379 69 22MB
English Pages 530 Year 1998
zy z
t L A
PLASTICS ENGINEERING
PLASTICS ENGINEERING
zy zyxwvuts zyxwv zyxw
Third Edition
R.J. Crawford, BSc, PhD, DSc, FEng, FIMechE, FIM Department of Mechanical, Aeronautical and Manufacturing Engineering The Queen’s University of Belfast
l E I N E M A N N
OXFORD AMSTERDAM BOSTON LONDON NEW YORK PARIS SAN DlEGO SAN FRANCISCO SINGAPORE SYDNEY TOKYO
ButterworthHeinemann An imprint of Elsevier Science Linacre House. Jordan Hill, Oxford OX2 8DP 225 Wildwood Avenue, Woburn, MA 018012041
zyxwvutsr
First published 1981 Second edition 1987 Reprinted with corrections 1990. 1992 Third edition 1998 Reprinted 1999.2001, 2002
Copyright 0 1987, 1998 R.J. Crawford. All rights reserved The right of R.J. Crawford to be identified as the author of this work has been asserted in accordance with the Copyright. Designs and Patents Act 1988
No part of this publication may be reproduced in any material form (including photocopying or storing in any medium by electronic means and whether or not transiently or incidentally to some other use of this publication) without the written permission of the copyright holder except in accordance with the provisions of the Copyright, Designs and Patents Act 1988 or under the terms of a licence issued by the Copyright Licensing Agency Ltd, 90 Tottenham Court Road, London, England WIT 4LP. Applications for the copyright holder’s written permission to reproduce any part of this publication should be addressed to the publishers.
zyxwvutsr zyxwvuts
British Library Cataloguing in Publication Data Crawford, R.J. (Roy J.) Plastics engineering. 3rd ed. 1. Plastics I. Title 668.4 ISBN 0 7506 3764 1
Library of Congress Cataloguing in Publication Data Crawford, R.J. Plastics engineering/R.J. Crawford  3rd ed. p. cm. Includes index. ISBN 0 7506 3764 1 (pbk). 1 Plastics. I Title TP1120 C74 668.4  dc21
9736604 CIP
For information on all ButterworthHeinemann publications visit our website at www.bh.com
Typeset by Laser Words, Chennai, India Printed by St Edmundsbury Press Ltd, Bury St Edmunds, Suffolk
Contents
zyxwvut zyxwv zyxw
Preface to the Third Edition Preface to the Second Edition Preface to the First Edition
Chapter 1  General Properties of Plastics 1.1 1.2
Introduction Polymeric Materials Plastics Available to the Designer 1.3 1.3.1 Engineering Plastics 1.3.2 Thermosets 1.3.3 Composites 1.3.4 Structural Foam 1.3.5 Elastomers 1.3.6 Polymer Alloys 1.3.7 Liquid Crystal Polymers 1.4 Selection of Plastics 1.4.1 Mechanical Properties 1.4.2 Degradation 1.4.3 Wear Resistance and Frictional Properties 1.4.4 Special Properties 1.4.5 Processing 1.4.6
Costs
xi
...
Xlll
xv
1
1 2 6 6 7 8 9 9 11 12 18 18 26 28 30 35 37
zyxwvu zyxwvut
vi
Contents
Chapter 2  Mechanical Behaviour of Plastics
2.1 Introduction 2.2 Viscoelastic Behaviour of Plastics 2.3 ShortTerm Testing of Plastics 2.4 LongTerm Testing of Plastics 2.5 Design Methods for Plastics using Deformation Data 2.6 Thermal Stresses and Strains 2.7 Multilayer Mouldings 2.8 Design of Snap Fits 2.9 Design of Ribbed Sections 2.10 Stiffening Mechanisms in Other Moulding Situations 2.1 1 Mathematical Models of Viscoelastic Behaviour 2.12 Intermittent Loading 2.12.1 Superposition Principle 2.12.2 Empirical Approach 2.13 Dynamic Loading of Plastics 2.14 TimeTemperature Superposition 2.15 Fracture Behaviour of Unreinforced Plastics 2.16 The Concept of Stress Concentration 2.17 Energy Approach to Fracture 2.18 Stress Intensity Factor Approach to Fracture 2.19 General Fracture Behaviour of Plastics 2.20 Creep Failure of Plastics 2.20.1 Fracture Mechanics Approach to Creep Fracture 2.20.2 Crazing in Plastics 2.21 Fatigue of Plastics 2.21.1 Effect of Cyclic Frequency 2.21.2 Effect of Waveform 2.21.3 Effect of Testing Control Mode 2.2 1.4 Effect of Mean Stress 2.21.5 Effect of Stress System 2.21.6 Fracture Mechanics Approach to Fatigue 2.22 Impact Behaviour of Plastics 2.22.1 Effect of Stress Concentrations 2.22.2 Effect of Temperature 2.22.3 Miscellaneous Factors Affecting Impact 2.22.4 Impact Test Methods 2.22.5 Fracture Mechanics Approach to Impact
41 42 43 45 48 61 66 71 74 81 84 95 95 103 110 116 119 121 121 127 131 134 136 137 138 140 142 142 143 145 145 147 148 150 152 152 154
zyxwvu
Chapter 3  Mechanical Behaviour of Composites 3.1 3.2
41
Deformation Behaviour of Reinforced Plastics Types of Reinforcement
168 168 168
Contents
zyxwvuts vii
Types of Matrix Forms of Fibre Reinforcement in Composites Analysis of Continuous Fibre Composites Deformation Behaviour of a Single Ply or Lamina Summary of Approach to Analysis of Unidirectional Composites 3.8 General Deformation Behaviour of a Single Ply 3.9 Deformation Behaviour of Laminates 3.10 Summary of Steps to Predict Stiffness of Symmetric Laminates 3.11 General Deformation Behaviour of Laminates 3.12 Analysis of Multilayer Isotropic Materials 3.13 Analysis of Nonsymmetric Laminates 3.14 Analysis of Short Fibre Composites 3.15 Creep Behaviour of Fibre Reinforced Plastics 3.16 Strength of Fibre Composites 3.16.1 Strength of Single Plies 3.16.2 Strength of Laminates 3.17 Fatigue Behaviour of Reinforced Plastics 3.18 Impact Behaviour of Reinforced Plastics
3.3 3.4 3.5 3.6 3.7
Chapter 4
170 171 172 182
188 195 202 206 208 218 223 226 232 232 234 236 238 240
zyxwvuts  Processing of Plastics
4.1 Introduction 4.2 Extrusion 4.2.1 General Features of Single Screw Extrusion 4.2.2 Mechanism of Flow 4.2.3 Analysis of Flow in Extruder 4.2.4 ExtruderDie Characteristics 4.2.5 Other Die Geometries 4.2.6 General Features of Twin Screw Extruders 4.2.7 Processing Methods Based on the Extruder 4.3 Injection Moulding 4.3.1 Introduction 4.3.2 Details of the Process 4.3.3 Moulds 4.3.4 Structural Foam Injection Moulding 4.3.5 Sandwich Moulding 4.3.6 Gas Injection Moulding 4.3.7 Shear Controlled Orientation in Injection Moulding (SCORIM) 4.3.8 Reaction Injection Moulding
245
245 246 246 25 1 252 257 259 262 264 278 278 279 285 297 298 299
30 1 302
...
Vlll
zyxwvu zyxwvutsrqpo zyx Contents
4.3.9 Injection Blow Moulding 4.3.10 Injection Moulding of Thermosetting Materials 4.4 Thermoforming 4.4.1 Analysis of Thermoforming 4.5 Calendering 4.5.1 Analysis of Calendering 4.6 Rotational Moulding 4.6.1 Slush Moulding 4.7 Compression Moulding 4.8 Transfer Moulding 4.9 Processing Reinforced Thermoplastics 4.10 Processing Reinforced Thermosets 4.10.1 Manual Processing Methods 4.10.2 SemiAutomatic Processing Methods 4.10.3 Automatic Processes Chapter 5  Analysis of polymer melt flow 5.1 Introduction 5.2 General Behaviour of Polymer Melts 5.3 Isothermal Flow in Channels: Newtonian Fluids Rheological Models for Polymer Melt Flow 5.4 Isothermal Flow in Channels: NonNewtonian Fluids 5.5 5.6 Isothermal Flow in NonUniform Channels Elastic Behaviour of Polymer Melts 5.7 5.8 Residence and Relaxation Times 5.9 Temperature Rise in Die 5.10 Experimental Methods Used to Obtain Flow Data 5.11 Analysis of Flow in Some Processing Operations 5.12 Analysis of Heat 'lkansfer during Polymer Processing 5.13 Calculation of Clamping force
303 304 306 309 313 315 318 323 323 326 327 328 330 332 337 343 343 344 346 35 1 354 357 363 367 368 369 375 39 1 40 1
Appendix A  Structure of Plastics
413
zyxwvu
A.l A.2 A.3
Structure of Long Molecules Conformation of the Molecular Chain Arrangement of Molecular Chains
413 415 420
Appendix B  Solution of Differential Equations
425
Appendix C  Stredstrain Relationships
426
Appendix D  Stresses in Cylindrical Shapes
429
zyxwvut zyxwv zyxwvu zyxwvutsr ix
Contents
Appendix E  Introduction to Matrix Algebra
E.1
E.2 E.3
E.4 E.5
Matrix definitions Matrix multiplication Matrix addition and subtraction Inversion of a matrix Symmetric matrix
Appendix F
 Abbreviations for some Common Polymers
43 1
43 1 432 432 433 433 434
Solutions to Questions
435
Index
50 1
Preface to the Third Edition
zyxw
Plastics continue to be exciting materials to use and a dynamic area in which to work. Every year new application areas are being developed to utilise more fully the unique properties of this class of materials. In addition, new processing technologies are emerging to exploit the versatility of plastics and to take advantage of their ease of manufacture into all types of end products. It is very important that students and those already working in the industry are kept fully informed about these new developments. In this new edition an attempt has been made to bring existing subject material up to date and many new sections have been added to cover the innovations introduced over the past decade. The number of Worked Examples has been increased and there are many more Set Questions at the end of each Chapter. As in the previous editions, a full set of solutions to the Set Questions is provided at the end of the book. In this new edition, some restructuring of the content has taken place. The subject material on Fracture that previously formed Chapter 3 has been brought forward to Chapter 2. This chapter now provides a more unified approach to the deformation and fracture behaviour of nonreinforced plastics. Chapter 3 is new and deals with all aspects of the mechanical behaviour of composites in much more detail than the previous editions. Composites are an extremely important class of material for modem design engineers and they must form an integral part of undergraduate and postgraduate teaching. There are many excellent textbooks devoted to this subject but it was felt that an introduction to the analysis of laminates would be a valuable addition to this text. It is hoped that the many worked examples in this new chapter will help the student, and the practising engineer, to gain a better understanding of this apparently complex subject area. Chapters 4 and 5 are essentially as before but they have been extensively updated. A more unified approach to the analysis of processing has also been adopted.
zyx zyxwvu
xii
Preface to the Third Edition
zyxwvu
As other authors will know, the preparation of a textbook is a demanding, challenging and timeconsuming occupation. I have been very fortunate to receive many encouraging comments on the previous editions and this has given me the enthusiasm to continue developing the subject material in the book. I am very grateful to all of those who have taken the trouble to contact me in the past and I continue to welcome comments and advice as to how the book could be improved in the future.
R.J.Crawford September 1997
Preface to the Second Edition
zyxw
In this book no prior knowledge of plastics is assumed. The text introduces the reader to plastics as engineering materials and leads on to the design procedures which are currently in use. Since the publication of the first edition the subject has developed in some areas, particularly processing and so this second edition contains the new and uptodate information. Other modifications have also been made to improve the presentation of the contents. In particular, Chapter 1 has been completely rewritten as an introduction to the general behaviour characteristics of plastics. The introduction to the structure of plastics which formed the basis of Chapter 1 in the first edition has been condensed into an Appendix in the new edition. Chapter 2 deals with the deformation behaviour of plastics. It has been expanded from the first edition to include additional analysis on intermittent loading and fibre composites. Chapter 3 deals with the fracture behaviour of plastics and here the importance of fracture mechanics has been given greater emphasis. Chapter 4 describes in general terms the processing methods which can be used for plastics. All the recent developments in this area have been included and wherever possible the quantitative aspects are stressed. In most cases a simple Newtonian model of each of the processes is developed so that the approach taken to the analysis of plastics processing is not concealed by mathematical complexity. Chapter 5 deals with the aspects of the flow behaviour of polymer melts which are relevant to the processing methods. The models are developed for both Newtonian and NonNewtonian (Power Law) fluids so that the results can be directly compared. Many more worked examples have been included in this second edition and there are additional problems at the end of each chapter. These are seen as an important aspect of the book because in solving these the reader is
zyxwvut zyxwvutsr
xiv
zy
Preface to the Second Edition
encouraged to develop the subject beyond the level covered in the text. To assist the reader a full set of solutions to the problems is provided at the back of the book.
R.J. Crawford January 1987
Preface to the First Edition
zyxw
This book presents in a single volume the basic essentials of the properties and processing behaviour of plastics. The approach taken and terminology used has been deliberately chosen to conform with the conventional engineering approach to the properties and behaviour of materials. It was considered that a book on the engineering aspects of plastics was necessary because there is currently a drive to attract engineers into the plastics industry and although engineers and designers are turning with more confidence to plastics there is still an underlying fear that plastics are difficult materials to work with. Their performance characteristics fall off as temperature increases and they are brittle at low temperatures. Their mechanical properties are time dependent and in the molten state they are nonNewtonian fluids. All this presents a gloomy picture and unfortunately most texts tend to analyse plastics using a level of chemistry and mathematical complexity which is beyond most engineers and designers. The purpose of this text is to remove some of the fears, by dealing with plastics in much the same way as traditional materials. The major part of this is to illustrate how quantitative design of plastic components can be carried out using simple techniques and how apparently complex moulding operations can be analysed without difficulty. Many of the techniques illustrated have been deliberately simplified and so they will only give approximate solutions but generally the degree of accuracy can be estimated and for most practical purposes it will probably be acceptable. Once the engineeddesigner has realised that there are proven design procedures for plastics which are not beyond their capabilities then these materials will be more readily accepted for consideration alongside established materials such as woods and metals. On these terms plastics can expect to be used in many new applications because their potential is limited only by the ingenuity of the user.
xvi
Preface to the First Edition
zyxwv
This book is intended primarily for students in the various fields of engineering but it is felt that students in other disciplines will welcome and benefit from the engineering approach. Since the book has been written as a general introduction to the quantitative aspects of the properties and processing of plastics, the depth of coverage is not as great as may be found in other texts on the physics, chemistry and stress analysis of viscoelastic materials. this has been done deliberately because it is felt that once the material described here has been studied and understood the reader will be in a better position to decide if he requires the more detailed viscoelastic analysis provided by the advanced texts. In this book no prior knowledge of plastics is assumed. Chapter 1 provides a brief introduction to the structure of plastics and it provides an insight to the way in which their unique structure affects their performance. There is a resume of the main types of plastics which are available. Chapter 2 deals with the mechanical properties of unreinforced and reinforced plastics under the general heading of deformation. The time dependent behaviour of the materials is introduced and simple design procedures are illustrated. Chapter 3 continues the discussion on properties but concentrates on fracture as caused by creep, fatigue and impact. The concepts of fracture mechanics are also introduced for reinforced and unreinforced plastics. Chapter 4 describes in general terms the processing methods which can be used for plastics and wherever possible the quantitative aspects are stressed. In most cases a simple Newtonian model of each of the processes is developed so that the approach taken to the analysis of plastics processing is not concealed by mathematical complexity. Chapter 5 deals with the aspects of the flow behaviour of polymer melts which are relevant to the processing methods. The models are developed for both Newtonian and NonNewtonian (Power Law) fluids so that the results can be directly compared. Throughout the book there are worked examples to illustrate the use of the theory and at the end of each chapter there are problems to be solved by the reader. These are seen as an important part of the book because in solving the problems the reader is encouraged to develop the subject material beyond the level covered in the text. Answers are given for all the questions.
zyxw R.J. Crawford
zyxwv
CHAPTER 1  General Properties of Plastics
1.1 Introduction
zyxwvu zyxwv
It would be difficult to imagine our modem world without plastics. Today they are an integral part of everyone’s lifestyle with applications varying from commonplace domestic articles to sophisticated scientific and medical instruments. Nowadays designers and engineers readily hun to plastics because they offer combinations of properties not available in any other materials. Plastics offer advantages such as lightness, resilience, resistance to corrosion, colour fastness, transparency, ease of processing, etc., and although they have their limitations, their exploitation is limited only by the ingenuity of the designer. The term plastic refers to a family of materials which includes nylon, polyethylene and PTFE just as zinc, aluminium and steel fall within the family of metals. This is an important point because just as it is accepted that zinc has quite different properties from steel, similarly nylon has quite different properties from ITFE. Few designers would simply specify metal as the material for a particular component so it would be equally unsatisfactory just to recommend plastic. This analogy can be taken still further because in the same way that there are different grades of steel there are also different grades of, say, polypropylene. In both cases the good designer will recognise this and select the most appropriate material and grade on the basis of processability, toughness, chemical resistance, etc. It is usual to think that plastics are a relatively recent development but in fact, as part of the larger family called polymers, they are a basic ingredient of animal and plant life. Polymers are different from metals in the sense that their structure consists of very long chainlike molecules. Namal materials such as silk, shellac, bitumen, rubber and cellulose have this type of structure. However, it was not until the 19th century that attempts were made to develop a synthetic
zyxwvutsr zyxw 1
2
zyxwvut zyxwvu zyxwvut General Properties of Plastics
polymeric material and the first success was based on cellulose. This was a material called Purkesine, after its inventor Alexander Parkes, and although it was not a commercial success it was a start and it led to the development of Celluloid. This material was an important breakthrough because it became established as a good replacement for natural materials which were in short supply  for example, ivory for billiard balls. During the early 20th century there was considerable interest in these new synthetic materials. Phenolformaldehyde (Bakelite) was introduced in 1909, and at about the time of the Second World War materials such as nylon, polyethylene and acrylic (Perspex) appeared on the scene. Unfortunately many of the early applications for plastics earned them a reputation as being cheap substitutes. It has taken them a long time to overcome this image but nowadays the special properties of plastics are being appreciated, which is establishing them as important materials in their own right. The ever increasing use of plastics in all kinds of applications means that it is essential for designers and engineers to become familiar with the range of plastics available and the types of performance characteristics to be expected so that these can be used to the best advantage. This chapter is written as a general introduction to design with plastics. It outlines the range of plastics available, describes the type of behaviour which they exhibit and illustrates the design process involved in selecting the best plastic for a particular application.
1.2 Polymeric Materials
zyxwv
Synthetic large molecules are made by joining together thousands of small molecular units known as monomers. The process of joining the molecules is called polymerisation and the number of these units in the long molecule is known as the degree of polymerisation. The names of many polymers consist of the name of the monomer with the suffix poly. For example, the polymers polypropylene and polystryene are produced from propylene and styrene respectively. Names, and symbols for common polymers are given in Appendix F. It is an unfortunate fact that many students and indeed design engineers are reluctant to get involved with plastics because they have an image of complicated materials with structures described by complex chemical formulae. In fact it is not necessary to have a detailed knowledge of the structure of plastics in order to make good use of them. Perfectly acceptable designs are achieved provided one is familiar with their performance characteristics in relation to the proposed service conditions. An awareness of the structure of plastics can assist in understanding why they exhibit a timedependent response to an applied force, why acrylic is transparent and stiff whereas polyethylene is opaque and flexible, etc., but it is not necessary for one to be an expert
zyxwvu zyx zyxwvu
General Properties of Plastics
3
in polymer chemistry in order to use plastics. Those who wish to to have a general introduction to the structure of plastics may refer to Appendix A. The words polymers and plastics are often taken as synonymous but in fact there is a distinction. The polymer is the pure material which results from the process of polymerisation and is usually taken as the family name for materials which have long chainlike molecules (and this includes rubbers). Pure polymers are seldom used on their own and it is when additives are present that the term plastic is applied. Polymers contain additives for a number of reasons. The following list outlines the purpose of the main additives used in plastics. Antistatic Agents. Most polymers, because they are poor conductors of current, build up a charge of static electricity. Antistatic agents attract moisture from the air to the plastic surface, improving its surface conductivity and reducing the likelihood of a spark or a discharge. Coupling Agents. Coupling agents are added to improve the bonding of the plastic to inorganic filler materials, such as glass fibres. A variety of silanes and titanates are used for this purpose. Fillers. Some fillers, such as short fibres or flakes of inorganic materials, improve the mechanical properties of a plastic. Others, called extenders, permit a large volume of a plastic to be produced with relatively little actual resin. Calcium carbonate, silica and clay are frequently used extenders. Flame Retardants. Most polymers, because they are organic materials, are flammable. Additives that contain chlorine, bromine, phosphorous or metallic salts reduce the likelihood that combustion will occur or spread. Lubricants. Lubricants such as wax or calcium stearate reduce the viscosity of the molten plastic and improve forming characteristics. Pigments. Pigments are used to produce colours in plastics. Plasticisers. Plasticisers are low molecular weight materials which alter the properties and forming characteristics of the plastic. An important example is the production of flexible grades of polyvinyl chloride by the use of plasticisers. Reinforcement. The strength and stiffness of polymers are improved by adding fibres of glass, carbon, etc. Stabilisers. Stabilisers prevent deterioration of the polymer due to environmental factors. Antioxidants are added to ABS, polyethylene and polystyrene. Heat stabilisers are required in processing polyvinyl chloride. Stabilisers also prevent deterioration due to ultraviolet radiation. There are two important classes of plastics.
(a) Thermoplastic Materials In a thermoplastic material the very long chainlike molecules are held together by relatively weak Van der Waals forces. A useful image of the structure is a mass of randomly distributed long strands of sticky wool. When the material is heated the intermolecular forces are weakened so that it becomes soft and flexible and eventually, at high temperatures, it is a viscous melt.
4
zyxwvutsr zyxwv zyxwv zyxwv zyxwvu zyxwv General Properties of Plastics
When the material is allowed to cool it solidifies again. This cycle of softening by heat and solidifying on cooling can be repeated more or less indefinitely and is a major advantage in that it is the basis of most processing methods for these materials. It does have its drawbacks, however, because it means that the properties of thermoplastics are heat sensitive. A useful analogy which is often used to describe these materials is that, like candle wax, they can be repeatedly softened by heat and will solidify when cooled. Examples of thermoplastics are polyethylene, polyvinyl chloride, polystyrene, nylon, cellulose acetate, acetal, polycarbonate, polymethyl methacrylate and polypropylene. An important subdivision within the thermoplastic group of materials is related to whether they have a crystalline (ordered) or an amorphous (random) structure. In practice, of course, it is not possible for a moulded plastic to have a completely crystalline structure due to the complex physical nature of the molecular chains (see Appendix A). Some plastics, such as polyethylene and nylon, can achieve a high degree of crystallinity but they are probably more accurately described as partially crystalline or semicrystalline. Other plastics such as acrylic and polystyrene are always amorphous. The presence of crystallinity in those plastics capable of crystallising is very dependent on their thermal history and hence on the processing conditions used to produce the moulded article. In turn, the mechanical properties of the moulding are very sensitive to whether or not the plastic possesses crystallinity. In general, plastics have a higher density when they crystallise due to the closer packing of the molecules. Qpical characteristics of crystalline and amorphous plastics are shown below.
I
Crystalline
Amorphous Broad soflening range  thermal agitation of the molecules breaks down the weak secondary bonds. The rate at which this occurs throughout the formless structure varies producing broad temperature range for softening. Usually transparent  the looser structure transmits light so the material appears transparent. Low shrinkage  all thermoplastics are processed in the amorphous state. On solidification, the random
a
Sharp melting point  the regular closepacked structure results in most of the secondary bonds being broken down at the same time. Usually opaque  the difference in refractive indices between the two phases (amorphous and crystalline) causes interference so the material appears translucent or opaque. High shrinkage  as the material solidifies from the
zyxwv
zyxwv zyx zyxwvut zyxwvu zyx zyx 5
General Properties of Plastics
Amorphous (continued)
Crystalline (continued)
arrangement of molecules produces little volume change and hence low shrinkage. Low chemical resistance  the more open random structure enables chemicals to penetrate deep into the material and to destroy many of the secondary bonds. Poor fatigue and wear resistance  the random structure contributes little to fatigue or wear properties.
a
amorphous state the polymers take up a closely packed, highly aligned structure. This produces a significant volume change manifested as high shrinkage. High chemical resistance  the tightly packed structure prevents chemical attack deep within the material. Good fatigue and wear resistance  the uniform structure is responsible for good fatigue and wear properties.
Examples of amorphous and crystalline thermoplastics Amorphous
Crystalline
zyxwv zyx
Polyvinyl Chloride (PVC) Polystyrene (PS) Polycarbonate (PC) Acrylic (PMMA) Acrylonitrilebutadienestyrene (ABS) Polyphenylene (PPO)
Polyethylene (PE) Polypropylene (PP) Polyamide (PA) Acetal (POM) Polyester (PEW, PBTF’) Fluorocarbons (PTFE, PFA, FEP and ETFE)
(b) Thermosetting Plastics A thermosetting plastic is produced by a chemical reaction which has two stages. The first stage results in the formation of long chainlike molecules similar to those present in thermoplastics, but still capable of further reaction. The second stage of the reaction (crosslinking of chains) takes place during moulding, usually under the application of heat and pressure. The resultant moulding will be rigid when cooled but a close network structure has been set up within the material. During the second stage the long molecular chains have been interlinked by strong bonds so that the material cannot be softened again by the application of heat. If excess heat is applied to these materials they will char and degrade. This type of behaviour is analogous to boiling an egg. Once the egg has cooled and is hard, it cannot be softened again by the application of heat. Since the crosslinking of molecules is by strong chemical bonds, thermosetting materials are characteristically quite rigid materials and their
6
zyxwvu zyxwvu zyxwvu General Properties of Plastics
mechanical properties are not heat sensitive. Examples of thermosets are phenol formaldehyde, melamine formaldehyde, urea formaldehyde, epoxies and some polyesters. 1.3 Plastics Available to the Designer
Plastics, more than any other design material, offer such a wide spectrum of properties that they must be given serious consideration in most component designs. However, this does not mean that there is sure to be a plastic with the correct combination of properties for every application. It simply means that the designer must have an awareness of the properties of the range of plastics available and keep an open mind. One of the most common faults in design is to be guided by preconceived notions. For example, an initial commitment to plastics based on an irrational approach is itself a serious design fault. A good design always involves a judicious selection of a material from the whole range available, including nonplastics. Generally, in fact, it is only against a background of what other materials have to offer that the full advantages of plastics can be realised. In the following sections most of the common plastics will be described briefly to give an idea of their range of properties and applications. However, before going on to this it is worthwhile considering briefly several of the special categories into which plastics are divided. 13.1 Engineering Plastics Many thermoplastics are now accepted as engineering materials and some are distinguished by the loose description engineering plastics. The term probably originated as a classification distinguishing those that could be substituted satisfactorily for metals such as aluminium in small devices and structures from those with inadequate mechanical properties. This demarcation is clearly artificial because the properties on which it is based are very sensitive to the ambient temperature, so that a thermoplastic might be a satisfactory substitute for a metal at a particular temperature and an unsatisfactory substitute at a different one. A useful definition of an engineering material is that it is able to support loads more or less indefinitely. By such a criterion thermoplastics are at a disadvantage compared with metals because they have low timedependent moduli and inferior strengths except in rather special circumstances. However, these rather important disadvantages are offset by advantages such as low density, resistance to many of the liquids that corrode metals and above all, easy processability. Thus, where plastics compete successfully with other materials in engineering applications it is usually because of a favourable balance of properties rather than because of an outstanding superiority in some particular respect, although the relative ease with which they can be formed into complex shapes tends to be a particularly dominant factor. In addition to conferring the
zyxwvu
General Properties of Plastics
zyxw zyx zyxw 7
possibility of low production costs, this ease of processing permits imaginative designs that often enable plastics to be used as a superior alternative to metals rather than merely as a tolerated substitute. Currently the materials generally regarded as making up the engineering plastics group are Nylon, acetal, polycarbonate, modified polyphenylene oxide (PPO), thermoplastic polyesters, polysulphone and polyphenylene sulphide. The newer grades of polypropylene also possess good basic engineering performance and this would add a further 0.5 m tonnes. And then there is unplasticised polyvinyl chloride (uPVC) which is widely used in industrial pipework and even polyethylene, when used as an artificial hip joint for example, can come into the reckoning. Hence it is probably unwise to exclude any plastic from consideration as an engineering material even though there is a subgroup specifically entitled for this area of application. In recent years a whole new generation of high performance engineering plastics have become commercially available. These offer properties far superior to anything available so far, particularly in regard to high temperature performance, and they open the door to completely new types of application for plastics. The main classes of these new materials are
(i) Polyarylethers and Polyarylthioethers polyarylethersulphones (PES) polyphenylene sulphide (PPS) polyethernitrile (PEN) polyetherketones (PEK and PEEK) (ii) Polyimides and Polybenzimidazole polyetherimide (PEI) thermoplastic polyimide (PI) polyamideimide (PAI)
(iii) Fluompolymers fluorinated ethylene propylene (FEiP) perfluoroalkoxy (PFA) A number of these materials offer service temperatures in excess of 200°C and fibrefilled grades can be used above 300°C.
1.3.2 Thermosets In recent years there has been some concern in the thermosetting material industry that usage of these materials is on the decline. Certainly the total market for thermoset compounds has decreased in Western Europe. This has happened for a number of reasons. One is the image that thermosets tend to have as oldfashioned materials with outdated, slow production methods. Other reasons include the arrival of high temperature engineering plastics
8
zyx
General Properties of Plastics
and miniaturisation in the electronics industry. However, thermosets are now fighting back and have a very much improved image as colourful, easyflow moulding materials with a superb range of properties. Phenolic moulding materials, together with the subsequently developed easyflowing, granular thermosetting materials based on urea, melamine, unsaturated polyester (UP) and epoxide resins, today provide the backbone of numerous technical applications on account of their nonmelting, high thermal and chemical resistance, stiffness, surface hardness, dimensional stability and low flammability. In many cases, the combination of properties offered by thermosets cannot be matched by competing engineering thermoplastics such as polyamides, polycarbonates, PPO, PET, PBT or acetal, nor by the considerably more expensive products such as polysulphone, polyethersulphone and PEEK.
zyxw
1.33 Composites One of the key factors which make plastics attractive for engineering applications is the possibility of property enhancement through fibre reinforcement. Composites produced in this way have enabled plastics to become acceptable in, for example, the demanding aerospace and automobile industries. Currently in the USA these industries utilise over 100,OOO tonnes of reinforced plastics out of a total consumption of over one million tonnes. Both thermoplastics and thermosets can reap the benefit of fibre reinforcement although they have developed in separate market sectors. This situation has arisen due to fundamental differences in the nature of the two classes of materials, both in terms of properties and processing characteristics. Thermosetting systems, hampered on the one hand by brittleness of the crosslinked matrix, have turned to the use of long, indeed often continuous, fibre reinforcement but have on the other hand been able to use the low viscosity state at impregnation to promote maximum utilization of fibre properties. Such materials have found wide application in large area, relatively low productivity, moulding. On the other hand, the thermoplastic approach with the advantage of toughness, but unable to grasp the benefit of increased fibre length, has concentrated on the short fibre, high productivity moulding industry. It is now apparent that these two approaches are seeking routes to move into each other’s territory. On the one hand the traditionally longfibre based thermoset products are accepting a reduction in properties through reduced fibre length, in order to move into high productivity injection moulding, while thermoplastics, seeking even further advances in properties, by increasing fibre length, have moved into longfibre injection moulding compounds and finally into truly structural plastics with continuous, aligned fibre thermoplastic composites such as the advanced polymer composite (APC)developed by IC1 and the stampable glass mat reinforced thermoplastics (GMT)developed in the USA. Glass fibres are the principal form of reinforcement used for plastics because they offer a good combination of strength, stiffness and price. Improved
zyxwv
General Properties of Plastics
9
strengths and stiffnesses can be achieved with other fibres such as aramid (Kevlar) or carbon fibres but these are expensive. The latest developments also include the use of hybrid systems to get a good balance of properties at an acceptable price. For example, the impact properties of carbonfibre composites can be improved by the addition of glass fibres and the stiffness of gfrp can be increased by the addition of carbon fibres. Another recent development is the availability of reinforced plastics in a form very convenient for moulding. One example is polyester dough and sheet moulding compounds (DMC and SMC respectively). DMC, as the name suggests, has a doughlike consistency and consists of short glass fibres (1520%) and fillers (up to 40%) in a polyester resin. The specific gravity is in the range 1.72.1. SMC consists of a polyester resin impregnated with glass fibres (203096). It is supplied as a sheet would into a roll with a protective polythene film on each side of the sheet. The specific gravity is similar to that of DMC and both materials are usually formed using heat and pressure in a closed mould (see Chapter 4 on moulding of gfrp).
zy
zyxwv
1.3.4 Structural Foam The concept of structural foams offers an unusual but exciting opportunity for designers. Many plastics can be foamed by the introduction of a blowing agent so that when moulded the material structure consists of a cellular rigid foam core with a solid tough skin. This type of structure is of course very efficient in material terms and offers an excellent strengthtoweight ratio. The foam effect is achieved by the dispersion of inert gas throughout the molten resin directly before moulding. Introduction of the gas is usually carried out by preblending the resin with a chemical blowing agent which releases gas when heated, or by direct injection of the gas (usually nitrogen). When the compressed gashesin mixture is rapidly injected into the mould cavity, the gas expands explosively and forces the material into all parts of the mould. An internal cellular structure is thus formed within a solid skin. Polycarbonate, polypropylene and modified PPO are popular materials for structural foam moulding. One of the main application areas is housings for business equipment and domestic appliances because the number of component parts can be kept to the absolute minimum due to integral moulding of wall panels, support brackets, etc. Other components include vehicle body panels and furniture. Structural foam mouldings may also include fibres to enhance further the mechanical properties of the material. Typical performance data for foamed polypropylene relative to other materials is given in Table 1.1. 1.3.5 Elastomers Conventional rubbers are members of the polymer family in that they consist of long chainlike molecules. These chains are coiled and twisted in a random
zy zyxwv
10
General Properties of Plastics
Table 1.1 Comparison of structural foams based on various grades of polypropylene with some traditional materials Unfilled copolymer
40% 30% talcfilled coupled glass Chiphomopolymer reinforced board
Pine
Alumi Mild nium steel
Solid Foam Solid Foam Solid Foam Flexural modulus MN/mz Specific gravity Relative thickness at equivalent rigidity Relative weight at equivalent rigidity
1.4 1.2 0.905 0.72
4.4 1.24
2.5 1.00
6.7 1.12
3.5 0.90
2.3 7.9 0.650 0.641
70 2.7
207 7.83
1
1.05
0.68
0.81
0.59
0.74
0.85
0.56
0.27
0.19
1
0.84
0.94
0.90
0.74
0.73
0.61
0.40
0.81
1.65
manner and have sufficient flexibility to allow the material to undergo very large deformations. In the green state the rubber would not be able to recover fully from large deformations because the molecules would have undergone irreversible sliding past one another. In order to prevent this sliding, the molecules are anchored together by a curing (vulcanisation) process. Thus the molecules are crosslinked in a way similar to that which occurs in thermosets. This linking does not detract from the random disposition of the molecules nor their coiled and twisted nature so that when the rubber is deformed the molecules stretch and unwind but do not slide. Thus when the applied force is removed the rubber will snap back to its original shape. Vulcanised rubbers possess a range of very desirable properties such as resilience, resistance to oils, greases and ozone, flexibility at low temperatures and resistance to many acids and bases. However, they require careful (slow) processing and they consume considerable amounts of energy to facilitate moulding and vulcanisation. These disadvantages led to the development of thermoplastic rubbers (elastomers).These are materials which exhibit the desirable physical characteristics of rubber but with the ease of processing of thermoplastics. At present there are five types of thermoplastic rubber (TPR).Three of these, the polyurethane, the styrenic and the polyester are termed segmented block copolymers in that they consist of thermoplastic molecules grafted to the rubbery molecules. At room temperature it is the thermoplastic molecules which clump together to anchor the rubbery molecules. When heat is applied the thermoplastic molecules are capable of movement so that the material may be shaped using conventional thermoplastic moulding equipment. The olefinic type of TPR is the latest development and is different in that it consists of fine rubber particles in a thermoplastic matrix as shown in Fig. 1.1.
zyxwvu
General Properties of Plastics
zyxwv zyxwvu 11
Rubber particles
Tkrmoplastic matrix Ipolypmpylenc~
zyxwv
zyx zyxw
Fig. 1.1 npical structure of olefinic TF'R
The matrix is usually polypropylene and it is this which melts during processing to permit shaping of the material. The rubber filler particles then contribute the flexibility and resilience to the material. The other type of TPR is the polyamide and the properties of all five types are summarised in Table 1.4.
1.3.6 Polymer Alloys The development of new polymer alloys has caused a lot of excitement in recent years but in fact the concept has been around for a long time. Indeed one of the major commercial successes of today, ABS, is in fact an alloy of acrylonitrile, butadiene and styrene. The principle of alloying plastics is similar to that of alloying metals  to achieve in one material the advantages possessed by several others. The recent increased interest and activity in the field of polymer alloys has occurred as a result of several new factors. One is the development of more sophisticated techniques for combining plastics which were previously considered to be incompatible. Another is the keen competition for a share of new market areas such as automobile bumpers, body panels etc. These applications call for combinations of properties not previously available in a single plastic and it has been found that it is less expensive to combine existing plastics than to develop a new monomer on which to base the new plastic. In designing an alloy, polymer chemists choose candidate resins according to the properties, cost, and/or processing characteristics required in the end product. Next, compatibility of the constituents is studied, tested, and either optimised or accommodated. Certain polymers have come to be considered standard building blocks of the polyblends. For example, impact strength may be improved by using polycarbonate, ABS and polyurethanes. Heat resistance is improved by using polyphenylene oxide, polysulphone, PVC, polyester (PET and PBT) and acrylic. Barrier properties are improved by using plastics such as ethylene vinyl alchol (EVA). Some modern plastic alloys and their main characteristics are given in Table 1.2.
zyxwv zy zyxwv zyx zyxwvu General Properties of Plastics
12
Table 1.2
vpical plastic alloys
Alloy PVClacrylic PVC/ABS Polycarbonate/ABS ABSPolysulphone Polyphenylene oxide/HIPS SAN/olefin Nylon/elastomer Modified amorphous nylon PolycarbonatePBT
Features
Tough with good flame and chemical resistance Easily processed with good impact and flame resistance Hard with high heat distortion temperature and good notch impact strength Less expensive than unmodified polysulphone Improved processability, reduced cost Good weatherability Improved notched impact strength Easily processed with excellent surface finish and toughness Tough engineering plastic
1.3.7 Liquid Crystal Polymers Liquid crystal polymers (LCP) are a recent arrival on the plastics materials scene. They have outstanding dimensional stability, high strength, stiffness, toughness and chemical resistance all combined with ease of processing. LCPs are based on thermoplastic aromatic polyesters and they have a highly ordered structure even in the molten state. When these materials are subjected to stress the molecular chains slide over one another but the ordered structure is retained. It is the retention of the highly crystalline structure which imparts the exceptional properties to LCPs. Typical Characteristics of Some Important Plastics (a) Semicrystalline plastics Low density polyethylene (LDPE). This is one of the most widely used plastics. It is characterised by a density in the range 918935 kg/m3 and is very tough and flexible. Its major application is in packaging film although its outstanding dielectric properties means it is also widely used as an electrical insulator. Other applications include domestic ware, tubing, squeeze bottles and cold water tanks. Linear Low Density Polyethylene (LLDPE). This new type of polyethylene was introduced in 1977. LLDPE is produced by a low pressure process and it has a regular structure with short chain branches. Depending on the cooling rate from the melt, the material forms a structure in which the molecules are linked together. Hence for any given density, LLDPE is stiffer than LDPE and exhibits a higher yield strength and greater ductility. Although the difference melt processing characteristics of LLDPE take a little getting used to, this new material has taken over traditional LDPE markets. High Density Polyethylene (HDPE). This material has a density in the range 935965 kg/m3 and is more crystalline than LDPE. It is also slightly more
General Properties of Plastics
13
expensive but as it is much stronger and stiffer it finds numerous applications in such things as dustbins, bottle crates, general purpose fluid containers and pipes. One of the most exciting recent developments in this sector has been the introduction to the marketplace of metallocenebased polyethylenes. Metallocenes have been recognised as suitable catalysts for the manufacture of polyethylenes since the 1950s. However, it is only recently that their use has been perfected. Their big advantage is that they are single site catalysts so that the polymer molecules which are produced tend to be all the same  a fact which offers an array of superior properties. Traditional catalysts for polyethylene (Ziegler Natta catalysts) are multisited so that they produce polymers with short, medium and long molecules. In the new metallocene grades of polyethylene, the absence of low molecular weight species results in low extractables, a narrow melting range and freeflowing material even at low densities. The absence of high molecular weight species contributes excellent melting point control, clarity and improved flexibility/toughness at low temperatures. Metallocenebased polyethylene does not offer the lower production costs associated with LLDPE. Hence there will be a price premium for the new materials but this is felt to be justified in view of their improved property profile. CrosslinkedPolyethylene (XLPE). Some thermoplastic materials such as polyethylene can have their structure altered so that the molecular chains become crosslinked and the material then behaves like a thermoset. In the case of polyethylene, a range of crosslinking methods are available. These include the use of radiation, peroxides and silanes. In some cases the crosslinking can occur during moulding whereas in other cases the endproduct shape is created before the crosslinking is initiated. The action of crosslinking has a number of beneficial effects including improved stress crack resistance, improved creep resistance, better chemical resistance, improved toughness and better general thermomechanical stability. Polypropylene (PP). Polypropylene is an extremely versatile plastic and is available in many grades and also as a copolymer (ethylene/propylene). It has the lowest density of all thermoplastics (in the order of 900 kg/m3 and this combined with strength, stiffness and excellent fatigue and chemical resistance make it attractive in many situations. These include crates, small machine parts, car components (fans, fascia panels etc), chair shells, cabinets for TV, tool handles, etc. Its excellent fatigue resistance is utilised in the moulding of integral hinges (e.g. accelerator pedals and forceps/tweezers). Polypropylene is also available in fibre form (for ropes, carpet backing) and as a film (for packaging). Polyamides (nylon). There are several different types of nylon (e.g. nylon 6, nylon 66, nylon 11) but as a family their characteristics of strength, stiffness and toughness have earned them a reputation as engineering plastics. Table 1.3 compares the relative merits of light metal alloys and nylon.
zyx zyxwvut zyxwvu
zyxwv
14
zyxwvuts zyxwv zyx General Properties of Plastics
Table 1.3
Comparison between die casting alloys and nylons
Points for comparison
Die casting alloys
Cost of raw materidtonne Cost of mould Speed of component production Accuracy of component Post moulding operations
LOW
Surface hardness
Low  scratches easily
Rigidity
Good to brittleness
Elongation
LOW
Toughness (flexibility)
LOW
Impact Notch sensitivity Youngs modulus (E) General mechanical properties Heat conductivity Electrical insulation Weight Component assembly
Low
Nylon
zyxwvu
High Slower than injection moulding of nylon Good Finishing  painting. Paint chips off easily
High Can be lower  no higher Lower component production costs Good Finishing not required painting not required. Compounded colour retention permanent. Much higher. Scratch resistant. Glass reinforced grades as good or better GR grades comparable unfilled grades excellent GR grades comparable unfilled grades excellent All grades good

LOW
LOW
Consistent Similar to GR grades of 66 nylon High Low High Snap fits difficult
Varies with load Higher compressive strength Low High Low very good
Typical applications for nylon include small gears, bearings, bushes, sprockets, housings for power tools, terminal blocks and slide rollers. An important design consideration is that nylon absorbs moisture which can affect its properties and dimensional stability. Glass reinforcement reduces this problem and produces an extremely strong, impact resistant material. Another major application of nylon is in fibres which are notoriously strong. The density of nylon is about 1100 kg/m3. Acetals. The superior properties of acetal in terms of its strength, stiffness and toughness have also earned it a place as an engineering plastic. It is more dense than nylon but in many respects their properties are similar and they can be used for the same types of light engineering application. A factor which may favour acetal in some cases is its relatively low water absorption. The material is available as both a homopolymer and a copolymer. The former is slightly stronger and stiffer whereas the copolymer has improved high temperature performance. This latter feature makes this material very attractive for hot water plumbing applications and as the body for electric kettles.
General Properties of Plastics
zy zyxwv 15
Polytetrafluoroethylene(PTFE). The major advantages of this material are its excellent chemical resistance and its extremely low coefficient of friction. Not surprisingly its major area of application is in bearings particularly if the environment is aggressive. It is also widely used in areas such as insulating tapes, gaskets, pumps, diaphragms and of course nonstick coatings on cooking utensils. Thermoplastic Polyesters. These linear polyesters are highly crystalline and exhibit toughness, strength, abrasion resistance, low friction, chemical resistance and low moisture absorption. Polyethylene terephthalate (PET) has been available for many years but mainly as a fibre (e.g. Terylene). As a moulding material it was less attractive due to processing difficulties but these were overcome with the introduction of polybutylene terephthalate (PBT). Applications include gears, bearings, housings, impellers, pulleys, switch parts, bumper extensions, etc. and of course PET is now renowned for its success as a replacement for glass in beverage bottles. PBT does not have such a high performance specification as PET but it is more readily moulded. Polyetheretherketone. This material, which is more commonly known as PEEK, is one of the new generation plastics which offer the possibility of high service temperatures. It is crystalline in nature which accounts in part for its high resistance to attack from acids, alkalis and organic solvents. It is easily processed and may be used continuously at 200°C where it offers good abrasion resistance, low flammability, toughness, strength and good fatigue resistance. Its density is 1300 kg/m3. Applications include wire coatings, electrical connections, fans, impellers, fibres, etc.
zyxw
(b) Amorphous plastics Polyvinyl Chloride (PVC). This material is the most widely used of the
amorphous plastics. It is available in two forms  plasticised or unplasticised. Both types are characterised by good weathering resistance, excellent electrical insulation properties, good surface properties and they are self extinguishing. Plasticised PVC is flexible and finds applications in wire covering, floor tiles, toy balls, gloves and rainwear. Unplasticised PVC (uPVC) is hard, tough, strong material which is widely used in the building industry. For example, pipes, gutters, window frames and wall claddings are all made in this material. The familiar credit cards are also made from uPVC. Polymethyl Methacrylate (PMMA). This material has exceptional optical clarity and resistance to outdoor exposure. It is resistant to alkalis, detergents, oils and dilute acids but is attacked by most solvents. Its peculiar property of total internal reflection is useful in advertising signs and some medical applications. Qpical uses include illuminated notices, control panels, domelights, lighting diffusers, baths, face guards, nameplates, lenses and display models. Polystyrene (PS). Polystyrene is available in a range of grades which generally vary in impact strength from brittle to very tough. The nonpigmented
16
zyxwvuts zyxw zyxwv General Properties of Plastics
grades have crystal clarity and overall their low cost coupled with ease of processing makes them used for such things as model aircraft kits, vending cups, yoghurt containers, light fittings, coils, relays, disposable syringes and casings for ballpoint pens. Polystyrene is also available in an expanded form which is used for such things as ceiling tiles and is excellent as a packaging material and thermal insulator. Acrylonitrilebutadienestyrene (ABS). ABS materials have superior strength, stiffness and toughness properties to many plastics and so they are often considered in the category of engineering plastics. They compare favourably with nylon and acetal in many applications and are generally less expensive. However, they are susceptible to chemical attack by chlorinated solvents, esters, ketones, acids and alkalis. Qpical applications are housings for TV sets, telephones, fascia panels, hair brush handles, luggage, helmets and linings for refrigerators. Polycarbonates. These materials also come within the category of engineering plastics and their outstanding feature is extreme toughness. They are transparent and have good temperature resistance but are attacked by alkaline solutions and hydrocarbon solvents. Qpical applications include vandalproof street lamp covers, baby feeding bottles, machine housings and guards, camera parts, electrical components, safety equipment and compact discs. Polyethersulphone. This material is one of the new high temperature plastics. It is recommended for load bearing applications up to 180°C. Even without flame retardants it offers low flammability and there is little change in dimensions of electrical properties in the temperature range 0200°C. It is easily processed on conventional moulding equipment. Applications include aircraft heating ducts, terminal blocks, engine manifolds, bearings, grilles, tool handles, nonstick coatings. Modified Polyphenylene Oxide (PPO). The word modijied in this material refers to the inclusion of high impact polystyrene to improve processability and reduce the cost of the basic PPO. This material offers a range of properties which make it attractive for a whole range of applications. For example, it may be used at 100150°C where it is rigid, tough and strong with good creep resistance and hydrolytic stability. Water absorption is very small and there is excellent dimensional stability. Applications include business machine parts, flow values, headlight parts, engine manifolds, fascia panels, grilles, pump casings, hair dryer housings, etc.
zyxw
(c) Thermoplastic Rubbers There are five types of thermoplastic rubbers currently available. These are based on (i) Olefinics (e.g. Alcryn, Suntoprene) (ii) Polyurethanes (e.g. EZustollun, Cuprolun, Pellethune) (iii) Polyesters (e.g. Hytrel, Arnitel) (iv) Styrenics (e.g. Solprene, CuriJlex) and (v) Polyamides (e.g. Pebax, Dinyl) Some typical properties are given in Table 1.4.
General Properties of Plastics
zyxwvu zyxw 17
zyxwvu zyxwv
Table 1.4
Physical characteristics of thermoplastic rubbers
5Pe
Olefinic
Hardness (Shore AD) Resilience (%) Tensile strength (MN/m2) Resistances Chemicals Oils Solvents Weathering Specific gravity Service temperature ("C)
60A to 60D 60A to 60D 30 to 40 40 to 50
40D to 72D 30A to 45D 40D to 63D 60 to 70 43 to62
8 to 20
30 to 55
21 to 45
25 to 45
F F PIF E 0.97 1.34 50130
PIG E F G 1.11 1.21 40130
E E G E 1.171.25 65 130
E F P
Polyurethane Polyester
Styrenic
PIE
0.931.0 30 120
Polyamide
PIE
PIE E 1.0 1.12 65130
(d) Thermosetting Plastics Aminos. There are two basic types of amino plastics  urea formaldehyde and melamine formaldehyde. They are hard, rigid materials with good abrasion resistance and their mechanical characteristics are sufficiently good for continuous use at moderate temperatures (up to 100°C). Urea formaldehyde is relatively inexpensive but moisture absorption can result in poor dimensional stability. It is generally used for bottle caps, electrical switches, plugs, utensil handles and trays. Melamine formaldehyde has lower water absorption and improved temperature and chemical resistance. It is typically used for tableware, laminated worktops and electrical fittings. Phenolics. Phenolformaldehyde (Bakelite) is one of the oldest synthetic materials available. It is a strong, hard, brittle material with good creep resistance and excellent electrical properties. Unfortunately the material is only available in dark colours and it is susceptible to attack by alkalis and oxidising agents. Typical applications are domestic electrical fittings, saucepan handles, fan blades, smoothing iron handles and pump parts. Polyurethanes. This material is available in three forms  rigid foam, flexible foam and elastomer. They are characterised by high strength and good chemical and abrasion resistance. The rigid foam is widely used as an insulation material, the flexible foam is an excellent cushion material for furniture and the elastomeric material is used in solid tyres and shock absorbers. Polyesters. The main application of this material is as a matrix for glass fibre reinforcement. This can take many forms and is probably most commonly known as a DIY type material used for the manufacture of small boats, chemical containers, tanks and repair kits for cars, etc. Epoxides. Epoxy resins are more expensive than other equivalent thermosets (e.g. polyesters) but they an generally outperform these materials due to better
18
zyxwvutsrq zyx zyx zyxw zyxwv zyxwv zy General Properties of Plastics
toughness, less shrinkage during curing, better weatherability and lower moisture absorption. A major area of application is in the aircraft industry because of the combination of properties offered when they are reinforced with fibres. They have an operating temperature range of 25 to 150°C.
1.4 Selection of Plastics
The previous section has given an indication of the range of plastics available to the design engineer. The important question then arises How do we decide which plastic, if any, is best for a particular application? Material selection is not as difficult as it might appear but it does require an awareness of the general behaviour of plastics as a group, as well as a familiarity with the special characteristics of individual plastics. The first and most important steps in the design process are to define clearly the purpose and function of the proposed product and to identify the service environment. Then one has to assess the suitability of a range of candidate materials. The following are generally regarded as the most important characteristics requiring consideration for most engineering components.
(1) mechanical properties  strength, stiffness, specific strength and stiffness, fatigue and toughness, and the influence of high or low temperatures on these properties; (2) corrosion susceptibility and degradation (3) wear resistance and frictional properties; (4) special properties, for example, thermal, electrical, optical and magnetic properties, damping capacity, etc; (5) moulding and/or other methods of fabrication. (6) total costs attributable to the selected material and manufacturing route.
In the following sections these factors will be considered briefly in relation to plastics.
1.4.1 Mechanical Properties Strength and Stiffness. Thermoplastic materials are viscoelastic which means that their mechanical properties reflect the characteristics of both viscous liquids and elastic solids. Thus when a thermoplastic is stressed it responds by exhibiting viscous flow (which dissipates energy) and by elastic displacement (which stores energy). The properties of viscoelastic materials are time, temperature and strain rate dependent. Nevertheless the conventional stressstrain test is frequently used to describe the (shortterm) mechanical properties of plastics. It must be remembered, however, that as described in detail in Chapter 2 the information obtained from such tests may only be used for an initial sorting of materials. It is not suitable, or intended, to provide design data which must usually be obtained from long term tests.
General Properties of Plastics
19
In many respects the stressstrain graph for a plastic is similar to that for a metal (see Fig. 1.2). At low strains there is an elastic region whereas at high strains there is a nonlinear relationship between stress and strain and there is a permanent element to the strain. In the absence of any specific information for a particular plastic, design strains should normally be limited to 1%. Lower values (0.5%) are recommended for the more brittle thermoplastics such as acrylic, polystyrene and values of 0.20.3% should be used for thermosets. The effect of material temperature is illustrated in Fig. 1.3. As temperature is increased the material becomes more flexible and so for a given stress the
Fig. 1.2 Qpical stressstrain graph for plastics
zy
zyxw
zyx f zyxwv zyxw 20°C
20°C 50°C
70°C
Strain (7")
Fig. 1.3 Effect of material temperature on stressstrain behaviour of plastics
zyxw zyxw General Properties of Plastics
20
material deforms more. Another important aspect to the behaviour of plastics is the effect of strain rate. If a thermoplastic is subjected to a rapid change in strain it appears stiffer than if the same maximum strain were applied but at a slower rate. This is illustrated in Fig. 1.4.
O
I
O
l
z
zyxwvu zyx
1 1
Z 3 4 Strain (“A)
5
Fig. 1.4 Effect of strain rate on stressstrain behaviour of plastics
zyxw
It is important to realise also that within the range of grades that exist for a particular plastic, there can be significant differences in mechanical properties. For example, with polypropylene for each 1 kg/m3 change in density there is a corresponding 4% change in modulus. Fig. 1.5 illustrates the typical variation which occurs for the different grades of ABS. It may be seen that very often a grade of material selected for some specific desirable feature (e.g. high impact strength) results in a decrease in some other property of the material (e.g. tensile strength). The stiffness of a plastic is expressed in terms of a modulus of elasticity. Most values of elastic modulus quoted in technical literature represent the slope of a tangent to the stressstrain curve at the origin (see Fig. 1.6). This is often referred to as Youngs modulus, E, but it should be remembered that for a plastic this will not be a constant and, as mentioned earlier, is only useful for quality
General Properties of Plastics 50
zyxw 21
zyx zyxwvu zyxwv Highheat grade
40
Mediumimpact Highimpact impact
Strain (%)
zy
Fig. 1.5 Effect of grade on mechanical properties of ABS
‘4/ /k sm
Slope represents tangent, OrYoung‘s modulus
0
zyxwvut c’
Strain
Fig. 1.6 Tangent and secant modulus
control purposes, not for design. Since the tangent modulus at the origin is sometimes difficult to determine precisely, a secant modulus is often quoted to remove any ambiguity. A selected strain value of, say 2% (point C’, Fig. 1.6) enables a precise point, C, on the stressstrain curve to be identified. The slope of a line through C and 0 is the secant modulus. npical shortterm mechanical
22
General Roperties of Plastics
properties of plastics are given in Table 1.5. These are given for illustration purposes. For each type of plastic there are many different grades and a wide variety of properties are possible. The literature supplied by the manufacturers should be consulted in specific instances.
zyxw zy zyxwvu zyxwvutsr zyxwvu Table 1.5
Shortterm properties of some important plastics
Material
A B S (high impact) Acetal (homopolymer) Acetal (copolymer) Acrylic Cellulose acetate CAB EPOXY Modified PPO Nylon 66 Nylon 66 (33% glass) PEEK PEEK (30% carbon) PET PET (36% glass) Phenolic (mineral filled) Polyamideimide Polycarbonate Polyetherimide Polyethersulphone Polyimide Polypropylene Polysulphone Polystyrene Polythene (LD) Polythene (HD)
rn
PVC (rigid) PVC (flexible) SAN DMC (polyester) SMC (polyester)
Density (kg/m3) 1040 1420 1410 1180 1280 1190 1200 1060
1140 1380 1300 1400 1360 1630 1690 1400 1150 1270 1370 1420 905 1240 1050 920 950
2100 1400 1300 1080 1800 1800
Tensile strength (MN/m*) 38 68 70 70 30 25 70 45 70 115 62 240 75 180 55 185 65 105 84 72 33 70
Flexural modulus (GN/m2) 2.2 2.8 2.6 2.9 1.7 1.3 3.0 2.3 2.8 5.1 3.8 14 3 12 8.O 4.5 2.8 3.3 2.6 2.5 1.5 2.6 3.0 0.2 1.2
%
elongation at break 8 40 65 2 30 60 3 70 60 4 4 1.6 70 3 0.8 12 100 60 60 8 150 80 1.5 400 150 200 80 300 2 2 3
Price* 2.1 3.5 3.3 2.5 3.2 8.3

3.9 4.0 42
44 3.0 3.5 1.25 67 4.2
zyxwvu 40 10 32 25
50
14 72 40 70
0.5
3.0 0.007 3.6 9.0 11.0

13.3 150 1 11 1.1 0.83 1.1 13.3 0.88 0.92 1.8 1.5 1.3
*On a weight basis, relative to polypropylene.
Material Selection for Strength If, in service, a material is required to have a certain strength in order to per€orm its function satisfactorily then a useful way to compare the structural efficiency of a range of materials is to calculate their strength desirability factor. Consider a structural member which is essentially a beam subjected to bending (Fig. 1.7). Irrespective of the precise nature of the beam loading the
zyxwvu zyxwvu zyxwv zyxw z zyx zyxwvuts zyxwv
General Properties of Plastics
23
Fig. 1.7 Beam subjected to bending
maximum stress, 0,in the beam will be given by (T=
MmaX(dl2) I
 MInaX(dl2) bd2/12
Assuming that we are comparing different materials on the basis that the mean length, width and loading is fixed but the beam depth is variable then equation (1.1) may be written as (T
= /?,Id2
(1.2)
where /?I is a constant. But the weight, w,of the beam is given by w = pbdL
(1.3)
So substituting for d from (1.2) into (1.3)
w = /32p/(T”2
(1.4)
where Bz is the same constant for all materials. Hence, if we adopt loading/weight as a desirability factor, Df,then this will be given by (Til2
Df = P
(1.5)
where cry and p are the strength and density values for the materials being compared. Similar desirability factors may be derived for other geometries such as struts, columns etc. This concept is taken further later where material costs are taken into account and Tables 1.1 1 and 1.12 give desirability factors for a range of loading configurations and materials.
Material Selection for Stiffness If in the service of a component it is the deflection, or stiffness, which is the limiting factor rather than strength, then it is necessary to look for a different desirability factor in the candidate materials. Consider the beam situation described above. This time, irrespective of the loading, the deflection, 6,
24
zyxwvu zyxw zyxwv zyxwvuts zyxwvut zyxw zy General Properties of Plastics
will be given by
6=a1
(G)
where a1 is a constant and W represents the loading. The stiffness may then be expressed as
W
where a2 is a constant and again it is assumed that the beam width and length are the same in all cases. Once again the beam weight will be given by equation (1.3) so substituting for d from equation (1.7) w = ( ~ 3 p / 1/3 E (1.8) Hence, the desirability factor, Df, expressed as maximum stiffness for minimum weight will be given by
where E is the elastic modulus of the material in question and p is the density. As before a range of similar factors can be derived for other structural elements and these are illustrated in Section 1.4.6. (Tables 1.11 and 1.12) where the effect of material cost is also taken into account. Note also that since for plastics the modulus, E, is not a constant it is often necessary to use a longterm (creep) modulus value in equation (1.9) rather than the shortterm quality control value usually quoted in trade literature. Ductility. A loadbearing device or component must not distort so much under the action of the service stresses that its function is impaired, nor must it fail by rupture, though local yielding may be tolerable. Therefore, high modulus and high strength, with ductility, is the desired combination of attributes. However, the inherent nature of plastics is such that high modulus tends to be associated with low ductility and steps that are taken to improve the one cause the other to deteriorate. The major effects are summarised in Table 1.6. Thus it may be seen that there is an almost inescapable rule by which increased modulus is accompanied by decreased ductility and vice versa. Creep and Recovery Behaviour. Plastics exhibit a timedependent strain response to a constant applied stress. This behaviour is called creep. In a similar fashion if the stress on a plastic is removed it exhibits a time dependent recovery of strain back towards its original dimensions. This is illustrated in
zyxwv
General Properties of Plastics
zyxwv 25
Table 1.6
Balance between stiffness and ductility in thermoplastics Effect on
Reduced temperature Increased straining rate Multiaxial stress field Incorporation of plasticizer Incorporation of rubbery phase Incorporation of glass fibres Incorporation of particulate filler
Modulus
Ductility
increase increase increase decrease decrease increase increase
decrease decrease decrease increase increase decrease decrease
zyx
zyxwvut zyxwv zyxwv t 1 zyxwvutsrqpo
2. As stress is maintained, sample deforms Icreeps) viscoelostically to Point B,
3. Load is removed, and sample recovers elastically to Paint C immediately.
Viscoelastic deformation
Elastic recowry
Viscoelastic recovery
Time
1.
Load is opplied instantaneously, resulting in strain A
4.
Sample recovers viscoelastically to Point D
Fig. 1.8 npical Creep and recovery behaviour of a plastic
Fig. 1.8 and because of the importance of these phenomena in design they are dealt with in detail in Chapter 2. Stress Relaxation. Another important consequence of the viscoelastic nature of plastics is that if they are subjected to a particular strain and this strain is held constant it is found that as time progresses, the stress necessary to maintain this strain decreases. This is termed stress relaxation and is of vital importance in the design of gaskets, seals, springs and snapfit assemblies. This subject will also be considered in greater detail in the next chapter. Creep Rupture. When a plastic is subjected to a constant tensile stress its strain increases until a point is reached where the material fractures. This is called creep rupture or, occasionally, static fatigue. It is important for designers
zyx
26
zyxwvuts zy General Properties of Plastics
to be aware of this failure mode because it is a common error, amongst those accustomed to dealing with metals, to assume that if the material is capable of withstanding the applied (static) load in the short term then there need be no further worries about it. This is not the case with plastics where it is necessary to use longterm design data, particularly because some plastics which are tough at short times tend to become embrittled at long times. Fatigue. Plastics are susceptible to brittle crack growth fractures as a result of cyclic stresses, in much the same way as metals are. In addition, because of their high damping and low thermal conductivity, plastics are also prone to thermal softening if the cyclic stress or cyclic rate is high. The plastics with the best fatigue resistance are polypropylene, ethylenepropylene copolymer and PVDF. The fatigue failure of plastics is described in detail in Chapter 2. Toughness. By toughness we mean the resistance to fracture. Some plastics are inherently very tough whereas others are inherently brittle. However, the picture is not that simple because those which are nominally tough may become embrittled due to processing conditions, chemical attack, prolonged exposure to constant stress, etc. Where toughness is required in a particular application it is very important therefore to check carefully the service conditions in relation to the above type of factors. At mom temperature the toughest unreinforced plastics include nylon 66, LDPE, LLDPE, EVA and polyurethane structural foam. At subzero temperatures it is necessary to consider plastics such as ABS, polycarbonate and EVA. The whole subject of toughness will be considered more fully in Chapter 2.
zyxwvu
1.4.2 Degradation Physical or Chemical Attack. Although one of the major features which might
prompt a designer to consider using plastics is corrosion resistance, nevertheless plastics are susceptible to chemical attack and degradation. As with metals, it is often difficult to predict the performance of a plastic in an unusual environment so it is essential to check material specifications and where possible carry out proving trials. Clearly, in the space available here it is not possible to give precise details on the suitability of every plastic in every possible environment. Therefore the following sections give an indication of the general causes of polymer degradation to alert the designer to a possible problem. The degradation of a plastic occurs due to a breakdown of its chemical structure. It should be recognised that this breakdown is not necessarily caused by concentrated acids or solvents. It can occur due to apparently innocuous mediums such as water (hydrolysis), or oxygen (oxidation). Degradation of plastics is also caused by heat, stress and radiation. During moulding the material is subjected to the first two of these and so it is necessary to incorporate stabilisers and antioxidants into the plastic to maintain the properties of the material. These additives also help to delay subsequent degradation for an acceptably long time.
General Properties of Plastics
27
zyxw zyxw
As regards the general behaviour of polymers, it is widely recognised that crystalline plastics offer better environmental resistance than amorphous plastics. This is as a direct result of the different structural morphology of these two classes of material (see Appendix A). Therefore engineering plastics which are also crystalline e.g. Nylon 66 are at an immediate advantage because they can offer an attractive combination of loadbearing capability and an inherent chemical resistance. In this respect the anival of crystalline plastics such as PEEK and polyphenylene sulfide (PPS) has set new standards in environmental resistance, albeit at a price. At room temperature there is no known solvent for PPS, and PEEK is only attacked by 98% sulphuric acid. Weathering. This generally occurs as a result of the combined effect of water absorption and exposure to ultraviolet radiation (uv). Absorption of water can have a plasticizing action on plastics which increases flexibility but ultimately (on elimination of the water) results in embrittlement, while uv causes breakdown of the bonds in the polymer chain. The result is general deterioration of physical properties. A loss of colour or clarity (or both) may also occur. Absorption of water reduces dimensional stability of moulded articles. Most thermoplastics, in particular cellulose derivatives, are affected, and also polyethylene, PVC, and nylons. Oxidation. This is caused by contact with oxidising acids, exposure to uv, prolonged application of excessive heat, or exposure to weathering. It results in a deterioration of mechanical properties (embrittlement and possibly stress cracking), increase in power factor, and loss of clarity. It affects most thermoplastics to varying degrees, in particular polyolefins, PVC, nylons, and cellulose derivatives. Environmental Stress Cracking (ESC). In some plastics, brittle cracking occurs when the material is in contact with certain substances whilst under stress. The stress may be externally applied in which case one would be prompted to take precautions. However, internal or residual stresses introduced during processing are probably the more common cause of ESC. Most organic liquids promote ESC in plastics but in some cases the problem can be caused by a liquid which one would not regard as an aggressive chemical. The classic example of ESC is the brittle cracking of polyethylene washingup bowls due to the residual stresses at the moulding gate (see injection moulding, Chapter 4) coupled with contact with the aqueous solution of washingup liquid. Although direct attack on the chemical structure of the plastic is not involved in ESC the problem can be alleviated by controlling structural factors. For example, the resistance of polyethylene is very dependent on density, crystallinity, melt flow index (MFI)and molecular weight. As well as polyethylene, other plastics which are prone to ESC are ABS and polystyrene. The mechanism of ESC is considered to be related to penetration of the promoting substance at surface defects which modifies the surface energy and promotes fracture.
zy
28
zy zyxwvuts zyxwvu zy General Properties of Plastics
1.43 Wear Resistance and Frictional Properties There is a steady rate of increase in the use of plastics in bearing applications and in situations where there is sliding contact e.g. gears, piston rings, seals, cams, etc. The advantages of plastics are low rates of wear in the absence of conventional lubricants, low coefficients of friction, the ability to absorb shock and vibration and the ability to operate with low noise and power consumption. Also when plastics have reinforcing fibres they offer high strength and load carrying ability. Qpical reinforcements include glass and carbon fibres and fillers include PTFE and molybdenum disulphide in plastics such as nylon, polyethersulphone (PES), polyphenylene sulfide (PPS), polyvinylidene fluoride (PVDF) and polyetheretherketone (PEEK). The friction and wear of plastics are extremely complex subjects which depend markedly on the nature of the application and the properties of the material. The frictional properties of plastics differ considerably from those of metals. Even reinforced plastics have modulus values which are much lower than metals. Hence metalkhennoplastic friction is characterised by adhesion and deformation which results in frictional forces that are not proportional to load but rather to speed. Table 1.7 gives some typical coefficients of friction for plastics. Table 1.7 Coefficients of friction and relative wear rates for plastics Coefficient of friction Material
Static
Dynamic
Relative wear rate
Nylon Nylodglass Nylodcarbon Polycarbonate Polycarbonate/glass Polybutylene terephthalate (PBT) PBT/glass Polyphenylene sulfide (PPS) PPS/glass PPS/carbon Acetal
0.2 0.24 0.1 0.31 0.18 0.19 0.11
0.28 0.3 1 0.11 0.38
33 13 1 420
0.20
5 35
0.3
0.24
90
0.15 0.16 0.2 0.04
0.17 0.15 0.21 0.05
19 13
m
0.25 0.12
2


The wear rate of plastics is governed by several mechanisms. The primary one is adhesive wear which is characterised by fine particles of polymer being removed from the surface. This is a smallscale effect and is a common occurrence in bearings which are performing satisfactorily. However, the other mechanism is more serious and occurs when the plastic becomes overheated to the extent where large troughs of melted plastic are removed. Table 1.7
General Properties of Plastics
29
shows typical primary wear rates for different plastics, the mechanism of wear is complex the relative wear rates may change depending on specific circumstances. In linear bearing applications the suitability of a plastic is usually determined from its PV rating. This is the product of P (the bearing load divided by the projected bearing area) and V (the linear shaft velocity). Fig. 1.9 shows the limiting PV lines for a range of plastics  combinations of P and V above the lines are not permitted. The PV ratings may be increased if the bearing is lubricated or the mode of operation is intermittent. The PV rating will be decreased if the operating temperature is increased. Correction factors for these variations may be obtained from materialhearing manufacturers. The plastics with the best resistance to wear are ultra high molecular weight polyethylene (used in hip joint replacements) and PTFE lubricated versions of nylon, acetal and PBT. It is not recommended to use the same plastic for both mating surfaces in applications such as gear wheels.
zyxw zyxw zyxw
zyxw zyxw
Rubbing velocity, ( V ( d s )
Fig. 1.9 Qpical PV ratings for plastics rubbing on steel
30
zy zyxw zyxwv zyxwv General Properties of Plastics
L4,4 Special Properties Thermal Properties. Before considering conventional thermal properties such as conductivity it is appropriate to consider briefly the effect of temperature on
the mechanical properties of plastics. It was stated earlier that the properties of plastics are markedly temperature dependent. This is as a result of their molecular structure. Consider first an amorphous plastic in which the molecular chains have a random configuration. Inside the material, even though it is not possible to view them, we know that the molecules are in a state of continual motion. As the material is heated up the molecules receive more energy and there is an increase in their relative movement. This makes the material more flexible. Conversely if the material is cooled down then molecular mobility decreases and the material becomes stiffer. With plastics there is a certain temperature, called the glass tramition temperature, Tg9 below which the material behaves like glass Le+it is hard and rigid. As can be seen from Table lm8the value for Tgfor a particular plastic i s
not necessarily a low temperature. This immediately helps to explain some of the differences which we observe in plastics. For example, at room tempera+ ture polystyrene and acrylic are below their respective Ts values and hence we observe these materials in their glassy state Note, however, that in contrast, at room temperature, polyethylene is above its glass transition temperature and so we observe a very flexible materialmWhen cooled below its Tgit then becomes a hard, brittle.solid, Plastics can have several transitions. The main Tgi s called the glassrubber transition and signifies a change from a flexible, tough material to a glassy state in which the material exhibits stiffness, low creep and toughness although with a sensitivity to notches. At lower temperatures there is then a secondary transition characterised by a change to a hard, rigid, brittle statet It should be noted that although Table 1.8 gives specific values of Tg for different polymers, in reality the glasstransition temperature is not a material constant, As with many other properties of polymers it will depend on the testing conditions used to obtain it. In the socalled crystalline plastics the structure consists of both crystalline (ordered) regions and amorphous (random) regions. When these materials are heated there is again increased molecular mobility but the materials remain relatively stiff due to the higher forces between the closely packed molecules. When the crystalline plastics have their temperature reduced they exhibit a glass transition temperature associated with the amorphous regions. At room temperature polypropylene, for example, is quite rigid and tough, not because it is below its T, but because of the strong forces between the molecules in the crystalline regions. When i t is cooled below 10°C it becomes brittle because the amorphous regions go below their Tg' In the past a major limitation to the use of plastics materials in the engineering sector has been temperature. T h i s limitation arises not only due to the
zyxwvu zyxwv zyxwvu 31
General Properties of Plastics
Table 1.8 TLPicd Thermd properties of materials
zyxwvutsrqpon zyxwvutsrq zyxwvutsrqp zyxw zyxw Thermal Coeff. of Density conductivity therm exp (ClmlmpC) (kg/m3) W k g K) ( W I M ) Specific heat
Material ABS
Acetal (homopolymer) Acetal (copdymer)
Acrylic
Cellulose acetate CAB EPOXY
Modified PPO Nylon 66 Nylon 66 (33% glass) PEEK PEEK (30% carbon)
PET
PET (36% glass)
Phenolic (glass filled)
Polyamideimide Polycarbonate Polyester Polyetherimide Poiyethersulphone Polyimide Polyphenylene sulfide Polypropylene Polysulphone Polystyrene
Polythene (LD) Polythene (HP) PTFE PVC (igid) PVC (flexible) SAN
DMC (plyester) SMC (polyester) Polystyrene foam PU foam Stainless steel Nickel chrome alloy
Zinc
1040 1420 1410 1180
1280
1190 1200 1060 1I 4 0 1380 1300 1400 1360 1630 1700 1400 1150
1200 1270 1370
I .3
1.5 I .5 1.5 16
0.25 0.2
90
0.2 0.2 0.15
95 70 100 100 70
1.6
0.14
0.8
0.23 0.22
80
0.72 1.09 1.04 27
85 105

1c




1.o
0.2
90 40
75



0.5 0.25
1.2
Ob2
1.2
0.2 0.22

18 36 65 100
0.20
€00
950 2100 1400
2.0 1.3 1.3 2.2 2.2 1 .o 0.9
0.15 0.24 0.25
56 80 200 120
0.25
140
1300
1.$
70 140
1080 1800 1800
1.3
0.16 0.14 0.17
32

32 7855 7950 7135

8940
115 85
I43


920
1.7 0.7
48 14


1240 1050
TJC)
0.24 0.52
1.7 1,6

905
IO'
60 90 30
56 55 45 49
1420 1340
Thermal Glass diffusivity transition (m2/s) Temp,


0,49 r
0.39 0.39
1.18

0.2 0.2 0.032 0.032
70 20 20 YL
90
10
12 111 400
14
39 16
Ul 1 &33 +
4
56 M
I y
d

260
1.47
149
Max. operating, Temp ("C) 70 85 90
50 60
60 130 120
90
100
204 255 110 150 185
220 125 
200
0.65
06 1.17 1.57 0.7
0.7 0.81
230 40 85  10 180 100
120 120 1 13 80 80
170 180 260 150 1 0 170 50 50 55 250 50
50
115
60

130 130




800
7
lrrr
900

reduction in mechanical properties at high temperatures, including increased propensity to creep, but also due to limitations on the continuous working temperature causing permanent damage to the material as a result of thermal and oxidative degradation. Significant gains in property retentiun at high temperatures with crystalline polymers have been derived fmrn the incorporation of
32
General Properties of Plastics
fibrous reinforcement, but the development of new polymer matrices is the key to further escalation of the useful temperature range. Table 1.8 indicates the service temperatures which can be used with a range of plastics. It may be seen that there are now commercial grades of unreinforced plastics rated for continuous use at temperatures in excess of 200°C. When glass or carbon fibres are used the service temperatures can approach 300°C. The other principal thermal properties of plastics which are relevant to design are thermal conductivity and coefficient of thermal expansion. Compared with most materials, plastics offer very low values of thermal conductivity, particularly if they are foamed. Fig. 1.10 shows comparisons between the thermal conductivity of a selection of metals, plastics and building materials. In contrast to their low conductivity, plastics have high coefficients of expansion when compared with metals. This is illustrated in Fig. 1.11 and Table 1.8 gives fuller information on the thermal properties of plastics and metals.
z zyx zyx zyxwvu zyxwvu
zyxwvu
25mm Wyurelhanc 4Omm Pdystyrrw LSmn Hlreral d
50mm Cork 65mn Fibnbmd 1 L O m softrrmd
3Barm Concrpl~blocks
zyxw zyxwvut
Equivalent thickness of common building and insulatm materials required to achieve the same degree of insulaiion
Fig. 1.10 Comparative Thermal conductivities for a range of materials
Electrical Properties Traditionally plastics have established themselves in applications which require electrical insulation. PTFE and polyethylene are among the best insulating materials available. The material properties which are particularly relevant to electrical insulation are dielectric strength, resistance and tracking. The insulating property of any insulator will break down in a sufficiently strong electric field. The dielectric strength is defined as the electric strength (V/m) which an insulating material can withstand. For plastics the dielectric strength can vary from 1 to loo0 MV/m. Materials may be compared on the basis of their relative permittivity (or dielectric constant). This is the ratio of the permittivity of the material to the permittivity of a vacuum. The ability of a
General Properties of Plastics
33
zy
zyx zyxwvuts 250
zyxwvuts zyxwvuts zyxwvuts
$150
a0
El 100
€
B
Fig. 1.1 1 lsrpical thermal propexties of plastics
material to resist the flow of electricity is determined by its volume resistivity, measured in ohm m. Insulators are defined as having volume resistivities greater than about 104 ohm m. Plastics are well above this, with values ranging from ohm m for about 108 to 10l6 ohm m. These compare with a value of about copper. Although plastics are good insulators, local breakdown may occur due to tracking. This is the name given to the formation of a conducting path (arc) across the surface of the polymer. It can be caused by surface contamination (for example dust and moisture) and is characterised by the development of carbonised destruction of the surface carrying the arc. Plastics differ greatly in their propensity to tracking  PTFE,acetal, acrylic and PP/PE copolymers offer very good resistance. It is interesting to note that although the electrical insulation properties of plastics have generally been regarded as one of their major advantages, in recent years there has been a lot of research into the possibility of conducting plastics. This has been recognised as an exciting development area for plastics because electrical conduction if it could be achieved would offer advantages in designing against the build up of static electricity and in shielding of computers, etc from electromagnetic interference (EM).There have been two approaches  coating or compounding. In the former the surface of the plastic is treated with a conductive coating (e.g. carbon or metal) whereas in the second, fillers such as brass, aluminium or steel are incorporated into the plastic. It is important that the filler has a high aspect ratio (1ength:diameter) and so fibres or flakes of metal are used. There has also been some work done using glass fibres which are coated with a metal before being incorporated into the plastic. Since the fibre aspect ratio is critical in the performance of conductive plastics there can
zyx
zyxwv zyxwv zyxw
34
General Properties of Plastics
be problems due to breaking up of fibres during processing. In this regard thermosetting plastics have an advantage because their simpler processing methods cause less damage to the fibres. Conductive grades of DMC are now available with resistivities as low as 7 x ohm m. Optical Properties. The optical properties of a plastic which are important are refraction, transparency, gloss and light transfer. The reader is referred to BS 4618:1972 for precise details on these terms. Table 1.9 gives data on the optical properties of a selection of plastics. Some plastics may be optically clear (e.g. acrylic, cellulosics and ionomers) whereas others may be made transparent. These include epoxy, polycarbonate, polyethylene, polypropylene, polystyrene, polysulphone and PVC. Table 1.9 Typical properties of plastics Material Acrylic Polycarbonate Polystyrene CAB SAN
Nylon 66
Refractive index
Light transmission
Dispersive power
1.49 1.59 1.59 1.49 1.57 1.54
92 89 88 85
58 3035 31

0
zyxw zyx 
36 
zy zyxwvu
Flammability. The fire hazard associated with plastics has always been difficult to assess and numerous tests have been devised which attempt to grade materials as regards flammability by standard small scale methods under controlled but necessarily artificial conditions. Descriptions of plastics as selfextinguishing, slow burning, $re retardant etc. have been employed to describe their behaviour under such standard test conditions, but could never be regarded as predictions of the performance of the material in real fire situations, the nature and scale of which can vary so much. Currently there is a move away from descriptions such as jreretardant or selfextinguishing because these could imply to uninformed users that the material would not bum. The most common terminology for describing the flammability characteristics of plastics is currently the Critical Oxygen Index (COI). This is defined as the minimum concentration of oxygen, expressed as volume per cent, in a mixture of oxygen and nitrogen that will just support combustion under the conditions of test. Since air contains 21% oxygen, plastics having a COI of greater than 0.21 are regarded as selfextinguishing. In practice a higher threshold (say 0.27) is advisable to allow for unforeseen factors in a particular fire hazard situation. Fig. 1.12 shows the typical COI values for a range of plastics.
General Properties of Plastics
z
zy zyxwv 35
COI
zyxwvutsr 
Fig. 1.12 Oxygen Index Values for Plastics
Permeability. The low density of plastics is an advantage in many situations but the relatively loose packing of the molecules means that gases and liquids can permeate through the plastic. This can be important in many applications such as packaging or fuel tanks. It is not possible to generalise about the performance of plastics relative to each other or in respect to the performance of a specific plastic in contact with different liquids and gases. Some plastics are poor at offering resistance to the passage of fluids through them whereas others are excellent. Their relative performance may be quantified in terms of a permeation constant, k, given by
zyxwv zyxwvutsr zyxw (1.10)
where Q = volume of fluid passing through the plastic d = thickness of plastic A = exposed area t = time p = pressure difference across surfaces of plastic.
The main fluids of interest with plastics are oxygen and water vapour (for packaging applications) and C02 (for carbonated drinks applications). Fig. 1.13 and Fig. 1.14 illustrate the type of behaviour exhibited by a range of plastics. In some cases it is necessary to use multiple layers of plastics because no single plastic offers the combination of price, permeation resistance, printability, etc. required for the application. When multilayers are used, an overall permeation constant for the composite wall may be obtained from (1.11)
1.4.5 Processing A key decision in designing with plastics is the processing method employed. The designer must have a thorough knowledge of processing methods because
36
z zyx
General Properties of Plastics
Cellophane
CA

PC

tl
zyxwvutsrqpon zyx zyxwvu 1
1
1
I
Oxygen permeability (cc25 pm/m224 hatm)
Fig. 1.13 Permeability data for a range of plastics
zyxwv Nylon
u)
2)
v
zyxwvuts
.3 looam
E
Y Z P L
a
0
a
9 tl
EVOH
10
c
1
10 100 lo00 10000 C02 permeability (cc25 pdm224 hatm)
1OOOOO
Fig. 1.14 Permeability data for a range of plastics
plastics are unique in design terms in that they offer a wider choice of conversion techniques than are available for any other material. A simple container for example could be made by injection moulding, blow moulding or rotational moulding; light fittings could be thermoformed or injection moulded. In this brief introduction to designing with plastics it is not possible to do justice to the
General Roperties of Plastics
zyxwvu zyx zy zy zyxw zyxwv 37
range of processing methods available for plastics. Therefore Chapter 4 will be devoted to processing. This describes the suitability of particular plastics for each moulding method and considers the limitations which these place on the designer.
L4,6 Costs It is a popular misconception that plastics are cheap materials. They are not. On a weight basis most plastics are more expensive than steel and only slightly less expensive than aluminium. Prices for plastics can range from about ;JE600 per tonne for polypropylene to abut €25,000 per tonne for carbon fibre reinforced PEEK. Table 1.5 compares the costs of a range of plastics. However, i t should always be remembered that it is bad design practice to select materials on the basis of cost per unit weight. In the mass production industries, in particular, the raw material cost i s of relatively little importance. It is the inposition cost which is all important. The inposition cost of a component is the sum of several independent factors i.c raw material costs, fabrication costs and performance costs. It i s in the second two of these cost components that, in relation to other materials, plastics can offer particular advantages. Fabrication costs include power, labour, consumables, etc and Table 1.10 shows that, in terms of the oveniH energy consumption, plastics come out much better than metals. Performance costs relate to servicing, warranty claims, etc. On this basis plastics can be very attractive to industries manufacturing consumer products because they can offer advantages such as colour fastness, resilience, toughness, corrosion resistance and uniform quality  all features which help to ensure a reliable product. However, in general these fabrication and performance advantages are common to all plastics and so a decision has to be made in regard to which plastic would be best for a particular application. Rather than compare the basic raw material costs it is better to use a cost index on the basis of the cost to achieve a certain perforname. Consider again the material selection procedures illustrated in Section 1.4.1 in relation to strength and stiffness.
zyxwvut
Selection for Strength at Minimum Cost If the cost of a material is C per unit weight then from equation (1.3) the cost of the beam considered in the analysis would be
(1.12) Substituting for d from (1.2) then the cost of the beam on a strength basis would be Cb
83
PC
(1.13)
38
zy zyxwvu zy zyxwv General Roperties of Plastics
Table 1.10
The energy required to manufacture and process a range of materials at typical design thickness Material
Energy Jlm2 x lo6
Design thickness
0
mm
Magnesium Aluminium sheet Zinc die casting Aluminium casting Steel Acetal Modified PPO S MC Rgid polyurethane foam Wycurbmate Acrylic Nylon 6 Nylon 66 LOPE HDPE Polystyrene RRlM polyurethane Polypropylene ABS PVC
1.9
1.3 1.3 1.3 0.8 2.0 2.0
3.3 5.3 2.0 2.0 1.8 1.8 2.7
2.4 2.0
3.2 2.5 1.9
zyxwvut
zyxwv
Feedstodc
2.0
Fuel
0
Process
where 83 is a constant, which will be the same for all materials. Therefore we can define a cost factor, Cf,where
Cf =
(5)
(1.14)
zyx
which should be minimised in order to achieve the best combination of price and performance. Alternatively we may take the reciprocal of Cf to get a desirability factor, Df,
Df=
(g)
(1.15)
and this may be compared to Df given by equation (1.5).
Selection for Stiffness at Minimum Cost Using equation (1.7) and an analysis similar to above it may be shown that on the basis of stiffness and cost, the desirability factor, Df,is given by
Df =
(s)
(1.16)
General Properties of Plastics
zyxwvu 39
zyxw zyxwvutsr zyxwvut zyxwvu zyxwv Table 1.1 1
Desirability factors for some common loading configurations
Desirability factor, Df
Component
Strength basis
Stiffness basis
a;/=/pc UYIPC aYlPC rmlPC
E113/pC EIPC
Rectangular beam with fixed width Struts or ties Thin wall cylinders under pressure Thin wall shafts in tension Long rods in compression (buckling)

GIPC E112/pC

Table 1.12
zyxwvutsr zyxwvuts zyxwvuts
Desirability factors for a range of materials Proof or fracture
Density, p
stress n
Material
kg/m3
(MN/m )
Aluminium (pure) Aluminium alloy Stainless steel Titanium alloy Spruce
2700 2810 7855 4420
2'
Modulus E (GN/m2)
*Y
E 
E112
~ 1 1 3


P
P (x103)
P (x103)
P (xIo~)
450
90 500 980 900 35
70 71 I85 107 9
0.033 0.178 0.125 0.204 0.078
0.026 0.025 0.024 0.024 0.020
3.51 7.95 4.0 6.78 13.15
3.12 3.0 1.73 2.34 6.67
1.53 I .47 0.73 1.07 4.62
2000
1240
48
0.62
0.024
17.6
3.46
1.82
1500 1140 Io40 1I50 1450
1050 70 35
21.6 8.34 5.68 6.73
9.16 0.77 1.05 1.23 2.7
3.82 0.81 1.02 1.09 I .72
GRP (80%
unidirectional glass in
polyester) CFRP (60%
unidirectional fibres in epoxy) Nylon 66 ABS
Polycarbonate PEEK (+ 30% C)
60 215
189 0.78* 1.2* 2.0* 15.5
0.126 0.7 0.061 6.8 x 0.034 1 I .5 0.052 17.4 x 0.19 0.011
10.1
* 1500 h creep modules
Tables 1.11 and 1.12 give desirability factors for configurations other than the beam analysed above and typical numerical values of these factors for a range of materials.
Bibliography Waterman, N.A. The Selection and Use of Engineering Materials, Design Council, London (1979) Crane, F.A.C. and Charles, J.A. Selection and Use of Engineering Materials Buttenvorths, London ( 1984)
40
zyxwvuts zy zyxwvutsrq zyxwv zyxwvut zy General Properties of Plastics
zyxw
Crawford, R.J. Plastics and RubberEngineering Design and Application, MEP, London (1985) Powell, P.C.Engineering with Polymers, Chapman and Hall, London (1984) Hall, C. Polymer Materials, Macmillan, London (1981) Birley, A.W. and Scott, M.J. Plustic Materials: ProDem'es and ADdications. Leonard Hall. Gkgow (1982) Benham, P.P. Crawford, R.J. and Armstrong, C.G Mechanics of Engineering Materials, Longmans (1996) Lancaster, J.K.Friction and Wear of Plastics, Chapter 14 in Polymer Science edited by A.D. Jenkins (vol2), NorthHolland Publ. Co., London (192) Bartenev, G.M.and Lavrentev, V.V. Friction and Wear in Polymers, Elsevier Science h b l . Co., Amsterdam (1981) Schwartz, S.S. and Goodman,S.H. Plastics Materials and Processes, Van Nostrand Reinhold, New York (1982) Blythe, A.R. Electrical Properties of Polymers, Cambridge Univ. Press (1980) Van Krevelen, D.W.Properties of Polymers 2nd Edition, Elsevier, Amsterdam (1976) Mills, N. Plastics, Edward Arnold, London (1986) Kemmish, D.J. High performance engineering plastics, RAPRA Review Reports, 8, 2 (1995) Oswald, T.A. and Menges, G. Materials Science of Polymers for Engineers, Hanser, Munich (1995) Birley, A.W. Haworth B. and Batchelor, J. Physics of Plastics, Hanser, Munich (1992) Belofsky, H. Plastics: Product Design und Process Engineering, Hanser, Munich (1995) Gruenwald, G. Plastics: How Structure Determines Properties, Hanser, Munich (1992) Dominghaus, H. Plastics for Engineers, Hanser, New York (1993) Chanier, J.M. Polymeric Materials and Processing, Hanser, New York (1990) Progelhof, R.C. and Throne, J.L. Polymer Engineering Principles, Hanser, New York (1993)
..
zyxwvu zyxwvu
CHAPTER 2  Mechanical Behaviour of Plastics
2 J Introduction
zyxwvut zyx
In Chapter 1 the general mechanical properties of plastics were introduced. In order to facilitate comparisons with the behaviour of other classes of materials the approach taken was tu refer to standard methods of data presentation, such as stressstrain graphs, etc. However, it is important to note that when one becomes involved in engineering design with plastics, such graphs are of limited value. The reason is that they are the results of relatively shortterrn tests and so heir use i s restricted to quality control and, perhaps, the initial sorting of materials in terms of stiffness, strength etc. Designs based on, say, the modulus obtained from a shortterm test would not predict accurately the longterm behaviour of plastics because they are viscoelastic materials. T h i s viscoelasticity means that quantities such as modulus, strength, ductility and coefficient of fiction are sensitive to straining rate, elapsed time, loading history, temperature, etc. It will also be shown later that the manufacturing method used for the plastic product can create changes in the structure of the material which have a pronounced effect on properties. The behaviour of the moulded product may therefore be different from the behaviour of a moulded testpiece of the same material. The timedependent change in the dimensions of a plastic article when subjected to a constant stress is called creep. As a result of this phenomenon the modulus of a plastic is not a constant, but provided its variation is known then the creep behaviour of plastics can be allowed for using accurate and well established design procedures Metals also display time dependent properties at high temperatures so that designers of turbine blades, for example, have to allow for creep and guard against creep rupture. At room temperature the creep behaviour of metals is negligible and so design procedures are simpler in that
zyxwvuts 41
42
Mechanical Behaviour of Plastics
the modulus may be regarded as a constant. In contrast, thermoplastics at room temperature behave in a similar fashion to metals at high temperatures so that design procedures for relatively ordinary loadbearing applications must always take into account the viscoelastic behaviour of plastics. For most traditional materials, the objective of the design method is to determine stress values which will not cause fracture. However, for plastics it is more likely that excessive deformation will be the limiting factor in the selection of working stresses. Therefore this chapter looks specifically at the deformation behaviour of plastics and fracture will be treated separately in the next chapter.
zy zy zyx zyxwv zy zyxw
2.2 Viscoelastic Behaviour of Plastics
For a component subjected to a uniaxial force, the engineering stress, (T, in the material is the applied force (tensile or compressive) divided by the original crosssectional area. The engineering strain, E, in the material is the extension (or reduction in length) divided by the original length. In a perfectly elastic (Hookean) material the stress, (T, is directly proportional to be strain, E, and the relationship may be written, for uniaxial stress and strain, as (T
= constant x
E
(2.1)
where the constant is referred to as the modulus of the material. In a perfectly viscous (Newtonian) fluid the shear stress, t is directly proportional to the rate of strain (dy/dt or p) and the relationship may be written as t = constant x
i.
(2.2)
where the constant in this case is referred to as the viscosity of the fluid. Polymeric materials exhibit mechanical properties which come somewhere between these two ideal cases and hence they are termed viscoelastic. In a viscoelastic material the stress is a function of strain and time and so may be described by an equation of the form
zyxwvu
zyxwv (J
= f(E, t )
(2.3)
This type of response is referred to as nonlinear viscoelastic but as it is not amenable to simple analysis it is often reduced to the form 0=E .
f(t)
(2.4)
This equation is the basis of linear viscoelasticity and simply indicates that, in a tensile test for example, for a fixed value of elapsed time, the stress will be directly proportional to the strain. The different types of response described are shown schematically in Fig. 2.1. The most characteristic features of viscoelastic materials are that they exhibit a time dependent strain response to a constant stress (creep) and a time dependent stress response to a constant strain (relaxation). In addition when the
Mechanical Behaviour of Plastics
zy zyxwvu
0
43
Strain
zyxw
Fig. 2.1 Stressstrain behaviour of elastic and viscoelastic materials at two values of elapsed time, t
applied stress is removed the materials have the ability to recover slowly over a period of time. These effects can also be observed in metals but the difference is that in plastics they occur at room temperature whereas in metals they only occur at very high temperatures.
zyxwvuts zyxw zyxwvu
2.3 ShortTerm Testing of Plastics
The simple tensile test is probably the most popular method for characterising metals and so it is not surprising that it is also widely used for plastics. However, for plastics the tensile test needs to be performed very carefully and the results of the single test should only be used as a means of quality control  not as design data. This is because, with plastics it is possible to obtain quite different results from the same material simply by changing the test conditions. Fig. 2.2 shows that at high extension rates (>1 d s ) unplasticised PVC is almost brittle with a relatively high modulus and strength. At low extension rates (
a(b Int) ctdlrlt
Logarithmic
Logarithmic Exponential
7. 8.
E
= sinh ut
Hyperbolic sine
= a +. b sinh ct 10. E = a + b sinh ct 1/3 9.
11.
Power
Hyperbolic
.+bt
E =
E=
Parabolic
bf
+I
1 +atb 5 . E = a ln(b
6.
zyxw
These take the form
E
E
= a(l
+ bt
113
)e
cf
Hyperbolic sine
Hyperbolic sine Powerkxponential
The mechanism of creep is not completely understuod but some aspects have been explained based on the structures described in Appendix A. For example, in a glassy plastic a particular atom is restricted from changing its position as a result of attractions and repulsions between it and (a) atoms in the same chain, (b) atums in adjacent chains. It is generally considered that for an atom to change its position it must overcome an energy barrier and the probability of it achieving the necessary energy is improved when a stress is applied. In a semicrystalline plastic there is an important structural difference in that the crystalline regions are set in an amorphous matrix. Movement of atoms can occur in both regions but in the majority of cases atum mobility is favoured in the noncrystalline material between the spherulites. Plastics also have the ability to recover when the applied stress is removed and to a first approximation this can often be considered as a reversal of creep. This was illustrated in Fig. 1.8 and will be studied again in Section 2.7. At present it is proposed to consider the design methods for plastics subjected to steady forces. 2+5Design Methods for Plastics using Deformation Data
Isochronous and Isometric Graphs The most common method of displaying the interdependence of stress, strain and time is by means of creep curves, However, it should be realised that these
zy zyx
Mechanical Behaviour of Plastics
49
represent a twodimensional view of (or slices through) the threedimensional stressstraintime behaviour of plastics shown in Fig. 2.6. It would be equally sensible to consider the other twodimensional views which could be taken of Fig. 2.6. These are the stressstrain plot (sometimes called the isochronous curve because it represents a constant time section) and the stresstime plot (sometimes called the isometric curve because it represents constant strain section). These two 'views' are shown in Fig. 2.7 and 2.8.
Strain
zyxwv zyxwv
1000 " '0
Fig. 2.6 Stressstraintime curves for polypropylene
z zyx zyxw
In practice, of course, it is most common to have the creep curves (straintime curve) since these can be obtained relatively simply by experiment. The other two curves can then be derived from it. For example, the isometric graph is obtained by taking a constant strain section through the creep curves and replotting as stress versus time (see Fig. 2.10(a)). This is termed an isometric graph and is an indication of the relaxation of stress in the material when the strain is kept constant. This data is often used as a good approximation of stress relaxation in a plastic since the latter is a less common experimental procedure than creep testing. In addition, if the vertical axis (stress) is divided by the strain, E, then we obtain a graph of modulus against time (Fig. 2.1O(b)). This is a good illustration of the time dependent variation of modulus which was referred to earlier. It should be noted that this is a Relaxation Modulus since it relates to a constant strain situation. It will be slightly different to the Creep Modulus which could be obtained by dividing the constant creep stress by the strain at various times. Thus fY
creep modulus, E ( t ) = E@)
(2.9)
50
zy zyxwvuts Mechanical Behaviour of Plastics
12
10
8
z6
B
cn
4
2
0 0
zyxw zyxwv 0.5
1
1.5
2
2.5
3
3.5
Stmln (%)
Fig. 2.7 Stressstrain curves for polypropylene
Fig. 2.8 Stresstime curves for polypropylene
4
4.5
5
zyxwv zyxwvutsrqp
Mechanical Behaviour of Plastics
51
zyxwvut
A
lo00 100 
10000
10

1
0.1 0.01

'
zyxw zyx b
Log (time)
Fig. 2.9 Typical variation of creep or relaxation moduli with time 18
14
20
16
d
zyxwvutsrqpon C.C
\
? l2
03
OL
Fig. 2.10 Construction of isometric and isochronous graphs
The creep modulus will vary with time, i.e. decrease as time increases, in a manner similar to that shown for the relaxation modulus. The classical variation of these moduli is illustrated in Fig. 2.9. On loglog scales it is observed that there is a high value of creep or relaxation modulus at short times. This is referred to as the Unrelaxed Modulus and is independent of time. Similarly at long times there is a low value Relaxed Modulus which is also independent of time.
52
zyxwvutsr zyxw zyxw zyx zyxw zy zy Mechanical Behaviour of Plastics
Occasionally in creep analysis it is convenient to use a Creep Compliance instead of the creep modulus. This is simply given by 1 at)
N)
Creep compliance, c(t)= = 
(2.10)
0
An alternative to the isometric graph may be obtained by taking a constant time section through the creep curves and plotting stress versus strain as shown in Fig. 2.10(c). This Isochronous Graph can also be obtained experimentally by performing a series of minicreep and recovery tests on a plastic. In this experiment a stress is applied to a plastic testpiece and the strain is recorded after a time, t (typically 100 seconds). The stress is then removed and the plastic allowed to recover, normally for a period of 4t. A larger stress is then applied to the same specimen and after recording the strain at time t, this stress is removed and the material allowed to recover. This procedure is repeated until sufficient points have been obtained for the isochronous graph to be plotted. These latter curves are particularly important when they are obtained experimentally because they are less time consuming and require less specimen preparation than creep curves. Isochronous graphs at several time intervals can also be used to build up creep curves and indicate areas where the main experimental creep programme could be most profitably concentrated. They are also popular as evaluations of deformational behaviour because the data presentation is similar to the conventional tensile test data referred to in Section 2.3. It is interesting to note that the isochronous test method only differs from that of a conventional incremental loading tensile test in that (a) the presence of creep is recognised, and (b) the memory which the material has for its stress history is accounted for by the recovery periods. Quite often isochronous data is presented on loglog scales. One of the reasons for this is that on linear scales any slight, but possibly important, nonlinearity between stress and strain may go unnoticed whereas the use of loglog scales will usually give a straightline graph, the slope of which is an indication of the linearity of the material. If it is perfectly linear the slope will be 45". If the material is nonlinear the slope will be less than this. As indicated above, the stressstrain presentation of the data in isochronous curves is a format which is very familiar to engineers. Hence in design situations it is quite common to use these curves and obtain a secant modulus (see Section 1.4.1, Fig. 1.6) at an appropriate strain. Strictly speaking this will be different to the creep modulus or the relaxation modulus referred to above since the secant modulus relates to a situation where both stress and strain are changing. In practice the values are quite similar and as will be shown in the following sections, the values will coincide at equivalent values of strain and time. That is, a 2% secant modulus taken from a 1 year isochronous curve will be the same as a 1 year relaxation modulus taken from a 2% isometric curve.
Mechanical Behaviour of Plastics
zyxwv zyx 53
PseudoElastic Design Method for Plastics
Throughout this chapter the viscoelastic behaviour of plastics has been described and it has been shown that deformations are dependent on such factors as the time under load and the temperature. Therefore, when structural components are to be designed using plastics, it must be remembered that the classical equations which are available for the design of springs, beams, plates, cylinders, etc., have all been derived under the assumptions that (i) the strains are small (ii) the modulus is constant (iii) the strains are independent of loading rate or history and are immediately reversible (iv) the material is isotropic (v) the material behaves in the same way in tension and compression
zyxwv
Since these assumptions are not always justified for plastics, the classical equations cannot be used indiscriminately. Each case must be considered' on its merits and account taken of such factors as mode of deformation, service temperature, fabrication method, environment and so on. In particular it should be noted that the classical equations are derived using the relation. stress = modulus x strain
where the modulus is a constant. From the foregoing sections it should be clear that the modulus of a plastic is not a constant. Several approaches have been used to allow for this and some give very accurate results. The drawback is that the methods can be quite complex, involving Laplace transforms or numerical methods and they are certainly not attractive to designers. However, one method that has been widely accepted is the so called Pseudo Elastic Design Method. In this method, appropriate values of time dependent properties, such as modulus, are selected and substituted into the classical equations. It has been found that this approach gives sufficient accuracy in most cases provided that the value chosen for the modulus takes into account the service life of the component and the limiting strain of the plastic. This of course assumes that the limiting strain for the material is known. Unfortunately this is not just a straightforward value which applies for all plastics or even for one plastic in all applications. It is often arbitrarily chosen although several methods have been suggested for arriving at a suitable value. One method is to plot a secant modulus which is 0.85 of the initial tangent modulus (see Fig. 1.6) and note the strain at which this intersects the stressstrain characteristic. However, for many plastics (particularly crystalline ones) this is too restrictive and so in most practical situations the limiting strain is decided in consultations between the designer and the material manufacturers. Once the limiting strain is known, design methods based on the creep curves are quite straightforward and the approach is illustrated in the following
zyxwvu
54
zyxwvu Mechanical Behaviour of Plastics
examples. When using this pseudoelastic design approach it should be remembered that the creep curves used to derive modulus values have normally been obtained on test pieces which are essentially isotropic. In practice the manufacture of the endproduct by injection moulding or extrusion, etc. will have resulted in some degree of anisotropy. This may make the predictions inaccurate because the creep data for the material is no longer appropriate for the structural morphology introduced by the moulding method. Similar comments could, of course, also be made about metals in that the test data may have been obtained on specimens of the material which do not accurately reflect the nature of the material in the endproduct. Therefore, pseudoelastic design is a valid analytical procedure but one should always be cautious about the way in which the manufacturing method has affected the behaviour of the material.
zyxwv z zy zyxwv zyx bw zyxwvu
Example 2.1 A ballpoint pen made from polypropylene has the clip design shown in Fig. 2.1 1. When the pen is inserted into a pocket, the clip is subjected to a deflection of 2 mm at point A. If the limiting strain in the material is to be 0.5%calculate (i) a suitable thickness, d, for the clip (ii) the initial stress in the clip when it is first inserted into the pocket and (iii) the stress in the clip when it has been in the pocket for 1 week. The creep curves in Fig. 2.5 may be used and the shortterm modulus of polypropylene is 1.6 GN/m2.
?+I
, width 6 mm
Fig. 2.11 Ballpoint pen clip design
Solution Strain, E , is given by the ratio of stress, u,to modulus, E. In the case of the pen clip, it is effectively a cantilever of length 40 mm. stress = MY I
where M = bending moment (WL) y = half beam depth (d/2)
I = second moment of area (= bd3/12)
(i) Hence
WLd strain, E = 2EI
(2.11)
Mechanical Behaviour of Plastics
zyxwv zyx zyxwv zyxwvu zyxw zyx zyxwv 55
Also, the classical elastic equation for the end deflection of a cantilever is:
WL3 deflection, 6 = 3EI Combining (2.11) and (2.12) gives 36d
strain, E = 2L2
so d=
(2.12)
(2.13)
2(40)* x 0.005 = 2.7 mm 3x2
(ii) The shortterm stress in the material is obtained from the shortterm modulus which is given in this question (or could be obtained from the creep/isometric curves, i.e. at 10 seconds, E = 8 x 106/0.5% = 1.6 GN/m2 or from the appropriate isometric curve). stress = EE = 1.6 x lo9 x 0.005 = 8 MN/m2
(iii) After 1 week (6.1 x lo5 seconds), the isometric curves (Fig. 2.8) derived from the creep curves show that at a strain of 0.5% the stress would have decayed to about 3.3 MN/m2.
Example 2.2 A polypropylene beam is 100 mm long, simply supported at each end and is subjected to a load W at its midspan. If the maximum permissible strain in the material is to be 1.5%, calculate the largest load which may be applied so that the deflection of the beam does not exceed 5 mm in a service life of 1 year. For the beam I = 28 mm4 and the creep curves in Fig. 2.5 should be used. Solution The central deflection in a beam loaded as shown in Fig. 2.12 is given by
a =  WL3
48EI 48EI6
w=
L3
W
Fig. 2.12 Simply supported beam with central load
56
zyxwvutsr Mechanical Behaviour of Plastics
0
zyxwvuts zyxwvu zyxw zyxwv
0
1
0.5
2 Strain ("74
1.5
2.5
3
3.5
Fig. 2.13 Isochronous curve for polypropylene (1 year)
zyx zyxwv zy
The only unknown on the right hand side is a value for modulus E. For the plastic this is timedependent but a suitable value may be obtained by reference to the creep curves in Fig. 2.5. A section across these curves at the service life of 1 year gives the isochronous graph shown in Fig. 2.13. The maximum strain is recommended as 1.5% so a secant modulus may be taken at this value and is found to be 347 MN/m2. This is then used in the above equation.
so
W =
48 x 347 x 28 x 5
(W3
= 2.33 N
As before, a similar result could have been achieved by taking a section across the creep curves at 1.5% strain, plotting an isometric graph (or a 1.5% modulus/time graph) and obtaining a value for modulus at 1 year (see Fig. 2.8) In this example it has been assumed that the service temperature is 20 "C.If this is not the case, then curves for the appropriate temperature should be used. If these are not available then a linear extrapolation between temperatures which are available is usually sufficiently accurate for most purposes. If the beam in the above example had been builtin at both ends at 20% and subjected to service conditions at some other temperature, then allowance would need to be made for the thermal strains set up in the beam. These could be obtained from a knowledge of the coefficient of thermal expansion of the beam material. This type of situation is illustrated later.
zyxwv zyxw zyxwv
Mechanical Behaviour of Plastics
57
For some plastics, particularly nylon, the moisture content can have a significant effect on the creep behaviour. For such plastics, creep curves are normally available in the wet and dry states and a knowledge of the service conditions enables the appropriate data to be used. For convenience so far we have referred generally to creep curves in the above examples. It has been assumed that one will be using the correct curves for the particular loading configuration. In practice, creep curves obtained under tensile and flexural loading conditions are quite widely available. Obviously it is important to use the creep curves which are appropriate to the particular loading situation. Occasionally it is possible to obtain creep curves for compressive or shear loading but these are less common. If only one type of data is available (e.g. tensile creep curves) then it is possible to make conversions to the other test modes. It should always be remembered, however, that these may not always be absolutely accurate for plastics under all situations. Generally there is a stiffening effect in compression compared to tension. As a first approximation one could assume that tension and compression behaviour are the same. Thomas has shown that typically for PVC, the compression modulus is about 10%greater than the tensile modulus. However, one needs to be careful when comparing the experimental data because normally no account is taken of the changes in crosssectional area during testing. In tension, the area will decrease so that the true stress will increase whereas in compression the opposite effect will occur. The classical relationship between moduli in tension, compression and flexure is
zyxw (2.14)
where
MR = Ec/ET
It may be seen that if E, = ET then Eflex= ET. However, if E, = 1 . 1 E ~ (for example), then Eflex= 1.05E~. The classical relationship between the shear modulus G, and the tensile modulus, E, for an isotropic material is
zyx zyxwv zyxw (2.15)
where v = Poissons ratio. Finally, although it is less commonly used for plastics, the bulk modulus, K, is given by K=
I7 c
3(1  2 ~ )
(2.16)
58
zyxwvutsrq zy zyxw zyxwvut zyxw Mechanical Behaviour of Plastics
The bulk modulus is appropriate for situations where the material is subjected to hydrostatic stresses. The proof of equations (2.15) and (2.16) is given by Benham et al.
zyx zyxwvut zy
Example 23 A cylindrical polypropylene tank with a mean diameter of 1 m is to be subjected to an internal pressure of 0.2 MN/m2. If the maximum strain in the tank is not to exceed 2% in a period of 1 year, estimate a suitable value for its wall thickness. What is the ratio of the hoop strain to the axial strain in the tank.The creep curves in Fig. 2.5 may be used.
Solution The maximum strain in a cylinder which is subjected to an internal pressure, p, is the hoop strain and the classical elastic equation for this is PR = (2
 U) 2hE where E is the modulus, R is the cylinder radius and h is the wall thickness (See Appendix C). The modulus term in this equation can be obtained in the same way as in the previous example. However, the difference in this case is the term u. For elastic materials this is called Poissons Ratio and is the ratio of the transverse strain to the axial strain (See Appendix C). For any particular metal this is a constant, generally in the range 0.28 to 0.35. For plastics u is not a constant. It is dependent on time, temperature, stress, etc and so it is often given the alternative names of Creep Contraction Ratio or Lateral Strain Ratio. There is very little published information on the creep contraction ratio for plastics but generally it varies from about 0.33 for hard plastics (such as acrylic) to almost 0.5 for elastomers. Some typical values are given in Table 2.1 but do remember that these may change in specific loading situations. Using the value of 0.4for polypropylene, €0
h = PR (2~)
~ E E 6.5 from Fig. 2.7, E = = 325 MNlm2 0.02
... h =
0.2 x 0.5 x 103 x 1.6 = 12.3 mm 2 x 0.02 x 325
For a cylindrical tank the axial strain is given by
so
PR
= (1  2u) 2hE 1.6 2 = 2u = =8 Ex 1  2v 0.2 Ex
()
zyxwv zyx zyxwvut
Mechanical Behaviour of Plastics
59
Table 2.1
zyxwvu zyxwvutsrq zyxw Qpical tensile and shear moduli for a range of polymers
Material
Polystyrene (PS) Polymethyl Methacrylate (PMMA) Polyvinyl Chloride (PVC) (Unplasticised) Nylon 66 (at 65% RH) Acetal Homopolymer (POM) Acetal Copolymer (POM) Polyethylene  High Density (HDPE) Polyethylene  Low Density (LDPE) Polypropylene Homopolymer (PP) Polypropylene Copolymer (PP) Polyethersulphone
Density (kg/m3)
Tensile modulus (E)? (GN/m2)
Shear modulus (G) (GN/mZ)
Poisson’s ratio ( u )
1050 1180
2.65 3.10
0.99 1.16
0.33 0.33
1480 1140 1410 1410 955 920 910 902 1390
3.15 0.99 3.24 2.52 1.05 0.32 1.51 1.13 2.76
1.13 0.34 1.15 0.93 0.39 0.1 1 0.55 0.40 0.98
0.39 0.44 0.41 0.39 0.34 0.45 0.36 0.40 0.41

tl00 second modulus at 20°C for small strains (t0.2%)
Note that the ratio of the ratio of the hoop stress ( p R / h ) to the axial stress (pR/2h) is only 2. From the data in this question the hoop stress will be 8.12 MN/m2. A plastic cylinder or pipe is an interesting situation in that it is an example of creep under biaxial stresses. The material is being stretched in the hoop direction by a stress of 8.12 MN/mz but the strain in this direction is restricted by the perpendicular axial stress of OS(8.12) MN/m2. Reference to any solid mechanics text will show that this situation is normally dealt with by calculating an equivalent stress, a,. For a cylinder under pressure a, is given where a0 is the hoop stress. This would permit the above question by OSa& to be solved using the method outlined earlier.
zyxwv
Example 2.4 A glass bottle of sparkling water has an acetal cap as shown in Fig. 2.14. If the carbonation pressure is 375 kN/m2, estimate the deflection at the centre of the cap after 1 month. The value of Poissons ratio for acetal may be taken as 0.33.
Solution The top of the bottle cap is effectively a plate with clamped edges. The central deflection in such a situation is given by Benham et al. as PP 640
6 =  where D =
Eh3 12(1  v2)
To calculate 6 after 1 month it is necessary to know the 1 month creep modulus. The stresses at the centre of the cap are biaxial (radial and circumferential) both
60
zyxwvuts zy zyx zyx Mechanical Behaviour of Plastics Thickness = 1.2 mm
zyxw zyx zyxwvu Fig. 2.14 Acetal bottle cap
given by
o=
+
3pR2(1 u )  3 x 0.375 x (13)2(1.33) 8h2 8( 1 .2)2 o = 22 m / m 2
After 1 month (2.6 x lo6 seconds) at this stress, the strain is obtained from Fig. 2.15 as 2.2%. Hence E = 22 x 106/0.022 = 1 GN/m2. p p 0.375(13)412(1  0.332) 6=640  64 x io00 x (1.213 S=lmm
Example 2.5 In a small polypropylene pump the flange on the cover plate is 2 mm thick. When the rigid clamping screws are tightened, the flange is reduced in thickness by 0.03 mm. Estimate the initial stress in the plastic and the stress after 1 week
Solution The strain in the material is given by E = 
0.03 x 100 = 1.5% 2
This is a stress relaxation problem and strictly speaking stress relaxation data should be used. However, for most purposes isometric curves obtained from the creep curves are sufficiently accurate. By considering the 1.5% isometric curve shown in Fig. 2.8 it may be seen that the initial stress is 16 MN/m2 and the stress after 1 week is 7 MN/m2.
Mechanical Behaviour of Plastics
61 22
zy
20 MWm2 18 16 14
12
zyxw
10 8 6 4
Fig. 2.15 Creep curves for acetal (20°C)
Accurately performed relaxation tests in which the strain in the material was maintained constant and the decaying stress monitored, would give slightly lower values than those values obtained from the isometric data. It should also be noted that in this case the material was loaded in compresion whereas the tensile creep curves were used. The vast majority of creep data which is available is for tensile loading mainly because this is the simplest and most convenient test method. However, it should not be forgotten that the material will behave differently under other modes of deformation. In compression the material deforms less than in tension although the effect is small for strains up to 0.5%. If no compression data is available then the use of tensile data is permissible because the lower modulus in the latter case will provide a conservative design.
zyxwvu zyxwvu zyx zyxwvu
2.6 Thermal Stresses and Strains
It is quite common in modem engineering designs, for plastics to be used in conjunction with other materials, particularly metals. In such cases it is wise to consider the possibility of thermal stresses being set up due to the differences in the thermal expansion (or contraction) in each material. The change in shape of a material when it is subjected to a change in . temperature is determined by the coefficient of thermal expansion, a ~Normally for isotropic materials the value of CYT will be the same in all directions. For convenience this is often taken to be the case in plastics but one always needs
62
zyxwvut zyxw zyxwvuts zyxwvu zyx zyx zyxwvut Mechanical Behaviour of Plastics
to bear in mind that the manufacturing method may have introduced anisotropy which will result in different thermal responses in different directions in the material. The coefficient of thermal expansion, UT, is given by
(2.17)
where SL is the change in length in the material L is the original length AT is the change in temperature.
There are standard procedures for determining UT (e.g. ASTM 696) and typical values for plastics are given in Table 1.2.It may be observed that the coefficients of thermal expansion for plastics are higher than those for metals. Thus if 50 mm lengths of polypropylene and stainless steel are each heated up by 60°Cthe changes in length would be (a) polypropylene, SZ = 100 x (b) stainless steel, SL = 10 x
x 50 x 60 = 0.3 mm x 50 x 60 = 0.03 mm
If these changes in length take place freely then we will have a thermally induced strain in the material (= 0.3 x 100/50= 0.6% in the polypropylene) but no stress. However, if the polypropylene was constrained in some way so that the 0.3 mm expansion could not happen when it is heated by 6O"C, then there would be a thermally induced stress in the material, i.e.
zyxwv
stress = modulus x strain
If the modulus of the material is 1.2 GN/m2 at the final temperature, then the stress in the material would be given by
stress = 1.2 x
io9
(;E)
 = 7.2 MN/m2
Note that the stress is compressive because the material is effectively compressed by 0.3 mm. Example 2.6 The bobbin shown in Fig. 2.16 has been manufactured by sliding the acetal ring on to the steel inner and then placing the endplate in position. At 20°C there are no stresses in the acetal and the distance between the metal endplates is equal to the length of the acetal ring. If the whole assembly is heated to lOO"C, calculate the axial stress in the acetal. It may be assumed that there is no friction between the acetal and the steel. The coefficients of thermal expansion for the acetal and the steel are 80 x 106"C'and 11 x 1060C1 respectively. The modulus of the acetal at 100°C is 1.5 GN/m*.
Mechanical Behaviour of Plastics Steel endplate rigidly fixed to steel bobbin
zyxw zyxwv 63
zy
Acetal
/
zyxwv LG4
Fig. 2.16 Metal bobbin with plastic sleeve
zyxw zyx
Solution Under free conditions, the acetal would expand more than the steel but in the configuration shown they will both expand to the same extent. Hence, the acetal will effectively be put in compression by an amount given by eqn (2.17)
S = (ao CY,)L.AT
= (80  11)106(40)(80)
= 0.22 mm 0.22 x 100 = 0.55% strain = 40 0.55 stress = EE = 1.5 x 10 x 100 = 8.3 MN/m2
Thus there will be a compressive stress of 8.3 MN/m2 in the acetal. It should be noted that the above analysis ignores the effect of the constraining effect which the acetal has on the thermal expansion of the steel. However, as the modulus of the steel is over 100 times greater than the acetal, this constraining
64
zyxwvut zyxwv zyxwv zyx zyxw zyx Mechanical Behaviour of Plastics
effect will be very small. Thus the above analysis is perfectly acceptable for engineering design purposes.
Example 2.7 A nylon ring with a nominal inside diameter of 30 mm, an outer diameter of 50 mm and a width of 5 mm is to be made an interference fit on a metal shaft of 30 mm diameter as shown in Fig. 2.17. The design condition is that the initial separation force is to be 1 kN. Calculate (a) the interference on radius needed between the ring and the shaft and (b) the temperature to which the nylon must be heated to facilitate easy assembly. What will be the maximum stress in the nylon when it is in position on the shaft? The coefficient of friction between nylon and steel is 0.25. The shortterm modulus of the nylon is 1 GN/m2, its Poisson's ratio is 0.4 and its coefficient of thermal expansion is 100 x IO~"C'.
D=50
Im* 1
q = m m m
Namlnal diameter
zyxwvu Fig. 2.17 Inte&rence fit of nylon ring on metal shaft
solution
(a) Force, F = p N
where N = PA
= pnDW
SO,
F = xppDW
zyxwv zyxwv zyxwvut zyxw zyxwv zyxw zyxw
Mechanicd Behaviour of Plastics Therefore
65
1 x 10" 8.5 MN/m2 P= n(0.25 )(30)(5 
The nylon ring may be considered as a duck wall cylinder subjected to this internal pressure (see Appendix D).At the inner surface of the ring there will be a hoop stress, uo, and a radial stress, crrmBenham et al. shows these to be
Hoop stress, cr,,= p
{ ;}
Radial stress, or = p
where k = ratio of outer to inner radius. Hence the hoop strain, 8 0 , at the bore of the ring is given by
SO
kZ
+1
E
This is the interference needed on radius to give the desired separation force. (b) To facilitate easy assembly, the nylon should be heated so that the inner radius expands by his mount. As shown in the previous section
AT=
0.32 .
100 x
. 
x 15
214'C
( c ) The maximum stress in the nylon ring when i t is on the shaft will be the hoop stress at the bore. This is given by 00
=p
k2
+1
66
zyxwvu zy zyxwvu zyxwv Mechanical Behaviour of Plastics
As a practical point, it should be noted that the separation force will change with time. This is because the modulus, E, will decrease with time. Suppose that in this Example, the assembly is to be maintained in position for 1 year and that during this time the modulus decreases to half its initial value (the 1 year modulus would be obtained from the creep curves in the normal way). The above analysis shows that the interface pressure would then be half its initial value (because 6r is fixed) and this in turn means that the separation force would become 500 N instead of 1 kN.
2.7 Multilayer Mouldings
It is becoming common practice to have the crosssection of a plastic moulding made up of several different materials. This may be done to provide a permeation barrier whilst retaining attractive economics by having a less expensive material making up the bulk of the crosssection. To perform stress analysis in such cases, it is often convenient to convert the crosssection into an equivalent section consisting of only one material. This new section will behave in exactly the same way as the multilayer material when the loads are applied. A very common example of this type of situation is where a solid skin and a foamed core are moulded to provide a very efficient stiffnesdweight ratio. This type of situation may be analysed as follows:
Example 2.8 A polypropylene sandwich moulding is 12 mm thick and consists of a foamed core sandwiched between solid skin layers 2 mm thick. A beam 12 mm wide is cut from the moulding and is subjected to a point load, W, at midspan when it is simply supported over a length of 200 mm. Estimate the depth of a solid beam of the same width which would have the same stiffness when loaded in the same way. Calculate also the weight saving by using the foam moulding. The density of the solid polypropylene is 909 kg/m3 and the density of the foamed core is 600 kg/m3.
zyx zyx
Solution The first step in analysing the foamed sandwich type structure is to calculate the second moment of area of the crosssection. This is done by converting the cross section to an equivalent section of solid plastic. This is shown in Fig. 2.18. The equivalent width of the flange in the I section is given by (2.18)
where E, and E, refer to the modulus values for the core ( c ) and solid (s) material. In most cases there is very little information available on the modulus of foamed plastics but fortunately an empirical relationship has been found to
Mechanical Behaviour of Plastics
67
zy
zyxwvut zyxw zyxwv zyxw
Fig. 2.18 Equivalent section for sandwich moulding
exist between density (p) and modulus (Mooreet ul.).
zyxw zyx 2
(2.19)
From the equivalent section the second moment of area can then be calculated as
I =  12(1213 12
12(813 12
= 1439 UTI^
+ 12 (  m )2 ( 909
The solid polypropylene beam which would have the same stiffness when loaded in the same way would need to have the same 2nd moment of area. So if its depth is d then 12(d)3  1439, d = 11.3 ~ U T I 
12 The weight per unit length of the solid beam would be
W,= 12 x 11.3 x
x 909 x lo3 = 123 g
The weight per unit length of the foamed beam is
W f = (909 x 2 x 12 x 2 x
+ (600 x 12 x 8 x
= 101.2 g Hence the weight saving is 17.7% Once the foamed plastic moulding has been converted to an equivalent section of solid plastic then the long term design procedures illustrated in the
68
zyx zyxwv zy zyxwv zyxwv zyxwvu zyxw zyxwvu Mechanical Behaviour of Plastics
previous questions can be used. For example, to determine the 1 year deflection of the beam in this question, the appropriate 1 year modulus from the polypropylene creep curves could be used. Throne has reported that the relationship between foam modulus and density can be generalised to other properties such as tensile strength, fatigue strength, creep properties as well as shear and compression modulus. Thus if X is the general material property then
“=(E)
2
(2.20)
X,
Example 2.9 A solid polyethylene beam is 10 mm thick and 15 mm wide. If it is to be replaced with a sandwich section with solid polyethylene in the two outer skins and polyethylene foam (density = 200 kg/m3) in the centre, calculate the dimensions of the sandwich beam if it is to have optimum stiffness at the same weight as the solid beam.If the foam material costs 20% more than the solid material, calculate the increase or decrease in cost of the sandwich beam.
Solution The weight per unit length, W , for the solid beam is W = 935 x lo3 x 15 x 10 x
= 140 g/m
For the sandwich section
+
W = p,bh p,2bd W  2 b d p   W_ 2d h= PCb bP,D D where D = density ratio ( p c / p s ) . The flexural stiffness of the beam will be proportional to EZ. So converting the section to an equivalent ‘I’ beam as in the previous example   + 12 (;)2$]
E,I = E,
h)3 bh3 Substituting for h from above, the stiffness may be optimised for constant W , by differentiating this expression and equating to zero. This gives the optimum beam depth as 1
48W
48W
2  1)(D  1 ) + 2 4 W d ( DbPsD2
1
Mechanical Behaviour of Plastics
zyxw 69
Solid skin
zyxwvuts zyxwvu Solid skin
zyxw zyxwv zyxwvutsr zyxw Original solid/foam/ Solid section
Equivalent solid section
Fig. 2.19
Using the information given
D = 200/935 = 0.214, so
p, = 935 x
g/mm3,
W = 0.14 g/m
d = 1.61 mm
Using the expression for h from above, the thickness of the foam is given by h = 31.6 IWII
The cost of the solid beam is given by (Cost), = 935 x 10 x 15 x
x C , = 0.14 C ,
The cost of the sandwich beam is given by (C0st)F = pcbhCc
+ pS2bdCs = 0.159 C ,
Hence the additional cost =
0.159  0.14 = 13.5% 0.14
It is interesting to generalise this solution for any core: skin density ratio. Fig. 2.20 shows how the optimum skin thickness varies with D. This is independent of the solid material density or modulus but is based on a weight
zy zy zyx zyxwvut
zyxwv Mechanical Behaviour of Plastics
70
per unit length of 140 g/m (equivalent to a solid thickness of 10 mm). If a different solid thickness is of interest then the optimum skin thickness would need to be scaled accordingly. For example, for a 5 mm thick solid beam which is to be converted to a foam sandwich beam of the same weight per unit length, the optimum skin thickness would be half of the value shown in Fig. 2.20. The optimum skidcore thickness ratios are shown in Fig. 2.21. 1.66
1.64
EZ;
d
1.6
5 1.58 1.56
f E
1.54 1.52 1.5 1.48 1.46
0
0.1
0.3
0.2
0.4
zy zyxw 0.5
0.6
0.7’
0.8
0.9
zyxwvutsr Densny ratk (core:)
Fig. 2.20 Variation of optimum skin t h i c h with core: skin density ratio 90 80 70
60 50
40
:; 30
0
0
0.1
0.2
0.3
0.4
0.5
0.6
Density ratlo (core:skln)
Fig. 2.21 Optimum skin to core ratio for constant weight
zyxw zyx zyxwv zyxwvu zyxwvuts
Mechanical Behaviour of Plastics
71
The stiffness ratios (Le. stiffness of the foam sandwich beam relative to the original solid beam) are also given in Fig. 2.21. In both cases the values given are independent of the original solid material or its dimensions, so this provides a good design chart. The design of solid/foam sandwich structures is also considered in Chapter 3 in the laminate analysis. 2.8 Design of Snap Fits
A major attraction of plastics to designers is the ease with which fast assembly mechanisms can be incorporated into the endproduct. A very good example of this is the snap fit. A typical design is shown in Fig. 2.22 although there
are many variations. Snap fits exploit the fact that thin plastic sections can undergo relatively large flexural deflections for a short period of time and exhibit complete recovery. The design of snap fits is straightforward and does not involve creep curves since the timescale of the deflectionlstress is small. The point that will be illustrated here is that in a real design situations it is necessary to choose combinations of dimensions which provide the necessary function but which do not overstress the plastic. In the following example a
Fig. 2.22 Snap fit for Example 2.10
72
zyxwvuts zyxwv zy z z z zyxw zyxwvu Mechanical Behaviour of Plastics
set of design curves are developed to show how the different combinations of dimensions might be selected.
Example 2.10 The polypropylene snap fit shown in Fig. 2.22 is to have a length of 1030 mm. If the insertion force is not to exceed 4 N and the yield stress of the plastic is 30 MN/m2, calculate suitable crosssectional dimensions for the snap fit. The shortterm modulus of the polypropylene is 900 MN/m2 and the coefficient of friction is 0.3. The safety factor on stress is to be 2. Solution
Resolving vertical forces gives V=NcosapNsina
= N(cos a  p sin a)
Resolving horizontal forces gives
1 F=Nsina+pNcosa = N(sina
+ pcosa)
b
Eliminating N from the above equations gives
V = F { 1ptana p+tana
}
The snap fit may be regarded as a cantilever and for this situation, the vertical deflection, ti, is given by VL3 3EI t i =  {FL3 3EI ti=
bd3 where I = 
1ptana p tana
+
Insertion force F=
(Lfd)l
{: E}
}
12
(2.21)
For polypropylene in the situation given, Fig. 2.23 shows a set of design curves linking F, b and ( L / d ) . For a limiting insertion force of 4 N and a typical maximum thickness, d , of 2 mm (to avoid excessive moulding times  Chapter 5). a length of 20 mm would give an L/d ratio of 10 which gives b = 18 mm.
zy zyxw
Mechanical Behaviour of Plastics
73
10
9
,a
J
P7 '
s6
4
6
a
10
zyxwvu zyxwv zyxwv zy
12
14
16
ia
Length to thickness ratb (Ud)
Fig. 2.23 Variation of insertion force with beam dimensions
zyxwvu
It is also necessary to check that the stress in the snap fit does not exceed the yield strength for the material (30 MN/m2). Allowing for a safety factor of 2, the maximum permissible stress will be 15 MN/m2. The stress in a cantilever beam of this type will be maximum at point A (Fig. 2.22) and is given by stress, UA = MY 
I
where M = bending moment (= VL) y = half depth of beam (= d/2) I = second moment of area (= bd3/12)
(2.22) For the conditions given, OA = 13.5 MN/m2 which is less than the permitted maximum of 15 MN/m2 and so the chosen dimensions are acceptable. Note that the stress is independent of the width, b. Fig. 2.24 gives a set of design curves for the situation considered so that it may be seen that other combinations of L, d and b could be chosen to meet the design specification. For example, L = 22 mm, d = 2.5 mm and b = 12 mm gives an insertion force of 4 N and a maximum stress of 14 MN/m2 which is again acceptable.
74
zyxwvuts zy
zyxwv zyxwvuts zyxwv Mechanical Behaviour of Plastics
L=10 mm
15 t"Un
40
35
20 mm
30
25
5E. 20
25 mm
5 15
30 mm
'
35 mm
10
zyxwv 40 mm
5
0 0
1
2 3 Beam thickness, d (mm)
4
5
Fig. 2.24 Variation of stress with beam dimensions
2.9 Design of Ribbed Sections
It will be shown later (Chapters 4 and 5 ) that it is normally good practice to design plastic products with crosssections which are as thin as possible. This is because thick sections cool very slowly and hence the moulding cycle times are long resulting in uneconomic production. Also, thick sections tend to shrink more and can lead to warpage and distortion. Of course thin sections tend to have low stiffness and so engineers usually adopt geometrical configurations which will enhance stiffness whilst retaining the required thinness in the wall section. In any particular material, the flexural stiffness will be defined by the second moment of area, I , for the crosssection. As with a property such as area, the second moment of area is independent of the material  it is purely a function of geometry. If we consider a variety of crosssections as follows, we can easily see the benefits of choosing carefully the crosssectional geometry of a moulded plastic component. All the sections have the same crosssectional area (and hence the same weight).
zyxwvut
(a) (b) (c) (d) (e)


Solid Rectangle Solid Rectangle Solid Rectangle Square Hollow rectangular box
(B = 1OD) (B = 4 0 ) (B = 2 0 ) (B = D ) (B = 2 0 , B = 1Oh)
zy zyxwvu zyxwv zyxwv
Mechanical Behaviour of Plastics (f)
(8) (h) (i)



Solid circular section Thin wall tube Thick wall tube Tsection
75
(D = 10h) (D = 4h) (B = 8h)
Fig. 2.25 illustrates the various crosssections and Fig. 2.26 compares their flexural stiffnesses. An important conclusion from this is that ‘T’ sections (or
B=4D
B=2D
B=D
(4
1
B = 2D and B = 10h
Fig. 2.25 Various crosssections
76
zyxwvuz Mechanical Behaviour of Plastics
zyx
Dia = 4h
zyxwvu zyxwv +IF?
Fig. 2.25 (continued)
indeed ‘L‘ or ‘U’sections) are very efficient at providing excellent stiffness per unit weight. The following Example illustrates how such sections can be designed into plastic products. Example 2.11 An aluminium cantilever beam is 50 mm wide, 80 mm long and 2 mm deep. The loading is 200 N spread uniformly over the cantilever. If the beam is to be replaced by one made from acetal and the design criteria is that the end deflections should be the same in each beam after one month, calculate the dimensions (a) of a solid acetal beam and (b) an acetal beam with unidirectional ribs. The modulus of the aluminium is 70 GN/m2.
Mechanical Behaviour of Plastics
4500 4000
zyxw 77
zyxwvut
3500
1500
1000
500
zyxwvut
0
zyxwvu zyxwv zyxwvu zyxwvutsrq Fig. 2.26 Effect of geometry of flexural stiffness
Solution
(a) In order that the two beams (aluminium and acetal) will have the same stiffness it is necessary that
(EOd = (EZ)aCetul
(2.23)
In order to get the 1 month modulus for acetal, the strain in the beam must be known. CJ MY  W(L/2)(dU1/2)Strain,  WLdar EI EI 4EI where W = total load (200 N) and d d = depth of beam. Also, deflection
6=
WL3 8EZ
So, strain,
Using the information for the aluminium 6=
200 x 803 x 12 = 5.5 mm 8 x 70 x lo3 x 50 x 23
78
zyxwvut zyxwvu zyx zyx zyxw zyx Mechanical Behaviour of Plastics
Therefore,
E=
2 x 5.5 x 2
802
= 0.34%
From the creep curves for acetal, at 1 month (2.6 x lo6 s) and 0.34% strain, ) approximately 1.3 GN/m2. the modulus ( 0 , ' ~is Therefore, using (2.23) and ignoring (W/12) on each side
70 x 23 = 1.3 x D3 D = 7.6 m m
Hence an acetal beam 7.6 mm deep and of the same width and length as the aluminium beam will perform in exactly the same way when the load of 200 N is applied. However, as will be shown in Chapters 4 and 5, it would not be good design practice to use a plastic beam Section 7.6 m m thick. Such a section would take a long time to mould and would probably have sink marks on its surface. It would be preferable to use thinner wall sections and introduce ribs to provide the desired stiffness. This is illustrated below. (b) Consider the flat beam to be replaced by a ribbed section as shown in Fig. 2.27. It is necessary for the second moment of area, I , to be the same for both sections. Clearly there are many permutations for the dimensions of the 4
W
zyxwv
Fig. 2.27 Flat beam and ribbed section, Example 2.11
zyx zyxw zy zyxwvut
Mechanical Behaviour of Plastics
79
ribbed section which would meet this requirement. One practical consideration is that the thickness of the rib should be less than the thickness of the top plate ( d ) in order that there will be no evidence (sink mark) to show the presence of the rib on the underside of the plate. A typical ratio (#?)of rib thickness to plate thickness is 0.6. In order to assist with the design of the ribbed plate, Fig. 2.28 shows a chart to enable permissible combinations of dimensions to be chosen. For example, suppose that we wish the plate thickness to be 2 mm and there are to be five ribs (= N) across the plate. 3
2.5
zyxwvutsr
2
n a
1.5
1
0.5
zyxwvuts
0 0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1
z
h/D
Fig. 2.28 Design of ribbed plates
Then
2 50 W I N D = = 0.66 and h / D =  = 0.26 5 x 7.6 7.6
From Fig. 2.28, d / D = 1.3. So the depth of the 5 ribs would be 1.3 x 7.6 = 9.9 mm and their width would be 0.6 x 2 = 1.2 m. Such a ribbed beam would perform in exactly the same way as the original aluminium beam or the flat acetal beam. However, an additional consideration is buckling of the ribs. If the ribs are thin and deep there is a possibility that they will buckle along the lower unsupported edge if they are loaded in compression (Le. downward deflection of the cantilever in this Example).
80
zyx zyxwvutsr zyxw zyxw zyxwv zyx zyxwvu Mechanical Behaviour of Plastics
Buckling is complex to analyse but if we consider the rib as a flat plate, clamped along one edge then Roark gives the formula for the critical buckling stress as
1.2E (1  9 )
or
2
(2.24)
If we take the critical stress as the yield stress then for many plastics, the ratio of UJE is approximately 35 x Using Poisson's ratio, u = 0.35 and taking /I = 0.6, as before, then
_h 
h D  0.267 d  5 ' 2 
or d
 = 3.75
D
h

D
This line may be superimposed on the rib design data as shown in Fig. 2.28. Combinations of dimensions above this line are likely to provide ribs which are too slender and so are liable to buckling. Combinations below the line are likely to be acceptable but do remember the assumptions made in the determination of the buckling line  in particular, the ratio of u,/E will increase with time due to creep and this will cause the buckling line to move downwards. Returning to the Example, it is apparent that the dimensions chosen lie above the buckling line. It is necessary therefore, to choose other dimensions. For example, h = 2.5 mm gives h D
 = 0.33,
W  = 0.66 (as before) ND
So d / D = 1.15 which gives d = 11.15(7.6) = 8.7 mm. These dimensions lie below the buckling line and so are acceptable. The solution would therefore be a ribbed beam with five ribs, plate thickness = 2.5 mm, rib thickness = 1.5 mm and rib depth = 8.7 mm. It should be noted that ribbed sections play an extremely important part in the design of plastic products. Not only do they reduce manufacturing times (because they utilise thinner sections), but they also save material. It may easily be shown in this case that the volume of the ribbed beam is half the volume of the flat acetal beam and this will result in a substantial cost saving. Fig. 2.29 shows a design chart for slightly thicker ribs (/I= 0.8) so as to reduce the likelihood of rib buckling.
zy zyxwvutsrq 81
Mechanical Behaviour of Plastics
zyxwvutsrq
3
2.5
2
1.5
1
0.5
0 0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1
hlD Fig. 2.29 Design of ribbed beams
2.10 Stiffening Mechanisms in Other Moulding Situations In some moulding methods such as blow moulding, thermoforming and rotational moulding, it is difficult if not impossible to produce stiffening ribs. Hence other stiffening configurations such as corrugations have to be used. Fig. 2.30 illustrates a typical repeat unit in such a corrugation. The second moment of
Fig. 2.30 Cormgation profile
zyx
82
z
zyxwvuts zyxw zyxw zyxw zyxwvuts zyxwvu Mechanical Behaviour of Plastics
area, I , will quantify the stiffening effect of the crosssection and if this is related to the I value for the flat sheet of the same length and thickness then it is possible to define a stiffness enhancement factor, q, as q=
L
{
mh+
(7
4>
2nh 24n +sin a +h sin a (7
2
+ph+
(7 ( n h +
q)lJ
:))
2
(2.25)
where 7 = distance to centre of area from the base of the crosssection, i.e.
+ + 0 . 5 +~ 
0.5m p n y=h
p+m+
tana
and b m=h'
B p=h'
D n=h
zyx
Clearly there are many permutations of D, b, h, a, etc and Fig. 2.31 shows how the stiffness enhancement factor, q, changes with various values of these parameters. In each case the angle a has been fixed at 85" and the corrugation dimensions have been expressed as a function of the wall thickness, h.
Fig. 2.31 Stiffness of cormgations as function of dimensions
zyxwv zyxw zyxw zyx zyxw zyxw zyx 83
Mechanical Behaviour of Plastics
The obvious question is ‘Is there an optimum design for the corrugations?’ Unforhmately the answer is ‘No’because if one wishes to increase transverse stiffness then the obvious thing to do is to increase D up to the point where buckling problems start to be a concern. Usually this is when D / h = 10, for shortterm loading and less than this for long term loading because of the decrease in modulus of viscoelastic materials. Another approach is to recognise that initially for a flat sheet, the axial stiffness is high but the transverse stiffness is relatively low. As the corrugation depth increases then the transverse stiffness increases but at the expense of the axial stiffness. It is readily shown that the axial deflection per unit load for the corrugations for the new geometry compared with the flat sheet is given by 4n3h Axial stiffness ratio = L sin2a
(2.26)
If this is then divided into the previous enhancement ratio, q, it is possible to observe the way in which one stiffness increases at the expense of the other. Fig. 2.32 shows this transverse/axial stiffness ratio as a function of the depth of the corrugations. It may be seen that when the depth is less than four times the wall thickness then the axial stiffness ratio is better than the transverse stiffness ratio. However, when the depth is greater than four times the wall thickness then the transverse stiffness ratio dominates. 14 12
3
lo
t
E E=
6
4 2 0
1
2
3
4
6
5
7
Dh
Fig. 2.32 Optimisation of Corrugation depth
a
9
10
84
zyxwvu zyxwv zyxwv
zyxw zyxw zyxw zyxw Mechanical Behaviour of Plastics
This would suggest that D / h = 4 offers the best balance of transverse and axial properties. In fact the ‘optimum’ ratio is essentially independent of the thickness, h, but it depends on B and b. Fig. 2.33 shows this relationship and reflects the combinations of B, b, D and h which will give the best design of cormgations. Generally it is desirable to have B and b approximately equal and it is also good design practice to keep D / h well below 10 (to avoid buckling). Hence values of B, h and D in the shaded area tend to be best. A combination of D / h = 4, b/h = 5 and B / h = 4 is known to give good results for rotationally moulded products where shape must be used very effectively to ensure good performance.
zyxwvuts B/h=
7
6
I
8
10
8
3 2
1
0
2
4
wh
6
8
10
Fig. 2.33 Variation of optimum Dlh with blh
2.11 Mathematical Models of Viioelastic Behaviour Over the years there have been many attempts to simulate the behaviour of viscoelastic materials. This has been aimed at (i) facilitating analysis of the behaviour of plastic products, (ii) assisting with extrapolation and interpolation of experimental data and (iii) reducing the need for extensive, timeconsuming creep tests. The most successful of the mathematical models have been based on spring and dashpot elements to represent, respectively, the elastic and viscous responses of plastic materials. Although there are no discrete molecular structures which behave like the individual elements of the models, nevertheless
Mechanical Behaviour of Plastics
zyxwvu zyxwv 85
they do aid in the understanding and analysis of the behaviour of viscoelastic materials. Some of the more important models will now be considered.
(a) Maxwell Model
The Maxwell Model consists of a spring and dashpot in series at shown in Fig. 2.34. This model may be analysed as follows.
zyxwvutsrqp zyxwvuts zyxwvu zyxwv zyxwvutsrq Stressa
Fig. 2.34 The Maxwell model

Stress Strain Relations
The spring is the elastic component of the response and obeys the relation 01
= ( . &I
(2.27)
where (TI and ~1 are the stress and strain respectively and 4 is a constant. The dashpot is the viscous component of the response and in this case the stress a2 is proportional to the rate of strain E 2 , ie 02
where
r)
= r) ’ E2
(2.28)
is a material constant.
Equilibrium Equation
zyxwvut
For equilibrium of forces, assuming constant area Applied Stress,
(T
= ( T ~= 0 2
(2.29)
Geometry of Deformation Equation The total strain,
so
E
is equal to the sum of the strains in the two elements. &=&1+&2
(2.30)
zyxwvu zyxw
86
Mechanical Behaviour of Plastics
From equations (2.27), (2.28) and (2.30)
(2.31) This is the governing equation of the Maxwell Model. It is interesting to consider the response that this model predicts under three common timedependent modes of deformation.
zyxw zy zyxw zyx
(i) creep If a constant stress, a,, is applied then equation (2.31) becomes . 1 €=*a,
(2.32)
r)
which indicates a constant rate of increase of strain with time. From Fig. 2.35 it may be seen that for the Maxwell model, the strain at any time, t, after the application of a constant stress, a,, is given by 00
€ ( t )= 
5
w
i
+r ta0)
t
'E
; i
0
b
tl
t2
t
Fig. 2.35 Response of Maxwell model
Time

zyxwvu zyxw zy zyxwvuts zyxw zyxw zyx zyxwv 87
Mechanical Behaviour of Plastics
Hence, the creep modulus, E ( t ) , is given by
(2.33)
(ii) Relaxation If the strain is held constant then equation (2.31) becomes
Solving this differential equation (see Appendix B) with the initial condition o = a,, at t = to then,
5,
a(r)= aoe
11
a(t)= oOef/TR
(2.34)
(2.35)
where T R = q / e is referred to as the relaxation rime. This indicates that the stress decays exponentially with a time constant of q/t (see Fig. 2.35).
(iii) Recovery When the stress is removed there is an instantaneous recovery of the elastic strain, E ' , and then, as shown by equation (2.31), the strain rate is zero so that there is no further recovery (see Fig. 2.35). It can be seen therefore that although the relaxation behaviour of this model is acceptable as a first approximation to the actual materials response, it is inadequate in its prediction for creep and recovery behaviour. (b) Kelvin or Voigt Model In this model the spring and dashpot elements are connected in parallel as shown in Fig. 2.36.
+
Stress. u
Fig. 2.36 The Kelvin or Voigt Model
88
zy z zyxwv zyx zy zyxw zyxwv Mechanical Behaviour of Plastics
StressStrain Relations These are the same as the Maxwell Model and are given by equations (2.27) and (2.28).
Equilibrium Equation For equilibrium of forces it can be seen that the applied load is supported jointly by the spring and the dashpot, so a = u1
+ a2
(2.36)
Geometry of Deformation Equation In this case the total strain is equal to the strain in each of the elements, i.e. &=E1
=E2
(2.37)
From equations (2.27), (2.28) and (2.36) a = 6 * El
or using equation (2.37)
+ qb2
a=f*&+q*&
(2.38)
This is the governing equation for the Kelvin (or Voigt) Model and it is interesting to consider its predictions for the common time dependent deformations. (3 c=p If a constant stress, a,, is applied then equation (2.38) becomes a, = 6 * E
+qi
and this differential equation may be solved for the total strain, E , to give
where the ratio q / ( is referred to as the retardation time, T R . This indicates an exponential increase in strain from zero up to the value, ao/t,that the spring would have reached if the dashpot had not been present. This is shown in Fig. 2.37. As for the Maxwell Model, the creep modulus may be determined as (2.39)
zy
Mechanical Behaviour of Plastics
zyxwv 89
zyxwvut
zyxw zyxwv zyxw zyxwvutsrq zyxwvu zyx
Fig. 2.37 Response of KelvinNoigt model
(ii) Relaxation
If the strain is held constant then equation (2.38) becomes U = C * E
That is, the stress is constant and supported by the spring element so that the predicted response is that of an elastic material, Le. no relaxation (see Fig. 2.37)
(iii) Recovery If the stress is removed, then equation (2.38) becomes
0=C . E +
r)€
Solving this differential equation with the initial condition E = E’ at the time of stress removal, then
i!
~ ( t=) de
(2.4)
This represents an exponential recovery of strain which is a reversal of the predicted creep.
(c) More Complex Models It may be seen that the simple Kelvin model gives an acceptable first approximation to creep and recovery behaviour but does not account for relaxation. The Maxwell model can account for relaxation but was poor in relation to creep
90
zyxwvut zyx zyx Mechanical Behaviour of Plastics
and recovery. It is clear therefore that some compromise may be achieved by combining the two models. Such a setup is shown in Fig. 2.38. In this case the stressstrain relations are again given by equations (2.27) and (2.28). The geometry of deformation yields.
Total strain, E = e1 + €2 + &k
(2.41)
52
Fig. 2.38 Maxwell and Kelvin models in series
where &k is the strain response of the Kelvin Model. From equations (2.27), (2.28) and (2.41).
(2.42) From this the strain rate may be obtained as
(2.43) The response of this model to creep, relaxation and recovery situations is the sum of the effects described for the previous two models and is illustrated in Fig. 2.39. It can be seen that although the exponential responses predicted in these models are not a true representation of the complex viscoelastic response of polymeric materials, the overall picture is, for many purposes, an acceptable approximation to the actual behaviour. As more and more elements are added to the model then the simulation becomes better but the mathematics become complex.
Example 2.12 An acrylic moulding material is to have its creep behaviour simulated by a four element model of the type shown in Fig. 2.38. If the creep curve for the acrylic at 14 MN/m2 is as shown in Fig. 2.40, determine the values of the four constants in the model.
zy
91
Mechanical Behaviour of Plastics
0
tl
zy
zyxwvu zyxwvuts 12
Time
Fig. 2.39 Response of combined Maxwell and Kelvin models
0
zyxwvutsrqpon zyxwvutsrq
0
300
200
100
400
500
Time (hours)
Fig. 2.40 Creep curve for acrylic at 20°C
zy zyxwv
Solution The spring element constant, 61, for the Maxwell model may be obtained from the instantaneous strain, ~ 1 Thus .
'
oo 14 ,= 2800 MN/m2  e1 0.005
The dashpot constant, V I , for the Maxwell element is obtained from the slope of the creep curve in the steady state region (see equation (2.32)). a0
?)I==
E
14 = 1.2 x io7 MN.iu/m2 1.167 x = 4.32 x 10" MN.s/m2
92
Mechanical Behaviour of Plastics
The spring constant, 62, for the KelvinVoigt element is obtained from the maximum retarded strain, ~ 2in, Fig. 2.40.
zy zyxwvut
The dashpot constant, q2, for the KelvinVoigt element may be determined by selecting a time and corresponding strain from the creep curve in a region where the retarded elasticity dominates (i.e. the knee of the curve in Fig. 2.40) and substituting into equation (2.42). If this is done then q2 = 3.7 x lo8 MN.s/m2. Having thus determined the constants for the model the strain may be predicted for any selected time or stress level assuming of course these are within the region where the model is applicable.
z
zyxwv zyx
(d) Standard Linear Solid Another model consisting of elements in series and parallel is that attributed to Zener. It is known as the Standard Linear Solid and is illustrated in Fig. 2.41. The governing equation may be derived as follows.
I Stress. u
Fig. 2.41 The standard linear solid
zyx
StressStrain Relations As shown earlier the stressstrain relations are 0 1 = 41&1 0 2 = E2&2 (73 = 7l3E3
(2.44) (2.45) (2.46)
Equilibrium Equation In a similar manner to the previous models, equilibrium of forces yields. (TI = a3 (2.47) (J = a 1 +a 2
zyxwv zyxwv zyxwvutsrq zyxwvuts zyxwvut 93
Mechanical Behaviour of Plastics
Geometry of Deformation Equation
In this case the total deformation, E , is given by E
= E2 = E l
+ E3
(2.48)
From equation (2.48)
&=&1+&3
but from equation (2.47)
a1 = a  a2
~ I I ~ U ~ = C T  U ~
Rearranging gives (2.49) This is the governing equation for this model. The behaviour of this model can be examined as before
zy zyxwv
(9 creep
If a constant stress, a,, is applied then the governing equation becomes
+ t2)1 + 6162e  6100 = 0
&{q3(6l
The solution of this differential equation may be obtained using the boundary 62) at t = 0. So condition E = a,/(ij1
+
(2.50)
zyx
It may be seen in Fig. 2.42 that this predicts the initial strain when the stress is first applied as well as an exponential increase in strain subsequently.
(ii) Relaxation If the strain is held constant at E', then the governing equation becomes v3a
+ 610  6162.s' = 0
This differential equation may be solved with the boundary condition that a = a, = ~ ' ( 6 1 62) when the strain is first kept constant.
+
Stress, a(t)=
~
61
+h
This predicts an exponential decay of stress as shown in Fig. 2.42.
(2.51)
z zy
zyxwvuts zyxwvutsrq Mechanical Behaviour of Plastics
94
Stress =0
zyxwvu
I. &I d
w Time
1
zyxwvutsrqponm Time
Fig. 2.42 Response of standard linear solid
(iii) Recovery
If the stress is at a value of equation becomes
0’
and then completely removed, the governing
+ e2)& + e1e2& = 0
1)3(e1
The solution of this differential equation may be obtained using the boundary condition that when the stress is removed, the strain is given by E’
= a’/(e1
+ (2)
(2.52)
This predicts an instantaneous recovery of strain followed by an exponential decay. It may be observed that the governing equation of the standard linear solid has the form U,O = b l i bo&
+
+
zyxwvuts zyx 95
Mechanical Behaviour of Plastics
where al, a,, bl and bo are all material constants. In the more modem theories of viscoelasticity this type of equation or the more general form given in equation (2.53) is favoured.
The models described earlier are special cases of this equation.
2.12 Intermittent Loading
The creep behaviour of plastics considered to date has assumed that the level of the applied stress is constant. However, in service the material may be subjected to a complex pattern of loading and unloading cycles. This can cause design problems in that clearly it would not be feasible to obtain experimental data to cover all possible loading situations and yet to design on the basis of constant loading at the maximum stress would not make efficient use of material or be economical. In these cases it is useful to have methods of predicting the extent of the recovered strain which occurs during the rest periods of conversely the accumulated strain after N cycles of load changes. There are several approaches that can be used to tackle this problem and two of these will be considered now.
2.12.1 Superposition Principle
zyxw zy zyxwvuts
The simplest theoretical model proposed to predict the strain response to a complex stress history is the Boltzmann Superposition Principle. Basically this principle proposes that for a linear viscoelastic material, the strain response to a complex loading history is simply the algebraic sum of the strains due to each step in load. Implied in this principle is the idea that the behaviour of a plastic is a function of its entire loading history. There are two situations to consider.
(a) Step Changes of Stress When a linear viscoelastic material is subjected to a constant stress, u1, at time, t l , then the creep strain, &(t),at any subsequent time, t, may be expressed as (2.54)
where E(t  t l ) is the timedependent modulus for the elapsed time (t  tl). Then suppose that instead of this stress q , another stress, a2 is applied at some arbitraxy time, t2, then at any subsequent time, t , the stress will have been applied for a time (t  t2) so that the strain will be given by &(t)=
1
 t2)
.fJ1
zyxwv zyxw zyxwv zyxw zyxwvutsrq zyxw zyx
96
Mechanical Behaviour of Plastics
Now consider the Situation in which the stress, 01, was applied at time, t l , and an additional stress, 02, applied at time, r2, then Boltzmanns’ Superposition Principle states that the total strain at time, t, is the algebraic sum of the two independent responses. E(t)
1 = E(t  t l ) a0
+ E(r 1 12)
*
61
This equation can then be generalised, for any series of N step changes of stress, to the form i=N
e(t) =
Eoi
(2.55)
i=l
where ai is the step change of stress which occurs at time, ti. To illustrate the use of this expression, consider the following example.
Example 2.13 A plastic which can have its creep behaviour described by a Maxwell model is to be subjected to the stress history shown in Fig. 2.43(a). If the spring and dashpot constants for this model are 20 GN/m2 and 1000 GNs/m2 respectively then predict the strains in the material after 150 seconds, 250 seconds, 350 seconds and 450 seconds.
zyxwvut zyxw
Solution From Section 2.1 1 for the Maxwell model, the strain up to 100s is given by a m E(t) = 
+
t t l
Also the time dependent modulus E ( t ) is given by O E(t) = 
ttl
 tl+
(2.56)
~
tt
Then using equation (2.54) the strains may be calculated as follows: (i) at t = 150 seconds; ai = 10 MN/m2 at tl = 0, a2 = 10 MN/m2 at t2 = 100 s
= 0.002  0.001 = 0.1%
(ii) at 250 seconds; 6 1 ,
a2
as above, a3 = 5 MN/m2 at t3 = 200 s
~ ( 2 5 0= ) 10
ttl
tl
+
*
= 0.003  0.002
(250  200)
+ 0.0005 = 0.15%
1
Mechanical Behaviour of Plastics
97
zy
zyxwv zyxwvu zyxwv zyxwvu Time (s)
0.5
0.4
3 v
9
0.3 0.2
0.1
0
0
100
200 300 Time (s)
5 K)
zyxwvutsr
Fig. 2.43 Strain predictions using superposition theory
(iii) at 350 seconds; 01, SO,
02,
zyxw
a3 as above, a4 = 10 MN/m2 at r4 = 300 s
~ ( 3 5 0= ) 0.003 = 0.3% (iv) and in the same way
~ ( 4 5 0= ) 0.004 = 0.4%
The predicted strain variation is shown in Fig. 2.43(b). The constant strain rates predicted in this diagram are a result of the Maxwell model used in this example to illustrate the use of the superposition principle. Of course superposition is not restricted to this simple model. It can be applied to any type of model or directly to the creep curves. The method also lends itself to a graphical solution as follows. If a stress 01 is applied at zero time, then the creep curve will be the time dependent strain response predicted by equation (2.54). When a second stress, a2 is added then the new creep curve will be obtained by adding the creep due to a2 to the anticipated creep if stress a1 had remained
98
zy zyxw zyxw zyxwvut Mechanical Behaviour of Plastics
alone. This is illustrated in Fig. 2.44(a). Then if all the stress is removed this is equivalent to removing the creep strain due to 6 1 and 02 independently as shown in Fig. 2.44(b). The procedure is repeated in a similar way for any other stress changes.
zyxwvuts 
1iI
0
4
Fig. 2.44(a)
tL
tsm
Stress history
Fig. 2.44(b) Predicted strain response using Boltzmann’s superposition principle
(b) Continuous Changes of Stress If the change in stress is continuous rather than a step function then equation (2.55) may be generalis4 further to take into account a continuous loading cycle. So
zyxwvuts t
(2.57)
where a(t) is the expression for the stress variation that begins at time, tl. The lower limit is taken as minus infinity since it is a consequence of the
zy zy zyxwv zyxwvu zyxwv
Mechanical Behaviour of Plastics
99
Superposition Principle that the entire stress history of the material contributes to the subsequent response. It is worth noting that in exactly the same way, a material subjected to a continuous variation of strain may have its stress at any time predicted by
(2.58)
m
To illustrate the use of equation (2.57) consider the following Example. Example 2.14 A plastic is subjected to the stress history shown in Fig. 2.45.
The behaviour of the material may be assumed to be described by the Maxwell model in which the elastic component 6 = 20 GN/m2 and the viscous component 9 = lo00 GNs/m2.Determine the strain in the material (a) after u1 seconds (b) after u2 seconds and (c) after u3 seconds. Stress (MN/m2)
100
U2
zyxwvu T'
Time (s)
Fig. 2.45 Stress history to be analysed
Solution As shown in the previous Example, the modulus for a Maxwell element may be expressed as
6v
E(t) = 9 6t (a) The stress history can be defined as
+
100
zy zyxw zyxwvutsrqp zyxwvu zyx Mechanical Behaviour of Plastics
Substituting into equation (2.57)
E(U1)
= .
zyxw
then for u1 = 50 seconds and K1 = 0.1 MN/m2s
E(100) = 0.1(100)
(20
lo3
+ E) = 0.1% 2 x lo6
It is interesting to note that if K1 was large (say K1 = 10 in which case T = 1 second) then the strain predicted after application of the total stress (10 MN/m*) would be ~ ( 1 = ) 0.0505%. This agrees with the result in the previous Example in which the application of stress was regarded as a step function. The reader may wish to check that if at time T = 1 second, the stress was held constant at 10 MN/m2 then after 100 seconds the predicted strain using the integral expression would be ~ ( 1 0 0 = ) 0.1495% which again agrees with the previous example. (b) After the time T, the change in stress is given by
zyxwvu
Hence,
where tl = 0 and t2 = T = 100 s.
 (K1 K2)U2
zyxwv
[6 + 1
u2

2a
1'a
zyxwvuts zyxwvuts zyxw
Mechanical Behaviour of Plastics
101
then for K2 = 0.2 MN/m2s, T = 100 seconds and u2 = 125 seconds ~ ( 1 2 5= ) 0.094%
(c) After the time T ' , the change in stress is given by Change in stress, a ( t ) = K2(t  T ' ) dm) dt
= K2
Hence,
zyxw zyxwvu zyxwvu
and from this, for u3 = 200 seconds and K z = 0.2 MNlm2 s ~ ( 2 0 0= ) 0.075%
This will in fact be constant for all values of u3 because the Maxwell Model cannot predict changes in strain if there is no stress. The overall variation in strain is shown in Fig. 2.46.
Example 2.15 In the previous Example, what would be the strain after 125 seconds if (a) the stress remained constant at 10 MN/m2 after 100 seconds and (b) the stress was reduced to zero after 100 seconds.
zy
Solution (a) If the stress was kept constant at 10 MN/m2 after 100 seconds as shown in Fig. 2.47 then the effective change in stress would be given by change in stress, a ( t ) =  K l ( t  T ) d 4 ) = K1 dt
so
E(U2)
K I U ~ TKIT
= +   
17 ~ ( 1 2 5 )= 0.125%
e
KlT2 217
zy zyxwvutsr Mechanical Behaviour of Plastics
102
0.1
zyxwvutsrqpo zyxwvutsrq 0.08
Sp
B 0.06
65
0.04
0.02
0
0
50
100
150
200
(SI
zy
Fig. 2.46 Variation of strain with time
Stress (MN/m*)
100
0

Time (s)
zyxwv
Fig. 2.47 Stress history: Example 2.15(a)
(b) If the stress was completely removed after 100 seconds as shown in Fig. 2.48 then the effective change in stress would be given by
change in stress,
a(t)=  K l ( t  T )  Au d a )  K1 dt
zyxwv zy zyxwvutsr
Mechanical Behaviour of Plastics Stress (MNlm2)
103
zy zyxwvuts 0
zyxwvutsrq zyxwvuts loo
*
Time (s)
up
Fig. 2.48 Stress history: Example 2.15(b)
so
/
u2
u2
E(U3)
=
rl +
11
E(U3)
rl

trl
Kldt+/ f2
+ 0  &2 (Kl)dt trl

zy AC7
E(U2 
T)
K,T~
=
211
~ ( 1 2 5 )= 0.05%
It is apparent therefore that the Superposition Principle is a convenient method of analysing complex stress systems. However, it should not be forgotten that the principle is based on the assumption of linear viscoelasticity which is quite inapplicable at the higher stress levels and the accuracy of the predictions will reflect the accuracy with which the equation for modulus (equation (2.33)) fits the experimental creep data for the material. In Examples (2.13) and (2.14) a simple equation for modulus was selected in order to illustrate the method of solution. More accurate predictions could have been made if the modulus equation for the combined MaxwellKelvin model or the Standard Linear Solid had been used.
2.12.2 Empirical Approach As mentioned earlier, it is not feasible to generate test data for all possible combinations of load variations. However, there have been a number of experimental investigations of the problem and these have resulted in some very
104
zyxwvut
z zy zyxwvuts zy Mechanical Behaviour of Plastics
useful design aids. From the experimental point of view the most straightforward situation to analyse and one that has considerable practical relevance is the loadnoload cycle. In this case a constant load is applied for a period and then completely removed for a period. The background to this approach is as follows. For a linear viscoelastic material in which the strain recovery may be regarded as the reversal of creep then the material behaviour may be represented by Fig. 2.49. Thus the timedependent residual strain, E,(?), may be expressed as (2.59) E,(?) = E,(?)  Ec(?  T )
zyxwvut
Fig. 2.49 wical creep and recovery behaviour of a plastic
where E, is the creep strain during the specified period denoted by (t) or (t  T). Since there can be an infinite number of combinations of creep and recovery periods it has been found convenient to express this behaviour in terms of two dimensionless variables. The first is called the Fractional Recovery, defined as Fractional recovery, F, =
Strain recovered  E,(T) E&) Max.creep strain &,(TI
(2.60)
where E,(T) is the creep strain at the end of creep period and E,(?) is the residual strain at any selected time during the recovery period. The second dimensionless variable is called the Reduced Time, t ~ , defined as Recovery time (2.61) Reduced time, t~ = Creep time Extensive tests have shown that if the final creep strain is not large then a graph of Fractional Recovery against Reduced Time is a master curve which
Mechanical Behaviour of Plastics
105
zy
zyxwv zyxwvu
zyxwv zyxwv zy zyx Reduced time, k
Fig. 2.50
meal recovery behaviour of a plastic
describes recovery behaviour with acceptable accuracy (see Fig. 2.50). The relationship between F, and f R may be derived in the following way. When creep curves are plotted on logarithmic strain and time scales they are approximately straight lines so that the creep strain, E,(?) may be expressed as E,(?)
= At"
(2.62)
and using this relationship in equation (2.59) E,(?)
= At"  A ( ?  T)"
and so the Fractional Recovery may be written as
F, =
AT"  [At"  A ( ?  T)"] AT"
= 1
(;)"+
(f  1)"
F, = 1 +?;  (?R + 1)"
(2.63)
In practice this relationship is only approximately correct because most plastics are not linearly viscoelastic, nor do they obey completely the power law expressed by equation (2.62). However this does not detract from the considerable value of this simple relationship in expressing the approximate solution to a complex problem. For the purposes of engineering design the expression provides results which are sufficiently accurate for most purposes. In addition,
106
zy zyx
Mechanical Behaviour of Plastics
zyxwvu zyxwvuts zyxw zyxw z
equation (2.63) permits the problem of intermittent loading to be analysed in a relatively straightforward manner thus avoiding uneconomical overdesign which would result if the recovery during the rest periods was ignored. From equation (2.63) and the definition of Fractional Recovery, F,, the residual strain is given by & r ( t ) = &c(T) Fr
*
&c(T)
If there have been N cycles of creep and recovery the accumulated residual strain would be x=N
&,(t)= EC(T)
x=l
[(F) (y 
?I
 1)
'1
where t p is the period of each cycle and thus the time for which the total accumulated strain is being calculated is t = t,N. Note also that the total accumulated strain after the load application for the (N 1)th time will be the creep strain for the loadon period ie cC(T)plus the residual strain s,(t).
+
ie
(&N+l)max
{ + [(F)"(y
= &c(T) 1
x=N x= I

 l)n]}
(2.65)
Tests have shown that when total strain is plotted against the logarithm of the total creep time (ie NT or total experimental time minus the recovery time) there is a linear relationship. This straight line includes the strain at the end of the first creep period and thus one calculation, for say the 10th cycle allows the line to be drawn. The total creep strain under intermittent loading can then be estimated for any combinations of loading/unloading times. In many design calculations it is necessary to have the creep modulus in order to estimate deflections etc from standard formulae. In the steady loading situation this is straightforward and the method is illustrated in the Examples (2.1)(2.5). For the intermittent loading case the modulus of the material is effectively increased due to the apparent stiffening of the material caused by the recovery during the rest periods. For example, if a constant stress of 17.5 MN/m2 was applied to acetal (see Fig. 2.51) for 9600 hours then the total creep strain after this time would be 2%. This would give a 2% secant modulus of 17.5/0.02 = 875 MN/m2. If, however, this stress was applied intermittently for 6 hours on and 18 hours off, then the total creep strain after 400 cycles (equivalent to a total time of 9600 hours) would only be 1.4%. This would be equivalent to a stress of 13 MN/m2 being applied continuously for 9600 hours and so the effective creep modulus would be 13/0.014 = 929 MN/m2.
zy
zyxw zy zyxwvut
Mechanical Behaviour of Plastics 2.4
2.2
107
2.0 1.8 1.6
.E 1.2
L
fj 1.0
0.8 0.6
0.4 0.2 n
yol
100
101
102
zyxwvutsr lo3
lo4
io5
Time (hours)
Fig. 2.51 Creep curves for acetal
zyx zyxwv zyxwvu
The effective increase in modulus due to intermittent loading is shown in Fig. 2.52. This illustrates that considerable material savings can be made if intermittent loading of the plastic can be ensured.
Example 2.16 Analysis of the creep curves given in Fig. 2.51 shows that they can be represented by an equation of the form E ( t ) = A m " where the constants n = 0.083 and A = 0.0486. A component made from this material is subjected to a loading pattern in which a stress of 10.5 MN/m2 is applied for 100 hours and then completely removed. Estimate (a) the residual strain in the material 100 hours after the stress has been removed, (b) the total creep strain after the 5th loading cycle in which the stress has been applied for 100 hours and removed for 100 hours in each cycle and (c) the residual strain after lo00 cycles of the type described in (b). Solution (a) The strain E , ( T )after 100 hours at 10.5 MN/m2 may be obtained from the creep curves in Fig. 2.23 or by calculation from the equation E,(T)= AatnAT".
so ~ ~ ( 1 0= 0 )0.0486(10.5)(100)0~083 = 0.51(100)0~083 = 0.747%
108
zyxwvuz Mechanical Behaviour of Plastics
zyxw
zy zyx zyx zyxwv Time (hours)
Fig. 2.52 Variation of modulus for continuous and intermittent loading
Now from equation (2.60)the Fractional Recovery is given by
Fr =
~c(l00) E r ( t ) =IE C ( W
Er ( t )
0.747 *
Also, the Reduced Time is given by tT tR=T
 200100 100
=1
Then from equation (2.63)
Fr = 1 + t i
E,(?)
 (tR+ 1)"
= 0.044%
Alternatively, since recovery may be regarded as the reverse of creep this part of the problem may be solved as follows. The projected creep strain after 200 hours at 10.5 MN/m2 is
~~(200) = 0.51(200)0.083= 0.792%
(see Fig. 2.51 to confirm this value of strain). However, since the stress was removed after 100 hours the recovered strain after a further 100 hours will be the same as E,(T), i.e. 0.747%. Thus the
zyxwv zyx zyxwvu zyxwvu zyxwvu zyxw
Mechanical Behaviour of Plastics
109
zyx
residual strain after the recovery period may be determined by superposition.
Er(t) = 0.792 0.747= 0.045%
This is simpler than the first solution but this approach is only convenient for the simple loading sequence of stress onstress off. If this sequence is repeated many times then this superposition approach becomes rather complex. In these cases the analytical solution shown below is recommended but it should be remembered that the equations used were derived on the basis of the superposition approach illustrated above. (b) If the stress is applied for 100 hours and removed for 100 hours then in equation (2.64),T = 100 hours and t , = 200 hours. Therefore after four cycles i.e. t = 800 hours. x=4
~ ~ ( 8 0=0~~(100) ) x=l
[(
y)fl 
x=4
x=l
+
= 0.747(0.059 0.0265
(7
I)']
+ 0.0174+ 0.0131)
= 0.0868%
Thus the total creep strain after the 5th load application for 100 hours would be 0.0868 0.747 = 0.834%. (c) The residual strain after the lOOOth cycle may be calculated as shown in (b) with the limits x = 1 to x = 1OOO. Clearly this repetitive calculation is particularly suitable for a computer and indeed there are many inexpensive desktop programmable calculators which could give the solution quickly and easily. Thus for a time, t , of lo00 x 200 hours.
+
= 0.342%.
However, in the absence of a programmable calculator or computer the problem may be solved as follows. If the residual strain is calculated for, say 10 cycles then the value obtained is
&(io3)= 0.121% The total creep strain after the stress of 10.5 MN/m2 has been applied for the 1lth time would be 0.121 0.747 = 0.868%. Now tests have shown that a plot of total creep strain plotted against the logarithm of the total creep time (i.e. ignoring the recovery times) is a straight line which includes the point E,(T).
+
zyx zyxw zyxw
110
Mechanical Behaviour of Plastics
Therefore after the 11th cycle the total creep time is 11 x 100 = 1.1 x io3 hours. If the total strain at this time is plotted on Fig. 2.51 then a straight line can be drawn through this point and the point E,(T), and this line may be extrapolated to any desired number of cycles. For the case in question the line must be extrapolated to (1001 x 100) hours at which point the total strain may be obtained as 1.09%. Thus the accumulated residual strain after lo00 cycles would be 1.09  0.747 = 0.343% as calculated on the computer. Of course it should always be remembered that the solutions obtained in this way are only approximate since the assumptions regarding linearity of relationships in the derivation of equation (2.64) are inapplicable as the stress levels increase. Also in most cases recovery occurs more quickly than is predicted by assuming it is a reversal of creep. Nevertheless this approach does give a useful approximation to the strains resulting from complex stress systems and as stated earlier the results are sufficiently accurate for most practical purposes.
zyxwvut
2.13 Dynamic Loading of Plastics
So far the deformation behaviour of plastics has been considered for situations where (i) the stress (or strain) is constant (ii) the stress (or strain) is changing relatively slowly or (iii) the stress (or strain) is changed intermittently but the frequency of the changes is small. In practice it is possible to have situations where the stress and strain are changing quite rapidly in a regular manner. This can lead to fatigue fracture which will be discussed in detail in later. However, it is also interesting to consider the stresdstrain relationships when polymers are subjected to dynamic loading. The simplest dynamic system to analyse is one in which the stress and strain are changing in a sinusoidal fashion. Fortunately this is probably the most common type of loading which occurs in practice and it is also the basic deformation mode used in dynamic mechanical testing of plastics. When a sinusoidally varying stress is applied to a material it can be represented by a rotating vector as shown in Fig. 2.53.Thus the stress at any moment in time is given by (T = 00 sinwt (2.66)
zyx zyx
where w is the angular velocity of the vector (= 2xf = 2x/T, where f is the cyclic frequency in hertz (H,) and T is the period of the sinusoidal oscillations). If the material being subjected to the sinusoidal stress is elastic then there will be a sinusoidal variation of strain which is in phase with the stress, i.e. E
= EO sinwt
However, for a viscoelastic material the strain will lag behind the stress. The strain is thus given by E = EO sin(wt  6) (2.67) where 6 is the phase lag.
Mechanical Behaviour of Plastics
z 111
I
z
zy
T zyxwvutsrqp zyxwvu
1
zyxwvutsrqp zyxwvut zyxwv 0
100
200
300
400
500
600
700
800
at
Fig. 2.53 Sinusoidal variation of stress and strain in viscoelastic material
zyxwvutsrqp
It is more usual to write these equations in a form which shows the stress leading the strain, i.e. E
(2.68)
= €0 sin wt
a = 00 sin(wt
+ 6)
(2.69)
The latter equation may be expanded to give o = 00
sin wt cos 6 + a0 coswt sin S
zyxwv
Thus the stress can be considered to have two components: (i) (ii)
(2.70)
00 cos S which is in phase with the strain and a0 sin6 which is 90" out of phase with the strain.
This leads to the definition of two dynamic moduli, El and E2: (i) E1 = (00 cos S ) / E O in phase with the strain (ii) E:! = (00 sin S ) / E O 90" out of phase with strain
We could thus represent these two moduli on a phasor diagram as shown in Fig. 2.54. E1 leads E2 by 90" (n/2 radians) and from this diagram it is possible to define a complex modulus, E* where
where i =
a.
112
zyxwvut zy Mechanical Behaviour of Plastics
zyxwv El
Fig. 2.54 Phasor diagram showing complex modulus (E*) relative to loss ( E 2 ) and storage ( E l ) moduli
zyxwvu zy zy zyxwv zyx
This presentation format leads to the terminology
E 1 = real modulus or storage modulus E2 = imaginary modulus or loss modulus.
Also, from Fig. 2.54 it is possible to relate El and E2 to the lag or phase angle, 6
E2 (2.72) tans= El In dynamic mechanical analysis of plastics, the material is subjected to a sinusoidal variation of stress and the strain is recorded so that E 1, E2 and 6 can be determined. The classical variation of these parameters is illustrated in Fig. 2.55. At very low frequencies the polymer is rubberlike and has a low modulus ( E l typically 0.1 MN/m2). At very high frequencies, the material behaves like a stiff, glassy solid with a high modulus (typically about lo3 MN/m2). It may be seen that this El plot is the inverse of that shown in Fig. 2.9 since o cx l/t. The loss modulus, E2, will be zero at low and high frequencies but will rise to a maximum close to the region where El is increasing most rapidly. The loss factor, tans(= E2/E1). will also have a maximum in the viscoelastic region but this will occur at a lower frequency than the peak in the E2 curve.
Example 2.17 Establish and plot the variation with frequency of the storage and loss moduli for materials which can have their viscoelastic behaviour described by the following models (i) A Maxwell model with i$ = 1 GN/m2 and Q = 0.1 GNs/m2. (ii) A Standard Linear Solid with ( 1 = 2 GN/m2, (2 = 0.1 GN/m2, r,~= 1 GNs/m2.
Mechanical Behaviour of Plastics
zyxwv 113
zyxwvuts zyxw zyxwvuts zyxwvut Log (4
zyxwv
Fig. 2.55 Typical variation of E l , E2 and loss tangent for a viscoelastic material
Solution As illustrated above, the stress and strain will be given by CT
= 00 sin(wr
E
= EO sin wt
+8)
However, in this type of question it is preferable to utilise complex numbers and so the transformations will be used so that CT
= ,oei(wr+6)
(2.73)
F
= EOe'af
(2.74)
(i) As shown earlier in this chapter, the governing equation for the Maxwell model is given by 1. 1
zyxwvut zyxwvuts &=U+CT
6 1 7
Then from equations (2.73) and (2.74) Eoiweiar
= looiWei(otC6)
4
iw iw=.
6
+ aOei(0t+6) 1
D
1
aoei(ot+a)
&Oeio'
+
;.
a,,ei(ot+a) &OeiWf
114
zyxwvuts zyxw zyxwv
zyxw zyxwvu Mechanical Behaviour of Plastics
where E* is the complex modulus. Rearranging gives
Using the fact that (a
E* =
+
iw6 E* = 6 oqi bi)(u  b i ) = u2 b2
+
iwqe
(6  wqi)  0 2 q 2 t+ or)t2i
(6 + wqi) (t wqi)
and since E* = El then storage modulus, El =
+
+ iE2
w2q2
+62
w2a25 ,2172
+62
and loss modulus,
zyxw
The variations of E l , E2 and tan8 with w are shown in Fig. 2.56. It may be seen that the variations of E1 and E2 are of the general shape that would be expected. The tan8 curve does not go through a maximum and so this is a further shortcoming of this simple model.
zyxwvu Fig. 2.56 Variation of E l , E2 and loss tangent for Maxwell model
(ii) For the Standard Linear Solid, the governing equation was derived earlier as vb + h a = r l 0 l + t 2 P + 4241s
zyxwvu zyxw zyxwvut zyx zyxw zyxw zyx zyxwv 115
Mechanical Behaviour of Plastics
substituting from equations (2.73) and (2.74) once again
3aoiweW+s) + tlaoeW+s) =~ Dividing across by
EOeiwrand
+ t 2 ) i w ~ o +e ~41t2&0eiwr ~~
letting E* = qei(wr+')/qgid
E* =
then,
( ( 1
v(t1 + t2)iw + t i t 2 t1 + tloi
Multiplying top and bottom by the conjugate of the denominator, we get
E* =
(532
+ 0 2 ( h + t2'2)w2)+ ( t 2 0 4 i 6:
and since E* = El
+ W2V2
+ iE2,
storage modulus,
E1 =
loss modulus,
E2 =
E2 tans = _ E1
t:w
,E%*
+ 3201 + h ) m 2
It may be seen in Fig. 2.57 that the variations of E 1, E2 and tan 6 follow the classicai pattern referrid to earlier in this section. 2.5
2
z g w
1.5 1
0.5
0
0.01
0.1
1
10
Log (4 Fig. 2.57 Variation of E , , Et and loss tangent for standard linear solid
100
116
zy zyx
Mechanical Behaviour of Plastics
2.14 TimeTemperature Superposition
It has been shown throughout this chapter that the properties of plastics are dependent on time. In Chapter 1 the dependence of properties on temperature was also highlighted. The latter is more important for plastics than it would be for metals because even modest temperature changes below 100°C can have a significant effect on properties. Clearly it is not reasonable to expect creep curves and other physical property data to be available at all temperatures. If information is available over an appropriate range of temperatures then it may be possible to attempt some type of interpolation. For example, if creep curves are available at 20°C and 60°C whereas the service temperature is 40°C then a linear interpolation would provide acceptable design data. If creep curves are available at only one temperature then the situation is a little more difficult. It is known that properties such as modulus will decrease with temperature, but by how much? Fortunately it is possible to use a timetemperature superposition approach as follows: It was shown earlier that the variation of creep or relaxation moduli with time are as illustrated in Fig. 2.9. If we now introduce temperature as a variable then a series of such curves will be obtained as shown in Fig. 2.58. In general the relaxed and unrelaxed modulus terms are independent of temperature. The remainder of the moduli curves are essentially parallel and so this led to the thought that a shift factor, UT, could be applied to move from one curve to another. Modulus
zyx
zyxwv zyxwvutsr
’ L
log (time)
Fig. 2.58 Modulustime curves for a range of temperatures
It may be seen from Fig. 2.59 that the two modulus curves for temperatures T I and T Z are separated by a uniform distance (1oguT). Thus, if the material behaviour is known at T I ,in order to get the modulus at time, f, and temperature
zy
Mechanical Behaviour of Plastics
117
Modulus
zy
[EITl
IE1T2
zyxw zyxwvu zyxwvutsr zyxwvuts zyxwvu t
VaT
log(time)
Fig. 2.59 Modulus curves at temperatures T I and T2
T2, it would be necessary to use a time @ / a T as ) shown in Fig. 2.59, in relation to the T1 data. This means that
(2.75)
where T2 > T I . Log ( U T ) is negative and so UT < 1. Williams, Landel and Feny developed an empirical relationship for this type of shift factor. This has the form
(2.76) where C1 and C2 are constants and Tref is a reference temperature. For many polymers it has been found that C1 and C2 are constants and T,j is taken as Tgrthe glass transition temperature for the polymer (values are given in Table 1.8). The WLF equation then takes the form logaT =
17.4(T  T g ) 51.6 (T  T g )
+
(2.77)
Thus all the different temperature related data in Fig. 2.58 could be shifted to a single master curve at the reference temperature (T,). Alternatively if the properties are known at T,f then it is possible to determine the property at any desired temperature. It is important to note that the shift factor cannot be applied to a single value of modulus. This is because the shift factor is on the horizontal timescale, not the vertical, modulus scale. If a single value of modulus ET^ is known as well as the shift factor UT it is not possible to
118
zyxwvuts zyxwvu zyx zy Mechanical Behaviour of Plastics
determine ET^ without knowing how the modulus varies with time. This is illustrated in Fig. 2.60 where it is readily seen that a knowledge of ET, and UT do not lead to a single value of ET* unless the E ( t ) relationship is known.
zyxwvu Fig. 2.60 Various modulustime curves
zyxwvu
Example 2.18 A particular grade of polypropylene can have its relaxation modulus described by the equation E ( t ) = 1.8tO”
where E ( t ) is in GN/m2 when ’t’ is in seconds. The temperature of the material is 20°C. Use the WLF equation to determine the 1 year modulus of the material at 60°C. The glass transition temperature for the polypropylene is 10°C.
Solution To use equation (2.76) it would be necessary to know the properties at  10°C. In this example, the properties are known at 20°C which becomes the reference temperature ( T I ) .The approach taken will be to get the shift factor at T2(= 60°C) and the shift factor at T I ( = 20°C) and then subtract these to get the shift factor from T1 to T2.
 17.4(20 + 10)  17.4(60 + 10) 51.6 + (20 + 10) = 3.62 UT
= 2.4 x 1 0  ~
51.6 + (60 + 10)
zyxwv zyxwvu zyxwv 119
Mechanical Behaviour of Plastics Therefore, using equation (2.75)
t
=
0.1
(2.4 x
[ E ( t ) l ~= * 0.78t'.' The modulus at T z ( = 60°C) can now be calculated at any desired time. For example, at 1 year (t = 3.15 x lo6 s)
[ E ( t ) ] m= 0.78(3.15 x lo6)'.' = 0.14 GN/m2
The two modulus curves at 20°C and 60°C are illustrated in Fig. 2.61 along with the shift factor.
zyxwvuts zyxwvuts zyxwvuts zyxwvutsrq zyxwvutsrqpo 1
0.9 0.8
0.7
N
E
f
f
0.6 0.5
1 0.4 5
0.3 0.2 0.1
0
1
Fig. 2.61 Variation of modulus with time and temperature for polypropylene
2.15 Fracture Behaviour of Unreinforced Plastics If a plastic moulding fails in the performance of its normal function it is usually caused by one of two factors  excessive deformation or fracture. In the previous sections it was pointed out that, for plastics, more often than not it will be excessive creep deformation which is the limiting factor. However, fracture,
120
zyxwvut
zyxw Mechanical Behaviour of Plastics
if it occurs, can have more catastrophic results. Therefore it is essential that designers recognise the factors which are likely to initiate fracture in plastics so that steps can be taken to avoid this. Fractures are usually classified as brittle or ductile. Although any type of fracture is serious, brittle fractures are potentially more dangerous because there is no observable deformation of the material prior to or during breakage. When a material fails in a ductile fashion, large nonrecoverable deformations are evident and these serve as a warning that all is not well. In polymeric materials, fracture may be ductile or brittle depending on such variables as the nature of the additives, the processing conditions, the strain rate, the temperature and the stress system. The principal external causes of fracture are the application of a stress in a very short period of time (impact), the prolonged action of a steady stress (creep rupture) or the continuous application of a cyclically varying stress (fatigue). In all cases the fracture processes will be accelerated if the plastic is in an aggressive environment. Basically there are two approaches to the fracture of a material. These are usually described as the microscopic and the continuum approaches. The former approach utilises the fact that the macroscopic fracture of the material must involve the rupture of atomic or molecular bonds. A study of the forces necessary to break these bonds should, therefore, lead to an estimate of the fracture strength of the material. In fact such an estimate is usually many times greater than the measured strength of the material. This is because any real solid contains multitudes of very small inherent flaws and microcracks which give rise to local stresses far in excess of the average stress on the material. Therefore although the stress calculated on the basis of the crosssectional area might appear quite modest, in fact the localised stress at particular defects in the material could quite possibly have reached the fracture stress level. When this occurs the failure process will be initiated and cracks will propagate through the material. As there is no way of knowing the value of the localised stress, the strength is quoted as the average stress on the section and this is often surprisingly small in comparison with the theoretical strength. The second approach to fracture is different in that it treats the material as a continuum rather than as an assembly of molecules. In this case it is recognised that failure initiates at microscopic defects and the strength predictions are then made on the basis of the stress system and the energy release processes around developing cracks. From the measured strength values it is possible to estimate the size of the inherent flaws which would have caused failure at this stress level. In some cases the flaw size prediction is unrealistically large but in many cases the predicted value agrees well with the size of the defects observed, or suspected to exist in the material. In this chapter the various approaches to the fracture of plastics are described and specific causes such as impact loading, creep and fatigue are described in detail.
zyxwv
zy zyxwvu
Mechanical Behaviour of Plastics
121
2.16 The Concept of Stress Concentration
Any material which contains a geometrical discontinuity will experience an increase in stress in the vicinity of the discontinuity. This stress concentration effect is caused by the redistribution of the lines of force transmission through the material when they encounter the discontinuity. Causes of stress concentration include holes, notches, keyways, comers, etc as illustrated in Fig. 2.62.
zyxwvu zyxw
Fig. 2.62 Stress concentration
zyx zyxw zyxw
The classical equation for calculating the magnitude of the stress concentration at a defect of the type shown in Fig. 2.62(b) is 0 ,
= a (1
+2 4 3 )
(2.79)
where a, is the local stress, a is the nominal stress on the material, 2a is the defect size and r is the radius of the defect at the area in question. The parameter (1 2 4 7 7 ) is commonly termed the stress concentration factor ( K , ) and for a hole where a = r then K, = 3, i.e. the stresses around the periphery of the hole are three times as great as the nominal stress in the material. It should be noted, however, that for a cracklike defect in which r + 0 then K, + 00. Obviously this does not occur in practice. It would mean that a material containing a crack could not withstand any stress applied to it. Therefore it is apparent that the stress concentration approach is not suitable for allowing for the effects of cracks. This has given rise to the use of Fracture Mechanics to deal with this type of situation.
+
2.17 Energy Approach to Fracture When a force is applied to a material there is work done in the sense that a force moves through a distance (the deformation of the material). This work is converted to elastic (recoverable) energy absorbed in the material and surface energy absorbed in the creation of new surfaces at cracks in the material. The original work on Fracture Mechanics was done by Griffith and he proposed that unstable crack growth (fracture) would occur if the incremental change in the net energy (work done  elastic energy) exceeded the energy which could be absorbed in the creation of the new surface. In mathematical terms this may
122
zyxwvuts zyxwvu zyxwvut zyxw zyxw Mechanical Behaviour of Plastics
be expressed as
(2.80)
where y is the surface energy per unit area. Note that for a situation where the applied force does no work (Le. there is no overall change in length of the material) then W = 0 and equation (2.80) becomes au aA (2.81) aa
'Yz
Now, for a through crack propagating in a sheet of material of thickness, B, we may write aA = 2Baa So equation (2.80) becomes
a
(W  U )> 2yB
aa
(2.83)
zy zy
In the context of fracture mechanics the term 2 y is replaced by the G, so that the condition for fracture is written as i a Baa
(W  U)> G,
(2.84)
G, is a material property which is referred to as the toughness, critical strain energy release rate or crack extension force. It is effectively the energy required to increase the crack length by unit length in a piece of material of unit width. It has units of J/m2. Equation (2.84) may be converted into a more practical form as follows. Consider a piece of material of thickness, B, subjected to a force, F, as shown in Fig. 2.63(a). The loaddeflection graph is shown as line (i) in Fig. 2.63(b). From this the elastic stored energy, U 1, may be expressed as
U1 = ZFS 1
(2.85)
If the crack extends by a small amount aa then the stiffness of the material changes and there will be a small change in both load, aF, and deflection, 86. This is shown as line (ii) in Fig. 2.63(b). The elastic stored energy would then be (2.86) U2 = aF)(6 36)
zyx i(F +
+
From equations (2.85) and (2.86) the change in stored energy as a result of the change in crack length 8~ would be given by
au = u2 u1= $(Fad + 6aF + aFas)
(2.87)
zyxwv zy zyxwvut
Mechanical Behaviour of Plastics F
123
t t t
1 7 Fo7
zyxw zyxwvu
Fig. 2.63 Force displacement behaviour of an elastic cracked plate
The work done, aW, as a result of the change in crack length &a is shown shaded in Fig. 2.63(b). This will be given by
aw = Fas + ;aFas
(2.88)
zyxwvu
Now using equations (2.87) and (2.88) in equation (2.84)
(2.89)
This equation may be simplified very conveniently if we consider the Compliance, C,of the material. This is the reciprocal of stiffness and is given by
c = sF
From this equation we may write
ad = FaC
+ CaF
and using this in equation (2.89) we get (2.91)
where F, is the applied force at fracture. This is a very important relationship in that it permits the fundamental material property G, to be calculated Erom the fracture force, F,, and the variation of compliance with crack length.
zyxwv zy zyxwv zyx zyxwvu zyxw Mechanical Behaviour of Plastics
124
Example 2.19 During tensile tests on 4 mm thick acrylic sheets of the type shown in Fig. 2.63(a), the forcedisplacement characteristics shown in Fig. 2.64(a) were recorded when the crack lengths were as indicated. If the sheet containing a 12 mm long crack fractured at a force of 330 N, determine the fracture toughness of the acrylic and calculate the applied force necessary to fracture the sheets containing the other crack sizes.
Solution The compliance ( S / F ) of each sheet may be determined from the slope of the graph in Fig. 2.64(a). A plot of compliance, C, against crack dimension, a, is shown in Fig. 2.64(b) and from this the parameter dC/da may be obtained. This is also shown plotted on Fig. 2.64(b). Using this, for NI. a = 6 mm, it may be seen that dC/da = 115 x Thus, from equation (2.91)
As this is a material constant, it may be used to calculate F, for the other N' so crack sizes. For example, for a = 2 mm, dC/da = 7 x
Fc = \/2(0.004)1.56 7 x 106x lo3 = 1.34 kN
Similarly for a = 3 , 4 , 5 and 5.5 mm the fracture loads would be 1.15 kN, 0.98 kN, 0.71 kN and 0.5 kN respectively. 1.6
1
1.4 1.2 A
B
1.0
8 o*8 0.6 0.4 0.2
0
10
20
30
40
50
60
Displacement (pm)
Fig. 2.64(a) Forcedisplacement characteristics for cracked plate
Mechanical Behaviour of Plastics
1
zyxwv zy 125
zyxwvut 2
3 4 a (mm)
5
6
zyxwv zyxw zyxw
Fig. 2.w) Compliance and rate. of change of compliance for various crack lengths
An alternative energy approach to the fracture of polymers has also been developed on the basis of nonlinear elasticity. This assumes that a material without any cracks will have a uniform strain energy density (strain energy per unit volume). Let this be UO.When there is a crack in the material this strain energy density will reduce to zero over an area as shown shaded in Fig. 2.65. This area will be given by &a2where k is a proportionality constant. Thus the loss of elastic energy due to the presence of the crack is given by
U = &a2BUo
and
(2.92) (2.93)
Comparing this with equation (2.84) and assuming that the external work is zero then it is apparent that G, = 2hU, (2.94) where U, is the value of strain energy density at which fracture occurs. Now, for the special case of a linear elastic material this is readily expressed in terms of the stress, a,,on the material and its modulus, E. (2.95)
126
zyxwvu zyxwv Mechanical Behaviour of Plastics
F
zyxw zyxwv zyxw zyxw zyxw zyxw
Fig. 2.65 Loading of cracked plate
So, combining equations (2.94) and (2.95)
and in practice it is found that k
2: R, so
nu;a G, = E
(2.96)
This is an alternative form of equation (2.91) and expresses the fundamental material parameter G, in terms the applied stress and crack size. From a knowledge of G, it is therefore possible to specify the maximum permissible applied stress for a given crack size, or vice versa. It should be noted that, strictly speaking, equation (2.96) only applies for the situation of plane stress. For plane strain it may be shown that material toughness is related to the stress system by the following equation.
nu:a GI,= (1 E
 v2 )
(2.97)
where v is the lateral contraction ratio (Poissons ratio). Note that the symbol GI,is used for the plane strain condition and since this represents the least value of toughness in the material, it is this value which is usually quoted. Table 2.2 gives values for GI,for a range of plastics.
z
zyxwv zyx zyxwv zyxwvuts 127
Mechanical Behaviour of Plastics
Table 2.2
spital fracture toughness parameters for a range of materials (at 20°C)
GI, (kJ/mz)
Material
ABS Acetal Acrylic
EPOXY
5 1.22 0.351.6 0.1 0.3 57 6.5 3.56.5 0.254 0.45
Glass reinforced polyester LDPE MDPEMDPE Nylon 66 Polycarbonate Polypropylene copolymer Polystyrene UPVC Glass Mild Steel
8 0.30.8 1.31.4 0.010.02
100
K I ~ (m/m3I2)
(5)
0.13 0.08 0.0140.023 0.0050.008 0.12 0.125 0.0250.25 0.06 0.020.5 0.150.2 0.02 0.030.13 0.01 0.5
24 4 0.91.6 0.30.5 57 1 0.55 3 12.6 34.5 0.71.1 14 0.75 140
2.18 Stress Intensity Factor Approach to Fracture
Ductility Factor (in mm) ($)'I2
17 6 0.20.5 0.020.06 14 16 5100 3.6 0.42.7 2240 0.4 1.118 0.1 250
zy
Although Griffith put forward the original concept of linear elastic fracture mechanics (LEFM), it was Irwin who developed the technique for engineering materials. He examined the equations that had been developed for the stresses in the vicinity of an elliptical crack in a large plate as illustrated in Fig. 2.66. The equations for the elastic stress distribution at the crack tip are as follows.
zyxw zyxwv zyxwvu
(f) { 1 sin (f) sin ( y ) } (4) { 1 + sin (:) sin ( ) } (2nr) sin (!) cos (i) cos (y ) (2nr) 12
cos  (2nr)l/2 K By = cos B
112
txy =
1
and for plane strain u 
 (2Irr)1/2
cos
(2) f H \
or for plane stress, a, = 0. Irwin observed that the stresses are proportional to (nu)'/2where 'u' is the half length of the crack. On this basis, a Stress Intensity Factor, K, was
128
z zyxwvut zyxwvu zyxw Mechanical Behaviour of Plastics
Normal
f
stnsro
t
t
hriation of uy along x axis (O=O)
zyxwvuts zyx zyxwv Fig. 2.66 Stress distribution in vicinity of a crack
defined as
K = o(Ru)'/~
The stress intensity factor is a means of charactensing the elastic stress distribution near the crack tip but in itself has no physical reality. It has units of MN m3/2 and should not be confused with the elastic stress concentration factor (K,)referred to earlier. In order to extend the applicability of LEFM beyond the case of a central crack in an infinite plate, K is usually expressed in the more general form K = Yo(Ru)'/~
(2.loo)
where Y is a geometry factor and 'u' is the half length of a central crack or the full length of an edge crack. Fig. 2.67 shows some crack configurations of practical interest and expressions for K are as follows. (a) Central crack of length 2u in a sheet of finite width (2.101)
(b) Edge cracks in a plate of finite width
(2.102)
Mechanical Behaviour of Plastics
la (a) Finite width plate
zyxw 129
zyx zyxwvu (b) Double edge crack
t" to
(c) Single edge crack
1. (d) Internal penny crack
Izyxwvu zyxwvu L zyxwvu zyx 02
0110
15
20
4
(1) Three point bending
(e) Ellipticalsurface crack
zyxwvu
Fa.2.67 Mal crack configurations
(c) Single edge cracks in a plate of finite width
{
K = ~ ( Z U ) ' ' ~ 1.12  0.23
+ 30.4 = (G)4} Note: in most cases
(5>+
10.6
(isi very ) s m d so Y =
(;)*
 21.7
(
;)3
(2.103) 1.12.
130
zyx zy Mechanical Behaviour of Plastics
zyxwvuts zyxwvu zyxw zyxwv zyxwv zyxw
(d) Penny shaped internal crack
(2.104)
assuming a
50). They can also be used to analyse laminates made up of materials other than unidirectional fibres, eg layers which are isotropic or made from woven fabrics can be analysed by inserting the relevant properties for the local 12 directions. Sandwich panels can also be analysed by using a thickness and appropriate properties for the core material. These types of situation are considered in the following Examples. Example 3.14 A blow moulded plastic bottle has its wall thickness made of three layers. The layers are:
Outside and inside skin  Material A thickness = 0.4 mm, El = E2 = 3 GN/m2, Gl2 = 1.1 GN/m2, u12 = 0.364 Core  Material B thickness = 0.4 mm, E1 = E2 = 0.8 GN/m2, Glz = 0.285 GN/m2, 1112 = 0.404.
zyxw zy zyxwvutsrq zyxwvuts zyxwv zyxwv zyxwvu zyxw
Mechanical Behaviour of Composites
219
If the diameter of the bottle is 160 mm, calculate the hoop and axial strains in the bottle wall when an internal pressure of 200 kN/m2 is applied. Calculate also the stresses in the individual layers.
Solution Although the composite wall is curved, the ( r / h ) value is large and so it can be analysed using the method illustrated for laminates. In this case, each ply is isotropic and so the properties do not vary with 6. It is thus necessary to get Q for each ply relative to the centre line of the wall thickness
h~ = 0.6,
h2 =O,
hl = 0.2,
h3 = 0 . 2 ,
h4
= 0.6
ie the wall section is treated as if it has four plies
[material A (0.4 mm)/material B (0.2 mm)],
Also
pr 0.2 x 80 = 13.33 MN/m2 hoop stress, cy=  = h 1.2 (or N , = c y h = 16 N/mm)
pr 0.2 x 80 axial stress, a, =  = = 6.67 MN/m2 2h 2 x 1.2 (or N R = a ~ = h 8 N/mm)

[ 3 , m O x io3 1.244 103 0 N/mm2, = 1.244 x io3 3.444 x io3 0 0 1.103 x lo3
Q2
956.5 376.7 = 376.7 956.5 0 0 285.8
[
;]
1
N/IM12
Also, and
zyx
Then the Extensional Stiffness Matrix is given by 4
ef(hf
A= f=1
u = A'
 hf,),
(since [BI = 0 ) .
The strains are related to the forces (or stresses) by
Nx
[;!yl
Therefore the axial and hoop strains are Ex
= 7.932
Ey
= 4.809
1 0  ~ ( ~ ,= , 01
220
zyxwvut zyxw zyxwv zyxwvu zy zyx Mechanical Behaviour of Composites
The effective elastic constants for the composite are: 1 1 1 E, =  E , = G ai1 h a22 * h ”  a66 h a12
a12
uxy = 
vyx = a22
all
so E, = 2.26 x lo3 MN/m2 E, = 2.26 x lo3 MN/m2 Gxy= 830.6 MN/m2 and vYx= 0.36
vXy = 0.36,
The stresses in the individual layers are obtained from TBxy
so, OA,
= 8.71 MN/m2
and
(TAX, = OB,
= 2.5 MN/m2 (TB,,
zy
[“]=a2.[;;,]
[::]=B.[;;,] TA*Y
CTA,
= 17.55 MN/m2
o MN/m2)
and
OB,
= 4.9 MN/m2
= 0 MN/m2)
The values of stress may be checked by simple equilibrium analysis. (i) Force equilibrium: N A
+ N B = N,
+
OA*AA O B ~ A= B Nx
(ii) Geometry of deformation:
zyxw zyx
0A.x = UBx
EA
EB
or ah =
(2) ((2)
(g)
OBx
+
UBAA OBAB= N,
OB,
=Nx/
ah =
AA + A B ) = 2.4 N/mm2
(A)
2.4 = 8.8 N / m 2
zyxwv zyx zyxwvutsrq zyxw [zyx I I] zyxw 1 zyxw 22 1
Mechanical Behaviour of Composites
To assist the reader the values of the terms in the matrices are [3.is; 103 1.16 x 103 A = 1.16 x IO3 3.158 x lo3 N/mm B= 0 996.7 0 3.670x 104 1.35 x 104 a = 1.35 x 104 3.67 x 104 0 0 1.003 x mdN
8]
[
This type of analysis could also be used for a sandwich structure with solid sluns and a foamed core. It is simply a matter of using the appropriate values of El, G12, E2, u12 for the skin and core material. This is illustrated in the following Example.
Example 3.15 A sandwich moulding is made up of solid skins with a foamed plastic core. The skins and core may be regarded as isotropic with the following the properties: Skin  Material A, El = E2 = 3.5 GN/m2,G12 = 1.25 GN/m2, u12 = 0.4. Foam Core  Material B, El = E2 = 0.06 GN/m2, Glz = 0.021 GN/m2, ~ 1= 2 0.43.
The skins are each 1 mm thick and the core is 20 mm thick. If moments of M , = 400 Nm/m and M y = 300 Nm/m are applied to the moulding, calculate the resulting curvatures and the stresses and strains in the crosssection.
Solution As the skins and core are isotropic, we only need to get the values for each:

[
e
Foamed Core
Skin
4 . 1 6 : ~lo3 1.667 x lo3
Ql = 1.667 x lo3 4.167 x lo3 0
Q2=
1.25 x io3I
 [
73.63 31.63 0 31.63 73.63 0 o 0 20.98
1
Assuming as before that there are four layers with the centre line at the midplane of the crosssection, then
zyxwvu
ho =  1 1 ,
hl = 10,
h2
= 0,
h3 =
10,
h4
= 1 1 mm
As these are only moments applied and the section is symmetric (B = 0) we only need the D and d matrices. These are given by .
4
222
[
zy zyxwv zyx x zy zyxwv zyxwv zyx Mechanical Behaviour of Composites
]
9.69; 1 6 3.89 x 1 6 D = 3.89 x 1 6 9.69 x I d Nmm, 0 2.89 x 105 i m 0 X 106 4.94 x 107 0 d = 4.94 x 1.23 x 3.45 xO 106 I 0 Then the curvatures, K, are given by
so, K,
= 3.44 x 1 0  ~mml,
K~
= 1.72 x 1 0  ~mm',
K , ~=
o
The strains will be directly proportional to the distance across the thickness, ie E=K*Z
At top surface, Z = 11 mm, so E~ = (3.44 x 104)(11) = 3.78 x stress, a, = EIE, = 3500(3.78 x
= 13.25 MN/m2
At interface (skin side), Z = 10 mm, so 3.44 x 103: stress, a, = E ~ E , = 3500(3.44 x
E,
= (3.44 x 104)(10) =
= 12.04 m / m 2
At interface (core side), E, = 3.44 x stress, a, = 60(3.44 x
= 0.21 MN/m2
Similarly in the ydirection, At top surface cy = 1.89 x
ay= 6.6 MN/m2
At interface (skin) = 1.72 x
ay= 6 MN/m2
At interface (core) = 1.72 x
ay= 0.1 m / m 2
In both cases the stresses and strains will be mirrored on the bottom section of the beam (ie positive instead of negative). These are illustrated in Fig. 3.26.
zy zyxwvutsr
Mechanical Behaviour of Composites X  strains 0.378%
223
X  stresses
0
0
0.378%
zyxwv 13.25
0


Y strains
Y stresses
Fig. 3.26 Stresses and strains, Example 3.15
zyxwv zyx zyxwv
3.13 Analysis of Nonsymmetric Laminates Example 3.16 A unidirectional carbon fibre/PEEK laminate has the stacking
sequence [0/352/352]~. If it has an inplane stress of a, = 100 MN/m2 applied, calculate the strains and curvatures in the global directions. The properties of the individual plies are El
= 145 GN/m2,
E2
= 15 GN/m2,
Each ply has a thickness of 0.1 mm.
G12 = 4
GN/m2,
u12
= 0.278
224
zyxwvuts zy zy zyxwvu zy Mechanical Behaviour of Composites
Solution This stacking sequence is similar to that in Example 3.1 1 except that in this case the laminate is not symmetrical. As shown in Fig. 3.27, the centre line of the laminate is in the middle of one of the plies and
IQ = 0.25,
hl = 0.15, h4 = 0.15,
h2 = 0.05, h5 = 0.25
h3
= 0.05,
zyxwv zyxw
Fig. 3.27 Nonsymmetric laminate
The approach is the same as before. must be determined for each layer as shown below and thus the values in the A, B and D matrices.

[
1.6; 16 4.20 x 1 6 Ql = 4.20 x lo3 1.51 x lo4 0 7.28 x 104 3.44 x 104 4.17 x lo4 3 . 4 4 ~104 2 . 8 0 ~104 1.98 x 104 4.17 x 104 1.98 x lo4 3.42 x 104 7.28 x 104 3.44 x lo4 4.17 x 104 3 . 4 4 ~104 2 . 8 0 ~104 1 . 9 8 ~104 4.17 x 104 1.98 x 104 3.42 x 104
[ Qs=[

Q4=

7.28 x 104 3.44 x 104 4.17 x 104 3.44 x 104 2.80 x 104 1.98 x 104 4.17 x 104 1.98 x lo4 3.42 x lo4
1 1
3.44 x 104 4.17 x 104 7.28 x 104 3.44 x 104 2.80 x 104 1.98 x lo4 4.17 x 104 1.98 x 104 3.42 x lo4
l 5 [(hf 3 f=1
D =
1
CDf
l3  WflP]
zyxwv zyxwvuts zyxwvuts zyxw zyx zyxwv
Mechanical Behaviour of Composites
225
In this case [B] # 0 and so [a]and [ d ] cannot be obtained by inverting the [A] and [D] matrices respectively. They must be obtained from
:] ;[
[;
=
;]l
The inplane strains and the moments and curvatures are all linked in this nonsymmetrical lamina and are obtained from
a61
a12 a22 a62
811
812
821 861
822 862
all
a21
where
bll
b12
b21
b61
b22 b62
dll
d12
a16 a26 a66 816
8 6
d21
866
d61
d22 d62
b16 b26
b66 d16
d26
d66
N = 0 . h(Nx = 50 N/mm)
which gives the strains and curvatures as ex = 3.326 x Kx
cy = 2.868 x
= 0.012 IlUl',
Ky
= 0.01 mm',
yxy= 3.405 x IOv5
K~~
= 0.019 mm'
The important point to note from this Example is that in a nonsymmetrical laminate the behaviour is very complex. It can be seen that the effect of a simple uniaxial stress, ax,is to produce strains and curvatures in all directions. This has relevance in a number of polymer processing situations because unbalanced cooling (for example) can result in layers which have different properties, across a moulding wall thickness. This is effectively a composite laminate structure which is likely to be nonsymmetrical and complex behaviour can be expected when loading is applied. The reader may wish to check the matrices in this Example:
zyxw
14.37: io4 1.41 io4 A = 1.41 x lo4 1.27 x 104 1.40 x 104 0 6.65 1 0  ~ 5.73 1 0  ~ 6.81
07
05]
B=
[
6.81 x 2.05 x 1.02 x 04 1.46 x io3 604.5 1.67 x io3 604.5 258.2 792 16.7 x lo3 792 604.4 2.30 1 0  ~ 2.09 10~ 3.77 1 0  ~ 2.24 x 1.49 x 5.34 x 9.55 1 0  ~ 2.01 1 0  ~ 2.03 x 1 0  ~
1
226
zyxw
zyxwvut zyxwv zy zyxwvu 1 Mechanical Behaviour of Composites
2.30 x 1 0  ~ 2.24 x 1 0  ~ 9.55 1 0  ~ 2.01 1 0  ~ x 10~ 1.49 x 1 0  ~ 3.77 x 104 5.34 x 105 2.03 x 104 1.05 x lo3 235.2 167.1 239.2 79.2 D= 235.2 167.1 79.2 233.0 2.15 x 103 1.60 103 1.64 103 1.601 x 6.65 x 4.04 x 1.64 x 1 0  ~ 4.04 x 1 0  ~ 8.74 1 0  ~
[ [
p = 2.09
1
3.14 Analysis of Short Fibre Composites
zyxwvz
In order to understand the effect of discontinuous fibres in a polymer matrix it is important to understand the reinforcing mechanism of fibres. Fibres exert their effect by restraining the deformation of the matrix as shown in Fig, 3.28. The external loading applied through the matrix is transferred to the fibres by shear at the fibdmatrix interface. The resultant stress distributions in the fibre and matrix are complex. In short fibres the tensile stress increases from zero at the ends to a value (af) which it would have if the fibre was continuous. This is shown in Fig. 3.29. From the previous section it may be seen that (of) may be determined from (3.42)
where a, is the stress applied to the composite and E1 may be determined from the rule of mixtures. Fibre
\
(a) Before force application
Matrix
t
+
(b) Force applied
t
+
Fig. 3.28 Effect of fibre on defonnation of matrix
zyxwv zy
Mechanical Behaviour of Composites
'7
227
zy
Stresses
1
+
34
zyxwvuts zyxwvuts
(a)
dia = d
1
4 It
+,It
34
T4
(c)
Fig. 3.29 Short Fibre Composites
zyx zyx
The stress distribution in short fibres is often simplified to the form shown in Fig. 3.29(c) It is evident from Fig. 3.29 that there is a minimum fibre length which will permit the fibre to achieve its full loadcarrying potential. The minimum fibR length in which the maximum fibre stress, (of), can be achieved is called the load transfer length, e,. The value of may be determined from a simple force balance force transmitted by shear at interface = ty(l/2)nd force exerted by fibre hence,
= 0f(nd2/4)
(3.43)
where, t,,is the shear strength of the fibrdmatrix interface. The maximum value of e, will occur when (of),, reaches the tensile strength of the fibre, ofu, and this is defined as the critical fibre length, e, (3.44)
228
zyxwvuts zyxwv Mechanical Behaviour of Composites
Example 3.17 Short carbon fibres with a diameter of 10 pm are to be used to reinforce nylon 66. If the design stress for the composite is 300 MN/m2 and the following data is available on the fibres and nylon, calculate the load transfer length for the fibres and also the critical fibre length. The volume fraction of the fibres is to be 0.3.
zy zyxwvuts Modulus (CN/m*)
Carbon fibres Nylon 66
230
2.8
Strength (GN/m2)
zy 2.9 
The interfacial shear strength for carbonhylon may be taken as 4 MN/m2
Solution
EI = EfVf
+ EmVm
zyxwv zyxw zyxw zyxw
El = 230(0.3) Using (3.42) = Ef
Using (3.43)
+ 2.8(0.7) = 71 GN/m2
(2) (11) = 230
300
972(10 x e, = (af),,,=d 2TY 2x4 Using (3.44)
ec  af,d   2900(10 x 2rY
2x4
= 972 MN/m2
= 1.2 mm
= 3.6
It may be seen from Fig. 3.29 that due to the ineffective end portions of short fibres, the average stress in the fibre will be less than in a continuous fibre. The exact value of the average stress will depend on the length of the fibres. Using the stress distributions shown in Fig. 3.29(b) the fibre stresses may be analysed as follows.
zyxwvut zyxwvu
Mechanical Behaviour of Composites
Now, for equilibrium of forces F1 = F2
229
+ F3
+
(rd2/4) (md)dx
( d / 4 ) d o f = r,dx
zy
Integrating this equation gives
of =
4ry (:t  x)
(3.45) d This is the general equation for the stress in the fibres but there are 3 cases to consider, as shown in Fig. 3.30
Stress
I
zyxwvutsr strest

Fig;. 3.30 Stress variations in short fibres
230
zyxwvut zyxwv zyxwvu zyxwv zy Mechanical Behaviour of Composites
(a) Fibre lengths less than Ct In this case the peak value of stress occurs at x = 0, so from equation (3.45) Of =
2Tyf
d
zyx
The average fibre stress, Ff,is obtained by dividing the area under the stresdfibre length graph by the fibre length.
zyx
zyxw ;e(?)

=
Uf
Now from (3.6) .
e
(2) +
I
Vf ak(1  Vf)
a, = (b) Fibre length equal to Ct
In this case the peak stress is equal to the maximum fibre stress. So at x = 0 2ryft Uf = (af ) = d
Average fibre stress = Ff =
So from (3.6) .~ a, =
(3.46)
(3.47)
4
(F)
Vf +ak(l Vf)
(c) Fibre length greater than Ct (i) For >x >  et)
CT~
= constant = (af),,,=
2ryet af = d
(3.48)
zyx zyxw zyxw zy zyxwv
Mechanical Behaviour of Composites
23 1
Also, as before, the average fibre stress may be obtained from f f f
[(af)max~(~ 
=
e,)
e
+ [ ( a f > m a x ~ + e , = [(af>max~(1

i)
So from (3.6)
(3.49) Note that in order to get the average fibre stress as close as possible to the maximum fibre stress, the fibres need to be considerably longer than the critical length. At the critical length the average fibre stress is only half of the value achieved in continuous fibres. Experiments show that equations such as (3.49) give satisfactory agreement with the measured values of strength and modulus for polyester sheets reinforced with chopped strands of glass fibre. Of course these strengths and modulus values are only about 2025% of those achieved with continuous fibre reinforcement. This is because with randomly oriented short fibres only a small percentage of the fibres are aligned along the line of action of the applied stress. Also the packing efficiency is low and the generally accepted maximum value for V f of about 0.4 is only half of that which can be achieved with continuous filaments. In order to get the best out of fibre reinforcement it is not uncommon to try to control within close limits the fibre content which will provide maximum stiffness for a fixed weight of matrix and fibres. In flexure it has been found that optimum stiffness is achieved when the volume fraction is 0.2 for chopped strand mat (CSM) and 0.37 for continuous fibre reinforcement.
zyxwvut
zy
Example 3.18 Calculate the maximum and average fibre stresses for glass fibres which have a diameter of 15 pm and a length of 2.5 mm. The interfacial shear strength is 4 MN/m2 and L , / L = 0.3. Solution Since L > L , then (gf)max
zy e,
A)= 2) y)
2tyC,  2tyL =d
2 x 4 x 2.5 x 15 x
(af),,, = 400 MN/m2
Also
f f f = (af)max (1 
5f= 340 MN/m2
= 400 (1 
x 0.3
In practice it should be remembered that short fibres are more likely to be randomly oriented rather than aligned as illustrated in Fig. 2.35. The problem of analysing and predicting the performance of randomly oriented short fibres
232
zyxwvuts zyxwv zy zy zyxw Mechanical Behaviour of Composites
is complex. However, the stiffness of such systems may be predicted quite accurately using the following simple empirical relationship.
Emdom = 3E1/8
+ 5E2/8
(3.50)
Hull also proposed that the shear modulus and Poisson’s Ratio for a random short fibre composite could be approximated by
Gmdm = gEi I 4 $E2
(3.51)
(3.52) =  1 2Gr El and E2 refer to the longitudinal and transverse moduli for aligned fibre composites of the type shown in (Fig. 3.29). These values can be determined experimentally or using specifically formulated empirical equations. However, if the fibres are relatively long then equation (3.5) and (3.13) may be used. These give results which are sufficiently accurate for most practical purposes. Vmdom
3.15 Creep Behaviour of Fibre Reinforced Plastics
The viscoelastic nature of the matrix in many fibre reinforced plastics causes their properties to be time and temperature dependent. Under a constant stress they exhibit creep which will be more pronounced as the temperature increases. However, since fibres exhibit negligible creep, the time dependence of the properties of fibre reinforced plastics is very much less than that for the unreinforced matrix. 3.16 Strength of Fibre Composites
Up to this stage we have considered the deformation behaviour of fibre composites. An equally important topic for the designer is avoidance of failure. If the definition of ‘failure’ is the attainment of a specified deformation then the earlier analysis may be used. However, if the Occurrence of yield or fracture is to be predicted as an extra safeguard then it is necessary to use another approach. In an isotropic material subjected to a uniaxial stress, failure of the latter type is straightforward to predict. The tensile strength of the material 6~will be known from materials data sheets and it is simply a question of ensuring that the applied uniaxial stress does not exceed this. If an isotropic material is subjected to multiaxial stresses then the situation is slightly more complex but there are well established procedures for predicting failure. If a, and ay are applied it is not simply a question of ensuring that . values of a, and ay below 3~ there can be neither of these exceed 8 ~At a plane within the material where the stress reaches 6~ and this will initiate failure.
zyxwv
zyxwvutsr zyx zyxwvutsr zyxwvu zy 233
Mechanical Behaviour of Composites
A variety of methods have been suggested to deal with the prediction of failure under multiaxial stresses and some of these have been applied to composites. The main methods are
(i) Maximum Stress Criterion: This criterion suggests that failure of the composite will occur if any one of five events happens oI2 CTT or
01
5 &c or
02
2
62T
or a2 5 & or
t12
2
312
That is, if the local tensile, compressive or shear stresses exceed the materials tensile, compressive or shear strength then failure will occur. Some typical values for the strengths of unidirectional composites are given in Table 3.5. Table 3.5
Typical strength properties of unidirectional fibre reinforced plastics
Material
GFRP (E glasdepoxy) GFRP (E glasdpolyester) KFRP (Kevlar 49/epoxy) CFRP (Carbodepoxy) CFRP (Carbon HWepoxy)
zyxwv zyxwv
Fibre volume fraction, Vf
(GN/m2)
32r (GN/m2)
(GN/m*)
(GN/m2)
32c (GN/m*)
0.6
1.4
0.05
0.04
0.22
0.1
0.42
0.52
0.034



0.6
1.5
0.027
0.047
0.24
0.09
0.6
1.8
0.08
0.1
1.57
0.17
0.62
1.24
0.02
0.04
0.29
0.03
3117
6 2
&IC
GFRP  Glass fibre reinforced plastic KFRP  Kevlar fibre reinforced plastic CRFP  Carbon fibre reinforced plastic
(ii) Maximum Strain Criterion: This criterion is similar to the above only it uses strain as the limiting condition rather than stress. Hence, failure is predicted to occur if (iii) TsaiHill Criterion: This empirical criterion defines failure as occur
The values in this equation are chosen so as to correspond with the nature of the loading. For example, if (TI is compressive, then 6 ~ is c used and so on.
234
Mechanical Behaviour of Composites
zy zyx zyxwvu zyx zy
In practice the second term in the above equation is found to be small relative to the others and so it is often ignored and the reduced form of the TsaiHill Criterion becomes (3.54)
3.16.1 Strength of Single Plies
These failure criteria can be applied to single ply composites as illustrated in the following Examples.
Example 3.19 A single ply Kevlar 49/epoxy composite has the following properties. E1
= 79 GN/m2, &IT
E2 = 4.1
GN/m2, G12 = 1.5 GN/m2,
= 1.5 GN/m2, 6 2 =~ 0.027 GN/m2, = 0.24 GN/m2,
?12
6 2= ~ 0.09
u12
= 0.43
= 0.047 GN/m2
GN/m2.
If the fibres are aligned at 15" to the xdirection, calculate what tensile value of a, will cause failure according to (i) the Maximum Stress Criterion (ii) the Maximum Strain Criterion and (iii) the TsaiHill Criterion. The thickness of the composite is 1 mm.
Solution (i) Maximum Stress Criterion Consider the situation where a, = 1 MN/m2. The stresses on the local (12) axes are given by
[:+.["] r12
Hence, 01 = 0.93 MN/m2,
02
tXY
= 0.067 MN/m2,
t12
= 0.25 MN/m2
so 31T
= 01
1608,
62T
 = 402, 02
$12 = 188 tl2
Hence, a stress of a, = 1608 MN/m2 would cause failure in the local 1direction. A stress of a, = 402 MN/m2 would cause failure in the local 2direction and a stress of a, = 188 MN/m2 would cause shear failure in the local 12 directions. Clearly the latter is the limiting condition since it will occur first.
zyxwvut
zyxwvu zyxwv zyxw zyxw zyx 235
Mechanical Behaviour of Composites
(ii) Maximum Strain Criterion Once again, let a, = 1 MN/m2. The limiting strains are given by &IC = 3.04 x
E1
212
i/12
0.031

G
10 3
zyxw I;:[zyxw zyxwvu
The strains in the local directions are obtained from
[ :;]
= s.
Y12 El
= 1.144
E2
;IT
=
TI2
= 1.128
1659,
i2T 
E2
El
io?
y12= 1.688 x 1 0  ~
~ 5 8 3 ,?I2  188 Y12
Thus once again, an applied stress of 188 MN/m2 would cause shear failure in the local 12 direction.
(iii) TsaiHill Criterion For an applied stress of 1 MN/m2 and letting X be the multiplier on this stress, we can determine the value of X to make the TsaiHill equation become equal to 1 .
x .a1
x2
'
ala2
x . a2
x . TI2
2
zyxwv
(TI2( ) + ( F ) 2 = *+ ( r ) Solving this gives X = 169. Hence a stress of a, = 169 MN/m2 would cause failure. It is more difficult with the TsaiHill criterion to identify the nature of the failure ie tensile, compression or shear. Also, it is generally found that for fibre angles in the regions 5"15" and 40"90",the TsaiHill criterion predictions are very close to the other predictions. For angles between 15" and 40" the TsaiHill tends to predict more conservative (lower) stresses to cause failure.
Example 3.20 The single ply in the previous Example is subjected to the stress system a, = 80 MN/m2,
ay = 40 MN/m2,
rxy= 20 MN/m2
Determine whether failure would be expected to occur according to (a) the Maximum Stress (b) the Maximum Strain and (c) the TsaiHill criteria.
zyxw
zyxwvuts [:]=.[:I zyxwvuts zyxwv zyxwvu
236
Mechanical Behaviour of Composites
Solution
(a) Maximum Stress Criterion The stresses in the 12 directions are
T12
a1 = 61.9 MN/m2,
02
TXY
= 21.9 MN/m2,
~ 1= 2 47.3
MN/m2
There are thus no problems in the tensile or compressive directions but the shear ratio has dropped below 1 and so failure is possible. (b) Maximum Strain Criterion The limiting strains are as calculated in the previous Example. The local strains are obtained from
[:I
=s.
Y12
~1
= 9.04 x
~2
[ :q r12
= 5.69 x
zyxwv yl2 = 0.032
Once again failure is just possible in the shear direction. (c) TsaiHill Criterion The TsaiHill equation gives (:)2 IT
(q2+ IT
( z02c )2+(E)2=1.08
As these terms equate to >1, failure is likely to occur.
3.16.2 Strength of Laminates When a composite is made up of many plies, it is unlikely that all plies will fail simultaneously. Therefore we should expect that failure will occur in one ply before it occurs in the others. To determine which ply will fail first it is simply a question of applying the above method to each ply in turn. Thus it is necessary to determine the stresses or strains in the local (1 2) directions for each ply and then check for the possibility of failure using any or all of the above criteria. This is illustrated in the following Example.
zy
Example 3.21 A carbonepoxy composite has the properties listed below. If the stacking sequence is [O/30/30], and stresses of ax= 400 MN/m2, ay =
zyxwvu zyxwv zyxwvutsr zyxwv zyx zyxw zyxw
Mechanical Behaviour of Composites
237
160 MN/m2 and txy= 100 MN/m2 are applied, determine whether or not failure would be expected to occur according to (a) the Maximum Stress (b) the Maximum Strain and (c) the TsaiHill criteria. The thickness of each ply is 0.2 mm. El = 125 GN/m2,
E2 = 9
GN/m2,
3 2 = ~ 0.08
61= ~ 1.8 GN/m2,
G12 = 4.4
GN/m2,
62~ = 0.17 GN/m2,
t12
GN/m2,
131= ~
u12
= 0.34
1.57 GN/m2
= 0.1 GN/m2
Solution It is necessary to work out the global strains for the laminate (these will be the same for each ply) and then get the local strains and stresses. Thus, for the 30" ply
Using ho = 0.6, hl = 0.4, h2 = 0.2, h3 = 0, h4 = 0.2, h5 = 0.4 and h6 = 0.6 (h = 1.2 mm) gives
[E;]
=
Yxy
[
2.94 7.51 5.46
10~
Thus
so
[
=
zyxw [z] MN/m2
If this is repeated for each ply, then the data in Fig. 3.31 is obtained. It may be seen that failure can be expected to occur in the +30" plies in the 2direction because the stress exceeds the boundary shown by the dotted line. The TsaiHill criteria gives the following values (i) 0" plies, (ii) 30 plies, (iii) 30 plies,
1.028 0.776 1.13
The failure in the 30" plies is thus confirmed. The TsaiHill criteria also predicts failure in the 0" plies and it may be seen in Fig. 3.31 that this is
z zyxwvuts zyxwvu zyxwvutsrqponml Mechanical Behaviour of Composites
238
Limit = 1800 I
Limit = 100
I
0
77
I
zyxwvut I
5
0 244
01
02
Limit = 0.09%
712
Limit = 2.3%
 ____
0 0.172%
I
0
0.07%!
0 0.12%
€2
Y12
Fig. 3.31 Stress and strain in the plies, Example 3.21
probably because the stress in the 2direction is getting very close to the limiting value.
3.17 Fatigue Behaviour of Reinforced Plastics In common with metals and unreinforced plastics there is considerable evidence to show that reinforced plastics are susceptible to fatigue. If the matrix is thermoplastic then there is a possibility of thermal softening failures at high stresses or high cyclic frequencies as described in Section 2.21.1. However, in general, the presence of fibres reduces the hysteritic heating effect and there is a reduced tendency towards thermal softening failures. When conditions are chosen to avoid thermal softening, the normal fatigue process takes place in the form of a progressive weakening of the material due to crack initiation and propagation. Plastics reinforced with carbon or boron are stiffer than glass reinforced plastics (grp)and they are found to be less vulnerable to fatigue. In shortfibre grp, cracks tend to develop relatively easily in the matrix and particularly at the interface close to the ends of the fibres. It is not uncommon for cracks to propagate through a thermosetting type matrix and destroy its integrity long before fracture of the moulded article occurs. With shortfibre composites it has been found that fatigue life is prolonged if the aspect ratio of the fibres is large. The general fatigue behaviour which is observed in glass fibre reinforced plastics is illustrated in Fig. 3.32. In most grp materials, debonding occurs
zyxw
zy zyxwvut
Mechanical Behaviour of Composites 120
20
0
239
zyxwvut zyxwvut zy zyxwv
10’
10’
103
104
105
106
107
Cycles to fracture
Fig. 3.32 1s.pical fatigue behaviour of glass reinforced polyester
after a small number of cycles, even at modest stress levels. If the material is translucent then the buildup of fatigue damage may be observed. The first signs are that the material becomes opaque each time the load is applied. Subsequently, the opacity becomes permanent and more pronounced. Eventually resin cracks become visible but the article is still capable of bearing the applied load until localised intense damage causes separation of the component. However, the appearance of the initial resin cracks may cause sufficient concern, for safety or aesthetic reasons, to limit the useful life of the component. Unlike most other materials, therefore, glass reinforced plastics give a visual warning of fatigue failure. Since grp does not exhibit a fatigue limit it is necessary to design for a specific endurance and factors of safety in the region of 34 are commonly employed. Most fatigue data is for tensile loading with zero mean stress and so to allow for other values of mean stress it has been found that the empirical relationship described in Section 2.21.4 can be used. In other modes of loading (e.g. flexural or torsion) the fatigue behaviour of grp is worse than in tension. This is generally thought to be caused by the setting up of shear stresses in sections of the matrix which are unprotected by properly aligned fibres. There is no general rule as to whether or not glass reinforcement enhances the fatigue behaviour of the base material. In some cases the matrix exhibits longer fatigue endurances than the reinforced material whereas in other cases the converse is true. In most cases the fatigue endurance of grp is reduced by the presence of moisture. Fracture mechanics techniques, of the type described in Section 2.21.6 have been used very successfully for fibre reinforced plastics. Qpical values of K
zyxwvu zyxw
240
zyxwvuts zyxw zyxw zyxw Mechanical Behaviour of Composites
for reinforced plastics are in the range 550 MN m3/2, with carbon fibre reinforcement producing the higher values.
3.18 Impact Behaviour of Reinforced Plastics
Reinforcing fibres are brittle and if they are used in conjunction with a brittle matrix (e.g. epoxy or polyester resins) then it might be expected that the composite would have a low fracture energy. In fact this is not the case and the impact strength of most glass reinforced plastics is many times greater than the impact strengths of the fibres or the matrix. A typical impact strength for polyester resin is 2 H/m2 whereas a CSWpolyester composite has impact strengths in the range 5080H/m2. Woven roving laminates have impact strengths in the range 100 150 kJ/m2. The much higher impact strengths of the composite in comparison to its component parts have been explained in terms of the energy required to cause debonding and work done against friction in pulling the fibres out of the matrix. Impact strengths are higher if the bond between the fibre and the matrix is relatively weak because if it is so strong that it cannot be broken, then cracks propagate across the matrix and fibres, with very little energy being absorbed. There is also evidence to suggest that in shortfibre reinforced plastics, maximum impact strength is achieved when the fibre length is at the critical value. There is a conflict therefore between the requirements for maximum tensile strength (long fibres and strong interfacial bond) and maximum impact strength. For this reason it is imperative that full details of the service conditions for a particular component are given in the specifications so that the sagacious designer can tailor the structure of the material accordingly.
zyxwvutsrq
Bibliography
Powell, P.C. Engineering with FibrePolymer Laminates, Chapman and Hall, London (1994). Daniel, LM. and Ishai, 0. Engineering Mechanics of Composite Materials, Oxford University Press (1994). Hancox, N.L. and Mayer, R.M. Design Data for Reinforced Plastics, Chapman and Hall, London (1993). Mayer, R.M. Design with Reinforced Plastics, HMSO,London (1993). Tsai, S.W. and Hahn, H.T. Introduction to Composite Materials, Technomic Westport, CT (1980). Folkes, M.J. Short Fibre Reinforced Thermoplastics, Research Studies Press, Somerset (1982). Mathews, F.L. and Rawlings, R.D. Composite Materials: Engineering and Science, Chapman and Hall, London (1993). Phillips, L.N.(ed.) Design with Advanced Composite Materials, Design Council, London (1989). Strong, B.A. High Performance Engineering Thermoplastic Composites, Technomic Lancaster, PA (1993). Ashbee, K. Fibre Reinforced Composites, Technomic Lancaster, PA (1993). Kelly, A (ed.) Concise Encyclopedia of Compiste Materials, Pergamon, Oxford (1994). Stellbrink, K.K.U. Micromechanics of Composites, Hanser, Munich (1996). Hull, D. An Intmducrion to Composite Materials, Cambridge University Press, (1981). Piggott, M.R. Load Bearing Fibre Composites, Pergamon, Oxford (1980). Richardson, M.O.W. Polymer Engineering Composites, Applied Science London (1977). Agarwal, B. and Broutman, L.J. Analysis and Performance of Fibre Composites, Wiley Interscience, New York (1980).
zyxwvut
zy zyxwvut 24 1
Mechanical Behaviour of Composites
zyxwvutsr zyxwvutsr
Questions
3.1 Compare the energy absorption capabilities of composites produced using carbon fibres, aramid fibres and glass fibres. Comment on the meaning of the answer, The data in Fig. 3.2 may be used. 3.2 A hybrid composite material is made up of 20% HS c d n fibres by weight and 30% Eglass fibres by weight in an epoxy matrix. If the density of the epoxy is 1300 kg/m3 and the data in Fig. 3.2 may be used for the fibres, calculate the density of the composite. 3.3 What weight of carbon fibres (density = 1800 kg/m3) must be added to 1 kg of epoxy (density = 1250 kg/m3) to produce a composite with a density of 1600 kg/m3. 3.4 A unidirectional glass fibre/epoxy composite has a fibre volume fraction of 60%. Given the data below, calculate the density, modulus and thermal conductivity of the composite in the fibre direction.
Epoxy
1250
6.1
0.25
Glass fibre
2540
80.0
1.05
3.5 In a unidirectional Kevlar/epoxy composite the modular ratio is 20 and the epoxy occupies 60% of the volume. Calculate the modulus of the composite and the stresses in the fibres and the matrix when a stress of 50 MN/m2 is applied to the composite. The modulus of the epoxy is 6 GN/m2. 3.6 In a unidirectional carbon fibdepoxy composite, the modular ratio is 40 and the fibres take up 50% of the crosssection. What percentage of the applied force is taken by the fibres? 3.7 A reinforced plastic sheet is to be made from a matrix with a tensile strength of 60 MN/m2 and continuous glass fibres with a modulus of 76 GN/m2. If the resin ratio by volume is 70% and the modular ratio of the composite is 25, estimate the tensile strength and modulus of the composite.
zyxwvutsr zyxwv zyxwvutsrq zyxwvutsrq
3.8 A single ply unidirectional carbon fibre reinforced PEEK material has a volume fraction of fibres of 0.58. Use the data given below to calculate the Poisson's Ratio for the composite in the fibre and transverse directions. Material
Modulus (GN/m2)
Poisson's Ratio
230 3.8
0.23 0.35
Carbon fibres (HS) PEEK
3.9 A single ply unidirectional glass fibre/epoxy composite has the fibres aligned at 40" to the global xdirection. If the ply is 1.5 mm thick and it is subjected to stresses of a, = 30 MN/m2 and uy = 15 MN/m2, calculate the effective moduli for the ply in the xy directions and the values of and E ~ The . properties of the ply in the fibre and transverse directions are El = 35 GN/m2,
E2
= 8 GN/m2,
Gl2
= 4 GN/m2 and
u12
= 0.26
3.10 A single ply unidirectional carbon fibre/epoxy composite has the fibres aligned at 30" to the xdirection. If the ply is 2 mm thick and it is subjected to a moment of M, = 180 Nm/m and to an axial stress of a, = 80 MN/m2, calculate the moduli, strains and curvatures in the xy directions. If an additional moment of M , = 250 Nm/m is added, calculate the new curvatures.
zy zyxwvuts Mechanical Behaviour of Composites
242
zyxwv zyx zyx zyx zyxw zyxw
3.11 State whether the following laminates are symmetric or nonsymmetric.
(i) [o/w/45/45/w/olT (ii) P/902/45/  45/45/902/01~ (iii) [0/90/45/  456/45/9o/o]T
3.12 A plastic composite is made up of three layers of isotropic materials as follows:
Skin layers: Core layer:
Material A, E = 3.5 GN/m2, G = 1.25 GN/m2, u = 0.4 Material B, E = 0.6 GN/m2, G = 0.222 GN/m2, u = 0.35.
The skins are each 0.5 mm thick and the core is 0.4 mm thick. If an axial stress of 20 MN/mz, a transverse stress of 30 MN/m2 and a shear stress of 15 MN/m2 are applied to the composite, calculate the axial and transverse stresses and strains in each layer. 3.13 A laminate is made up of plies having the following elastic constants El = 133 GN/m2, E2 = 9 GN/m2,
G12
= 5 GN/m2,
u12
= 0.31
If the laminate is based on (60, 30, 0, 30, 60, 90)s and the plies are each 0.2 mm thick, calculate E,, E,, Gxyand uxy. If a stress of 100 MN/m2 is applied in the x direction, what will be the axial and lateral strains in the laminate? 3.14 A unidirectional carbon fibrdepoxy composite has the following layup [40, 40,40, 401,
The laminate is 8 mm thick and is subjected to stresses of a, = 80 MN/mz and a, = 40 MN/m2, determine the strains in the x and y directions. The properties of a single ply are
E1 = 140 GN/m2,
E2
= 9 GN/m2,
Gl2
= 7 GN/m2
and
u12
= 0.3
3.15 A filament wound composite cylindrical pressure vessel has a diameter of 1200 m m and a wall thickness of 3 mm. It is made up of 10 plies of continuous glass fibres in a polyester resin. The arrangement of the plies is [03/60/ 601,. Calculate the axial and hoop strain in the cylinder when an internal pressure of 3 MN/m2 is applied. The properties of the individual plies are
E l = 32 GN/m2, E2 = 8 GN/mz, G12= 3 GN/mz,
u12
= 0.3
3.16 Compare the response of the following laminates to an axial force N, of 40 N/mm. The plies are each 0.1 mm thick. (a) [30/  301  30/30]T (b) [30/  30/30/  3 0 1 ~ The properties of the individual plies are El
= 145 GN/m2,
E2
= 15 GN/m2,
Gl2
= 4 GN/m2,
u12
= 0.278
3.17 A unidirectional carbon fibre/PEEK laminate has the stacking sequence [0/35/  3%. If the properties of the individual plies are E1 = 145 GN/m2, E2 = 15 GN/m2, G12 = 4 GN/m2,
u12
= 0.278
If the plies are each 0.1 mm thick, calculate the strains and curvatures if an inplane stress of 100 MN/m2 is applied. 3.18 A sinfle ply of carbodepoxy composite has the properties listed below and the fibres are aligned at 25 to the xdirection. If stresses of a, = 80 MN/m2, a, = 20 MN/m2 and
r,, = 10 MN/m2
L
zyxwvutsr zyxwvuts zyxwvuts C
n
K,(MN rn1I2)
CSM
3.3 x 1018
12.7
13.5
WR
2.7
6.4
26.5
1014
244
zyxwvuts zy zyxwvuts Mechanical Behaviour of Composites
zyxwvut
3.25 A sheet of chopped strand matreinforced polyester is 5 mm thick and 10 mm wide. If its modulus is 8 GN/mz calculate its flexural stiffness when subjected to a point load of 200 N midway along a simply supported span of 300 mm. Compare this with the stiffness of a composite beam made up of two 2.5 mm thick layers of this reinforced material separated by a 10 mm thick core of foamed plastic with a modulus of 40 m / m Z .
3.26 A composite of gfrp skin and foamed core is to have a fixed weight of 200 g/m. If its width is 15 mm investigate how the stiffness of the composite varies with skin thickness. The density of the skin material is 1450 kg/m3 and the density of the core material is 450 kg/m3. State the value of skin thickness which would be best and for this thickness calculate the ratio of the weight of the skin to the total composite weight.
3.27 In a short carbon fibre reinforced nylon moulding the volume fraction of the fibres is 0.2. Assuming the fibre length is much greater that the critical fibre length, calculate the modulus of the moulding. The modulus values for the fibres and nylon are 230 GN/m2 and 2.8 GN/m2 respectively.
zyxwvu zyxwvu
CHAPTER 4  Processing of Plastics
4.1 Introduction
zyxwvu
One of the most outstanding features of plastics is the ease with which they can be processed. In some cases semifinished articles such as sheets or rods are produced and subsequently fabricated into shape using conventional methods such as welding or machining. In the majority of cases, however, the finished article, which may be quite complex in shape, is produced in a single operation. The processing stages of heating, shaping and cooling may be continuous (eg production of pipe by extrusion) or a repeated cycle of events (eg production of a telephone housing by injection moulding) but in most cases the processes may be automated and so are particularly suitable for mass production. There is a wide range of processing methods which may be used for plastics. In most cases the choice of method is based on the shape of the component and whether it is thermoplastic or thermosetting. It is important therefore that throughout the design process, the designer must have a basic understanding of the range of processing methods for plastics since an illconceived shape or design detail may limit the choice of moulding methods. In this chapter each of the principal processing methods for plastics is described and where appropriate a Newtonian analysis of the process is developed. Although most polymer melt flows are in fact NonNewtonian, the simplified analysis is useful at this stage because it illustrates the approach to the problem without concealing it by mathematical complexity. In practice the simplified analysis may provide sufficient accuracy for the engineer to make initial design decisions and at least it provides a quantitative aspect which assists in the understanding of the process. For those requiring more accurate models of plastics moulding, these are developed in Chapter 5 where the NonNewtonian aspects of polymer melt flow are considered.
zyx 245
246
zyxwvuts zy zyxwv Processing of Plastics
4.2 Extrusion
4.2.1 General Features of Single Screw Extrusion One of the most common methods of processing plastics is Extrusion using a screw inside a barrel as illustrated in Fig. 4.1. The plastic, usually in the form of granules or powder, is fed from a hopper on to the screw. It is then conveyed along the barrel where it is heated by conduction from the barrel heaters and shear due to its movement along the screw flights. The depth of the screw channel is reduced along the length of the screw so as to compact the material. At the end of the extruder the melt passes through a die to produce an extrudate of the desired shape. As will be seen later, the use of different dies means that the extruder screwharrel can be used as the basic unit of several processing techniques. Powder or granules
Heoter bands
Die
zyxwvutsr zyxwvut I
Filter plate
.
__
.
Rototing screw 
_  .
Fig. 4.1 Schematic view of single screw extruder
Basically an extruder screw has three different zones. (a) Feed Zone The function of this zone is to preheat the plastic and convey it to the subsequent zones. The design of this section is important since the constant screw depth must supply sufficient material to the metering zone so as not to starve it, but on the other hand not supply so much material that the metering zone is overrun. The optimum design is related to the nature and shape of the feedstock, the geometry of the screw and the frictional properties of the screw and barrel in relation to the plastic. The frictional behaviour of the feedstock material has a considerable influence on the rate of melting which can be achieved. (b) Compression Zone In this zone the screw depth gradually decreases so as to compact the plastic. This compaction has the dual role of squeezing any
zyxw zyxwvutsrq
Processing of Plastics
247
trapped air pockets back into the feed zone and improving the heat transfer through the reduced thickness of material. (e) Metering Zone In this section the screw depth is again constant but much less than the feed zone. In the metering zone the melt is homogenised so as to supply at a constant rate, material of uniform temperature and pressure to the die. This zone is the most straightforward to analyse since it involves a viscous melt flowing along a uniform channel. The pressure buildup which occurs along a screw is illustrated in Fig. 4.2. The lengths of the zones on a particular screw depend on the material to be extruded. With nylon, for example, melting takes place quickly so that the compression of the melt can be performed in one pitch of the screw. PVC on the other hand is very heat sensitive and so a compression zone which covers the whole length of the screw is preferred. Pressure
Pressure Metering
1
Feed
Compression
..___
zyxwv
I
I
zyxwvut
0
Fig. 4.2 Typical zones on a extruder screw
zyxwvuts
As plastics can have quite different viscosities, they will tend to behave differently during extrusion. Fig. 4.3 shows some typical outputs possible with different plastics in extruders with a variety of barrel diameters. This diagram is to provide a general idea of the ranking of materials  actual outputs may vary f25% from those shown, depending on temperatures, screw speeds, etc.
248
zyxwvutsr zy Processing of Plastics
zyxw
Fig. 4.3 Typical extruder outputs for different plastics
In commercial extruders, additional zones may be included to improve the quality of the output. For example there may be a mixing zone consisting of screw flights of reduced or reversed pitch. The purpose of this zone is to ensure uniformity of the melt and it is sited in the metering section. Fig. 4.4 shows some designs of mixing sections in extruder screws.
pclra\Ie\ Interrupted mixing t W t s
Undercut spiral barriertype
Ringtype barrier mixer
Mixing pins
RAPRA cavity tmnsfer mixer
Fig. 4.4 'I)lpical designs of mixing zones
Processing of Plastics
zyxwv zyxwv 249
Some extruders also have a venting zone. This is principally because a number of plastics are hygroscopic  they absorb moisture from the atmosphere. If these materials are extruded wet in conventional equipment the quality of the output is not good due to trapped water vapour in the melt. One possibility is to predry the feedstock to the extruder but this is expensive and can lead to contamination. Vented barrels were developed to overcome these problems. As shown in Fig. 4.5, in the first part of the screw the granules are taken in and melted, compressed and homogenised in the usual way. The melt pressure is then reduced to atmospheric pressure in the decompression zone. This allows the volatiles to escape from the melt through a special port in the barrel. The melt is then conveyed along the barrel to a second compression zone which prevents air pockets from being trapped. Pressure
Pressure Decompression zone
Volatiles
Feed
/
zyxwvut zyxwvu
Zones on a vented extruder
Fig. 4.5 Zones on a vented extruder
zyx
The venting works because at a typical extrusion temperature of 250°C the water in the plastic exists as a vapour at a pressure of about 4 MN/m2. At this pressure it will easily pass out of the melt and through the exit orifice. Note that since atmospheric pressure is about 0.1 MN/m2 the application of a vacuum to the exit orifice will have little effect on the removal of volatiles.
250
zyxwvuts zyx Processing of Plastics
Another feature of an extruder is the presence of a gauze filter after the screw and before the die. This effectively filters out any inhomogeneous material which might otherwise clog the die. These screen packs as they are called, will normally filter the melt to 120150 pm. However, there is conclusive evidence to show that even smaller particles than this can initiate cracks in plastics extrudates e.g. polyethylene pressure pipes. In such cases it has been found that fine melt filtration (245 pm) can significantly improve the performance of the extrudate. Since the filters by their nature tend to be flimsy they are usually supported by a breaker plate. As shown in Fig. 4.6 this consists of a large number of countersunk holes to allow passage of the melt whilst preventing dead spots where particles of melt could gather. The breaker plate also conveniently straightens out the spiralling melt flow which emerges from the screw. Since the fine mesh on the filter will gradually become blocked it is periodically removed and replaced. In many modem extruders, and particularly with the fine filter systems referred to above, the filter is changed automatically so as not to interrupt continuous extrusion.
zyxwvuts *l
Filter pack
Section A A A
zyxwvu
Fig. 4.6 Breaker plate with filter pack
It should also be noted that although it is not their primary function, the breaker plate and filter also assist the buildup of back pressure which improves
zy zyxwvutsr
Processing of Plastics
25 1
mixing along the screw. Since the pressure at the die is important, extruders also have a valve after the breaker plate to provide the necessary control. 4.2.2 Mechanism of Flow As the plastic moves along the screw, it melts by the following mechanism. Initially a thin film of molten material is formed at the barrel wall. As the screw rotates, it scrapes this film off and the molten plastic moves down the front face of the screw flight. When it reaches the core of the screw it sweeps up again, setting up a rotary movement in front of the leading edge of the screw flight. Initially the screw flight contains solid granules but these tend to be swept into the molten pool by the rotary movement. As the screw rotates, the material passes further along the barrel and more and more solid material is swept into the molten pool until eventually only melted material exists between the screw flights. As the screw rotates inside the barrel, the movement of the plastic along the screw is dependent on whether or not it adheres to the screw and barrel. In theory there are two extremes. In one case the material sticks to the screw only and therefore the screw and material rotate as a solid cylinder inside the barrel. This would result in zero output and is clearly undesirable. In the second case the material slips on the screw and has a high resistance to rotation inside the barrel. This results in a purely axial movement of the melt and is the ideal situation. In practice the behaviour is somewhere between these limits as the material adheres to both the screw and the barrel. The useful output from the extruder is the result of a drag flow due to the interaction of the rotating screw and stationary barrel. This is equivalent to the flow of a viscous liquid between two parallel plates when one plate is stationary and the other is moving. Superimposed on this is a flow due to the pressure gradient which is built up along the screw. Since the high pressure is at the end of the extruder the pressure flow will reduce the output. In addition, the clearance between the screw flights and the barrel allows material to leak back along the screw and effectively reduces the output. This leakage will be worse when the screw becomes worn. The external heating and cooling on the extruder also plays an important part in the melting process. In high output extruders the material passes along the barrel so quickly that sufficient heat for melting is generated by the shearing action and the barrel heaters are not required. In these circumstances it is the barrel cooling which is critical if excess heat is generated in the melt. In some cases the screw may also be cooled. This is not intended to influence the melt temperature but rather to reduce the frictional effect between the plastic and the screw. In all extruders, barrel cooling is essential at the feed pocket to ensure an unrestricted supply of feedstock. The thermal state of the melt in the extruder is frequently compared with two ideal thermodynamic states. One is where the process may be regarded as
zyxwvu
252
zyxwvutsr zyxwvu zyxwvut Processing of Plastics
adiabatic. This means that the system is fully insulated to prevent heat gain or loss from or to the surroundings. If this ideal state was to be reached in the extruder it would be necessary for the work done on the melt to produce just the right amount of heat without the need for heating or cooling. The second ideal case is referred to as isothermal. In the extruder this would mean that the temperature at all points is the same and would require immediate heating or cooling from the barrel to compensate for any loss or gain of heat in the melt. In practice the thermal processes in the extruder fall somewhere between these ideals. Extruders may be run without external heating or cooling but they are not truly adiabatic since heat losses will occur. Isothermal operation along the whole length of the extruder cannot be envisaged if it is to be supplied with relatively cold granules. However, particular sections may be near isothermal and the metering zone is often considered as such for analysis.
zyxw zyx zyx
4.2.3 Analysis of Flow in Extruder As discussed in the previous section, it is convenient to consider the output from the extruder as consisting of three components  drag flow, pressure flow and leakage. The derivation of the equation for output assumes that in the metering zone the melt has a constant viscosity and its flow is isothermal in a wide shallow channel. These conditions are most likely to be approached in the metering zone. (a) Drag Flow Consider the flow of the melt between parallel plates as shown in Fig. 4.7(a). For the small element of fluid ABCD the volume flow rate d Q is given by dQ= V*dy*dx Assuming the velocity gradient is linear, then
(4.1)
Substituting in (4.1)and integrating over the channel depth, H,then the total drag flow, Qd, is given by
This may be compared to the situation in the extruder where the fluid is being dragged along by the relative movement of the screw and barrel. Fig. 4.8 shows the position of the element of fluid and (4.2) may be modified to include terms relevant to the extruder dimensions. For example
vd
= RDN cos $

Processing of Plastics
vd
z 253
Moving plate
zy
Y
Stationary plate (a) Drag Flow
High Pressure
Low Pressure
F3
zyxwvut zyxwv zyxwvuts (b) Pressure Flow
zyxwv
In both cases, AB = dz, element width = dx and channel width = T
Fig. 4.7 Melt Flow between parallel plates
zyxw
where N is the screw speed (in revolutions per unit time). T = (IrDtan4  e)cos4
so
Qd
4
= (XDtan 4  e)(XDN cos2 4 ) H
In most cases the term, e, is small in comparison with (nDtan4) so this expression is reduced to Qd
=~
I ~ ~ D Zsin N H4 cos 4
Note that the shear rate in the metering zone will be given by V d / H .
(4.3)
254
zyxwvuts zy zyxwvuts Processing of Plastics
Pitch =KO ton @
Axial velocity, VO
!el
qXN
zyxwvuts
zyxwvu zyx zy zyxw Element ot fluid
Fig. 4.8 Details of extruder screw
(b) Pressure flow: Consider the element of fluid shown in Fig. 4.7(b). The forces are
F2 = P  d y d X F3 = tyd z d x
where P is pressure and d t is the shear stress acting on the element. For steady flow these forces are in equilibrium so they may be equated as follows:
F1 = F2
which reduces to
+ 2F3
dP Y z =tY
(4.4)
Now for a Newtonian fluid, the shear stress, ty,is related to the viscosity, r,~, and the shear rate, 9, by the equation
.
ty = v y
dV = r)dY
Using this in equation (4.4)
dP dV Yx = tlby
Integrating V
255
Processing of Plastics
so
zyxwv zyxwv zyxwvutsrq
Also, for the element of fluid of depth, d y , at distance, y , from the centre line (and whose velocity is V) the elemental flow rate, d e , is given by dQ = V T d y
This may be integrated to give the pressure flow, Q p
zyxwvuts
HI2
eP=2J1  dP .~(;$)dy 0 Q
77 dz
    . 1T HdP  1277 dz
Referring to the element of fluid between the screw flights as shown in Fig. 4.8, this equation may be rearranged using the following substitutions. Assuming e is small, T = nDtan$. cos4 Also,
zyxwv
dL dP dP sin$ =  so  = sin$ dz dL dz
Thus the expression for Q p becomes
QP
nDH3sin2@. d P 12rl

dL
(4.7)
(c) Leakage The leakage flow may be considered as flow through a wide slit which has a depth, 6, a length (ecos4) and a width of (nDlcos4). Since this is a pressure flow, the derivation is similar to that described in (b). For convenience therefore the following substitutions may be made in (4.6). h=S
zyxwvu
T = nD/
COS
AP Pressure gradient = (see Fig. 4.9) e cos 4 So the leakage flow, QL, is given by QL
=
n2D2d3 dP tan 4dL 1277e
~
(4.8)
A factor is often required in this equation to allow for eccentricity of the screw in the barrel. Typically this increases the leakage flow by about 20%.
256
zyxwvuts zyxwvut zyxwvutsr zyxwvu zyxwvu , Processing of Plastics
Pitch
= nD tan 0
e
~
r
KD
\ \ 'WA\\ AIPI
zyxw zyxw zyxw
Fig. 4.9 Development of screw
The total output is the combination of drag flow, back pressure flow and leakage. So from (4.3), (4.7) and (4.8)
Q=$T~D NH~ sin4cos4 
nDH3sin2I$ dP
n2D2J3
1 2 ~ dL
12~e
dP dL
tan+
(4.9)
For many practical purposes sufficient accuracy is obtained by neglecting the leakage flow term. In addition the pressure gradient is often considered as linear so dP  P _ dL L where 'L' is the length of the extruder. In practice the length of an extruder screw can vary between 17 and 30 times the diameter of the barrel. The shorter the screw the cooler the melt and the faster the moulding cycle. In the above analysis, it is the melt flow which is being considered and so the relevant pressure gradient will be that in the metering zone. However, as shown in Fig. 4.2 this is often approximated by P / L . If all other physical dimensions and conditions are constant then the variation of output with screw flight angle, 4, can be studied. As shown in Fig. 4.10 the maximum output would be obtained if the screw flight angle was about 35°C. In practice a screw flight angle of 17.7" is frequently used because
257
Processing of Plastics
zy
2.5E005 2E005
1 E405
0
zyxwvuts zyxwvuts zyxwv 0
10
20
30
40
50
60
70
80
90
Screw flight angle
Fig. 4.10 Variation of drag flow and pressure flow
zyxwvu zyxw
(i) this is the angle which occurs if the pitch of the screw is equal to the diameter and so it is convenient to manufacture, (ii) for a considerable portion of the extruder length, the screw is acting as a solids conveying device and it is known that the optimum angle in such cases is 17" to 20".
It should also be noted that in some cases correction factors, F d , and Fp are applied to the drag and pressure flow terms. They are to allow for edge effects and are solely dependent on the channel width, T, and channel depth, h, in the metering zone. Qpical values are illustrated in Fig. 4.11. 4.2.4 Extruderme Characteristics From equation (4.9) it may be seen that there are two interesting situations to consider. One is the case of free discharge where there is no pressure build up at the end of the extruder so Q=
emax = ; X ~ D * N Hsin4cos4
(4.10)
The other case is where the pressure at the end of the extruder is large enough to stop the output. From (4.9) with Q = 0 and ignoring the leakage flow P=P,,=
6rDLNq H2tan4
(4.11)
In Fig. 4.12 these points are shown as the limits of the screw characteristic. It is interesting to note that when a die is coupled to the extruder their requirements
258
z
z zyxwvu Processing of Plastics
0.96 0.94
0.82 0.8
zyxwvutsr Es zyxw zyxwvu LdLL
0
0.05
0.1
0.2
0.15
0.25
0.3
zy zyxw
Ratio (hiT)
Fig. 4.11 Flow correction factors as a function of screw geometry
are conflicting. The extruder has a high output if the pressure at its outlet is low. However, the outlet from the extruder is the inlet to the die and the output of the latter increases with inlet pressure. As will be seen later the output, Q , of a Newtonian fluid from a die is given by a relation of the form Q=KP
nP
(4.12)
where K = for a capillary die of radius R and length Ld. 87& Equation (4.12) enables the die characteristics to be plotted on Fig. 4.12 and the intersection of the two characteristics is the operating point of the extruder. This plot is useful in that it shows the effect which changes in various parameters will have on output. For example, increasing screw speed, N , will move the extruder characteristic upward. Similarly an increase in the die radius, R, would increase the slope of the die characteristic and in both cases the extruder output would increase. The operating point for an extrudeddie combination may also be determined from equations (4.9) and (4.12)  ignoring leakage flow
So for a capillary die, the pressure at the operating point is given by POP =
2nqD2NH sin 4 cos 4 (R4/2Ld) (OH3 sin24 ) / 3 ~
+
(4.13)
Processing of Plastics
zyxwv z 259
output,
Q"
P,
0
Pressure, P
zy
zy zyxw
Fig. 4.12 Extruder and die characteristics
4.2.5 Other Die Geometries For other die geometries it is necessary to use the appropriate form of equation (4.12).The equations for a capillary and a slit die are derived in Chapter 5. For other geometries it is possible to use the empirical equation which was developed by Boussinesq. This has the form Fbd3 12qLdeP
Q=
(4.14)
zyx
where b is the greatest dimension of the crosssection d is the least dimension of the crosssection F is a nondimensional factor as given in Fig. 4.13.
Using equation (4.14)it is possible to modify the expression for the operating pressure to the more general form 2 1 r q p N H sin 4 cos 4
+ (OH3sin24/3L)
(4.15)
260
zy zyxwvuts Processing of Plastics
1
0.9
zyxwvu zyxwvuts zyxwvutsrq 0.8
U
c 0.7 Q)
I
0
zy
E 0.6
8g 0.5
E 0.4
0.3 0.2
0 Fig. 4.13
0.4 0.6 Aspect ratio (db)
0.2
zyxw 0.8
Flow coefficient as a function of channel geometry
For a capillary die, one may obtain a value of F from Fig. 4.13 as 0.295 and substituting b = d = 2R, this equation reduces to the same form as equation (4.13).
Example 4.1 A single screw extruder is to be designed with the following characteristics. L/D ratio = 24, screw flight angle = 17.7" Max. screw speed = 100 rev/min, screw diameter = 40 mm flight depth (metering zone) = 3 mm. If the extruder is to be used to process polymer melts with a maximum melt viscosity of 500 Ns/m2, calculate a suitable wall thickness for the extruder barrel based on the von Mises yield criterion. The tensile yield stress for the barrel metal is 925 MN/m2 and a factor of safety of 2.5 should be used.
Solution The maximum pressure which occurs in the extruder barrel is when there is no output. Therefore the design needs to consider this worst case blockage situation. As given by equation (4.1 1) P,,

6nDLr) =H 2 tan #J
6~ x 40 x (24 x 10) x (100/60) x 500 = 210 m / m 2 (3)2tan 17.7O
The von Mises criterion relates the tensile yield stress of a material to a state of multiaxial stress in a component made from the material. In a cylinder (the
zy zyxwvut zyxwv zyxwvut zyxw 26 1
Processing of Plastics
barrel of the extruder in this case), the principal stresses which exist as a result of an internal pressure are
PmmD 2h PmaxD =4h
hoop stress, 01 = axial stress, a 2
~
where h = wall thickness of the barrel. The von Mises criterion simply states that yielding (failure) will occur if
where
ay = tensile yield stress of material
FS = factor of safety.
In this case, therefore
8h2
h = 9.8 mm
Hence a barrel wall thickness of 10 mm would be appropriate.
Example 4.2 A single screw extruder is to be used to manufacture a nylon rod 5 mm in diameter at a production rate of 1.5 ndmin. Using the following information, calculate the required screw speed. Nylon Extruder Die = 4 mm Length Viscosity = 42.0 Ns/m2 Diameter = 30 mm Diameter = 5 mm Density (solid) = 1140 kg/m3 Length = 750 mm Density (melt) = 790 kg/m3 Screw flight angle = 17.7" Metering channel depth = 2.5 mm Die swelling effects may be ignored and the melt viscosity can be assumed to be constant.
zyxw
Solution The output rate of solid rod = speed x crosssectional area = 1.5 x ~ ( 2 . 5x 1OW3)*/60 = 49.1 x m3/s
zyxw
As the solid material is more dense than the melt, the melt flow rate must be greater in the ratio of the solid/melt densities. Therefore Melt flow rate through die = 49.1 x lop6
(g)
= 70.8 x
m3/s
262
zy zyxw zyxwvu zyxwv zyxw zyxw Processing of Plastics
The pressure necessary to achieve this flow rate through the die is obtained from XPP
Q=8qLd
P=
8 x 420 x 4 x n(2.5
x 70.8 x
= 7.8 MNIm’
103)4
At the operating point, the die output and the extruder output will be the same. Hence Q = 70.8 x
= in2(30x 103)2N(2.5 x
 n(30 x
sin 17.7 cos 17.7
(
)
1OP3)(2.6x 103)3 sin 17 7.8 x lo6 12 x 420 0.75 N = 22 revlmin
4.2.6 General Features of Twin Screw Extruders In recent years there has been a steady increase in the use of extruders which have two screws rotating in a heated barrel. These machines permit a wider range of possibilities in terms of output rates, mixing efficiency, heat generation, etc compared with a single screw extruder. The output of a twin screw extruder can be typically three times that of a single screw extruder of the same diameter and speed. Although the term ‘twinscrew’ is used almost universally for extruders having two screws, the screws need not be identical. There are in fact a large variety of machine types. Fig. 4.14 illustrates some of the possibilities with counterrotating and corotating screws. In addition the screws may be conjugated or nonconjugated. A nonconjugated screw configuration is one in which the screw flights are a loose fit into one another so that there is ample space for material between the screw flights (see Fig. 4.15).
(a) Counter rotating (intermeshing)
(b) Corotating
(intermeshing)
(c) Counterrotating (d) Corotating (nonintemshlng) (nonintemhing)
Fig. 4.14 Different types of twin screw extruder
263
Processing of Plastics
zyxwvutsrqp
lo) Nonconjugated screws showing some
I bl
passages around each screw
Fig. 4.15
Conjugoted screws showing closed passages around each screw
Two types of twin screw extruder
In a counterrotating twin screw extruder the material is sheared and pressurised in a mechanism similar to calendering (see Section 4.5), i.e. the material is effectively squeezed between counterrotating rolls. In a corotating system the material is transferred from one screw to the other in a figureofeight pattern as shown in Fig. 4.16. This type of arrangement is particularly suitable for heat sensitive materials because the material is conveyed through the extruder quickly with little possibility of entrapment. The movement around the screws is slower if the screws are conjugated but the propulsive action is greater. Table 4.1
zy zyxwvut
Comparison of singlescrew, corotating and counterrotating twinscrew extruders Corotating screw Single screw
Principle
Conveying efficiency Mixing efficiency Shearing action Selfcleaning effect Energy efficiency Heat generation Temp distribution Max. revolving
speed (rpm) Max. effective length of screw L/D
Friction between cylinder and materials and the same between material and screw LOW Low High Slight LOW High Wide
Low speed type
I
High speed type
Mainly depend on the frictional action as in the case of single screw extruder
Medium Mediudigh Medium High Medium/High High Medium/High Medium High Medium Narrow
100300
25  35
250300
3032
7 18
3040
Counterrotating twin screw
Forced mechanical conveyance based on gear pump principle
High High Low Low High LOW Narrow
zyxwv 3545
1021
264
zyxwvuts zyxwvu zyxw Processing of Plastics
Fig. 4.16 Material flow path with corotating scres
The following table compares the single screw extruder with the main types of twin screw extruders.
4.2.7 Processing Methods Based on the Extruder Extrusion is an extremely versatile process in that it can be adapted, by the use of appropriate dies, to produce a wide range of products. Some of the more common of these production techniques will now be described.
(a) Granule ProductiodCompounding In the simplest case an extruder may be used to convert polymer formulations and additives into a form (usually granules) which is more convenient for use in other processing methods, such as injection moulding. In the extruder the feedstock is melted, homogenised and forced through a capillary shaped die. It emerges as a continuous lace which is cooled in a long water bath so that it may be chopped into short granules and packed into sacks. The hauloff apparatus shown in Fig. 4.17 is used to draw down the extrudate to the required dimensions. The granules are typically 3 mm diameter and about 4 mm long. In most cases a multihole die is used to increase the production rate.
(b) Profile Production Extrusion, by its nature, is ideally suited to the production of continuous lengths of plastic mouldings with a uniform crosssection. Therefore as well as producing the laces as described in the previous section, the simple operation of a die change can provide a wide range of profiled shapes such as pipes, sheets, rods, curtain track, edging stsips, window frames, etc (see Fig. 4.18). The successful manufacture of profiled sections depends to a very large extent on good die design. Generally this is not straightforward, even for a simple crosssection such as a square, due to the interacting effects of postextrusion swelling and the flow characteristics of complex viscoelastic fluids. Most dies are designed from experience to give approximately the correct shape and then sizing units are used to control precisely the desired shape. The extrudate is then cooled as quickly as possible. This is usually done in a water bath the length of which depends on the section and the material being cooled. For example,
Processing of Plastics
zyxwvu zyx 265
zyxwvutsrq Feedstock
Cutter
haul
,Laces,
Water bath
Fig. 4.17 Use of extruder to produce granules
Fig. 4.18 (a) Extruded panel sections (b) Extruded window profile
longer baths are needed for crystalline plastics since the recrystallisation is exothermic. The storage facilities at the end of the profile production line depend on the type of product (see Fig. 4.19). If it is rigid then the cooled extrudate may be cut to size on a guillotine for stacking. If the extrudate is flexible then it can be stored on drums. (c) Film Blowing
Although plastic sheet and film may be produced using a slit die, by far the most common method nowadays is the film blowing process illustrated in Fig. 4.20. The molten plastic from the extruder passes through an annular die and emerges as a thin tube. A supply of air to the inside of the tube prevents it from collapsing and indeed may be used to inflate it to a larger diameter.
266
zyxwvut zy zy Processing of Plastics
Controlled temperature
zyxwv
(1)
Fig. 4.19(a) Sheet extrusion (1) thick sheet (2) thin sheet
Fig. 4.19(b) Pipe extrusion ( 1 ) rigid pipe (2) flexible pipe Bubble
Ian
Fig. 4.20 Film blowing process
267
Processing of Plastics
Initially the bubble consists of molten plastic but a jet of air around the outside of the tube promotes cooling and at a certain distance from the die exit, a freeze line can be identified. Eventually the cooled film passes through collapsing guides and nip rolls before being taken off to storage drums or, for example, gussetted and cut to length for plastic bags. Most commercial systems are provided with twin storage facilities so that a full drum may be removed without stopping the process. The major advantage of film blowing is the ease with which biaxial orientation can be introduced into the film. The pressure of the air in the bubble determines the blowup and this controls the circumferential orientation. In addition, axial orientation may be introduced by increasing the nip roll speed relative to the linear velocity of the bubble. This is referred to as drawdown. It is possible to make a simple estimate of the orientation in blown film by considering only the effects due to the inflation of the bubble. Since the volume flow rate is the same for the plastic in the die and in the bubble, then for unit time
zyxw
TtDdhdLd
zyxwvut = TtDbhbLb
where D, h and L refer to diameter, thickness and length respectively and the subscript ‘d’ is for the die and ‘b’ is for the bubble. So the orientation in the machine direction, OMD,is given by b Ddhd hd OMD = L=  Ld
hbDb
hbBR
where BR = blowup ratio ( D b / D d ) Also the orientation in the transverse direction, OTD,is given by
zyxwvu
Therefore the ratio of the orientations may be expressed as
(4.16)
Example 4.3 A plastic shrink wrapping with a thickness of 0.05 mm is to be produced using an annular die with a die gap of 0.8 mm. Assuming that the inflation of the bubble dominates the orientation in the film, determine the blowup ratio required to give uniform biaxial orientation. Solution Since OMD = OTD then the blowup ratio,
BR =

/%hb
Common blowup ratios are in the range 1.5 to 4.5.
268
zyxwvu zyxwv zyxwvu zyxwv zyxw Processing of Plastics
This example illustrates the simplified approach to film blowing. Unfortunately in practice the situation is more complex in that the film thickness is influenced by drawdown, relaxation of induced stresses/strains and melt flow phenomena such as die swell. In fact the situation is similar to that described for blow moulding (see below) and the type of analysis outlined in that section could be used to allow for the effects of die swell. However, since the most practical problems in film blowing require iterative type solutions involving melt flow characteristics, volume flow rates, swell ratios, etc the study of these is delayed until Chapter 5 where a more rigorous approach to polymer flow has been adopted.
(d) Blow Moulding This process evolved originally from glass blowing technology. It was devel
oped as a method for producing hollow plastic articles (such as bottles and barrels) and although this is still the largest application area for the process, nowadays a wide range of technical mouldings can also be made by this method e.g. rear spoilers on cars and videotape cassettes. There is also a number of variations on the original process but we will start by considering the conventional extrusion blow moulding process.
Extrusion Blow Moulding Initially a molten tube of plastic called the Parison is extruded through an annular die. A mould then closes round the parison and a jet of gas inflates it to take up the shape of the mould. This is illustrated in Fig. 4.21(a). Although this process is principally used for the production of bottles (for washingup liquid, disinfectant, soft drinks, etc.) it is not restricted to small hollow articles. Domestic cold water storage tanks, large storage drums and 200
Extruder
(i) Parison descends
(ii) Inflating
(iii) Cooling
Fig. 4.21 Stages in blow moulding
(iv) Ejecting
Processing of Plastics
269
gallon containers have been blowmoulded. The main materials used are PVC, polyethylene, polypropylene and PET. The conventional extrusion blow moulding process may be continuous or intermittent. In the former method the extruder continuously supplies molten polymer through the annular die. In most cases the mould assembly moves relative to the die. When the mould has closed around the parison, a hot knife separates the latter from the extruder and the mould moves away for inflation, cooling and ejection of the moulding. Meanwhile the next parison will have been produced and this mould may move back to collect it or, in multimould systems, this would have been picked up by another mould. Alternatively in some machines the mould assembly is fixed and the required length of parison is cut off and transported to the mould by a robot arm. In the intermittent processes, single or multiple parisons are extruded using a reciprocating screw or ram accumulator. In the former system the screw moves forward to extrude the parisons and then screws back to prepare the charge of molten plastic for the next shot. In the other system the screw extruder supplies a constant output to an accumulator. A ram then pushes melt from the accumulator to produce a parison as required. Although it may appear straightforward, in fact the geometry of the parison is complex. In the first place its dimensions will be greater than those of the die due to the phenomenon of post extrusion swelling (see Chapter 5). Secondly there may be deformities ( e g curtaining) due to flow defects. Thirdly, since most machines extrude the parison vertically downwards, during the delay between extrusion and inflation, the weight of the parison causes sagging or drawdown. This sagging limits the length of articles which can be produced from a free hanging parison. The complex combination of swelling and thinning makes it difficult to produce articles with a uniform wall thickness. This is particularly true when the cylindrical parison is inflated into an irregularly shaped mould because the uneven drawing causes additional thinning. In most cases therefore to blow mould successfully it is necessary to program the output rate or die gap to produce a controlled nonuniform distribution of thickness in the parison which will give a uniform thickness in the inflated article. During moulding, the inflation rate and pressure must be carefully selected so that the parison does not burst. Inflation of the parison is generally fast but the overall cycle time is dictated by the cooling of the melt when it touches the mould. Various methods have been tried in order to improve the cooling rate e.g. injection of liquid carbon dioxide, cold air or high pressure moist air. These usually provide a significant reduction in cycle times but since the cooling rate affects the mechanical properties and dimensional stability of the moulding it is necessary to try to optimise the cooling in terms of production rate and quality. Extrusion blow moulding is continually developing to be capable of producing even more complex shapes. These include unsymmetrical geometries and double wall mouldings. In recent years there have also been considerable
zyxw zyxwv
270
zyxwvutsr zyx Processing of Plastics
developments in the use of inthemould transfers. This technology enables lables to be attached to bottles and containers as they are being moulded. Fig. 4.22 illustrates three stages in the blow moulding of a complex container.
zyxw zyxwvutsr zyxwvutsrq d zyx
Parlscn pinched as it emerges from die and then stretched between two halves d open mwid
Mould closes to deform patison into shape
side cores rotate inwards to complete fming
zyxw zyxwvu Fig. 4.22 Stages in blow moulding of complex hollow container
Analysis of Blow Moulding As mentioned previously, when the molten plastic emerges from the die it swells due to the recovery of elastic deformations in the melt. It will be shown later that the following relationship applies: BSH = B& (from Chapter 5 )
where
BSH = swelling of the thickness (= hl/hd)
BST = swelling of the diameter (= D l / D d ) 2
therefore hl = hd (BST )2
(4.17)
Now consider the situation where the parison is inflated to fill a cylindrical die of diameter, Om.Assuming constancy of volume and neglecting drawdown effects, then from Fig. 4.23 7tDlhl = ZDmh
Processing of Plastics
zyxw zyxwvu 27 1
Mould
Fig. 4.23 Analysis of blow moulding
zy zyxwvu (4.18)
This expression therefore enables the thickness of the moulded article to be calculated from a knowledge of the die dimensions, the swelling ratio and the mould diameter. The following example illustrates the use of this analysis. A further example on blow moulding may be found towards the end of Chapter 5 where there is also an example to illustrate how the amount of sagging of the parison may be estimated.
Example 4.4 A blow moulding die has an outside diameter of 30 mm and an inside diameter of 27 mm. The parison is inflated with a pressure of 0.4 MN/m2 to produce a plastic bottle of diameter 50 mm. If the extrusion rate used causes a thickness swelling ratio of 2, estimate the wall thickness of the bottle. Comment on the suitability of the production conditions if melt fracture occurs at a stress of 6 MN/m2. Solution From equation (4.18)
Now
so
(2)
zyxwvuts wall thickness, h = B&hd
hd = :(30  27) = 1.5 mm
h = (1.414)3(1.5)  = 2.42 mm
(2:>
272
zy zyxwvut zyxw zyxwv Processing of Plastics
The maximum stress in the inflated parison will be the hoop stress, 0 0 , which is given by
PO, 2h
oo=
. 4 50 ~ 2 x 2.42
0
= 4.13 MN/m2
Since this is less than the melt fracture stress (6 MN/m2) these production conditions would be suitable. These are more worked examples on extrusion blow moulding towards the end of Chapter 5. Extrusion Stretch Blow Moulding Molecular orientation has a very large effect on the properties of a moulded article. During conventional blow moulding the inflation of the parison causes molecular orientation in the hoop direction. However, biaxial stretching of the plastic before it starts to cool in the mould has been found to provide even more significant improvements in the quality of blowmoulded bottles. Advantages claimed include improved mechanical properties, greater clarity and superior permeation characteristics. Cost savings can also be achieved through the use of lower material grades or thinner wall sections. Biaxial orientation may be achieved in blow moulding by
zyxw
(a) stretching the extruded parison longitudinally before it is clamped by the mould and inflated. This is based on the Neck Ring process developed as early as the 1950s. In this case, molten plastic is extruded into a ring mould which forms the neck of the bottle and the parison is then stretched. After the mould closes around the parison, inflation of the bottle occurs in the normal way. The principle is illustrated in Fig. 4.24.
U
Extrusion / Injection of plastic into pull rod
Stretching of parison
Fig. 4.24 Neck ring stretch blow moulding
zyx
Inflation and ejection
zyxwvu 273
Processing of Plastics
(b) producing a preform ‘bottle’ in one mould and then stretching this longitudinally prior to inflation in the full size bottle mould. This is illustrated in Fig. 4.25.
(11 Extruscon
zyxwvutsrq zyxwvuts (111
Inflation of preform
l a ) Manufacture of prefwm
(I )
(ii) Inflation
Stretching
Ib) Manufacture of bottle
Fig. 4.25
zyxwvu
(iiil Ejection
Extrusion stretch blow moulding
Injection Stretch Blow Moulding This is another method which is used to produce biaxially oriented blow moulded containers. However, as it involves injection moulding, the description of this process will be considered in more detail later (Section 4.3.9).
zyxw
(e) Extrusion Coating Processes There are many applications in which it is necessary to put a plastic coating on to paper or metal sheets and the extruder provides an ideal way of doing this. Normally a thin film of plastic is extruded from a slit die and is immediately brought into contact with the medium to be coated. The composite is then passed between rollers to ensure proper adhesion at the interface and to control the thickness of the coating (see Fig. 4.26). Another major type of coating process is wire covering. The tremendous demand for insulated cables in the electrical industry means that large tonnages of plastic are used in this application. Basically a bare wire, which may be heated or have its surface primed, is drawn through a special die attached
274
zyxwvuts zy Processing of Plastics
(driven)
Coated fabric
Fig. 4.26 Extrusion coating process
be coated
Fig. 4.27
Wire
Covering Die
to an extruder (see Fig. 4.27). The drawing speed may be anywhere between 1 d m i n and lo00 d m i n depending on the diameter of the wire. When the wire emerges from the die it has a coating of plastic, the thickness of which depends on the speed of the wire and the extrusion conditions. It then passes into a cooling trough which may extend for a linear distance of several hundred metres. The coated wire is then wound on to storage drums. Wire covering can be analysed in a very similar manner to that described for extrusion. The coating on the wire arises from two effects:
zyxw zyxwvuts zyxwvuts
(a) Drug Flow due to the movement of the wire (b) Pressure Flow due to the pressure difference between the extruder exit and the die exit.
Processing of Plastics
zyxwvut zyxwvu zyxwv 275
From (4.2) the drag flow, Qd, is given by
From (4.6) the pressure flow, Q p , is given by 1 dP Q TH  124 d z
So combining these two equations, the total output, Q, is given by (4.19) This must be equal to the volume of coating on the wire so
+ Q = nVdh(2R + h )
Q = nVd((R h)*  R 2 )
(4.20)
Combining equations (4.19) and (4.20) nVdh(2R
TH3 P + h ) = iTHVd + .12q L
zyx zyxwvu
from which
p =  6qLvd (2H  H ) H3
(4.21)
This is an expression for the pressure necessary at the extruder exit and therefore enables the appropriate extrusion conditions to be set.
(f) Recent Developments in Extrusion Technology (i) CoExtrusion As a result of the wide range of requirements which occur in practice it is not surprising that in many cases there is no individual plastic which has the correct combination of properties to satisfy a particular need. Therefore it is becoming very common in the manufacture of articles such as packaging film, yoghurt containers, refrigerator liners, gaskets and window frames that a multilayer plastic composite will be used. This is particularly true for extruded film and thermoforming sheets (see Section 4.4). In coextrusion two or more polymers are combined in a single process to produce a multilayer film. These coextruded films can either be produced by a blown film or a cast film process as illustrated in Figs 4.28(a) and (b). The cast process using a slot die and chill roll to cool the film, produces a film with good clarity and high gloss. The film blowing process, however, produces a stronger film due to the transverse orientation which can be introduced and this process offers more flexibility in terms of film thickness.
276
Processing of Plastics
zy
Extruder die
I b ) Cast film process
zyxw zy zyxwv
Fig. 4.28 Coextrusion of plastic film
In most cases there is insufficient adhesion between the basic polymers and so it is necessary to have an adhesive film between each of the layers. Recent investigations of coextrusion have been centred on methods of avoiding the need for the adhesive layer. The most successful seems to be the development
Processing of Plastics
zyxwvut zyxwv zyxwv zyxw 277
of reactive bonding processes in which the coextruded layers are chemically crosslinked together. The main reason for producing multilayer coextruded films is to get materials with better barrier properties  particularly in regard to gas permeation. The following Table shows the effects which can be achieved. Data on permeability of plastics are also given in Figs 1.13 and 1.14. Table 4.2
Transmission rates for a range of plastics
zyxw zyxw zyxwvut zyxw Transmission rates
Polymer ABS UPVC Polypropylene PET LDPE HDPE PSEVOH*IPE PSIPVdCIPE PPEVO WPP
Oxygen (cm3/m2 24 hr atm)
Layer distribution (Pm) lo00 lo00 loo0 loo0 lo00
loo0 825/25/150 8251501125 3001401660
1050 1390 910 1360 920 960 1050 1070 930
30 5 60 1 140
60 5t 1 It
Water vapour (glrn’ 24 hr) 2 0.75 0.25 2 0.5 0.3 1.6 0.4 0.25
‘EVOH ethyl vinyl alcohol. tDepends on humidity.
(ii) Highly Oriented Grids: Netlike polymer grids have become an extremely important development  particularly to civil engineers. The attraction in civil engineering applications is that the open grid structure permits soil particles to interlock through the apertures thus providing an extremely strong reinforcement to the soil. These geogrids under the trade name ‘Tensar’ are now widely used for road and runway construction, embankment supports, landslide repairs, etc. The polymer grid achieves its very high strength due to the orientation of the polymer molecules during its manufacture. The process of manufacture is illustrated in Fig. 4.29. An extruded sheet, produced to a very fine tolerance and with a controlled structure, has a pattern of holes stamped into it. The hole shapes and pattern can be altered depending on the performance required of the finished product. The perforated sheet is then stretched in one direction to give thin sections of highly orientated polymer with the tensile strength of mild steel. This type of grid can be used in applications where uniaxial strength is required. In other cases, where biaxial strength is necessary, the sheet is subjected to a second stretching operation in the transverse direction. The advantages of highly oriented grids are that they are light and very easy to
278
zyxwvuts Processing of Plastics
zyxwvu
Fig. 4.29 Tensar manufacturing process
handle. The advantage of obtaining a highly oriented molecular structure is also readily apparent when one compares the stiffness of a HDPE grid (10 GN/m2) with the stiffness of unoriented HDPE ( 2 1 GN/m2).
zy
(iii) Reactive Extrusion: The most recent development in extrusion is the use of the extruder as a ‘minireactor’. Reactive extrusion is the name given to the process whereby the plastic is manufactured in the extruder from base chemicals and once produced it passes through a die of the desired shape. Currently this process is being used the manufacture of low tonnage materials (4000tonnes p.a.) where the cost of a full size reactor run could not be justified. In the future it may be simply part of the production line. 4.3 Injection Moulding
4.3.1 Introduction One of the most common processing methods for plastics is injection moulding. Nowadays every home, every vehicle, every office, every factory contains a multitude of different types of articles which have been injection moulded. These include such things as electric drill casings, yoghurt cartons, television
Processing of Plastics
zyxw 279
housings, combs, syringes, paint brush handles, crash helmets, gearwheels, typewriters, fascia panels, reflectors, telephones, brief cases  the list is endless. The original injection moulding machines were based on the pressure die casting technique for metals. The first machine is reported to have been patented in the United States in 1872, specifically for use with Celluloid. This was an important invention but probably before its time because in the following years very few developments in injection moulding processes were reported and it was not until the 1920s, in Germany, that a renewed interest was taken in the process. The first German machines were very simple pieces of equipment and relied totally on manual operation. Levers were used to clamp the mould and inject the melted plastic with the result that the pressures which could be attained were not very high. Subsequent improvements led to the use of pneumatic cylinders for clamping the injection which not only lifted some of the burden off the operator but also meant that higher pressures could be used. The next major development in injection moulding, i.e. the introduction of hydraulically operated machines, did not occur until the late 1930s when a wide range of thermoplastics started to become available. However, these machines still tended to be hybrids based on die casting technology and the design of injection moulding machines for plastics was not taken really seriously until the 1950s when a new generation of equipment was developed. These machines catered more closely for the particular properties of polymer melts and modern machines are of the same basic design although of course the control systems are very much more sophisticated nowadays. In principle, injection moulding is a simple process. A thermoplastic, in the form of granules or powder, passes from a feed hopper into the barrel where it is heated so that it becomes soft. It is then forced through a nozzle into a relatively cold mould which is clamped tightly closed. When the plastic has had sufficient time to become solid the mould opens, the article is ejected and the cycle is repeated. The major advantages of the process include its versatility in moulding a wide range of products, the ease with which automation can be introduced, the possibility of high production rates and the manufacture of articles with close tolerances. The basic injection moulding concept can also be adapted for use with thermosetting materials.
zyxw zyxwvutsr
4.3.2 Details of the Process The earliest injection moulding machines were of the plunger type as illustrated in Fig. 4.30 and there are still many of these machines in use today. A predetermined quantity of moulding material drops from the feed hopper into the barrel. The plunger then conveys the material along the barrel where it is heated by conduction from the external heaters. The material is thus plasticised under pressure so that it may be forced through the nozzle into the mould cavity. In order to split up the mass of material in the barrel and improve the heat transfer, a torpedo is fitted in the barrel as shown.
280
zyxwvut zy Processing of Plastics
Material hopper
Electrical
Feed adjustment
zyxwv material
plunger
Fig. 4.30 Plunger type injection moulding machine
Unfortunately there are a number of inherent disadvantages with this type of machine which can make it difficult to produce consistent moulding. The main problems are: There is little mixing or homogenisation of the molten plastic. It is difficult to meter accurately the shot size. Since metering is on a volume basis, any variation in the density of the material will alter the shot weight. Since the plunger is compressing material which is in a variety of forms (varying from a solid granule to a viscous melt) the pressure at the nozzle can vary quite considerably from cycle to cycle. The presence of the torpedo causes a significant pressure loss. The flow properties of the melt are pressure sensitive and since the pressure is erratic, this amplifies the variability in mould filling. Some of the disadvantages of the plunger machine may be overcome by using a preplasticising system. This type of machine has two barrels. Raw material is fed into the first barrel where an extruder screw or plunger plasticises the material and feeds it through a nonreturn valve into the other barrel. A plunger in the second barrel then forces the melt through a nozzle and into the mould. In this system there is much better homogenisation because the melt has to pass through the small opening connecting the two barrels. The shot size can also be metered more accurately since the volume of material fed to the second barrel can be controlled by a limit switch on its plunger. Another advantage is that there is no longer a need for the torpedo on the main injection cylinder.
Processing of Plastics
28 1
However, nowadays this type of machine is seldom used because it is considerably more complicated and more expensive than necessary. One area of application where it is still in use is for large mouldings because a large volume of plastic can be plasticised prior to injection using the primary cylinder plunger. For normal injection moulding, however, the market is now dominated by the reciprocating screw type of injection moulding machine. This was a major breakthrough in machine design and yet the principle is simple. An extruder type screw in a heated barrel performs a dual role. On the one hand it rotates in the normal way to transport, melt and pressurize the material in the barrel but it is also capable, whilst not rotating, of moving forward like a plunger
Fig. 4.31 Spica1 cycle in reciprocating screw injection moulding machine
z
zy
282
zyxwvu Processing of Plastics
to inject melt into the mould. A typical injection moulding machine cycle is illustrated in Fig. 4.31.It involves the following stages:
(a) After the mould closes, the screw (not rotating) pushes forward to inject melt into the cooled mould. The air inside the mould will be pushed out through small vents at the furthest extremities of the melt flow path. (b) When the cavity is filled, the screw continues to push forward to apply a holding pressure (see Fig. 4.31).This has the effect of squeezing extra melt into the cavity to compensate for the shrinkage of the plastic as it cools. This holding pressure is only effective as long as the gate@) remain open. (c) Once the gate@) freeze, no more melt can enter the mould and so the screwback commences. At this stage the screw starts to rotate and draw in new plastic from the hopper. This is conveyed to the front of the screw but as the mould cavity is filled with plastic, the effect is to push the screw backwards. This prepares the next shot by accumulating the desired amount of plastic in front of the screw. At a preset point in time, the screw stops rotating and the machine sits waiting for the solidification of the moulding and runner system to be completed. (d) When the moulding has cooled to a temperature where it is solid enough to retain its shape, the mould opens and the moulding is ejected. The mould then closes and the cycle is repeated (see Fig. 4.32).
zy
zyxw Holding pressure
Screw back
Fig. 4.32 Stages during injection moulding
There are a number of important features in reciprocating screw injection moulding machines and these will now be considered in turn.
Screws The screws used in these machines are basically the same as those described earlier for extrusion. The compression ratios are usually in the range 251 to 4:l and the most common UD ratios are in the range 15 to 20.Some screws are capable of injecting the plastic at pressures up to 200 MN/m*. One important difference from an extruder screw is the presence of a backflow check valve at the end of the screw as illustrated in Fig. 4.33.The purpose of this valve is to stop any back flow across the flights of the screw when it is acting as a plunger. When material is being conveyed forward by the rotation of the screw, the valve opens as shown. One exception is when injection moulding
Processing of Plastics
283
zy
zyxwvutsrqponm
( 0 1 Valve closed
f b ) Valve open
Fig. 4.33 Typical check valve
heatsensitive materials such as PVC. In such cases there is no check valve because this would provide sites where material could get clogged and would degrade.
Barrels and Heaters These are also similar to those in extruder machines. In recent years, vented barrels have become available to facilitate the moulding of water sensitive plastics without the need for predrying. Water sensitivity in plastics can take several forms. If the plastic absorbs water then dimensional changes will occur, just as with wood or paper. The plastic will also be plasticised by the water so that there will be property changes such as a reduction in modulus and an increase in toughness. All these effects produced by water absorption are reversible. Another event which may occur is hydrolysis. This is a chemical reaction between the plastic and water. It occurs extremely slowly at room temperature but can be significant at moulding temperatures. Hydrolysis causes degradation, reduction in properties (such as impact strength) and it is irreversible. Table 4.3 indicates the sensitivity of plastics to moisture. Note that generally extrusion requires a lower moisture content than injection moulding to produce good quality products. Table 4.3
zyxwvuts zyxw
Water sensitivity of some common plastics Drying not required (Materials do not hydrolyse) Polyethylene Polypropylene Polystyrene PVC
Drying required
Absorbs only
Hydrolyses
Acrylic (0.02/0.08)* ABS (O.OU0.08) SAN (0.02/0.08)
PET (0.002/0.002) Polycarbonate (0.01/0.02) Nylon 66 (0.08/0.15)
*Required maximum moisture content for extrusionhjection moulding (%)
Nozzles The nozzle is screwed into the end of the barrel and provides the means by which the melt can leave the barrel and enter the mould. It is also a region where the melt can be heated both by friction and conduction from a
284
Processing of Plastics
heater band before entering the relatively cold channels in the mould. Contact with the mould causes heat transfer from the nozzle and in cases where this is excessive it is advisable to withdraw the nozzle from the mould during the screwback part of the moulding cycle. Otherwise the plastic may freeze off in the nozzle. There are several types of nozzle. The simplest is an open nozzle as shown in Fig. 4.34(a). This is used whenever possible because pressure drops can be minimised and there are no hold up points where the melt can stagnate and decompose. However, if the melt viscosity is low then leakage will occur from this type of nozzle particularly if the barrelhozzle assembly retracts from the mould each cycle. The solution is to use a shutoff nozzle of which there are many types. Fig. 4.34(b) shows a nozzle which is shut off by external means. Fig. 4.34(c) shows a nozzle with a spring loaded needle valve which opens when the melt pressure exceeds a certain value or alternatively when the nozzle is pressed up against the mould. Most of the shutoff nozzles have the disadvantage that they restrict the flow of the material and provide undersirable stagnation sites. For this reason they should not be used with heat sensitive materials such as PVC.
zyxwv
zyxwvu zyxwv
(b) External shutoff nozzle
IC)
Needle
nozzle
zyxwvutsr Fig. 4.34 bpes of nozzle
zy
Clamping Systems In order to keep the mould halves tightly closed when the melt is being injected under high pressures it is necessary to have a clamping system. This may be either (a) hydraulic or (b) mechanical (toggle)  or some combination of the two.
Processing of Plastics
285
In the hydraulic system, oil under pressure is introduced behind a piston connected to the moving platen of the machine. This causes the mould to close and the clamp force can be adjusted so that there is no leakage of molten plastic from the mould. The toggle is a mechanical device used to amplify force. Toggle mechanisms tend to be preferred for high speed machines and where the clamping force is relatively small. The two main advantages of the toggle system are that it is more economical to run the small hydraulic cylinder and since the toggle is self locking it is not necessary to maintain the hydraulic pressure throughout the moulding cycle. On the other hand the toggle system has the disadvantages that there is no indication of the clamping force and the additional moving parts increase maintenance costs.
zyxwvu zyxwv zyxwv
4.3.3 Moulds In the simplest case an injection mould (or ‘tool’) consists of two halves into which the impression of the part to be moulded is cut. The mating surfaces of the mould halves are accurately machined so that no leakage of plastic can occur at the split line. If leakage does occur the flash on the moulding is unsightly and expensive to remove. A typical injection mould is illustrated in Fig. 4.35. It may by seen that in order to facilitate mounting the mould in the machine and cooling and ejection of the moulding, several additions are made to the basic mould halves. Firstly, backing plates permit the mould to be bolted on to the machine platens. Secondly, channels are machined into the mould to allow the mould temperature to be controlled. Thirdly, ejector pins are included to that the moulded part can be freed from the mould. In most cases the ejector pins are operated by the shoulder screw hitting a stop when the mould opens. The mould cavity is joined to the machine nozzle by means of the sprue. The sprue anchor pin then has the function of pulling the sprue away from the nozzle and ensuring that the moulded part remains on the moving half of the mould, when the mould opens. For multicavity moulds the impressions are joined to the sprue by runners  channels cut in one or both halves of the mould through which the plastic will flow without restriction. A narrow constriction between the runner and the cavity allows the moulding to be easily separated from the runner and sprue. This constriction is called the gate. A production injection mould is a piece of high precision engineering manufactured to very close tolerances by skilled craftsmen. A typical mould can be considered to consist of (i) the cavity and core and (ii) the remainder of the mould (often referred to as the bolster). Of these two, the latter is the more straightforward because although it needs to be accurately made, in general, conventional machine tools can be used. The cavity and core, however, may be quite complex in shape and so they often need special techniques. These can include casting, electrodeposition, hobbing, pressure casting, spark erosion and NC machining.
286
Processing of Plastics
zy
zyxwvu
Fig. 4.35 Details of injection mould
Finishing and polishing the mould surfaces is also extremely important because the melt will tend to reproduce every detail on the surface of the mould. Finally the mould will have to be hardened to make it stand up to the treatment it receives in service. As a result of all the time and effort which goes into mould manufacture, it is sometimes found that a very complex mould costs more than the moulding machine on which it is used. Several features of the mould are worthy of special mention. (a) Gates: As mentioned earlier the gate is the small orifice which connects the runner to the cavity. It has a number of functions. Firstly, it provides a convenient weak link by which the moulding can be broken off from the runner system. In some moulds the degating may be automatic when the mould opens. The gate also acts like a valve in that it allows molten plastic to fill the mould but being small it usually freezes off first. The cavity is thus sealed off from the runner system which prevents material being sucked out of the cavity during screwback. As a general rule, small gates are preferable because no finishing
zy
Processing of Plastics
287
is required if the moulding is separated cleanly from the runner. So for the initial trials on a mould the gates are made as small as possible and are only opened up if there are mould filling problems. In a multicavity mould it is not always possible to arrange for the runner length to each cavity to be the same. This means that cavities close to the sprue would be filled quickly whereas cavities remote from the sprue receive the melt later and at a reduced pressure. To alleviate this problem it is common to use small gates close to the sprue and progressively increase the dimensions of the gates further along the runners. This has the effect of balancing the fill of the cavities. If a single cavity mould is multigated then here again it may be beneficial to balance the flow by using various gate sizes. Examples of gates which are in common use are shown in Fig. 4.36. Sprue gates are used when the sprue bush can feed directly into the mould cavity as, for example, with single symmetrical moulding such as buckets. Pin gates are particularly successful because they cause high shear rates which reduce the viscosity of the plastic and so the mould fills more easily. The side gate is the most common type of gate and is a simple rectangular section feeding into the side of the cavity. A particular attraction of this type of gate is that mould filling can be improved by increasing the width of the gate but the freeze time is unaffected because the depth is unchanged.
zyxw zyxwvut zyxwvutsrq zyxwvut zyx (a1 Sprue gate
( b l Pin gate
( c ) Side gate
Fig. 4.36 Types of gate
(b) Runners: The runner is the flow path by which the molten plastic travels from the sprue (i.e. the moulding machine) to the gates (i.e. the cavity). To prevent the runner freezing off prematurely, its surface area should be small so as to minimise heat transfer to the mould. However, the cross sectional area of the runner should be large so that it presents little resistance to the flow of the plastic but not so large that the cycle time needs to be extended to allow the runner to solidify for ejection. A good indication of the efficiency of a runner is, therefore, the ratio of its crosssectional area to its surface area. For example, a semicircular channel cut into one half of the mould is convenient to machine but it only has an area ratio of 0.153 D where D is the diameter of the semicircle. A full round runner, on the other hand, has a ratio of 0.25 D. A square section also has this ratio but is seldom used because it is difficult to
288
zyxwvu zyx Processing of Plastics
eject. A compromise is a trapezoidal section (cut into one half of the mould) or a hexagonal section.
(c) Sprues: The sprue is the channel along which the molten plastic first enters the mould. It delivers the melt from the nozzle to the runner system. The sprue is incorporated in a hardened steel bush which has a seat designed to provide a good seal with the nozzle. Since it is important that the sprue is pulled out when the mould opens it is tapered as shown in Fig. 4.35 and there is a sprue pulling device mounted directly opposite the sprue entry. This can take many forms but typically it would be an undercut or reversed taper to provide a key for the plastic on the moving half of the mould. Since the sprue, like the runner system, is effectively waste it should not be made excessively long.
(d) Venting: Before the plastic melt is injected, the cavity in the closed mould contains air. When the melt enters the mould, if the air cannot escape it become compressed. At worst this may affect the mould filling, but in any case the sudden compression of the air causes considerable heating. This may be sufficient to bum the plastic and the mould surface at local hot spots. To alleviate this problem, vents are machined into the mating surfaces of the mould to allow the air to escape. The vent channel must be small so that molten plastic will not flow along it and cause unsightly flash on the moulded article. 'I)lpically a vent is about 0.025 mm deep and several millimeters wide. Away from the cavity the depth of the vent can be increased so that there is minimum resistance to the flow of the gases out of the mould. (e) Mould Temperature Control: For efficient moulding, the temperature of the mould should be controlled and this is normally done by passing a fluid through a suitably arranged channel in the mould. The rate at which the moulding cools affects the total cycle time as well as the surface finish, tolerances, distortion and internal stresses of the moulded article. High mould temperatures improve surface gloss and tend to eliminate voids. However, the possibility of flashing is increased and sink marks are likely to occur. If the mould temperature is too low then the material may freeze in the cavity before it is filled. In most cases the mould temperatures used are a compromise based on experience. In Chapter 5 we will consider ways of estimating the time taken for a moulding to cool down in a mould.
zyxwv
Example 4.5 The runner layout for an eight cavity mould is illustrated in Fig. 4.37.If the mould is to be designed so that the pressure at the gate is the same in all cases, determine the radius of the runner in section A. The flow may be assumed to be isothermal.
Solution Although this runner system is symmetrical, it is not balanced. If the runner had the same diameter throughout all sections, then the mouldings close to the sprue would fill first and would be overpacked before the outermost
Processing of Plastics
z
zyxwvu zy 289
zyxw zyxwv 50
i
r
rad = 6 mm
rad = 8 mm
Fig. 4.37 Layout for eight cavity mould
cavities were filled. In a good mould design, all the cavities fill simultaneously at the same pressure. In this case it is necessary to ensure that the pressure drop in Sections 1 and 3 is the same as the pressure drop in Section 2. It will be shown in Chapter 5 that the pressure drop, AP, for isothermal flow in a circular section channel is given by
zyx (4.22)
where
q = viscosity of the plastic
L = length of channel
Q = volume flow rate R = radius of channel
If the volume flow rate towards point J is q (ie the input at the sprue is 2q) then at J the flow will split as follows:
zyx
Flow along runner 1 = xq
Flow along runner 2 = 1/2( 1  x)q Flow along runner 3 = 1/2xq where
(A refers to the area of the relevant runner). Using equation (4.22) we can write 8rlL1xq Pressure loss in runner 1 = 
n@
290
zyxwvut zyxw zyxwv zyxwvu Processing of Plastics
Pressure loss in runner 2 =
Pressure loss in runner 3 =
Thus, equating pressure losses after point J
Substituting for x and rearranging to get R2
For the dimensions given:
R2 = 3.8 mm In practice there are a number of other factors to be taken into account. For example, the above analysis assumes that this plastic is Newtonian, ie that it has a constant viscosity, 11. In reality the plastic melt is nonNewtonian so that the viscosity will change with the different shear rates in each of the three runner sections analysed. In addition, the melt flow into the mould will not be isothermal  the plastic melt immediately in contact with the mould will solidify. This will continuously reduce the effective runner crosssection for the melt coming along behind. The effects of nonNewtonian and nonisothermal behaviour are dealt with in Chapter 5.
MultiDaylight Moulds This type of mould, also often referred to as a three plate mould, is used when it is desired to have the runner system in a different plane from the parting line of the moulding. This would be the case in a multicavity mould where it was desirable to have a central feed to each cavity (see Fig. 4.38). In this type of mould there is automatic degating and the runner system and sprue are ejected separately from the moulding.
Hot Runner Moulds The runners and sprues are necessary in a mould but they are not part of the endproduct. Unfortunately, it is not economically viable to discard them so they must be reground for subsequent reprocessing. Regrinding is expensive and can introduce contamination into the material so that any system which avoids the accumulation of runners and sprues is attractive. A system has been developed to do this and it is really a logical extension of three plate moulding. In this system, strategically placed heaters and insulation in the mould keep the
29 1
Processing of Plastics
zyx
zyxwvutsrqp
Eject 01 pins
Split Ime
Spltt line
Fig. 4.38 Typical 3plate mould
plastic in the runner at the injection temperature. During each cycle therefore the component is ejected but the melt in the runner channel is retained and injected into the cavity during the next shot. A typical mould layout is shown in Fig. 4.39. Additional advantages of hot runner moulds are (i) elimination of trimming and (ii) possibility of faster cycle times because the runner system does not have to freeze off. However, these have to be weighed against the disadvantages of the system. Since the hot runner mould is more complex than a conventional mould it will be more expensive. Also there are many areas in the hot runner manifold where material can get trapped. This means that problems can be experienced during colour or grade changes because it is difficult to remove all of the previous material. As a practical point it should also be realised that the system only works as long as the runner remains molten. If the runner system freezes off then the hot runner manifold needs to be dismantled to remove the runners. Note also that hot runner system are not suitable for heat sensitive materials such as PVC.
zyxwv zyxwvu
Insulated Runner Moulds This is similar in concept to the hot runner mould system. In this case, instead of having a specially heated manifold in the mould, large runners (1325 mm diameter) are used. The relatively cold mould causes a frozen skin to form in
292
Processing of Plastics
zy
zyxwvu runner
channels
Fig. 4.39 Layout of hot runner mould
the runner which then insulates its core so that this remains molten. As in the previous case the runner remains in the mould when the moulding is ejected and the molten part of the runner is then injected into the cavity for the next shot. If an undue delay causes the whole runner to freeze off then it may be ejected and when moulding is restarted the insulation layer soon forms again. This type of system is widely used for moulding of fast cycling products such as flower pots and disposable goods. The main disadvantage of the system is that it is not suitable for polymers or pigments which have a low thermal stability or high viscosity, as some of the material may remain in a semimolten form in the runner system for long periods of time. A recent development of the insulated runner principle is the distribution tube system. This overcomes the possibility of freezingoff by insertion of heated tubes into the runners. However, this system still relies on a thick layer of polymer forming an insulation layer on the wall of the runner and so this system is not suitable for heat sensitive materials. Note that both the insulated runner and the distribution tube systems rely on a cartridge heater in the gate area to prevent premature freezing off at the gate (see Fig. 4.40).
zyxwv zyx
Processing of Plastics Cavity
zyxwvu zyx zyxw zyxw 293
Large runnel
Cavity I
Large runner
,
(b) Distributedrunner system
Fig. 4.40 Insulated and distributed runner systems
zyxw
Mould Clamping Force In order to prevent ‘flashing’, i.e. a thin film of plastic escaping out of the mould cavity at the parting line, it is necessary to keep the mould tightly closed during injection of the molten plastic. Before setting up a mould on a machine it is always worthwhile to check that there is sufficient clamping force available on the machine. To do this it is necessary to be able to estimate what clamping force will be needed. The relationship between mould area and clamp requirements has occupied the minds of moulders for many years. Practical experience suggests that the clamping pressure over the projected area of the moulding should be between 10 and 50 MN/m2 depending on factors such as shape, thickness, and type of material. The mould clamping force may also be estimated in the following way. Consider the moiilding of a disc which is centre gated as shown in Fig. 4.41(a). The force on the shaded element is given by
zy zyxwvuts zyxw zyx
Force, F =
i o
Pr2nrdr
(4.23)
The cavity pressure will vary across the disc and it is necessary to make some assumption about this variation. Experimental studies have suggested that an empirical relation of the form P , = P o (1 
(i)“)
(4.24)
is most satisfactory. Po is the pressure at the gate and rn is a constant which is usually between 0.3 and 0.75. It will be shown later (Chapter 5 ) that ‘tn’ is in fact equal to (1 n) where ‘n’ is the index in the Power Law expression for polymer melt flow.
294
zyxw zyxwv zyxw zyx Processing of Plastics
Substituting (4.24) in (4.23) then
F
= nR2Po (L)
(4.25)
m+2
This is a simple convenient expression for estimating the clamping force required for the disc. The same expression may also be used for more complex shapes where the projected area may be approximated as a circle. It will also give sufficiently accurate estimates for a square plate when the radius, R, in Fig. 4.41(a) is taken as half of the diagonal.
(a) Disc moulding
(b) Strip moulding
Fig. 4.41 Clamp force analysis
zyx
zyxw
An alternative way of looking at this equation is that the clamping pressure, based on the projected area of the moulding, is given by Clamping pressure =
2) x
+
Injection pressure
For any particular material the ratio (rn/(rn 2)) may be determined from the flow curves and it will be temperature and (to some extent) pressure dependent. In practice the clamping pressure will also depend on the geometry of the cavity. In particular the flow ratio (flow lengwchannel lateral dimension) is important. Fig. 4.42 illustrates typical variations in the Mean Effective Pressure in the cavity for different thicknesses and flow ratios. The data used here is typical for easy flow materials such as polyethylene, polypropylene and polystyrene. To calculate the clamp force, simply multiply the appropriate Mean Effective Pressure by the projected area of the moulding. In practice it is
Processing of Plastics
0
295
50
zy
zyxwvutsr zyxwvu zyxwvuts 100
200
150
Flow ratlo
Fig. 4.42 Claming pressures for different cavity geometries (typical values for easy flow materials)
prudent to increase this value by 1020% due to the uncertainties associated with specific moulds. For plastics other than the easy flow materials referred to above, it would be normal to apply a factor to allow for the higher viscosity. Typical viscosity factors are given below.
Material Polyethylene, polypropylene, polystyrene Nylon 66 ABS Acrylic PVC Polycarbonate
Viscosity Factor 1 1.2 + 1.4 1.3 + 1.4 1.5 + 1.7 1.6 + 1.8 1.7 + 2.0
Example 4.6 The mould shown in Fig. 4.35 produces four cup shaped ABS mouldings. The depth of the cups is 60 mm, the diameter at the is 90 mm and the wall thickness is 1.0 mm. The distance from the sprue to the cavity is 40 mm and the runner diameter is 6 mm. Calculate the clamp force necessary on the moulding machine and estimate how the clamp force would change if the mould was designed so as to feed the cups through a pin gate in the centre of the base (as illustrated in Fig. 4.38). The clamp pressure data in Fig. 4.42 should be used and the taper on the side of the cups may be ignored. Solution (a) Within the cavity, the maximum flow length for the plastic melt will be from the gate, along the side of the cup and across the base of the cup, ie
Flow length = 60
+ 90 = 150 mm
296
zyxwvutsr zyx zyx Processing of Plastics
The thickness of the moulding is 1 mm, hence the flow ratio = 150/1 = 150. From Fig. 4.42 at this thickness and flow ratio, the mean effective pressure is 75 MN/m2. Allowing an extra 15% for uncertainties and applying the viscosity factor of 1.4 for ABS, then the appropriate mean effective pressure is 75 x 1.15 x 1.4 = 120 MN/m2. For each cavity, the projected area is ( ~ / 4 ) ( 9 0 )= ~ 6360 mm2 = 6.36 x m2. = 763 kN. Hence, clamp force per cavity = 120 x 6.36 x The projected area of the runners is 4 x 40 x 6 = 960 mm2. Assuming that the mean effective pressure also applies to the runner system, then = 115 kN
clamp force for runners = 120 x 0.96 x
Hence total clamp force for 4 cavities and 1 runner system is given by Total clamp force = (4 x 763)
+ 115 = 3167 kN
zyx
The required clamp force is therefore 317 tonnes. (b) If a pin gate in the middle of the base is used instead of an edge gate, then the flow ratio will be different. In this case
+
flow length = i(90) 60 = 105
This is also the flow ratio, so from Fig. 4.42 the mean effective pressure is 50 MN/m2. Applying the viscosity factor, etc as above, then
Clamp force per cavity = 50 x 1.15 x 1.4 x
(:)
(90)2 x
= 512 kN
In this case the runner system will be almost totally in the ‘shadow’ of the projected area of the cavities and so they can be ignored.
zyxwvu
Hence, total clamp force = 4 x 5 12 = 2048 kN = 205 tonnes.
Another common shape which is moulded is a thin rectangular strip. Consider the centre gated strip as shown in Fig. 4.41(b). In the same way as before the clamping force, F, is given by (4.26)
zyxwv zyxwvut zyxwvut zyxwv zyxwvu zyx
Processing of Plastics i.e.
297
F = TPoL
()m m+ l
(4.27)
The calculation of clamp force is considered in more detail in Chapter 5 .
4.3.4 Structural Foam Injection Moulding Foamed thermoplastic articles have a cellular core with a relatively dense (solid) skin. The foam effect is achieved by the dispersion of inert gas throughout the molten resin directly before moulding. Introduction of the gas is usually carried out either by preblending the resin with a chemical blowing agent which releases gas when heated or by direct injection of the gas (usually nitrogen). When the compressed gashesin mixture is rapidly injected into the mould cavity, the gas expands explosively and forces the material into all parts of the mould. The advantages of these types of foam moulding are (a) for a given weight they are many times more rigid than a solid moulding (b) they are almost completely free from orientation effects and the shrinkage is uniform (c) very thick sections can be moulded without sink marks.
zyxw
Foamed plastic articles may be produced with good results using normal screwtype injection moulding machines (see Fig. 4.43(a)). However, the limitations on shot size, injection speed and platen area imposed by conventional
T7 '. .... ... ...:.a
;.
( 0 1 Stondord injection moulding press
zyxwvut
Fig. 4.43 Structural foam moulding equipment
298
zyxw zyxwvu zy Processing of Plastics
injection equipment prevent the full largepart capabilities of structural foam from being realised. Specialised foam moulding machines currently in use can produce parts weighing in excess of 50 kg (see Fig. 4.43(b)). Wall sections in foam moulding are thicker than in solid material. Longer cycle times can therefore be expected due to both the wall thickness and the low thermal conductivity of the cellular material. In contrast, however, the injection pressures in foam moulding are low when compared with conventional injection moulding. This means that less clamping force is needed per unit area of moulding and mould costs are less because lower strength mould materials may be used. 4.3.5 Sandwich Moulding This is an injection moulding method which permits material costs to be reduced in large mouldings. In most mouldings it is the outer surface of an article which is important in terms of performance in service. If an article has to be thick in order that it will have adequate flexural stiffness then the material within the core of the article is wasted because its only function is to keep the outer surfaces apart. The philosophy of sandwich moulding is that two different materials (or two forms of the same material) should be used for the core and skin. That is, an expensive high performance material is used for the skin and a lowcost commodity or recycled plastic is used for the core. The way that this can be achieved is illustrated in Fig. 4.44.
zyxw
II Q I
II
c., I I
I
Fig. 4.44 Stages in sandwich moulding process
Initially the skin material is injected but not sufficient to fill the mould. The core material is then injected and it flows laminarly into the interior of the core. This continues until the cavity is filled as shown in Fig. 4.44(c). Finally the
299
Processing of Plastics
nozzle valve rotates so that the skin material is injected into the sprue thereby clearing the valve of core material in preparation for the next shot. In a number of cases the core material is foamed to produce a sandwich section with a thin solid skin and a cellular core. It is interesting that in the latest applications of sandwich moulding it is the core material which is being regarded as the critical component. This is to meet design requirements for computers, electronic equipment and some automotive parts. In these applications there is a growing demand for covers and housings with electromagnetic interference (EMI) shielding. The necessity of using a plastic with a high loading of conductive filler (usually carbon black) means that surface finish is poor and unattractive. To overcome this the sandwich moulding technique can be used in that a good quality surface can be moulded using a different plastic.
zyxwvu
4.3.6 Gas Injection Moulding
In recent years major developments have been made in the use of an inert gas to act as the core in an injection moulded plastic product. This offers many advantages including greater stiffnesdweight ratios and reduced mouldedin stresses and distortion. The first stage of the cycle is the flow of molten polymer into the mould cavity through a standard feed system. Before this flow of polymer is complete, the injection of a predetermined quantity of gas into the melt begins through a special nozzle located within the cavity or feed system as shown in Fig. 4.45. The timing, pressure and speed of the gas injection is critical. The pressure at the polymer gate remains high and, therefore, the gas chooses a natural path through the hotter and less viscous parts of the polymer melt towards the lower pressure areas. The flow of gas cores out a hollow centre extending from its point of entry towards the last point of fill. By controlling the amount of gas injected into the hollow core, the pressure on the cooling polymer is controlled and maintained until the moulding is packed. The final stage is the withdrawal of the gas nozzle, prior to mould opening, which allows the gas held in the hollow core to vent. The gas injection process overcomes many of the limitations of injection mouldings such as mouldedin stress and distortion. These limitations are caused by laminar flow and variation in pressure throughout the moulding. With the gas injection process, laminar flow is considerably reduced and a uniform pressure is maintained. The difficulty of transmitting a very high pressure uniformly throughout a moulding can also cause inconsistent volumetric shrinkage of the polymer, and this leads to isolated surface sink marks. Whilst cycle times are comparable with those of conventional injection moulding, clamping forces are much lower. Also, by using gas to core out the polymer instead of mixing with it, gasinjection overcomes a number of shortcomings of the structural foam process. In particular there are no surface imperfections
300
zyxwvut z zyxwvu Processing of Plastics
Plastic
J injection
I Plastic
Stage 1
Hydraulic cylinder
&
zyxwvut
Fig. 4.45 Stages in the gas injection moulding of an automotive handle (courtesy of cinpress Ltd)
z zyx zyxwvuts zyx zyxwv
Processing of Plastics
301
(caused by escaping gas bubbles in structural foam moulding) and cycle times are lower because thinner sections are being cooled.
4.3.7 Shear Controlled Orientation in Injection Moulding (SCORIM) One of the major innovations in recent years is the use of pulsed pressure through the gates to introduce and control the orientation of the structure (or fillers) in injection moulded products. A special manifold is attached to the machine nozzle as illustrated in Fig. 4.46. This diagram relates to the double livefeed of melt although up to four pistons, capable of applying oscillating pressure may be used.
Mould cavity
Nozzle
zyx
/
/
Piston D
Injection moulder barrel
7A f
Piston E
s ring of the melt
/
DoNuble livefeed delvice
\
Fig. 4.46 One embodiment of SCORIM where the device (B) for producing shear during solidification, by the action of pistons @) and (E), is placed between the injection moulding machine barrel (A) and the mould (C) (Courtesy of Brunei University)
Shear controlled orientation in injection moulding (SCORIM)is based on the progressive application of macroscopic shears at the meltsolid interface during solidification in the moulding of a polymer matrix. Macroscopic shears of specified magnitude and direction, applied at the meltsolid interface provide several advantages: (i) Enhanced polymer matrix or fibre alignment by design in moulded polymers or fibre reinforced polymers. (ii) Elimination of mechanical discontinuities that result from the initial mould filling process, including internal weld lines. (iii) Reduction in the detrimental effects of a change in moulded section thickness. (iv) Elimination or reduction in defects resulting from the moulding of thick sectioned components.
302
zy zyxwvu zyxwvut zyx Processing of Plastics
43.8 Reaction Injection Moulding Although there have been for many years a number of moulding methods (such as hand layup of glass fibres in polyester and compression moulding of thermosets or rubber) in which the plastic material is manufactured at the same time as it is being shaped into the final article, it is only recently that this concept has been applied in an injection moulding type process. In Reaction Injection Moulding (RIM), liquid reactants are brought together just prior to being injected into the mould. Inmould polymerisation then takes place which forms the plastic at the same time as the moulding is being produced. In some cases reinforcing fillers are incorporated in one of the reactants and this is referred to as Reinforced Reaction Injection Moulding (RRIM) The basic RIM process is illustrated in Fig. 4.47. A range of plastics lend themselves to the type of fast polymerisation reaction which is required in this process  polyesters, epoxies, nylons and vinyl monomers. However, by far the most commonly used material is polyurethane. The components A and B are an isocyanate and a poly01 and these are kept circulating in their separate systems until an injection shot is required. At this point the two reactants are brought together in the mixing head and injected into the mould.
Fig. 4.47 Schematic view of reaction injection moulding
Since the reactants have a low viscosity, the injection pressures are relatively low in the RIM process. Thus, comparing a conventional injection moulding machine with a RIM machine having the same clamp force, the RIM machine could produce a moulding with a much greater projected area (typically about 10 times greater). Therefore the RIM process is particularly suitable for large
Processing of Plastics
303
area mouldings such as car bumpers and body panels. Another consequence of the low injection pressures is that mould materials other than steel may be considered. Aluminium has been used successfully and this permits weight savings in large moulds. Moulds are also less expensive than injection moulds but they must not be regarded as cheap. RIM moulds require careful design and, in particular, a good surface finish because the expansion of the material in the mould during polymerisation causes every detail on the surface of the mould to be reproduced on the moulding.
z
zyxw zyxw zyxwvuts
4.3.9 Injection Blow Moulding In Section 4.2.7 we considered the process of extrusion blow moulding which is used to produce hollow articles such as bottles. At that time it was mentioned that if molecular orientation can be introduced to the moulding then the properties are significantly improved. In recent years the process of injection blow moulding has been developed to achieve this objective. It is now very widely used for the manufacture of bottles for soft d r i n k s . The steps in the process are illustrated in Fig. 4.48. Initially a preform is injection moulded. This is subsequently inflated in a blow mould in order to produce the bottle shape. In most cases the second stage inflation step occurs immediately after the injection moulding step but in some cases the preforms are removed from the injection moulding machine and subsequently reheated for inflation.
I
Heating of injection
Clamping
Inflation
moulded preform
Fig. 4.48
Injection blow moulding process
Ejection
.i
304
Processing of Plastics
z
zy zyxwv
The advantages of injection blow moulding are that
(i) the injection moulded parison may have a carefully controlled wall thickness profile to ensure a uniform wall thickness in the inflated bottle. (ii) it is possible to have intricate detail in the bottle neck. (iii) there is no trimming or flash (compare with extrusion blow moulding).
A variation of this basic concept is the Injection Orientation Blow Moulding technique developed in the 1960s in the USA but upgraded for commercial use in the 1980s by AOKI in Japan. The principle is very similar to that described above and is illustrated in Fig. 4.49. It may be seen that the method essentially combines injection moulding, blow moulding and thermoforming to manufacture high quality containers.
zyxwv U
Injection moulding of disc preform
f
Clamping
zyxwvu zyxw Stretching
Inflation
Ejection
Fig. 4.49 Injection orientation strech blow moulding
4.3.10 Injection Moulding of Thermosetting Materials
In the past the thought of injection moulding thermosets was not very attractive. This was because early trials had shown that the feedstock was not of a consistent quality which meant that continual alterations to the machine settings were necessary. Also, any undue delays could cause premature curing of the resin and consequent blockages in the system could be difficult to remove. However, in recent years the processing characteristics of thermosets have been improved considerably so that injection moulding is likely to become one of the major production methods for these materials. The injection moulding of fibre reinforced thennosets, such as DMC (Section 4.10.2), is also becoming very common. Nowadays, the injection moulder can be supplied with uniform quality granules which consist of partially polymerised resin, fillers and additives. The formulation of the material is such that it will flow easily in the barrel with a slow rate of polymerisation. The curing is then completed rapidly in the mould.
Processing of Plastics
zyxwvu zyxw zyxwv 305
In most respects the process is similar to the injection moulding of thermoplastics and the sequence of operations in a single cycle is as described earlier. For thermosets a special barrel and screw are used. The screw is of approximately constant depth over its whole length and there is no check value which might cause material blockages (see Fig. 4.50). The barrel is only kept warm (80110°C) rather than very hot as with thermoplastics because the material must not cure in this section of the machine. Also, the increased viscosity of the thermosetting materials means that higher screw torques and injection pressures (up to 200 MN/m2 are needed).
zyxwvutsrq
Warming jacket
Nafzle
I
zyxwvuts
Fig. 4.50 Injection modding of thermosets and rubbers
zyxwvu
On the mould side of the machine the major difference is that the mould is maintained very hot (150200°C) rather than being cooled as is the case with thermoplastics. This is to accelerate the curing of the material once it has taken up the shape of the cavity. Another difference is that, as thermosetting materials are abrasive and require higher injection pressures, harder steels with extra wear resistance should be used for mould manufacture. As a result of the abrasive nature of the thermosets, hydraulic mould clamping is preferred to a toggle system because the inevitable dust from the moulding powder increases the wear in the linkages of the latter. When moulding thermosetting articles, the problem of material wastage in sprues and runners is much more severe because these cannot be reused. It is desirable therefore to keep the sprue and runner sections of the mould cool so that these do not cure with the moulding. They can then be retained in the mould during the ejection stage and then injected into the cavity to form the next moulding. This is analogous to the hot runner system described earlier for thermoplastics. The advantages of injection moulding thermosets are as follows: (a) fast cyclic times (see Table 4.4) (b) efficient metering of material (c) efficient preheating of material (d) thinner flash  easier finishing (e) lower mould costs (fewer impressions).
306
zy zyxw Processing of Plastics
Table 4.4 For the same part, injection moulding of thermosets can offer up to 25%production increase and lower partcosts than compression. Compression moulding Open mould, unload piece Mould cleaning Close machine, start pressure Moulding cycle time Total compression cycle Injection moulding Unload piece, opedclose machine Moulding cycle time Total injection cycle
Minutes 0.105 0.140 0.100 2.230 2.575
zy zy
0.100 1.goo 2.000
4.4 Thennoforming When a thermoplastic sheet is heated it becomes soft and pliable and the techniques for shaping this sheet are known as thermoforming. This method of manufacturing plastic articles developed in the 1950s but limitations such as poor wall thickness distribution and large peripheral waste restricted its use to simple packaging applications. In recent years, however, there have been major advances in machine design and material availability with the result that although packaging is still the major market sector for the process, a wide range of other products are made by thermoforming. These include aircraft window reveals, refrigerator liners, baths, switch panels, car bumpers, motorbike fairings etc. The term ‘thermoforming’ incoroporates a wide range of possibilities for sheet forming but basically there are two subdivisions  vacuum forming and pressure forming.
zyx zy
(a) Vacuum Forming In this processing method a sheet of thermoplastic material is heated and then shaped by reducing the air pressure between it and a mould. The simplest type of vacuum forming is illustrated in Fig. 4.5 l(a). This is referred to as Negative Forming and is capable of providing a depth of draw which is 113112 of the maximum width. The principle is very simple. A sheet of plastic, which may range in thickness from 0.025 mm to 6.5 mm, is clamped over the open mould. A heater panel is then placed above the sheet and when sufficient softening has occurred the heater is removed and the vacuum is applied. For the thicker sheets it is essential to have heating from both sides. In some cases Negative Forming would not be suitable because, for example, the shape formed in Fig. 4.5 1 would have a wall thickness in the comers which is considerably less than that close to the clamp. If this was not acceptable then
307
Processing of Plastics Heater
Vents
Plastic sheet
zy
zyxwvutsrq
zyxw zyxwvut Fig. 4.51 Vacuum forming process
the same basic shape could be produced by Positive Forming. In this case a male (positive) mould is pushed into the heated sheet before the vacuum is applied. This gives a better distribution of material and deeper shapes can be formed  depth to width ratios of 1:1 are possible. This thermoforming method is also referred to as Drupe Forming. Another alternative would be to have a female mould as in Fig. 4.5 1 but after the heating stage and before the vacuum is applied, a plug comes down and guides the sheet into the cavity. When the vacuum is applied the base of the moulding is subjected to less draw and the result is a more uniform wall thickness distribution. This is called Plug Assisted Forming. Note that both Positive Forming and Plug Assisted Forming effectively apply a prestretch to the plastic sheet which improves the performance of the material quite apart from the improved wall thickness distribution. In the packaging industry skin and blister vacuum machines are used. Skin packaging involves the encapsulation of articles between a tight, flexible transparent skin and a rigid backing which is usually cardboard. Blister packs are preformed foils which are sealed to a rigid backing card when the goods have been inserted. The heaters used in thermoforming are usually of the infra red type with typical loadings of between 10 and 30 kW/m2. Normally extra heat is concentrated at the clamped edges of the sheet to compensate for the additional heat losses in this region. The key to successful vacuum forming is achieving uniform heating over the sheet. One of the major attractions of vacuum forming is that since only atmospheric pressure is used to do the shaping, the moulds do not have to be very strong. Materials such as plaster, wood and thermosetting resins have all been used successfully. However, in long production runs mould cooling becomes essential in which case a metal mould is necessary. Experience has shown that the most satisfactory metal is undoubtedly aluminium. It
308
zy zy zyxw zyxwvu zyxwvu pn>cessing of Plastics
is easily shaped, has good thermal conductivity, can be highly polished and has an almost unlimited life. Materials which can be vacuum formed satisfactorily include polystyrene, ABS, PVC, acrylic, polycarbonate, polypropylene and high and low density polyethylene. Coextruded sheets of different plastics and multicolour laminates are also widely used nowadays. One of the most recent developments is the thennoforming of crystallisablePET for high temperature applications such as oven trays. The PET sheet is manufactured in the amorphous form and then during thennoforming it is permitted to crystallise. The resulting moulding is thus capable of remaining stiff at elevated temperatures.
(b) Pressure Forming
This is generally similar to vacuum forming except that pressure is applied above the sheet rather than vacuum below it. This advantage of this is that higher pressures can be used to form the sheet. A typical system is illustrated in Fig. 4.52 and in recent times this has become attractive as an alternative to injection moulding for moulding large area articles such as machine housings.
*
Plug moves
Fig. 4.52
..
Processing of Plastics
zyxwvu zyxwv zyx 309
(c) Matched Die Forming A variation of thermoforming which does not involve gas pressure or vacuum is matched die forming. The concept is very simple and is illustrated in Fig. 4.53. The plastic sheet is heated as described previously and is then sandwiched between two halves of a mould. Very precise detail can be reproduced using this thermoforming method but the moulds need to be more robust than for the more conventional process involving gas pressure or vacuum.
Sheet heating
Forming
Ejection
Fig. 4.53 Thermofonning between matched dies
(d) DualSheet Thennoforming This technique, also known as TwinSheet Forming, is a recent development. It is essentially a hybrid of blow moulding and thermofonning. Two heated sheets are placed between two mould halves and clamped as shown in Fig. 4.54. An inflation tube at the parting line then injects gas under pressure so that the sheets are forced out against the mould. Alternatively, a vacuum can be drawn between the plastic sheet and the mould in each half of the system. This technique has interesting possibilities for further development and will compete with blow moulding, injection moulding and rotational moulding in a number of market sectors. It can be noted that the two mould halves can be of different shapes and the two plastic sheets could be of different materials, provided a good weld can be obtained at the parting line.
zyx zyxwvu zyxw
4.4.1 Analysis of Thennoforming If a thermoplastic sheet is softened by heat and then pressure is applied to one of the sides so as to generate a freely blown surface, it will be found that the shape so formed has a uniform thickness. If this was the case during thermoforming, then a simple volume balance between the original sheet and the final shape could provide the wall thickness of the end product. Aihi = A f h f
(4.28)
where A = surface area, and h = wall thickness (‘i’ and ‘f’ refer to initial and final conditions).
310
zy
zyxwvu z Processing of Plastics
t
Air +
Heated sheets placed between open mould halves
Air
I
Inflation
Ejection
Fig. 4.54 Dual sheet forming
zyxwv zyxw
Example 4.7 A rectangular box 150 mm long, 100 mm wide and 60 mm deep is to be thermoformed from a flat sheet 150 mm x 100 mm x 2 mm. Estimate the average thickness of the walls of the final product if (a) conventional vacuum forming is used and (b) plug assisted moulding is used (the plug being 140 mm x 90 mm).
Solution (a) The initial volume of the sheet is given by
Aihj = 150 x 100 x 2 = 3 x lo4 mm3
The surface area of the final product is A j = (150 x 100) = 4.5
+ 2(100 x 60) + 2(150 x 60)
io4 mm2
Therefore, from equation (4.28)
3 x 104 = 0.67 mm hf = 4.5 x 104 (b) If plug assist is used then it could be assumed that over the area 140 mm x 90 mm, the wall thickness will remain at 2 mm. The volume of this part of the moulding will be Val= 140 x 90 x 2 = 2.52 x lo4 mm3
This would leave a volume of (3 x 1042.52 x lo4) to form the walls. The area of the walls is A , = ( 2 ~ 1 0 0 ~ 6 0 ) + ( 2 ~ 1 5 0 ~ 6 0 l ) O= 34 ~~ *
zyxwvu zyxw zyxwvu zyxwvuts zyxw zyx 31 1
Processing of Plastics
This ignores a small area in the base of the box, outside the edges of the plug. Hence, the thickness of the walls in this case would be (3 x
IO")  (2.52 x IO")
= 0.16 m n ~ 3 x 104 These calculations can give a useful first approximation of the dimensions of a thermoformed part. However, they will not be strictly accurate because in a real situation, when the plastic sheet is being stretched down into the cold mould it will freeze off at whatever thickness it has reached when it touches the mould. Consider the thermoforming of a plastic sheet of thickness, h,into a conical mould as shown in Fig. 4.55(a). At this moment in time, t, the plastic is in contact with the mould for a distance, S, and the remainder of the sheet is in the form of a spherical dome of radius, R, and thickness, h. From the geometry of the mould the radius is given by
h, =
R=
H  Ssina
(4.29)
sinatana D
Fig. 4.55 Analysis of thermo forming
Also the surface area, A, of the spherical bubble is given by A = 2zR2(1  COSCY)
+
(4.30)
At a subsequent time, ( t dt), the sheet will be formed to the shape shown in Fig. 4.55(b). The change in thickness of the sheet in this period of time may
312
zyxwvuts zyxwvu zyxwvu zy zyxw zy zyxw Processing of Plastics
be estimated by assuming that the volume remains constant.
2nR2(1  cos a ) h = 2n(R
+ dR)2(1  cos a)(h+ dh) + 2xrh dS sin a
Substitutingfor r(= R sina) and for R from (4.29) this equation may be reduced to the form sin a d s sin2a tan a (4.31) h 1  cosa (H  S sina)
This equation may be integrated with the boundary condition that h = hl at S = 0. As a result the thickness, h, at a distance, S, along the side of the conical mould is given by H  s sina secal (4.32) h=h1(
)
Now consider again the boundary condition referred to above. At the point when the softened sheet first enters the mould it forms part of a spherical bubble which does not touch the sides of the cone. The volume balance is therefore
2(0/2)2( 1  cos a)h1 sin2a
so.
hi =
sin2a *h 2( 1  cos a)
Making the substitution for hl in (4.32)
h= or
zyxwvu
2( 1  cos a) 1 +cosa
hlh=( 2
H
L
)[XI
(4.33)
This equation may also be used to calculate the wall thickness distribution in deep truncated cone shapes but note that its derivation is only valid up to the point when the spherical bubble touches the centre of the base. Thereafter the analysis involves a volume balance with freezingoff on the base and sides of the cone.
Example 4.8 A small flower pot as shown in Fig. 4.56 is to be thermoformed using negative forming from a flat plastic sheet 2.5 mm thick. If the diameter of the top of the pot is 70 mm, the diameter of the base is 45 mm and the depth is 67 mm estimate the wall thickness of the pot at a point 40 mm from the top. Calculate also the draw ratio for this moulding.
Processing of Plastics
313
zy
zyxwvut zyxwv zyxwvu zyxwvut Fig. 4.56 Thermofomed flower pot
Solution (a)
al= tan'
(E) = 79.4" 12.5
Using the terminology from Fig. 4.39(b)
zyxwv
H = 35tana = 187.6 mm From equation (4.33)
who =
( 1 + cos 79.C) ( 187.6  40)(E79.4)' = 0.203
2 187.6 h = 0.203 x 2.5 = 0.51 mm
(b) The drawratio for a thennoformed moulding is the ratio of the area of the product to the initial area of the sheet. In this case therefore Draw ratio =
R J [ ( R  r)2
 nJ[(35
+ h2](R+ r ) + nr2 RR~
 22.5)2 + 672](35+ 22.5) + ~ ( 2 2 . 5 ) ~ lr(35)2
= 3.6
4.5 Calendering Calendering is a method of producing plastic film and sheet by squeezing the plastic through the gap (or 'nip') between two counterrotating cylinders. The art of forming a sheet in this way can be traced to the paper, textile and metal industries. The first development of the technique for polymeric materials was in the middle 19th century when it was used for mixing additives into rubber. The subsequent application to plastics was not a complete success because the
3 14
zyxwvu zy zyxwvut Processing of Plastics
early machines did not have sufficient accuracy or control over such things as cylinder temperature and the gap between the rolls. Therefore acceptance of the technique as a viable production method was slow until the 1930s when special equipment was developed specifically for the new plastic materials. As well as being able to maintain accurately roll temperature in the region of 200°C these new machines had power assisted nip adjustment and the facility to adjust the rotational speed of each roll independently. These developments are still the main features of modem calendering equipment. Calenders vary in respect of the number of rolls and of the arrangement of the rolls relative to one another. One typical arrangement is shown in Fig. 4.57  the inverted Ltype. Although the calendering operation as illustrated here looks very straightforward it is not quite as simple as that. In the production plant a lot of ancillary equipment is needed in order to prepare the plastic material for the calender rolls and to handle the sheet after the calendering operation. A typical sheet production unit would start with premixing of the polymer, plasticiser, pigment, etc in a ribbon mixer followed by gelation of the premix in a Banbury Mixer and/or a short screw extruder. At various stages, strainers and metal detectors are used to remove any foreign matter. These preliminary operations result in a material with a doughlike consistency which is then supplied to the calender rolls for shaping into sheets.
1 Supply plastic
zyxwvut of

Sheet off to cooling drums and windup I
Fig. 4.57 'Qpical arrangement of calender rolls
However, even then the process is not complete. Since the hot plastic tends to cling to the calender rolls it is necessary to peel it off using a high speed roll of smaller diameter located as shown in Fig. 4.57. When the sheet leaves the calender it passes between embossing rolls and then on to cooling drums before being trimmed and stored on drums. For thin sheets the speed of the winding drum can be adjusted to control the drawdown. Outputs vary in the range 0.12 m/s depending on the sheet thickness.
Processing of Plastics
315
zyxwv
Calendering can achieve surprising accuracy on the thickness of a sheet. Typically the tolerance is f0.005 mm but to achieve this it is essential to have very close control over roll temperatures, speeds and proximity. In addition, the dimensions of the rolls must be very precise. The production of the rolls is akin to the manufacture of an injection moulding tool in the sense that very high machining skills are required. The particular features of a calender roll are a uniform specified surface finish, minimal eccentricity and a special barrel profile (‘crown’) to compensate for roll deflection under the very high presurres developed between the rolls. Since calendering is a method of producing sheedfilm it must be considered to be in direct competition with extrusion based processes. In general, film blowing and die extrusion methods are preferred for materials such as polyethylene, polypropylene and polystyrene but calendering has the major advantage of causing very little thermal degradation and so it is widely used for heat sensitive materials such as PVC.
zyxwv
4.5.1 Analysis of Calendering A detailed analysis of the flow of molten plastic between two rotating rolls is very complex but fortunately sufficient accuracy for many purposes can be achieved by using a simple Newtonian model. The assumptions made are that (a) (b) (c) (d)
zyxwvu zyxwvuts zyxw zyxwv zyxwv
the flow is steady and laminar the flow is isothermal the fluid is incompressible there is no slip between the fluid and the rolls.
If the clearance between the rolls is small in relation to their radius then at any section x the problem may be analysed as the flow between parallel plates at a distance h apart. The velocity profile at any section is thus made up of a drag flow component and a pressure flow component. For a fluid between two parallel plates, each moving at a velocity V d , the drag flow velocity is equal to V d . In the case of a calender with rolls of radius, R, rotating at a speed, N, the drag velocity will thus be given by 2nRN. The velocity component due to pressure flow between two parallel plates has already been determined in Section 4.2.3(b).
v
1 dP 2~ dx
  ( y 2 
 (h/212>
Therefore the total velocity at any section is given by
zyxwvuts zyxwvut zy zyxwv zyxw
zyx
3 16
Processing of Plastics
Considering unit width of the calender rolls the total throughput, Q , is given by hI2
Q=2/Vdy 0
=2 7 b d 0
1 dP + (3 2q dx
1
 (h/2)2) d y
(4.34)
Since the output is given by VdH then
(4.35)
zyx
dP From this it may be seen that  = 0 at h = H . dx To determine the shape of the pressure profile it is necessary to express h as a function of x. From the equation of a circle it may be seen that h = Ho
+ 2(R  (R2  x2)'I2)
(4.36)
However, in the analysis of calendering this equation is found to be difficult to work with and a useful approximation is obtained by expanding (R2  x2)'/* using the binomial series and retaining only the first two terms. This gives (4.37)
Therefore as shown earlier dP/dx will be zero at H=Ho
( L?) l+
x =f J H
 Ho)R'
(4.38)
This gives a pressure profile of the general shape shown in Fig. 4.58. The value of the maximum pressure may be obtained by rearranging (4.35) and substituting for h from (4.37)
 dx
(H0+;)3
(4.39)
Processing of Plastics
zyxwvu zy zyxwvutsrq 317
Pressure Drofile \
+
zyxw zyxwv zyxwvu zyx zy zyxw
Fig. 4.58 Melt flow between calender rolls
If this equation is integrated and the value of x from (4.38) substituted then the maximum pressure may be obtained as P,,
=
HO
(4.40) J(H H o w (4.41) where w= H Example 4.9 A calender having rolls of diameter 0.4 m produces plastic sheet 2 m wide at the rate of 1300 kghour. If the nip between rolls is 10 mm and the exit velocity of the sheet is 0.01 m / s estimate the position and magnitude of the maximum pressure. The density of the material is 1400 kg/m3 and its viscosity is 104 Ns/m2.
Solution Flow rate, Q = 1300 kg/hour = 0.258 x
m3/s
Q = HWVd where W = width of sheet
but
0.258 x = 12.9 mm 2 x 0.01 The distance upstream of the nip at which the pressure is a maximum is given by equation (4.38)
so
H =
x = d(12.9  10)200 = 24.08 ~III
Also from (4.37) Pmax
=
3 x 104 x 0.01 {(2 x 1.865) 0.13[1.865 io x 103
= 96 kNim2
+ (4.45)(0.494)1)
z zyxwvut
318
Processing of Plastics
4.6 Rotational Moulding
Rotational moulding, like blow moulding, is used to produce hollow plastic articles. However, the principles in each method are quite different. In rotational moulding a carefully weighed charge of plastic powder is placed in one half of a metal mould. The mould halves are then clamped together and heated in an oven. During the heating stage the mould is rotated about two axes at right angles to each other. After a time the plastic will be sufficiently softened to form a homogeneous layer on the surface of the mould. The latter is then cooled while still being rotated. The final stage is to take the moulded article from the mould. The process was originally developed in the 1940s for use with vinyl plastisols in liquid form. It was not until the 1950s that polyethylene powders were successfully moulded in this way. Nowadays a range of materials such as nylon, polycarbonate, ABS, high impact polystyrene and polypropylene can be moulded but by far the most common material is polyethylene. The process is attractive for a number of reasons. Firstly, since it is a low pressure process the moulds are generally simple and relatively inexpensive. Also the moulded articles can have a very uniform thickness, can contain reinforcement, are virtually strain free and their surface can be textured if desired. The use of this moulding method is growing steadily because although the cycle times are slow compared with injection or blow moulding, it can produce very large, thick walled articles which could not be produced economically by any other technique. Wall thicknesses of 10 mm are not a problem for rotationally moulded articles. There is a variety of ways in which the cycle of events described above may be carried out. For example, in some cases (particularly for very large articles) the whole process takes place in one oven. However, a more common setup is illustrated in Fig. 4.59. The mould is on the end of an arm which first carries the cold mould containing the powder into a heated oven. During heating the mould rotates about the arm (major) axis and also about its own (minor) axis (see Fig. 4.60). After a preset time in the oven the arm brings the mould into a cooling chamber. The rate of cooling is very important. Clearly, fast cooling is desirable for economic reasons but this may cause problems such as warping. Normally therefore the mould is initially cooled using blown air and this is followed by a water spray. The rate of cooling has such a major effect on product quality that even the direction of the air jets on the mould during the initial gradual cooling stage can decide the success or otherwise of the process. As shown in Fig. 4.59 there are normally three arms (mould holders) in a complete system so that as one is being heated another is being cooled and so on. In many machines the arms are fixed rigidly together and so the slowest event (heating, cooling or charging/discharging) dictates when the moulds progress to the next station. In some modem machines, the arms are
zyxwv
zy
Processing of Plastics
zyxwvu zyxw zyxwv 319
independent so that if cooling is completed then that arm can leave the cooling bay whilst the other arms remain in position. It is important to realise that rotational moulding is not a centrifugal casting technique. The rotational speeds are generally below 20 rev/min with the ratio of speeds about the major and minor axes being typically 4 to 1. Also since all mould surfaces are not equidistant from the centre of rotation any centrifugal forces generated would tend to cause large variations in wall thickness. In fact in order to ensure uniformity of all thickness it is normal design practice to arrange that the point of intersection of the major and minor axis does not coincide with the centroid of the mould. The heating of rotational moulds may be achieved using infrared, hot liquid, open gas flame or hotair convection. However, the latter method is the most common. The oven temperature is usually in the range 250450°C and since the mould is cool when it enters the oven it takes a certain time to get up to a temperature which will melt the plastic. This time may be estimated as follows. When the mould is placed in the heated oven, the heat input (or loss) per unit time must be equal to the change in internal energy of the material (in this case the mould).
zyxwvutsr zyxwv zyxw (4.42)
where h A To T,
and
is the convective heat transfer coefficient is the surface area of mould is the temperature of the oven is the temperature of the mould at time t p is the density of the mould material C , is the specific heat of the mould material V is the volume of the walls of the mould t is time
Rearranging this equation and integrating then
(4.43) where Ti is the initial temperature of the mould and fi is the surface area to volume ratio ( A I V ) . This equation suggests that there is an exponential rise in mould temperature when it enters the oven, and in practice this is often found to be the case.
320
z zyxw Processing of Plastics
CharQino area Powder
halves

Cooling chamber
Fig. 4.59
’I)pical rotational moulding process
zyxw
CP Minor axis
‘Oft set arm”
zyxw
Fig.4.60 meal ‘offset arm’ rotation
zy zyxwvut zyxwvuts zyxwv zyxwv zyx zyxw
Processing of Plastics
321
Fig. 4.61 illustrates typical temperature profiles during the rotational moulding of polyethylene. With typical values of oven temperatures and data for an aluminium mould
To = 300"C,
Ti = 30°C,
h = 22 W/m2K
T , = 20°C
C, = 917 J k g K,
p = 2700 kg/m3
350

T, Inside surface of mould
300
T,  Air inside mould
250
E E I
200
ls0 100 50
0 0
5
10
15
20 25 Time (min)
35
30
40
zy 45
Fig. 4.61 Temperature profiles during rotational moulding
then for an aluminium cube mould 330 mm side and 6 mm thick, as was used to produce Fig. 4.61 then T o  Tt 2700 x 917 330  220 r=*loge{}= T o  Ti lo00 x 22 loge 330  30 Bh r = 1.9 minutes
{
}
For a steel mould of the same dimensions and thickness, a quick calculation (h = 11 W/m2K, C , = 480 J k g K and p = 7850 kg/m3) shows that the steel mould would take three times longer to heat up. However, in practice, steel moulds are less than a third of the thickness of aluminium. Therefore, although aluminium has a better thermal conductivity, steel moulds tend to heat up more quickly because they are thinner. It is important to note that the above calculation is an approximation for the time taken to heat the mould to any desired temperature. Fig. 4.61 shows that in practice it takes considerably longer for the mould temperature to get to 220°C.This is because although initially the mould temperature is rising at the rate predicted in the above calculation, once the plastic starts to melt, it absorbs a significant amount of the thermal energy input.
322
zyxwvuts zyxwvu zyxw zyxwv zyxwv zy Processing of Plastics
Fig. 4.61 illustrates that the mould temperature is quite different from the set oven temperature (330°C) or indeed the actual oven temperature, throughout the moulding cycle. An even more important observation is that in order to control the rotational moulding process it is desirable to monitor the temperature of the air inside the mould. This is possible because there is normally a vent tube through the mould wall in order to ensure equal pressures inside and outside the mould. This vent tube provides an easy access for a thermocouple to measure the internal air temperature. The internal air temperature characteristic has a unique shape which shows clearly what is happening at all stages throughout the process. Up to point A in Fig. 4.61 there is simply powder tumbling about inside the mould. At point A the mould has become sufficiently hot that plastic starts to melt and stick to the mould. The melting process absorbs energy and so over the region AB, the internal air temperature rises less quickly. It may also be seen that the temperature of the mould now starts to rise less quickly. At B all the plastic has melted and so a larger proportion of the thermal energy input goes to heating the inner air. This temperature rises more rapidly again, at a rate similar to that in the initial phase of the process. Over the region BC the melt is effectively sintering because at B it is a powdery mass loosely bonded together whereas at C it has become a uniform melt. The value of temperature at C is very important because if the oven period is too short, then the material will not have sintered properly and there will be an excess of pinholes. These are caused where the powder particles have fused together and trapped a pocket of air. If the oven period is too long then the pinholes will all have disappeared but thermaYoxidative degradation will have started at the inner surface of the moulding. Extensive tests have shown that this is a source of brittleness in the mouldings and so the correct choice of temperature at C is a very important quality control parameter. For most grades of polyethylene the optimum temperature is in the region of 200°C 43°C. Once the mould is removed from the oven the mould starts to cool at a rate determined by the type of cooling  blown air (slow) or water spray (fast). There may be a overshoot in the internal air temperature due to the thermal momentum of the melt. This overshoot will depend on the wall thickness of the plastic product. In Fig. 4.61 it may be seen that the inner air temperature continues to rise for several minutes after the mould has been taken out of the oven (at about 13.5 minutes). During cooling, a point D is reached where the internal air temperature decreases less quickly for a period. This represents the solidification of the plastic and because this process is exothermic, the inner air cannot cool so quickly. Once solidification is complete, the inner air cools more rapidly again. Another kink (point E) may appear in this cooling curve and, if so, it represents the point where the moulding has separated from the mould wall. In practice this is an important point to keep consistent because it affects shrinkage, warpage,
zyxwvu zyxwvu
Processing of Plastics
323
etc in the final product. Once the moulding separates from the mould, it will cool more slowly and will tend to be more crystalline, have greater shrinkage and lower impact strength. Developments in rotational moulding are continuing, with the ever increasing use of features such as (i) mould pressurisation (to consolidate the melt, remove pinholes, reduce cycle times and provide more consistent mould release), (ii) internal heatingkooling (to increase cycle times and reduce warpage effects).
In overall terms the disadvantages of rotational moulding are its relative slowness and the limited choice of plastics which are commercially available in powder form with the correct additive package. However, the advantages of rotational moulding in terms of stressfree moulding, low mould costs, fast lead times and easy control over wall thickness distribution (relative to blow moulding) means that currently rotational moulding is the fastest growing sector of the plastics processing industry. s p i c a l annual growth rates are between 10 and 12% p.a. 4.6.1 Slush Moulding This is a method for making hollow articles using liquid plastics, particularly PVC plastisols. A shelllike mould is heated to a predetermined temperature (typically 130°C for plastisols) and the liquid is then poured into the mould to completely fill it. A period of time is allowed to elapse until the required thickness of plastic gels. The excess liquid is then poured out and the plastic skin remaining in the mould is cured in an oven. The moulding is then taken from the mould. It should be noted that when the plastisol liquid gels it has sufficient strength to remain in position on the inside surface of the mould. However, it has insufficient tear strength to be useful and so it has to go through the higher temperature curing stage to provide the necessary toughness and strength in the endproduct. The mould is not rotated during slush moulding. 4.7 Compression Moulding
zyxwv zyxw
Compression moulding is one of the most common methods used to produce articles from thermosetting plastics. The process can also be used for thermoplastics but this is less common  the most familiar example is the production of LP records. The moulding operation as used for thermosets is illustrated in Fig. 4.62. A preweighed charge of partially polymerised thermoset is placed in the lower half of a heated mould and the upper half is then forced down. This causes the material to be squeezed out to take the shape of the mould. The application of the heat and pressure accelerates the polymerisation of the
324
zyxwvuts zy Processing of Plastics
Pressure
zyxwvu zyxw zyxw zyx z zyxwv Houldikg
Fig. 4.62 Principle of compression moulding
thermoset and once the crosslinking (‘curing’) is completed the article is solid and may be ejected while still very hot. Mould temperatures are usually in the range of 130200°C.Cycle times may be long (possibly several minutes) so it is desirable to have multicavity moulds to increase production rates. As a result, moulds usually have a large projected area so the closing force needed could be in the region of 100500 tonnes to give the 725 MN/m2 cavity pressure needed. It should also k noted that compression moulding is also used for Dough Moulding Compounds (DMC)  these will be considered in Section 4.10.2 During compression moulding, the charge of material may be put into the mould either as a powder or a preformed ‘cake’. In both cases the material is preheated to reduce the temperature difference between it and the mould. If the material is at a uniform temperature in the mould then the process may be analysed as follows. Consider a ‘cake’ of moulding resin between the compression platens as shown in Fig. 4.63. When a constant force, F,is applied to the upper platen the resin flows as a result of a pressure gradient. If the flow is assumed Newtonian then the pressure flow equation derived in Section 4.2.3 may be used 1 flow rate, Q p = TH3 (4.6) 1217 dz For the annular element of radius, r, in Fig. 4.63 it is more convenient to use cylindrical coordinates so this equation may be rewritten as
(E)
1 dP eP= () .( 2 n r ) ~ 3 1217 d r
Now if the top platen moves down by a distance, dH, the volume displaced is (nr2dH)and the volume flow rate is nr2(dH/dt). Therefore
nr2
(f)1( E ) =
1217
dr
(2nr)~3
Processing of Plastics
zyxwv
zyxwvu zy 325
I
Force, F
I
/of
Annular element fluid
zyxw zy zy
Fig. 4.63 Analysis of compression moulding
12q .  =dH H 3 dt
2dP (4.44) r dr This simple differential equation is separable and so each side may be solved in turn. 2 dP A where A = f ( H ) Let r dr P
so
j d p=
zyxw
4
r
Jrdr
R
0
A 4
P = (r2  R ~ )
or
Now the force on the element is 2rcrdr(P) so the total force, F, is given by integrating across the platen surface. F =]2nr
(a)
RAR4
(r2  R2)dr = 
0
This may be rearranged to give
where V = xR2H Substituting for A in (4.44) 8rcFH2 12qdH  V2
H 3 dt
8
326
zyxwvuts zyxwvu zyxw zyx zyxw zyxw Processing of Plastics
Jq H
t
so
 J w 2nF dt=
H
0
Ho
Since Ho >> H then (l/H;) may be neglected. As a result the compaction force F, is given by
zyxwv (4.45)
where H is the platen separation at time, t .
Example 4.10 A circular plate with a diameter of 0.3 m is to be compression moulded from phenol formaldehyde. If the preform is cylindrical with a diameter of 50 mm and a depth of 36 mm estimate the platen force needed to produce the plate in 10 seconds. The viscosity of the phenol may be taken as lo3 Ns/m2. Solution Volume,
V=n
so
H=lmm
(;)2
x 36=n
(7)’H
3qV2 3 x lo3 x (n x 625 x 36)’ From (4.45) F = = 59.6 kN 8ntH4  106 x 8n x io x (1)4
4.8 Transfer Moulding Transfer moulding is similar to compression moulding except that instead of the moulding material being pressurized in the cavity, it is pressurized in a separate chamber and then forced through an opening and into a closed mould. Transfer moulds usually have multicavities as shown in Fig. 4.64. The advantages of transfer moulding are that the preheating of the material and injection through a narrow orifice improves the temperature distribution in the material and accelerates the crosslinking reaction. As a result the cycle times are reduced and there is less distortion of the mouldings. The improved flow of the material also means that more intricate shapes can be produced. The success of transfer moulding prompted further developments in this area and clearly it was only a relatively small step to an injection moulding process for thermosets as described in Section 4.3.10.
327
Processing of Plastics
zy
zyxwvutsrqp zyxw
(a) pretorm in position
(b) Melerial forced into cavities
Fig. 4.64 Transfer moulding of thermosetting materials
4.9 Processing Reinforced Thermoplastics Fibre reinforced thermoplastics can be processed using most of the conventional thermoplastic processing methods described earlier. Extrusion, rotational moulding, blow moulding and thermoforming of short fibre reinforced thermoplastics are all possible, but the most important commercial technique is injection moulding. In most respects this process is similar to the moulding of unreinforced thermoplastics but there are a number of important differences. For example the melt viscosity of a reinforced plastic is generally higher than the unreinforced material. As a result the injection pressures need to be higher, by up to 80% in some cases. In addition the cycle times are generally lower because the greater stiffness of the material allows it to be ejected from the mould at a higher temperature than normal. However, the increased stiffness can also hamper ejection from the mould so it is important to have adequate taper on side walls of the cavity and a sufficient number of strategically placed ejector pins. Where possible a reciprocating screw machine is preferred to a plunger machine because of the better mixing, homogenisation, metering and temperature control of the melt. However, particular attention needs to be paid to such things as screw speed and back pressure because these will tend to break up the fibres and thus affect the mechanical properties of the mouldings. A practical difficulty which arises during injection moulding of reinforced plastics is the increased wear of the moulding machine and mould due to the abrasive nature of the fibres. However, if hardened tool steels are used in the manufacture of screws, barrels and mould cavities then the problem may be negligible. An inherent problem with all of the above moulding methods is that they must, by their nature, use short fibres (typically 0.20.4 mm long). As a result the full potential of the reinforcing fibres is not realised (see Section 2.8.5). In recent years therefore, there have been a number of developments in reinforced
zyx
328
zyxwvut zyxwv Processing of Plastics
thermoplastics to try to overcome these problems. One approach has been to produce continuous fibre tapes or mats which can be embedded in a thermoplastic matrix. The best known materials of this type are the Aromatic Polymer Composites (APC) and the glass mat reinforced thermoplastics (GMT). One of the most interesting of these consists of unidirectional carbon fibres in a matrix of polyetheretherketone (PEEK).The material comes in the form of a wide tape which may be arranged in layers in one half of a mould to align the unidirectional fibres in the desired directions. The assembly is then pressurised between the two matched halves of the heated mould. The result is a laminated thermoplastic composite containing continuous fibres aligned to give maximum strength and stiffness in the desired directions. Another recent development has been the arrival of special injection moulding grades of thermoplastics containing long fibres. At the granule production stage the thermoplastic lace contains continuous fibres and to achieve this it is produced by pultrusion (see Section 4.10.3) rather than the conventional compounding extruder. The result is that the granules contain fibres of the same length as the granule (210 mm). These long fibres give better product performance although injection moulding machine modifications may be necessary to prevent fibre damage and reduce undesirable fibre orientation effects in the mould.
4.10 Processing Reinforced Thermosets There is a variety of ways in which fibre reinforcement may be introduced into thermosetting materials and as a result there is a range of different methods used to process these materials. In many cases the reinforcement is introduced during the fabrication process so that its extent can be controlled by the moulder. Before looking at the possible manufacturing methods for fibre reinforced thermosetting articles it is worth considering the semantics of fibre technology. Because of their fibre form, reinforcing materials have borrowed some of their terminology from the textile industry.
zyxw zyxwv
Filament This is a single fibre which is continuous or at least very long compared with its diameter.
Yarn or Roving Continuous bundle of filaments generally fewer than 10,OOO in number.
Tow A large bundle of fibres generally 10,OOO or more, not twisted.
Fabric, Cloth or Mat Woven strands of filament. The weave pattern used depends on the flexibility and balance of strength properties required in the warp and fill directions. Fig. 4.65 shows a plain weave in which the strength is uniform in both directions. The warp direction refers to the direction parallel to
Processing of Plastics
zyxwvu zy zyxwvuts 329
A W a r p ends
Fill ends
zyxw
Plain WeaveIn this construction. one warp end is repetitively woven over one till yam and under the next. It is the firmest. mort stabte construction,which provides for porosity and minimum slippage. Strength is uniformin both directions.
Fig. 4.65 Plain weave fibre fabric
the length of the fabric. Fabrics are usually designated in terms of the number of yams of filament per unit length of warp and fill direction.
zyxwv
Chopped Fibres These may be subdivided as follows Milled Fibres: These are finely ground or milled fibres. Lengths range from 30 to 3000 microns and the fibre (WD)ratio is typically about 30. Fibres in this form are popular for closed mould manufacturing methods such as injection moulding. Short Chopped Fibres: These are fibres with lengths up to about 6 mm. The fibre (WD)ratio is typically about 800. They are more expensive than milled fibres but provide better strength and stiffness enhancement. Long Chopped Fibres: These are chopped fibres with lengths up to 50 mm. They are used mainly in the manufacture of SMC and DMC (see Section 4.10.2).
Chopped Strand Mat This consists of strands of long chopped fibres deposited randomly in the form of a mat. The strands are held together by a resinous binder.
zyxwvutsr
Manufacturing Methods The methods used for manufacturing articles using fibre reinforced thermosets are almost as varied as the number of material variations that exist. They can, however, be divided into three main categories. These are manual, semiautomatic and automatic. The Manual processes cover methods such as hand layup, sprayup, pressure bag and autoclave moulding.
330
zyxwvu zyxwvut zyxw zyx Processing of Plastics
The SemiAutomatic processes include processes such as cold pressing, hot pressing, compression moulding of SMC and DMC, resin injection. The Automatic processes are those such as pultrusion, filament winding, centrifugal casting and injection moulding. Qpical market shares for the different methods are shown in Fig. 4.66. Injection moulding
Contact moulding (hand layup   > ;prayup)
zyx
Continuous lamination
ilament winding r
Pressure forming
niM
Pultrusion
Fig. 4.66 npical market shares for composite moulding methods in Europe
4.10.1 Manual Processing Methods (a) Hand LayUp: This method is by far the most widely used processing method for fibre reinforced materials. In the UK it takes up about 40% of the FRP market. Its major advantage is that it is a very simple process so that very little special equipment is needed and the moulds may be made from plaster, wood, sheet metal or even FRP. The first step is to coat the mould with a release agent to prevent the moulding sticking to it. This is followed by a thin layer (approximately 0.30.4 mm) of pure resin (called a gelcoat) which has a number of functions. Firstly it conceals the irregular mesh pattern of the fibres and this improves the appearance of the product when it is taken from the mould. Secondly, and probably most important, it protects the reinforcement from attack by moisture which would tend to break down the fibrehesin interface. A tissue mat may be used on occasions to back up the gelcoat. This improves the impact resistance of the surface and also conceals the coarse texture of the reinforcement. However, it is relatively expensive and is only used if considered absolutely necessary. When the gelcoat has been given time to partially cure the main reinforcement is applied. Initially a coat of resin (unsaturated polyester is the most common) is brushed on and this is followed by layers of tailored glass mat positioned by hand. As shown in Fig. 4.67 a roller is then used to consolidate the mat and remove any trapped air. The advantage of this technique is that the strength and stiffness of the composite can be controlled by building up the thickness with further layers of mat and resin as desired. Curing takes place at room temperature but heat is sometimes applied to accelerate this. Ideally any trimming should be carried out before the curing is complete because the
Processing of Plastics
zyxwv zyxwvut 33 1
Resin brushed on
cures inair
Layers of resin ond fibres (a1 Basic hand layup method
Flexible bag
Mould
zyxwvu zyxwvuts
/
IbIVacuum bag
Mould VIng .
‘Mwld
(cl Pressure bog
zyxw zyx zy
Fig. 4.67 Hand layup techniques
material will still be sufficiently soft for knives or shears to be used. After curing, special cutting wheels may be needed. Variations on this basic process are (i) vacuum bug moulding and (ii) pressure bug moulding. In the former process a flexible bag (frequently rubber) is clamped over the layup in the mould and a vacuum is applied between the moulding and the bag. This sucks the bag on to the moulding to consolidate the layers of reinforcement and resin. It also squeezes out trapped air and excess resin. The latter process is similar in principle except that pressure is applied above the bag instead of a vacuum below it. The techniques are illustrated in Fig. 4.67(b) and (c). (b) SprayUp: In this process, the preparatory stages are similar to the previous method but instead of using glass mats the reinforcement is applied using a spray gun. Roving is fed to a chopper unit and the chopped strands are sprayed on to the mould simultaneously with the resin (see Fig. 4.68). The thickness of the moulding (and hence the strength) can easily be built up in sections likely to be highly stressed. However, the success of the method depends to a large extent on the skill of the operator since he controls the overall thickness of the composite and also the glasshesin ratio.
332
zyxwvuz Processing of Plastics
Chopped fibre
Mould
zyxwvu
’
‘ Moulding
Fig. 4.68 Sprayup technique
(c) Autoclave Moulding: In order to produce high quality, high precision mouldings for the aerospace industries, for example, it is necessary to have strict control over fibre alignment and consolidation of the fibres in the matrix. To achieve this, fabric ‘prepregs’ (i.e. a fabric consisting of woven fibre yarns preimpregnated with the matrix material) are carefully arranged in layers in an open mould. The arrangement of the layers will determine the degree of anisotropy in the moulded article. A typical layer arrangement is shown in Fig. 4.69(a). The prepreg stack is then covered with a series of bleeder and breather sheets, as shown in Fig. 4.69(b) and finally with a flexible vacuum bag. When the air is extracted from between the flexible bag and the prepreg stack, the latter will be squeezed tightly on to the mould. The whole assembly is then transferred to a very large oven (autoclave) for curing.
Pwous releose
Fig. 4.69 Diagramatic cross section of a bagged layup
4.10.2 SemiAutomatic Processing Methods (a) Cold Press Moulding: The basis of this process is to utilise pressure applied to two unheated halves of a mould to disperse resin throughout a
z
Processing of Plastics
zy zyxwv 333
prepared fabric stack placed in the mould. The typical procedure is as follows. Release agent and gelcoat are applied to the mould surfaces and the fibre fabric is laid into the lower part of the open mould. The activated resin is then poured on top of the mat and when the mould is closed thb resin spreads throughout the reinforcement. High pressures are not necessary as the process relies on squeezing the resin throughout the reinforcement rather than forcing the composite into shape. A typical value of cycle time is about 1015 minutes compared with several hours for hand layup methods. The process is illustrated in Fig. 4.70.
zyx zyxwvutsrqpon zyxwvutsrq cantrol thickness
lo1 would with gel coat and reinforced
I bl Mould opend and moulding released
layers pnpositioned
Fig. 4.70 Basic cold press moulding process
zyxwvut
(b) Hot Press Mouldings: In this type of moulding the curing of the reinforced plastic is accelerated by the use of heat (2:18OoC) and pressure (15 MN/m2). The general heading of Hot Press Moulding includes both preform moulding and compression moulding. (i) Prefom Moulding: This technique is particularly suitable for mass production and/or more complex shapes. There are two distinct stages. In the first a preform is made by, for example, spraying chopped fibres on to a perforated metal screen which has the general shape of the article to be moulded. The fibres are held on the screen by suction applied behind it (see Fig. 4.71). A resin binder is then sprayed on the mat and the resulting preform is taken from the screen and cured in an oven at about 150°C for several minutes. Other methods by which the preform can be made include tailoring a continuous fibre fabric to shape and using tape to hold it together. The preform is then transferred to the lower half of the heated mould and the activated resin poured on top. The upper half of the mould is then brought into position to press the composite into shape. The cure time in the mould depends on the temperature, varying typically from 1 minute at 150°C to 10 minutes at 80°C. If the mould was suitably prepared with release agent the moulding can then
334
zyxwvuts zy Processing of Plastics
Y
P
P
fibres l Y of
Supply of
,' p,rotated
(b)
zyx
Heated mould
Exhaust fan (a)
\
\
\
zyxw zyx
Preform \, transferred \ to mould ,,\
63
/p
zyxw
Fig. 4.71 Reform moulding of GFRP
be ejected easily. This method would not normally be considered for short production runs because the mould costs are high. (ii) Compression Moulding (see also Section 4.7): Sheet Moulding Compounds: SMC is supplied as a pliable sheet which consists of a mixture of chopped strand mat or chopped fibres (25% by weight) preimpregnated with resin, fillers, catalyst and pigment. It is ready for moulding and so is simply placed between the halves of the heated mould. The application of pressure then forces the sheet to take up the contours of the mould. The beauty of the method is that the moulding is done 'dry' i.e. it is not necessary to pour on resins. Fig. 4.72 illustrates a typical method used to manufacture SMC material. Dough Moulding Compounds: DMC (also known as BMC  Bulk Moulding Compound) is supplied as a dough or rope and is a mixture of chopped strands (20% by weight) with resin, catalyst and pigment. It flows readily and so may be formed into shape by compression or transfer moulding techniques. In compression moulding the charge of dough may be placed in the lower half of the heated mould, in a similar fashion to that illustrated in Fig. 4.50(b) although it is generally wise to preform it to the approximate shape of the cavity. When the mould is closed, pressure is applied causing the DMC to flow in all sections of the cavity. Curing generally takes a couple of minutes for mould temperatures in the region of 12W160"C although clearly this also depends on the section thickness. In general, SMC moulds less well than DMC on intricate shapes but it is particularly suitable for large shelllike mouldings  automotive parts such as
zyxw
Processing of Plastics
zyxwvu zy 335
Canier film
Continuous
zyxw zyx
Take  up roll for SMC
Canier film
Fig. 4.72 Manufacture of SMC material
body panels and fascia panels are ideal application areas. An engine inlet manifold manufactured from SMC has recently been developed in the UK. DMC finds its applications in the more complicated shapes such as business machine housings, electric drill bodies, etc. In France, a special moulding method, called ZMC, but based on DMC moulding concepts has been developed. Its most famous application to date is the rear door of the Citroen BX saloon and the process is currently under active consideration for the rear door of a VW saloon car. Injection moulding of DMC is also becoming common for intricately shaped articles (see Section 4.3.10). Other types of compression moulding and stamp forming used for continuous fibre reinforced composites are illustrated in Fig. 4.73. (c) Resin Injection: This is a cold mould process using relatively low pressures (approximately 450 kN/m2). The mould surfaces are prepared with release agent and gelcoat before the reinforcing mat is arranged in the lower half of the mould. The upper half is then clamped in position and the activated resin is injected under pressure into the mould cavity. The advantage of this type of production method is that it reduces the level of skill needed by the operator because the quality of the mould will determine the thickness distribution in the moulded article (see Fig. 4.74).In recent times there has been a growing use of preformed fabric shells in the resin injection process. The preform is produced
336
zyxwvuts zy zyxwvu & Processing of Plastics
Heater
Laminate
Laminate Hot compression moulding
1
zyxwvu
20
Cold muid stamp f0llnlng process
3D
Fig. 4.73 Other types of compression moulding and stamp forming
zyxwv
using one of the methods described above and this is placed in the mould. This improves the quality and consistency of the product and reinforcements varying from chopped strand mat to close weave fabric in glass, aramid, carbon or hybrids of these may be used. It is possible, with care, to achieve reinforcement loadings in the order of 65%. (d) Vacuum Injection: This is a development of resin injection in which a vacuum is used to draw resin throughout the reinforcement. It overcomes the
Processing of Plastics
zyxwvu zy 337
zyxwvutsr Resin feed pipes
Mould clamping screws
\
Resin injection
Reinforced material in mould cavity
Fig. 4.74 Resin injection process
problem of voids in the residfibre laminate and offers faster cycle times with greater uniformity of product. 4.10.3 Automatic Pr~~esses (a) Filament Winding: In this method, continuous strands of reinforcement are used to gain maximum benefit from the fibre strength. In a typical process rovings or single strands are passed through a resin bath and then wound on to a rotating mandrel. By arranging for the fibres to traverse the mandrel at a controlled and/or programmed manner, as illustrated in Fig. 4.75, it is possible to lay down the reinforcement in any desired fashion. This enables very high strengths to be achieved and is particularly suited to pressure vessels where reinforcement in the highly stressed hoop direction is important. In the past a limitation on this process was that it tended to be restricted to shapes which were symmetrical about an axis of rotation and from which the mandrel could be easily extracted. However, in recent years there have been major advances through the use of collapsible or expendable cores and in particular through the development of computercontrolled winding equipment. The latter has opened the door to a whole new range of products which can be filament wound  for example, spaceframe structures. Braiding machines for complex shapes are shown in Fig. 4.76. (b) Centrifugal Casting: This method is used for cylindrical products which can be rotated about their longitudinal axis. Resin and fibres are introduced into the rotating mould/mandrel and are thrown out against the mould surface. The method is particularly suited to long tubular structures which can have a slight taper e.g. street light columns, telegraph poles, pylons, etc.
zy
zyxwvu
(c) Pultrusion: This is a continuous production method similar in concept to extrusion. Woven fibre mats and/or rovings are drawn through a resin bath and then through a die to form some desired shape (for example a ‘plank’
338
zyxwvuts zy Processing of Plastics
Rotating mandrel
zyxw
Fig. 4.75 Filament winding of fibre composites
zyxwvu
zyxwv
Fig. 4.76 ' b o types of filament winding
as illustrated in Fig. 4.77). The profiled shape emerges from the die and then passes through a tunnel oven to accelerate the curing of the resin. The pultruded composite is eventually cut to length for storage. A wide range of pultruded shapes may be produced  U channels, I beams, aerofoil shapes, etc.
(d) Injection Moulding: The injection moulding process can also be used for fibre reinforced thermoplastics and thermosets, for example DMC materials. This offers considerable advantages over compression moulding due to the higher production speeds, more accurate metering and lower product costs which can be achieved. The injection moulding process for thermosets has
Processing of Plastics
339
zyxwvu zyxw zyxwvutsrqp zyxwvuts zyxwvut zyxwvut Fig. 4.77 Pultrusion process
already been dealt with in Section 4.3.8. See also the section on Reaction Injection Moulding (RIM) since this offers the opportunity to incorporate fibres.
Bibliography
Fisher, E.G, Extrusion of Plastics, NewnesButterworth, 1976. Schenkel, G, Plastics Extrusion Technology and Practice, Iliffe, 1966. Fisher, E.G, Blow Moulding of Plastics, Iliffe, 1971. Rubin, I, Injection MouldingTheory and Practice, Wiley, 1972. HolmesWalker, W.A. Polymer Conversion, Applied Science Publishers, 1975. Bown, J, Injection Moulding of Plastic Covonents, McGrawHill, 1979. Dym, J.B, Injecrion Moulds and Moulding, Van Nostrand Rheinhold, 1979. Pye, R.G.W, Injection Mould Design, George Godwin, 1978. Elden, R.A. and Swann, A.D, Calendering ofPlastics, Plastics Institute Monograph, Iliffe, 1971. Rosenzweig, N., Marks, M., and Tadmar, Z., Wall Thickness Distribution in Thennoforming Polym. Eng. Sci. October 1979 Vol 19 No. 13 pp 946950. Parker, F.J, The Status of Thermoset Injection Moulding Today, Progress in Rubber and Plastic Technology. October 1985, vol 1, No 4, pp 2259. Whelm, A and Brydson, J.A. Developments with Thennosetting P h t i c s App. Sci. Pub. London 1975.
Monk, J.F. Thennosetting Plastics  Practical Moulding Technology, George Godwin, London 1981.
zy
Rosato, D.V. ed. Rosato. D.V. (ed.) Blow Moulding Handbook,Hanser, Munich (1989). Hepbum, C. Polyurethane Elastomers (ch 6RIM) Applied Science Publishers, London (1982). Martin, J., Pultrusion Ch 3 in ‘Plastics Product Design Handbook  B’ ed by E. Miller, Dekker Inc, New York (1983). Titow, W.V. and Lanham, B.J, Reinforced Thermoplastics, Applied Science Publisher, 1975. Penn, W.S. GRP Technology,Maclaren, 1966. Beck, R.D, Plastic Product Design, Van Nostrand Reinhold Co. 1980. S c h w a , S.S.and Goodman, S.H.Plastic Marerials and Processes, Van Nostrand, New York, 1982.
Crawford, R.J. Rotational Moulding of Plastics, Research Studies Press 2nd edition (1996).
340
zyxwvu zy zyxwvut zyx Processing of Plastics
Rosato, D.V. and Rosato, D.V. Injection Molding Handbook, 2nd edn, Chapman and Hall, New York (1995). Stevens, M.J. and Covas, J.A. Exlruder Principles and Operation, 2nd edn, Chapman and Hall, London (1995). Michaeli, W. Extrusion Dies, Hanser, Munich (1984). Baird, D.G. and Collias, D.I. Polymer Processing, ButterworthHeinemann,Newton, USA (1995). Michaeli, W. Polymer Processing, Hanser, Munich (1992). Lee, N. (ed.), Plasric Blow Moulding Handbook, Van Nostrand Reinhold, New York (1990). Throne, J.L. Technology of Thennofonning, Hanser, Munich (19%). Florian, J. Practical Thennoforming, Marcel Dekker, New York (1987). Boussinesq, M.J., J. Math Pures et Appl., 2, 13 (1868) pp. 377424. Meng Hou, Lin Ye and YiuWing Mai, Advances in processing of continuous fibre reinforced composites Plastics, Rubber and Composites Proc. and Appl., 23, 5 (1995) pp. 279292. Mitchell, P. (ed.) Tool and Manufacturing Engineers Handbook, Vol 8, 4th edition, Soc. Man. Eng., Michigan (1996).
zyxwvu zyx
Questions 4.1 In a particular extruder screw the channel depth is 2.4 mm, the screw diameter is 50 mm, the screw speed is 100 rev/min, the flight angle is 17' 42' and the pressure varies linearly over the screw length of lo00 mm from zero at entry to 20 MN/m* at the die entry. Estimate
(a) the drag flow (b) the pressure flow (c) the total flow. The plastic has a viscosity of 200 Ns/mz. Calculate also the shear rate in the metering zone.
zyxwvuts
4.2 Find the operating point for the above extruder when it is combined with a die of length 40 mm and diameter 3 mm. What would be the effect on pressure and output if a plastic with viscosity 400 Ns/mZwas used. 4.3 A single screw extruder has the following dimensions:
screw length = 500 mm screw diameter = 25 mm flight angle = 17'42' channel depth = 2 mm channel width = 22 mm
If the extruder is coupled to a die which is used to produce two laces for subsequent granulation, calculate the output from the extrudeddie combination when the screw speed is 100 rev/min. Each of the holes in the lace die is 1.5 m m diameter and 10 mm long and the viscosity of the melt may be taken as 400 Ns/mz. 4.4 An extruder is coupled to a die, the output of which is given by ( K P / q ) where P is the pressure drop across the die, q is the viscosity of the plastic and K is a constant. What are the optimum values of screw helix angle and channel depth to give maximum output from the extruder. 4.5 A circular plate of diameter 0.5 m is to be moulded using a sprue gate in its centre. If the melt pressure is 50 MN/mz and the pressure loss coefficient is 0.6 estimate the clamping force required. 4.6 The container shown at the top of p. 341 is injection moulded using a gate at point A. If the injection pressure at the nozzle is 140 MN/mz and the pressure loss coefficient, m, is 0.5, estimate (i) the flow ratio and (ii) the clamping force needed. 4.7 Compare the efficiencies of the runners shown on p. 341. 4.8 A calender having rolls of diameter 0.3 m produces plastic sheet 1 m wide at the rate of 2000 kghour. If the roll speed is 5 revlminute and the nip between the rolls is 4.5 mm, estimate
zy
Processing of Plastics
34 1
t
220 dia
4
zyxwvutsr zyxwvutsrqp zyxwvu zyxwvuts 3
the position and magnitude of the maximum pressure. The density of the material is 1400 kg/m3 and its viscosity is 1.5 x 104 Ns/m2. 4.9 A calender having rolls of 0.2 m diameter produces 2 mm thick plastic sheet at a linear velocity of 0.1 d s . Investigate the effect of nips in the range 0.8 to 1.9 mm on the pressure profile. The viscosity is lo3 Ns/m2.
4.10 A hemispherical dome of 200 mm diameter has been vacuum formed from a flat sheet 4 m m thick. What is the thickness of the dome at the point furthest away from its diameter. 4.11 A disposable tumbler which has the shape of a frustrum of a cone is to be vacuum formed from a flat plastic sheet 3 mm thick. If the diameter of the mouth of the tumbler is 60 mm, the diameter of the base is 40 mm and the depth is 60 mm estimate the wall thickness at (a) a point 35 m m from the top and (b) in the centre of the base. 4.12 A blow moulding die which has an outside diameter of 40 mm and a die gap of 2 m m is used to produce a plastic bottle with a diameter of 70 mm. If the swelling ratio of the melt in the thickness direction is 1.8 estimate
(a) the parison dimensions (b) the thickness of the bottle and (c) a suitable inflation pressure if melt fracture occurs at a stress of 10 MN/m2. 4.13 A plastic film, 0.1 mm thick, is required to have its orientation in the transverse direction twice that in the machine direction. If the film blowing die has an outer diameter of 100 mm and an inner diameter of 98 mm estimate the blowup ratio which will be required and the lay flat film width. Neglect extrusion induced effects and assume there is no drawdown.
zyx
4.14 A molten polymer is to be. coated on a cable at a speed of 0.5 d s . The cable diameter is 15 mm and the coating thickness required is 0.3 mm. The die used has a length of 60 mm and an internal diameter of 16 mm. What pressure must be developed at the die entry if the viscosity of the polymer under these operating conditions is 100 Ns/m2.
4.15 During a rotational moulding operation an aluminium mould with a uniform thickness of 3 mm is put into an oven at 300°C. If the initial temperature of the mould is 23°C. estimate the time taken for it to reach 250°C. The natural convection heat transfer coefficient is 28.4 J/m2s.
342
zy zyxwv zyx zyxwvuts Processing of Plastics
K and the thermal diffusivity and conductivity of aluminium may be taken as 8.6 x lo’ m2/s
and 230.1 J/m.s.K respectively.
4.16 A billet of PVC weighing 150 g is to be compression moulded into a long playing record of diameter 300 mm. If the maximum force which the press can apply is 100 kN estimate the time needed to fill the mould. The density and viscosity of the the PVC may be taken as 1200 kg/m3 and 10 Ndm2 respectively.
zyxwvu zyxwvu
CHAPTER 5  Analysis of polymer melt flow
5.1 Introduction
zyxwvu zyxwv
In general, all polymer processing methods involve three stages  heating, shaping and cooling of a plastic. processing However, this apparent simplicity can be deceiving. Most plastic moulding methods are not straightforward and the practical knowhow can only be gained by experience, often using trial and error methods. In most cases plastics processing has developed from other technologies (e.g. metal and glass) as an art rather than as a science. This is principally because in the early days the flow of polymeric materials was not understood and the rate of increase in the usage of the materials was much greater than the advances in the associated technology. Nowadays the position is changing because, as ever increasing demands are being put on materials and moulding machines it is becoming essential to be able to make reliable quantitative predictions about performance. In Chapter 4 it was shown that a simple Newtonian approach gives a useful first approximation to many of the processes but unfortunately the assumption of constant viscosity can lead to serious errors in some cases. For this reason a more detailed analysis using a NonNewtonian model is often necessary and this will now be illustrated. Most processing methods involve flow in capillary or rectangular sections, which may be uniform or tapered. Therefore the approach taken here will be to develop first the theory for Newtonian flow in these channels and then when the NonNewtonian case is considered it may be seen that the steps in the analysis are identical although the mathematics is a little more complex. At the end of the chapter a selection of processing situations are analysed quantitatively to illustrate the use of the theory. It must be stressed however, that even the more complex analysis introduced in this chapter will not give precisely accurate
343
zyx zyxwvuts zyx zy zyxwvu
344
Analysis of polymer melt flow
solutions due to the highly complex nature of polymer melt flow. This chapter simply attempts to show how a quantitative approach may be taken to polymer processing and the methods illustrated are generally sufficiently accurate for most engineering design situations. Those wishing to take a more rigorous approach should refer to the work of Pearson, for example. 5.2 General Behaviour of Polymer Melts
In a fluid under stress, the ratio of the shear stress, t. to the rate of strain, p, is called the shear viscosity, q, and is analogous to the modulus of a solid. In an ideal (Newtonian) fluid the viscosity is a material constant. However, for plastics the viscosity varies depending on the stress, strain rate, temperature etc. A typical relationship between shear stress and shear rate for a plastic is shown in Fig. 5.1.
0
zyxwv Shear strain rate. y
Fig. 5.1 Relations Between Shear Stress and Shear Rate
As a starting point it is useful to plot the relationship between shear stress and shear rate as shown in Fig. 5.1 since this is similar to the stressstrain characteristics for a solid. However, in practice it is often more convenient to rearrange the variables and plot viscosity against strain rate as shown in Fig. 5.2. Logarithmic scales are common so that several decades of stress and viscosity can be included. Fig. 5.2 also illustrates the effect of temperature on the viscosity of polymer melts. When a fluid is flowing along a channel which has a uniform crosssection then the fluid will be subjected to shear stresses only. To define the flow behaviour we may express the fluid viscosity, q , as the ratio of shear stress, r,
Analysis of polymer melt flow
10 1
zyxwv zy 345
zyxwvuts zyxwvu
zyxwvu zyxwvut zyxwvu zyx 10
100 Shear rate (s1)
lo00
loo00
Fig. 5.2 Viscosity curves for polypropylene
to shear rate, Y ,
If, on the other hand, the channel section changes then tensile stresses will also be set up in the fluid and it is often necessary to determine the tensile viscosity, A, for use in flow calculations. If the tensile stress is (T and the tensile strain rate is E then cr A = T &
(5.2)
For many polymeric melts the tensile viscosity is fairly constant and at low stresses is approximately three times the shear viscosity. To add to this picture it should be realised that so far only the viscous component of behaviour has been referred to. Since plastics are viscoelastic there will also be an elastic component which will influence the behaviour of the fluid. This means that there will be a shear modulus, G, and, if the channel section is not uniform, a tensile modulus, E, to consider. If YR and ER are the recoverable shear and tensile strains respectively then
(5.3)
(5.4)
346
zyxwvutsr Analysis of polymer melt flow
zy
These two moduli are not material constants and typical variations are shown in Fig. 5.3. As with the viscous components, the tensile modulus tends to be about three times the shear modulus at low stresses. Fig. 5.3 has been included here as an introduction to the type of behaviour which can be expected from a polymer melt as it flows. The methods used to obtain this data will be described later, when the effects of temperature and pressure will also be discussed.
100 0.1
1
10
zyxwv zyxwvu
100
strain rate (sd)
loo0
loo00
Fig. 5.3 Flow curves for polyethylene at 170'
5.3 Isothermal Flow in Channels: Newtonian Fluids In the analysis of flow in channels the following assumptions are made:
1. There is no slip at the wall. 2. The melt is incompressible. 3. The flow is steady, laminar and time independent. 4. Fluid viscosity is not affected by pressure changes along the channel. 5. End effects are negligible. The steady isothermal flow of incompresible fluids through straight horizontal tubes is of importance in a number of cases of practical interest.
(a) Flow of Newtonian Fluid along a Channel of Uniform Circular Crosssection Consider the forces acting on an element of fluid as shown in Fig. 5.4.
Analysis of polymer melt flow High pressure
zyxwv zy zyxw 347
Low pressure
T
dr
L
V
Fig. 5.4 Element of Fluid in a Capillary F2
R
A
zyxw
= R?P
F3 = 2nr d z tr
Since the flow is steady X F z = 0
zyxw zyx zyxw
In many cases the pressure gradient is uniform, so that for a pressure drop, P , over a length, L, the maximum shear stress will be at the wall where r = R tw
Also since
PR 2L
=
.
av
t = r)y = r)
So using equation (5.5)
ar
Integrating this gives V
0
r
R
1 dP
erdr
(5.6)
zyxwvu zyxwvuts zyxwvuts
348
Analysis of polymer melt flow
zyxwvu
At r = 0, V = VO
so
and
dP .R2 Vo = .1 4r) d z
v = vo (1

(5.7)
(a)’)
The volume flow rate, Q,may be obtained from R
Q = 127trV d r 0
This can be rearranged using (5.7) to the form
zyx zyx I)’);(zy zyx zyxw
Once again if the pressure drop is uniform this may be expressed in the more common form
(5.10)
It is also convenient to derive an expression for the shear rate i,.
.
y=
then
2
i, = ar
bo
av ar
(1 
(5.11)
This may be rearranged using the relation between flow rate and Vo to give the shear rate at r = R as 4Q (5.12) Yo = nR3 The negative signs for velocity and flow rate indicate that these are in the opposite direction to the chosen zdirection. (b) Flow of Newtonian Fluid between Parallel Plates Consider an element of fluid between parallel plates, T wide and spaced a distance H apart. For unit width of element the forces acting on it are:
Analysis of polymer melt flow
zy zyxw
zyxwvu zyxw 349
Low pressure
High pressure
T
Y
4
I
I
,
F3
Fig. 5.5 Element of Fluid Between Parallel Plates
zyxwv zy zyxw
F2 = P t y F3 = tydZ
For steady flow there must be equilibrium of forces so
ap Y z = SY
(5.13)
In many cases the pressure gradient is uniform (aP/az = A P / L ) so the maximum shear stress will be at the wall where y = 4H tw
PH =2L
For a Newtonian Fluid the shear stress, t,is also given by
. = q av
t = qy
So using (5.13)
aY
av = y ap
q
ay
Integrating this gives V
V
az
(5.14)
350
zyxwvut zy zyxwv
zyxwvut zy zyxw Analysis of polymer melt flow
V=
211 d z
Now at y = 0, V = V O
so
1dP vo = 211 d z
(Hz)
(5.15)
Substituting aP/az in the expression for V gives V=Vo(l
(z)2)
(5.16)
The volume flow rate, Q, is given by
Q =2 T T V d y 0
Using equation (5.16) this may be expressed in the form
Q =2 TT.0 ( 1 
(2)’) dy
0
= 2TVo
):(
e=.TH3 1211
dP dz
(5.17)
zyxw
which, for a uniform pressure gradient, reduces to TPH3 12qL
Q=
zyxw
An expression for the shear rate,
=
9, may also be derived from
a [vo( 1 aY
($)2)]
= 8Voy/H 2
but as shown above
(5.18)
3Q vo = 2TH
(5.19)
zyxw zyxw zyxwv zyxwv zyxw zyxwv zyx
Analysis of polymer melt flow
so At the wall
351
.
12Qy TH3
y=
H
y=
2
yo = 6Q
TH2
(5.20)
It is worth noting that the equations for flow between parallel plates may also be used with acceptable accuracy for flow along  a circular annular slot. The relevant terms are Tllustrated in Fig. 5.6.
zyxwvu
Fig. 5.6 Flow in an Annular Slot
5.4 Rheological Models for Polymer Melt Flow
When log (viscosity) is plotted against log (shear rate) or log (shear stress) for the range of shear rates encounterd in many polymer processing operations, the result is a straight line. This suggests a simple power law relation of the type
zyxwv (5.21)
where n is the Power Law index and ro and M, refer to the shear stress and shear rate at some reference state. This is often taken as 90 = 1 sl and so the
352
zyxwvutsr z zyxwv zyxwv zyxwv Analysis of polymer melt flow
zyxwvu zyxwvu zyxw
Power Law may be expressed as
t = to y:
(5.22)
It is common practice nowadays to express the apparent viscosity as a function of the shear rate, ya. This may be obtained using the definition of apparent viscosity qa as the ratio of shear stress to shear rate, ie
So using
t=  .tla
Ya
to
Po
tlo
n1
(5.23)
or rearranging to use shear stress instead of shear rate n1
(5.24) tl0
Equations (5.21), (5.22) and (5.23) are useful for the high strain rates experienced in injection moulding or extrusion but unfortunately they do not predict the low strain rate situation very well where plastic melts tend towards Newtonian behaviour (ie n + 1). This is illustrated in Fig. 5.7. Carreau proposed an alternative equation to overcome this problem. It has the form fl1
Jln = [1 + (Alj/.)2]
(5.25)
tl0
where At is a material constant. It may be seen that when 9 >> 1, this equation reduces to the Power Law (5.23) but as shown in Fig. 5.7, it also predicts the low shear rate situation very well. In order to allow for the effect of temperature on viscosity a shift factor, UT is often used. The Carreau equation then becomes
zyx (5.26)
where typically the shift factor, U T , may be obtained from
logu= = CI(T1  To)  Cl(T2  To) c2 + (T1 To) c2 (T2 To)
+
(5.27)
Analysis of polymer melt flow
zyxwvu 353
zyxwvuts zyxwvu
zyxwvutsr zyxwvuts zyxwvut zyxw Fig. 5.7 Comparison of Models for Flow Behaviour
where C1 and C2 are material constants, T1 ("C) is the temperature at which the viscosity is known, T2 ("C)is the temperature at which the viscosity is required and To ("C)is a reference temperature. When To = Tg then C1 = 17.4 and C2 = 51.6. With the widespread use of software packages to assist with computational fluid dynamics (CFD) of polymer flow situations, other types of viscosity relationships are also used. For example, the regression equation of Klien takes the form In qa = a0
+ ai In ya + all(ln p)2 + a2T + 42T2 + a12 . T . In ya
(5.28)
where ai, are material constants and T is the temperature of the melt ("C). It should be noted that if all is small (which is often the case) then this equation also reduces to the Power Law. The polynomial of Muenstedt is also popular. It takes the form logqa = logaT
+A0 +A1
log ( a ~ i / a+A2[log(a~j.)I~ )
+ ~3 [ W a T Pa )i3 + A ~ [ W ~ T P ) I ~
(5.29)
However, for the high strain rates appropriate for the analysis of typical extrusion and injection moulding situations it is often found that the simple Power Law is perfectly adequate. Thus equations (5.22), (5.23) and (5.27) are important for most design situations relating to polymer melt flow.
zyxwvu zyxwv zyxwvut zyx zy Analysis of polymer melt flow
354
Example 5.1 Applying the Carreau model to polypropylene, the following constants are known at 190°C. qo = 2350 Ns/m2, AT = 0.05,
n = 0.33
zyx zyxwvu
Estimate the viscosity of polypropylene at 230°C and a shear rate of lo00 s'. The glass transition temperature for the polypropylene is  10°C.
Solution The temperature shift factor from 190°Cto 230°C may be obtained from logaT =
C l V I  T,) c2 (TI  T g )
+
 Tg) c2 + (T2  Tg) Cl(T2
+ 10)  17.4(230+ 10) 51.6 + (190 + 10) 51.6 + (230 + 10)
 17.4(190
aT
= 0.324
Using the Carreau model
= QOUT (1
+ UT(ATg)2)T*
0.331
+ 0.324(0.05 x 103)2)0.33
= 2350(0.324) (1
so,
qa = 80.7 Ns/m2 at
230°C and p = lo00
5.5 Isothermal Flow in Channels: NonNewtonian Fluids
(a) Flow of Power Law Fluid Along a Channel of Uniform Circular Crosssection Referring to Fig. 5.4 and remembering that equilibrium of forces was the only condition necessary to derive (5.5) then this equation may be used as the starting point for the analysis of any fluid.
zyxw zyxw
.='(E) Now so but from (5.23)
(5.5)
az
2
. =aq v
t = qy
ar
a v  _r a p _ aR
 2q
(a,)
zyxwvu zyxwvu zyx 355
Analysis of polymer melt flow
So from above
av _ ar
r
Integrating this between the limits Velocity = V at radius = r and Velocity = 0 at radius = R
The equation for velocity at any radius may then be expressed as
At r = 0, V = VO
v=v0[1(;)
]
(5.31)
The volume flow rate, Q, is given by
(;)(n+1)7] zyxwvut zyxw
Q=
()n + l 3n
Also Shear Rate,
nR2Vo
+1
av
a
ar
ar
(5.32)
[ (
i. =  =  V O 1 
(5.33)
The shear rate at the wall is obtained by letting r = R and the equation is more convenient if V Ois replaced by Q from (5.33). In this case Shear Rate at wall
356
zyxwvuts zyxwvu zyxwvuts zyxwvut zyxwvu zyxw zyxw zyxw Analysis of polymer melt flow
It is worth noting that since a Newtonian Fluid is a special case of the Power Law fluid when n = 1, then the above equations all reduce to those derived in Section 5.3(a) if this substitution is made.
(b) Flow of Power Law Fluid between Parallel Plates Referring to Fig. 5.5 and recognising that equation (5.13) is independent of the fluid then ap t=y
az
but
av
t = q a Y
.
n1
and q = q o [ i ]
Integrating this equation between the limits velocity = V at distance = y velocity = 0 at distance = H / 2
And using this to simplify the expression for V
zyxwvu (5.35)
The flow rate, Q, may then be obtained from the expression Hi2
Q = 2T
J 0
Vdy
Q=
And as before
zyx zyxw
zyxwvu zyxwvut zyxwvut zyxwvutsrq
Analysis of polymer melt flow
357
(*)2n + 1
av
a
aY
aY
(5.36)
TVoH
[ ( (23(n+17]
i. =  =  V O 1 

(5.37)
At the wall y = H / 2 and substituting for Vo from (5.36) then
2n
+1
TH2
It can be seen that in the special case of n = 1 these equations reduce to those for Newtonian Now.
zyxwv
5.6 Isothermal Flow in NonUniform Channels
In many practical situations involving the flow of polymer melts through dies and along channels, the crosssections are tapered. In these circumstances, tensile stresses will be set up in the fluid and their effects superimposed on the effects due to shear stresses as analysed above. Cogswell has analysed this problem for the flow of a power law fluid along conicylindrical and wedge channels. The flow in these sections is influenced by three factors: (1) entry effects given suffix 0
( 2 ) shear effects given suffix S (3) extensional effects given suffix E Each of these will contribute to the behaviour of the fluid although since each results from a different deformation mode, one effect may dominate depending on the geometry of the situation. This will be seen more clearly later when specific design problems are tackled.
zyxwv
(a) Flow in ConiCylindrical Dies Consider the channel section shown in Fig. 5.8(a) from which the element shown in Fig. 5.8(b) may be taken.
(i) Pressure Drop Due to Shear, Ps Assuming that the different modes of deformation are separable then considering equilibrium of forces in regard to the shear stress only, gives dP,~nr2=2nrdlsect?.rcos0 2t
dP, =  * dl r
(5.38)
zz
Analysis of polymer melt flow
358
L
zyxw zyx zyxwv zyx
Fig. 5.8 Analysis of ConiCylindrical Die
but for a power law fluid
t=q$
dr and using dl = tane
then (5.38) becomes
and p = 3( n + y 1 ) pQ
2to d P s = tane  ( ( y ) 3)n + 1
Q
dr y1+3n
zyxwvuts zy zyxwv zyxwvu
Analysis of polymer melt flow Integrating
359
tan 0
RI
(5.39)
(ii) Pressure Drop Due to Extensional Flow PE
dPE . nr2 = a [ n ( r + dr)2  nr2] 20 dr dPE = r
Integrating (5.40)
In order to integrate the right hand side of this equation it is necessary to get an equation for (T in terms of r. This may be obtained as follows. Consider a converging annulus of thickness, h, and radius, a, within the die. If the angle of convergence is 4 then simple geometry indicates that for uniform convergence a r
zyxwv
tan4=tanO
Now if the simple tensile strain,
E,
dh h
da a
  
and
is given by
E=
dA A
then the strain rate, i,will be given by E,
but
1 d(2nah)  _2 d_ a 1 d(area) = ~ . area dt 2nah dt a dt ~
da dl a  = tan4 .  =  [email protected] dt dt r
360
zyxw zyxwvu zyxwv zyx zyxwv zyxw zyxwvu Analysis of polymer melt flow
where V is the velocity of the fluid parallel to the centre line of the annulus. From (5.31) and (5.32) this velocity is given by 3n
so
+1
The average extensional stress is obtained by integrating across the element so m r 2 = ]ua2na
da
0
and since by definition 0, = Ab,
ff =)I ($)tan9
(5.41)
So in (5.40)
Using (5.41) (5.42)
(iii) Pressure Drop at Die Entry, PO When the fluid enters the die from a reservoir it will conform to a streamline shape such that the pressure drop is a minimum. This will tend to be of a conicylindrical geometry and the pressure drop, PO, may be estimated by considering an infinite number of very short frustrums of a cone. Consider a conicylindrical die with outlet radius, Ro, and inlet radius, Ri, and an included angle 2ao. From (5.40) From (5.42)
zyxwvu zyxwvut zyxwvutsrqp zyxwvut zyxwv
Analysis of polymer melt flow
(t) 3
where x =
zyxw 361
for convenience
The pressure drop, P I , for such a die is
p1 = P S + P E a btanao tan a0
+
where
For minimum pressure drop the differential of pressure drop with respect to the angle a0 should be zero dP1  a + b = O d(tanao) tan200
zyxwvut
So the minimum value of pressure is given by
p 1 = .1/2b1/2 + .1/2b1/2 = h1/2b1/2
If this procedure is repeated for other short conicylindrical dies then it is found that p 2 = X(l+n)/2p 1 P3 = (x(1+n)/2)2Pland so on.
So the total entry pressure loss, PO,is given by
where
f ( x ) = [(I x")(l
)]'/2.
[1 + . ( l + n ) / 2
+ ( X ( l + n ) / 2 ) 2 + ( X ( l + n ) / 2)3
+**.I
and q = viscosity corresponding to shear rate at die entry.
41/2 Po = 3(n 1)
+
Also
(5)(t7W2
(5.43)
362
zyxwvuts zyxwv zyxw zyxw zyx I")$(zy
zyx Analysis of polymer melt flow
So that from (5.44)
Po =
8a 3(n 1)
+
(5.44)
(b) Flow in Wedge Shaped Die Referring to the terminology in Fig. 5.9 and using analysis similar to that for the conicylindrical die, it may be shown that the shear, extensional and die entry pressure losses are given by
Ps = t l[I 
(5.45)
2n tan@
PE
= 2 [l
(32]
Po =
(5.47)
zyxw
Fig. 5.9 Analysis of How in Tapered Wedge
where q corresponds to shear rate at die entry Also
y= &
2n + 1 (y) ($)
= (9/3)tan@
(5.48)
(5.49)
zyxwvuts zyxwvuts
Analysis of polymer melt flow and
363
(5.50)
where Po is the half angle of convergence to the die.
5.7 Elastic Behaviour of Polymer Melts
As discussed earlier, polymer melts can also exhibit elasticity. During flow they have the ability to store strain energy and when the stresses are removed, this strain is recoverable. A good example of elastic recovery is post extrusion swelling. After extrusion the dimensions of the extrudate are larger than those of the die, which may present problems if the dimensions of the extrudate are critical. In these circumstances some knowledge of the amount of swelling likely to occur is essential for die design. If the die is of a nonuniform section (tapered, for example) then there will be recoverable tensile and shear strains. If the die has a uniform crosssection and is long in relation to its transverse dimensions then any tensile stresses which were set up at the die entry for example, normally relax out so that only the shear component contributes to the swelling at the die exit. If the die is very short (ideally of zero length) then no shear stresses will be set up and the swelling at the die exit will be the result of recoverable tensile strains only. In order to analyse the phenomenon of post extrusion swelling it is usual to define the swelling ratio, B, as dimension of extrudate B= dimension of die
zyxw zyxwvu zyxw
Swelling Ratios Due to Shear Stresses (a) Long Capillary
Fig. 5.10 shows an annular element of fluid of radius r and thickness dr subjected to a shear stress in the capillary. When the element of fluid emerges from the die it will recover to the form shown by ABCD. If the shear strain at radius r is yr then ED yr = tana = AE Also
area of swollen annulus =27rr dr'  AD initial area of annulus 2xr dr AE  (AE* ~ 0 ~ 1 ~ 1 ~ AE
+
364
z
zy zyxwvuts Analysis of polymer melt flow
/
/
Polymer melt
zyxw zyxw
Fig. 5.10 Polymer Melt Emerging from a Long Die
So from the definition of swelling ratio and using the subscripts S and R to denote Shear swelling in the Radial direction then R
/ ( I + y,2)'/227rr d r area of swollen extrudate = area of capillary
~i~
R
1 2 n r dr
zyxwvut / zyxwvu zyx 0
Assuming that the shear strain, yr, varies linearly with radius, r, then r yr = RyR where y~ is the shear strain at the wall (1
so
B ; ~=
+ $y2R)
112
2nr d r
7FR2
(b) Long Rectangular Channel When the polymer melt emerges from a die with a rectangular section there will be swelling in both the width (T) and thickness (H)directions. By a similar analysis to that given above; expressions may be derived for the swelling in
Analysis of polymer melt flow
zyxw zyxwv zyxw 365
these two directions. The resulting equations are
Equations (5.51), (5.52) and (5.53) can be cumbersome if they are to be used regularly so the relationships between swelling ratio and recoverable strain are often presented graphically as shown in Fig. 5.11.
zyxwvuts zyxwvutsr zyxwvutsr
2.6
2.4
2.2 0 .c
E
2
C UJ
I 1.8 a, 3
v,
1.6 1.4 1.2 1
0
1
2
zyx
3 4 5 Recoverable shear strain
6
7
8
Fig. 5.11 Variation of Swelling Ratio for Capillary and Slit Dies
Swelling Ratio Due to Tensile Stresses
(a) Short Capillary (zero length) Consider the annular element of fluid shown in Fig. 5.12. The true tensile strain ER in this element is given by ER
zyxwv
= ln(1
+E)
where E is the nominal strain (extension f original length) ..=ln(l+
(
dr' dr dr
))
366
zyxwvut zyxwvuts zyxwvut Analysis of polymer melt flow
Swelling = ratio
 R'
€a
Short die
Fig. 5.12 Polymer Melt Emerging from a Short Die
zyxwvu e"R= 1
(e""  1)dr
Now,
zyx
+
(
dr'  d r dr
)
+ d r = dr'
area of swollen annulus 2nr dr' dr' original area of annulus 2nr d r dr  (e""  1)dr d r dr = e"R
+
zy zyxwvuts
So from the definition of swelling ratio and using the subscript, E, to denote extensional stresses then
j2nre" dr
of swollen extrudate ~i~= area area of capillary
J2nr dr 0
&R
BER= (e )
112
zyx (5.54)
(b) Short Rectangular Channel By similar analysis it may be shown that for a short rectangular slit the swelling ratios in the width (T) and thickness (H)directions are given by BET=(^E R 1114
(5.55)
Analysis of polymer melt flow
zyxwvu zyx 367
BEH = ( e ER 1112
(5.56)
zyxwvutsr
Although these expressions are less difficult to use than the expressions for shear, it is often convenient to have the relationships available in graphical form as shown in Fig. 5.13.
zyxwvutsrq zyxwvu zyxwvut zyxwvutsrqponm 3
2.5
0 .L m L
.2 2 
s
v)
1.5
1 0.5
0
1 Recoverable extensional strain
1.5
2
Fig. 5.13 Variation of Swelling Ratio for Capillary and Slit Dies
5.8 Residence and Relaxation Times
zyxw
(a) Residence (or Dwell) Time This refers to the time taken for the polymer melt to pass through the die or channel section. Mathematically it is given by the ratio
Volume of channel (5.57) Volume flow rate For the uniform channels analysed earlier, it is a simple matter to show that the residence times are: Residence time, t R =
Newtonian Flow Circular Cross Section
tR
Rectangular Cross Section
tR
8qL2 PR2 12QL2 =PH2 =
(5.58) (5.59)
368
zyxwvu zyxwvu zyxwvut zyxwvu zyxwv Analysis of polymer melt flow
Power Law Fluid
Circular Cross Section
Rectangular Cross Section
(5.61)
(b) Relaxation (or Natural) Time In Chapter 2 when the Maxwell and Kelvin models were analysed, it was found that the time constant for the deformations was given by the ratio of viscosity to modulus. This ratio is sometimes referred to as the Relaxation or Natural time and is used to give an indication of whether the elastic or the viscous response dominates the flow of the melt. To do this, a Deborah Number Ndeb, has been defined as Ndeb =
Relaxation or Natural Time Timescale of the process
(5.62)
If Ndeb > 1 then the process is predominantly elastic whereas if Ndeb < 1 then viscous effects dominate the flow.
5.9 Temperature Rise in Die Power is the work done per unit time, where work in the simplest sense is defined as Work = (force) x (distance) Therefore Power = (force) x (distance per unit time) = (Pressure drop x area) x (velocity)
But the volume flow rate, Q, is given by Q = area x velocity
(5.63)
So Power = P Q
where P is the pressure drop across the die. Using this expression it is possible to make an approximation for the temperature rise of the fluid during extrusion through a die. If it is assumed that all the work is changed into shear heating and that all the heat is taken up evenly by the polymer, then the work done may be equated to the temperature rise in the polymer. Power = Heat required to change temperature = mass x specific heat x temperature rise
zyxwvu zy zyxwv zyxwvutsrqpon zyxwv zyx
Analysis of polymer melt flow SO
369
P Q = p Q x C , x AT
(5.64)
P
AT=
PCP
where p is the density of the fluid and C p is its specific heat. 5.10 Experimental Methods Used to Obtain Flow Data
In Section 5.1 1 design examples relating to polymer processing will be illustrated. In these examples the flow data supplied by material manufacturers will be referred to, so it is proposed in this section to show how this data may be obtained. The equipment used to obtain flow data on polymer melts may be divided into two main groups. (a) Rotational Viscometers  these include the cone and plate and the concentric cylinder. (b) Capillary Viscometer  the main example of this is the ram extruder.
Cone and Plate Viscometer In this apparatus the plastic to be analysed is placed between a heated cone and a heated plate. The cone is truncated and is placed above the plate in such a way that the imaginary apex of the cone is in the plane of the plate. The angle between the side of the cone and the plate is small (typically 4"). The cone is rotated relative to the plate and the torque. T, necessary to do this is measured over a range of rotational rates, 6 . Refemng to Fig. 5.14
zyxwv
Area of annulus
= 217r. dr
Force
= 2nn. dr
Torque
= 217r'r. dr
SOTotal Torque, T =
I
2rcr't .dr
0
T=
($)3rR3t
zyxwvuts zyxwv (5.65)
Also shear strain,
X I  8 y===
Strain rate,
y=
h
.
e
a!
ra!
6
ct
(5.66)
370
zy zyxwvuts Analysis of polymer melt flow
zyxwvutsrq Molten plastic
Heated plate [fixed I
zyxw zyxwvu zyxwv Fig. 5.14 Cone and Plate Viscometer
t
zyxwvut
And since viscosity
q=
Y
3T a 2 n ~ 3b
9=*
(5.67)
The disadvantage of this apparatus is that it is limited to strain rates in the region 10 to 1 s' whereas in plastics processing equipment the strain rates are in the order of 10 s3l to IO4 s'.
Concentric Cylinder Viscometer In this apparatus the polymer melt is sheared between concentric cylinders. The torque required to rotate the inner cylinder over a range of speeds is recorded so that viscosity and strain rates may be calculated. Referring to Fig. 5.15 Torque,
T = 2nRL R
t = 2nR2Lt
(5.68)
Strain rate,
(5.69)
Viscosity,
(5.70)
37 1
Analysis of polymer melt flow
zy
zyxwvu zyxwvutsrq Molten /plastic
Hwted concentric cylinders,
zyxwvu zyxw zyxwv zyx Fig. 5.15 Concentric Cylinder Viscometer
As in the previous case, this apparatus is usually restricted to relatively low strain rates.
Ram Extruder
In this apparatus the plastic to be tested is heated in a barrel and then forced through a capillary die as shown in Fig. 5.16. Normally the ram moves at a constant velocity to give a constant volume flow rate, Q. From this it is conventional to calculate the shear rate from the Newtonian flow expression.
p =  4Q
nR3 Since it is recognised that the fluid is NonNewtonian, this is often referred to as the apparent shear rate to differentiate it from the true shear rate. If the pressure drop, P, across the die is also measured then the shear stress, t,may be calculated from PR This leads to a definition of apparent viscosity as the ratio of shear stress to apparent shear rate
A plot of apparent viscosity against shear rate produces a unique flow curve for the melt as shown in Fig. 5.3. Occasionally this information may be based on the true shear rate. As shown in Section 5.4(a) this is given by
372
z
zyxwvutsr zy r zyxw Analysis of polymer melt flow
1/
Piston
kzyxw xtrudote
zyx zyx
Fig. 5.16 Section Through Ram Extruder
However, this then means that the true shear rate must always be used in the flow situation being analysed. Experience has shown that this additional complexity is unnecessary because if the Newtonian shear rate is correlated with flow data which has been calculated using a Newtonian shear rate, then no error is involved. Note that rotational viscometers give true shear rates and if this is to be used with Newtonian based flow curves then, from above, a correction factor of (4n/3n 1) needs to be applied to the true shear rate. The ratio (3n 1)/4n is called the Rabinowitsch Correction Factor and it is used to convert Newtonian shear rates to true shear rates. There are two other points worth noting about this test. Firstly the flow data is produced using a capillary die so that its use on channels of a different geometry would require a correction factor. However, in most cases of practical interest, the factor is not significantly different from 1 and so there is no justification for the additional complication caused by its inclusion. Secondly, the pressure drop, P, in the above expression is the pressure drop due to shear flow along the die. If a pressure transducer is used to record the
+
+
zyxwvu zyxwv zyxwvuts zyxw
Analysis of polymer melt flow
373
pressure drop as shown in Fig. 5.16, then it will also pick up the pressure losses at the die entry. This problem may be overcome by carrying out further tests using either a series of dies having different lengths or a die with a very short (theoretically zero) length. In the former case, the pressure drops for the various lengths of die may be extrapolated to give the pressure drop for entry into a die of zero length. In the second case this pressure is obtained directly by using the socalled zero length die. This is then subtracted from the measured pressure loss, PL, on the long die being considered, so that (5.71)
In addition, if the swelling of the extrudate is measured in each of these two tests then the swelling ratio using the long die will be BSR and the swelling ratio using the short die will be BER (see Section 5.6). Using equation (5.44) and (5.47) this enables the shear and tensile components of the recoverable strains to be calculated and from them the shear and tensile moduli. From this relatively simple test, therefore, it is possible to obtain complete flow data on the material as shown in Fig. 5.3. Note that shear rates similar to those experienced in processing equipment can be achieved. Variations in melt temperature and hydrostatic pressure also have an effect on the shear and tensile viscosities of the melt. An increase in temperature causes a decrease in viscosity and an increase in hydrostatic pressure causes an increase in viscosity. Wically, for low density polyethlyene an increase in temperature of 40°C causes a vertical shift of the viscosity curve by a factor of about 3. Since the plastic will be subjected to a temperature rise when it is forced through the die, it is usually worthwhile to check (by means of Quation 5.64) whether or not this is significant. Fig. 5.2 shows the effect of temperature on the viscosity of polypropylene. A change in pressure from atmospheric (= 0.1 MN/m2) to about 100 MN/m2 (a pressure likely to be experienced during processing) causes a vertical shift of the viscosity curve by a factor of about 4 for LDPE. This effect may be important during processing because the material can be subjected to large changes in pressure in sections such as nozzles, gates, etc. However, it should be noted that in some cases the increase or decrease in pressure results in, or is associated with, an increase or decrease in temperatures so that the net effect on viscosity may be negligible. Other factors such as the use of additives also have an effect on the shape of the flow curves. Flame retardants, if used, tend to decrease viscosity whereas pigments tend to increase viscosity. Fig. 5.17 shows flow curves for a range of plastics.
zyxwv zyxwvuts
Melt Flow Rate (also known as Melt Flow Index) The Melt Flow Rate Test is a method used to characterise polymer melts. It is, in effect, a single point r a m extruder test using standard testing conditions (BS
374
zyxwvutz Analysis of polymer melt flow
IO000
 1 m N I
66(290"C)
E
PVC (170°C) PMMA POM(21OOC)
10
1
100
1000
10000
Shear rate (s1)
zyx 100000
Fig. 5.17 Viscosity Curves for a Range of Plastics (230°C unless otherwise shown)
w I
Weight
Oil filled t hermomete wells
'r=%il
Barrel 'Heater ,
lnsulation
Polymei. melt
Fig. 5.18 Diagram of Apparatus for Measuring Melt Flow Index
zyxwv zyxwv zyxwv zyxw zyxwvut
Analysis of polymer melt flow
375
2782) as illustrated in Fig. 5.18. The polymer sample is heated in the barrel and then extruded through a standard die using a standard weight on the piston, and the weight (in gms) of polymer extruded in 10 minutes is quoted as the melt flow rate (MFR) of the polymer.
Flow Defects
When a molten plastic is forced through a die it is found that under certain conditions there will be defects in the extrudate. In the worst case this will take the form of gross distortion of the extrudate but it can be as slight as a dullness of the surface. In most cases flow defects are to be avoided since they affect the quality of the output and the efficiency of the processing operation. However, in some cases if the flow anomaly can be controlled and reproduced, it can be used to advantage  for example, in the production of sheets with matt surface finish. Flow defects result from a combination of melt flow properties, die design and processing conditions but the exact causes and mechanisms are not completely understood. The two most common defects are
(a) Melt Fracture When a polymer melt is flowing through a die, there is a critical shear rate above which the extrudate is no longer smooth. The defect may take the form of a spiralling extrudate or a completely random configuration. With most plastics it is found that increasing the melt temperature or the W D ratio of the die will increase the critical value of shear rate. It is generally believed that the distortion of the extrudate is caused by slipstick mechanism between the melt and the die wall due to the high shear rates. If there is an abrupt entry to the die then the tensilelshear stress history which the melt experiences is also considered to contribute to the problem. (b) Sharkskin Although this defect is also a visual imperfection of the extrudate it is usually differentiated from melt fracture because the defects are perpendicular to the flow direction rather than helical or irregular. In addition, experience has shown that this defect is a function of the linear output rate rather than the shear rate or die dimensions. The most probable mechanism of sharkskin relates to the velocity of skin layers of the melt inside and outside the die. Inside the die the skin layers are almost stationary whereas when the extrudate emerges from the die there must be a rapid acceleration of the skin layers to bring the skin velocity up to that of the rest of the extrudate. This sets up tensile stresses in the melt which can be sufficient to cause fracture. 5.11 Analysis of Flow in Some Processing Operations Design methods involving polymer melts are difficult because the flow behaviour of these materials is complex. In addition, flow properties of the melt are usually measured under well defined uniform conditions whereas unknown effects such as heating and cooling in processing equipment make service conditions less than ideal. However, sufficient experience has been gathered
376
zyxwvuts zyxw zyxwv zyxwv zyxw zyxwv zyxwvu Analysis of polymer melt flow
using the equations derived earlier that melt flow problems can be tackled quantitatively and with an accuracy which compares favourably with other engineering design situations. In this section a number of polymer processing methods will be analysed using the tools which have been assembled in this chapter. In some cases the heating and cooling of the melt may have an important effect on the flow behaviour and methods of allowing for this are developed.
Example 5.2 In a plungertype injection moulding machine the torpedo has a length of 40 mm, a diameter of 23 mm and is supported by three spiders. If, during moulding of polythene at 170°C, the plunger moves forward at a speed of 15 mm/s, estimate the pressure drop along the torpedo and the shear force on the spiders. The barrel diameter is 25 mm. Solution Assume that the flow is isothermal. Volume flow rate, Q = area x velocity IC
= (25
10~
1 0  ~ ) ~ 15
4 = 7.36 x
m3/s.
The gap between the torpedo and the barrel may be considered as a rectangular slit with T = (IC x 24 x 10F3)m and H = 1 x 10 m3. So apparent strain rate,
=
~
6Q TH2
 6 x 7.36 x  IC x 24 x
= 585
S'
From Fig. 5.3, at this strain rate,
r]
so
T=
2Lt p== H
x
= 400 Ns/m2.
r]p = 400 x 585 = 2.34 x
lo5 N/m2
x 2.34 x 105
2 x 40 x
1 x 103
= 18.7 MN/m2
The force on the spider results from (a) the force on the torpedo due to the pressure difference across it and (b) the force on the torpedo due to viscous drag. Crosssectional area of torpedo = nr2 So force due to pressure = Rr2P = ~ ( 1 1 . 5x 103)2x 18.7 x lo6
= 7.8 kN
Analysis of polymer melt flow
zyxwvu zyxw zyxw zyxwvu zyxw zyxw zyxwv zyxw 377
Surface area of torpedo = RDL
Viscous drag force = R D L ~
x 1OW3)(2.34x lo5)
= n(23 x
= 0.68 kN
So Total Force = 8.48 kN
m3/s. Example 5.3 The output of polythene from an extruder is 30 x If the breaker plate in this extruder has 80 holes, each being 4 mm diameter and 12 mm long, estimate the pressure drop across the plate assuming the material temperature is 170°C at this point. The flow curves in Fig. 5.3 should be used.
Solution Assume the flow is isothermal. Flow rate through each hole
So Apparent shear rate,
=
30 x
80
m3/s
4Q i, = nR3
4 x 30 x x go x 23 x 109
59.6 sl
From Fig. 5.3 the shear stress, t,is 1.2 x 1 6 N/m2 and since PR t=2L 2 12 103 x 1.2 x 105 P= 2 x 103 = 1.44 m / m 2
Example 5.4 Eight polypropylene mouldings, each weighing 10 g are to be moulded using the runner layout shown in Fig. 5.19. If the injection time is 2 seconds and the melt temperature is 210°C calculate the pressure at each cavity if the injection pressure at the sprue is 80 MN/m2. The density of the polypropylene is 909 kg/m3 and the volume of the sprue is 5000 mm3. Assume that the flow is isothermal and ignore the pressure losses at comers. Solution Firstly it is necessary to determine the volume flow rate through the runners and gates. The total volume of the runners, gates and cavities may be calculated as follows: Volume of 8 cavities
= 8 x 10 x 103/909 = 8.8 x = 88 x lo3 mm3
m3
Analysis of polymer melt flow
378
z
5 mm
1Wmm
z
zyxwv zyxw zyxwv zyxwv zyx zyxw zyxwv Gate 3 mm wide, 2 mm deep, 1.6mm long
Fig. 5.19 Runner Layout, Example 5.4
Volume of long runners = 4 x nR2 x L =4
n(3)2
100 = 11.3 x 103 mm3
Volume of short runners = 8 x ~ ( 2 . 5 x) ~50 = 7.85 x lo3 mm3 Volume of sprue
=5
Total volume
= 112.2
io3 m3
103 m3
The fill time is 2 seconds so the total volume flow rate, Q, is given by
Q=
112.2 x 103
= 56.1 x lo3 mm3/s = 56.1 x
m3/s
To get the pressure loss in the runners and gates. The flow rate in the long runner is Q/4, hence 4Q (i) For long runners i, = = RR~
4 x 56.1 x lo3 = 661 4x~ ( 3 ) ~
S'
zyx zyxwvutsrqponmlkji zyxwv 379
Analysis of polymer melt flow
From the flow curves for polypropylene at 210°C, at this shear rate,
17 = 130 Ns/m2, so the shear stress, t,is given by
zyxw zyxw zyxw zyxw zyxw
PR 130 x 661 = 85.9 kN/m2 = 2L 2 x 100 x 85.9 2Lt = 5.73 m / m 2 Hence, Pressure loss, P =  = R 3 (ii) For the short runners, the flow rate is Q/8, and so t=
i. = 571 sI,
q = 160 Ns/m2, t = 91.4 kN/m2
and these give the pressure loss = 3.66 MN/m2. (iii) For the gates, the flow rate is Q/8 and so
.
6Q 6 x 56.1 x lo3 = 3506 s' TH2 8 x 3 ~ 2 ~
y=
17 = 44 Ns/m2, t = 154.3 kN/m2
From the flow curves,
2Lr p== H = 5.73
So pressure loss, Total pressure loss
+
2 x 1.6 x 154.3 = 247 kN/m2 2 3.66 0.247
+
= 9.64 MN/m2
Thus, pressure available at cavity
= 80  9.64
= 70.4 MN/m2
Example 5.5 In a polyethylene film blowing die the geometry of the die lips is as shown in Fig. 5.20. If the output is 300 kghour and the density of the polythene is 760 kg/m3, estimate the pressure drop across the die lips. Solution Volume flow rate =
300 = 109.6 x 60 x 60 x 760
m3/s
The die lips may be considered in three sections A, B and C and the total pressure drop is the sum of the losses in each. Section A: Since this section is of a uniform section there will only be a pressure drop due to shear. For a rectangular slot, as shown earlier, the apparent shear rate, i. at A1 is given by 6 x 109.6 x = 1.64 T H :  ~ ( 2 6 0x 103)(0.7 x 103)2
y. =  6Q 
io3 sl
380
z zyxwvuts Analysis of polymer melt flow Tube
Tube
zyxwv zyxwv zyxw zyxwv zyxwv I
Fig. 5.20 Tube Extrusion Die
So from Fig. 5.3, t = 3.3 x 16 Nlm2
2Ltl ps,* = H1  2 x 4 x 3.3 x 16 0.7 = 3.77 m / m 2 Section B: This section is tapered so there will be pressure losses due to both shear and extensional flows. From simple geometry H3 = H2 (2Ltana) where (I! is half the included angle and L = 11 mm. H 2 = 0.7 mm, H3 = 1.28 mm
zyxwvu +
Now at B2,
i, = 1.64 x lo3 sl
.h
= ( i , / 3 ) t a n ~ t= 1/3 x 1.64 x 1O3tan(1So) = 14 s  ~
At B3,
6 x 109.6 x i, = 6Q TH;  n x 260 x 103(1.276 x 103)2 = 494.5 s1
zyxwvu zyxw zyxw
Analysis of polymer melt flow
381
i = 1/3(494.5)tan 1.5" = 4.3 sl
From Fig. 5.3 the flow curve can be taken as a straight line for the shear rate range 500 sl to 1600 sl and the power law index n may be taken as 0.33.

2(0.3) tan 1.5
= 6.9 M N h 2
zyxwvutsr
Also from (5.46)
Now t5 = 14 sl so from Fig. 5.3 0 2 = 3.15 x lo6 Nm2 (ie 2.25 x 16 x 14)
= 1.1 MN/m2
Section C: Although this section is tapered on one side only, since the angle is small the error in assuming it is tapered on both sides will be negligible. The included angle is taken as 8".
zyxwv zyxwvut zyx H4 = H3 + Ltan8" = 1.28
At
C3
+ 40 tan 8" = 6.9 mm
)j= 494.5
s1
6 = 1/3(494.5) tan 4" = 11.52 s  ~
At C4 y. =   6Q
TH:

7~
6 x 109.6 x = 16.9 s  ~ x 260 x 103 x (6.9 x 10312
i = 1/3(16.9)tan4" = 0.39 sl
zyxw zy zyxwv zyxw zy zy I'):( Analysis of polymer melt flow
382 As before
(Z,"]
psM= A [l . 2n tana from Fig. 5.3,
t3
= 2.1 x lo5 Nm2 at y = 494.5 2.1 x 1 6 = 0.6tan4"
sl
[' (z)] 1.28

= 3.36 MNlm2 Also
 3. PEB 2

($332]
k = 11.52 sl so from Fig. 5.3 a 3 = 2.6 x lo6 Nm2 (ie 2.25 x 1 6 x 11.52) PEM =
2.6 x lo6 . 2
[
 
= 1.26 MNlm2
In this case there will also be a pressure loss due to flow convergence at the die entry. This may be obtained from (5.47).
At
C4,
zyxw zyx zyxwvut
9
=7 6Q = 16.9, so Q = 4 x lo3 Nsm2, h = 2.25 x lo5 Nsm2 TH4
4 Po = (16.9)(4 x lo3 x 2.25 x lO5)'l2 1.9 = 1.07 MNlm2
So the total pressure drop through the die is given by
P = 3.77 + 6.9 + 1.1 + 3.36 + 1.26 + 1.07 = 17.5 MN/m2
Example 5.6 Estimate the dimensions of the tube which will be produced by the die in Example 5.5 assuming that there is no drawdown.
Solution Since the final section of the die lips is not tapered it may be assumed that the swelling at the die exit is due to shear effects only. At exit,
y. =   'Q
TH2
 1.64
103 sl
zyxwvut zyxwvu zyxwvu zyxwv zyxwvu zyxwvuts
Analysis of polymer melt flow
383
From Fig. 5.3, r = 3.3 x 1 6 Nm2 and G = 5 x lo4 Nm2
r 3.3 x 1 6 = 6.6 G 5.0 x 104 Then using equations (5.52) and (5.53), or more conveniently Fig. 5.11, the swelling ratios may be obtained as
So recoverable strain,
YR =  =
BSH = 2.31 and BST = 1.52
Therefore swollen thickness of film = H Ix BSH
= 0.7 x 2.31 = 1.62 mm
and swollen diameter of bubble = D x BST = 260 x 1.52 = 395 mm
Example 5.7 In many practical situations it is the dimensions of the output which are known or specified and it is necessary to work back (often using an iterative procedure) to design a suitable die. Design a die which will produce plastic film 0.52 mm thick at a linear velocity of 20 d s . The layflat width of the film is to be 450 mm and it is known that a blowup ratio of 1.91 will give the necessary orientation in the film. Assume that there is no drawdown.
Solution Using the terminology from the analysis of blow moulding in Section 4.2.5. 2(LFW) = 7tDb 2 x 450 Db = ___ = 286.5 mm n Now it makes the solution simpler to assume that the blow up ratio is given by Db/D1 (ie rather than Db/Dm).Also this seems practical because the change from D1 to Db is caused solely by inflation whereas the change from Dm to Db includes die swell effects.
. ’. D1 = 286.5/1.91 = 150 mm Then, for constant volume nDlhl = n&hb 286.5 x 0.52 hi = =lmm 150 So having obtained the dimensions of the tube to be produced, the procedure is to start by assuming that there is no die swell. This means that the die dimensions will be the same as those of the tube.
zyxw
6Q Apparent shear rate, i/ = TH2
384
zyxwvuts zyxwvu zyxw zyxwvu zyxw Analysis of polymer melt flow
but volume flow rate, Q = VTH
where V is the velocity of the plastic melt.
p = 6V
H 6 = x 20  120 s1 1
from Fig. 5.3, t = 1.3 x 16 N/m2 and G = 3 x 104 N/m2 So recoverable shear strain, YR, is given by t )/R==
G
1.3 x 16 = 4.33 3x104
Assuming that swelling results from shear effects only then from Fig. 5.13 at YR = 4.33, the swelling ratios are
BSH= 1.81 and BST = 1.35
The initial die dimension must now be adjusted to allow for this swelling. New die gap = H' = 1/1.81 = 0.55 mm R x 150
New die circumference = T' = = 349 mm 1.35
The volume flow rate, Q, will be constant so the velocity of the melt in the die will also be adjusted. Q = VTH = V'T'H'
New shear rate, From Fig. 5.3,
=
6V' H'
~
t = 2.36 x
 6 x 20 x 2 x 0.55
1.35
= 589 s  ~
lo5 N/m2 and G = 4 x
so
YR
104 N/m2
= 5.9
and from Fig. 5.13 BSH = 2.18
and BST = 1.48
1 So new die gap = HI' = = 0.459 mm 2.18 II x 150 new die circumference = TI' =  318 mm 1.48
zyxwvu zyxwv zyxw zyx zyxwv zyxwvu zyx 385
Analysis of polymer melt flow
If this iterative procedure is repeated again the next values obtained are
die gap, H"' = 0.455 mm R x 150 die circumference, T'" = ___ mm 1.49 These values are sufficiently close to the previous values so the die exit dimensions are Gap = 0.455 mm R x 150 Diameter = = 100.67 mm 1.49 x ~t The shear rate, 9, in the die land is 6 x 20 x 1.49 x 2.2 . Y= 0.455 = 864.5 S'
From Fig. 5.3 it may be seen that this exceeds the shear rate for nonlaminar flow (approximately 30 s') so that the entry to this region would need to be streamlined. Fig. 5.3 also shows that the extensional strain rate, k, in the tapered entry region should not exceed about 15 sl if turbulence is to be avoided. Therefore since
k = 1/39tana
=tan'
()3
x 15
864.5 = 2.97"
So the full angle of convergence to the die land must be less than (2 x 2.97")= 5.94". To complete the die design it is likely that a third tapered section will be necessary as shown in Fig. 5.20. This will be designed so that the entry to the die is compatible with the outlet of the die body on the extruder. The maximum angle of convergence of this section can be estimated as shown earlier and the lengths of the two tapered sections selected to ensure the angle is not exceeded for the fixed die inlet dimension. If the length of the 5.94" tapered region is chosen as 10 mm it may be shown that the maximum angle of convergence for the entry to this taper is 58.5". If the length of this section is fixed at 40 mm and the annular gap at the exit from the extruder is 16 mm, then a suitable angle of convergence would be about 40".
Example 5.8 It is desired to blow mould a plastic bottle with a diameter of 60 mm and a wall thickness of 2 mm. If the extruder die has an annular slot of
zyxwvutsr zyxw zyxwvu zyxwv zyxwvu zyxw zyxwvut zyxwvutsr zyxwv
386
Analysis of polymer melt flow
outside diameter = 32 mm and inside diameter = 28 mm, calculate the output rate needed from the extruder and recommend a suitable inflation pressure. Use the flow characteristics given in Fig. 5.3. Density of molten polythene = 760 kg/m3.
Solution In the analysis of blow moulding in Section 4.2.7, it was shown that the thickness, h, of the inflated bottle is given by
where hd = die gap = 2 mm 0, = mould diameter = 60 mm Dd = die diameter = 1/2(28 + 32) = 30 mm
so
2x60
BST
=
BST = 1.26
From Fig. 5.11 at BST = 1.26, y~ = 3.15
so
3.15 = t / G
From Fig. 5.3 it is now necessary to determine the combination of satisfy this equation. For example, at 9 = 5 s' G = 1.5 x
SO
At
lo4 N/m2,
t=5 x
lo4 N/m2,
t = 5.9 x
lo4 N/m2, t / G = 4.2
lo4 N/m2,
t = 5.9 x
lo4 N/m2, t / G = 3.1
8.8 x
x
lo4 N/m2
t / G = 2.93
y = 50 s'
G = 2.5 x
At
lo3 = 4.4
y = 10 s'
G = 1.9 x
Therefore the latter combination is correct.
and
t and
Q=
i o x IT x 30 x 22 x
= 1.26 x
6
10~ = 1.26 x
m3/s
x 760 x 3600 = 3.45 kg/hOw
G to
z
zyxwvu zyxw zyxwv zyxw zyxwv zyxwv zyxw
Analysis of polymer melt flow
387
To calculate the inflation pressure it is necessary to get the melt fracture stress. From Fig. 5.3 it may be seen that this is 4 x lo6 N/m2 Therefore since the maximum stress in the inflated bubble is the hoop stress, a, the maximum inflation pressure, P , is given by 2 x 2 x 4 x lo6 60
2ha p==
Dm
= 0.13 MN/m2
h
7
“1
f
I
I
i
I
I
I
I
I
1
Example 5.9 Calculate the time taken to inflate the bottle in the previous example if the inflation pressure is 50 kN/m2. The flow curves given in Fig. 5.3 may be used. Solution It is necessary to derive an expression for the inflation time. Referring to Fig. 5.22 where R is the radius of the inflated tube at any time, t, and h, is the wall thickness at this time, then a force balance on the shaded element gives (for unit length).
);(
(RdB)PI  ( R + h,)dB P2  2 a h, sin
(t)
=O
zyxwvu
Letting sin
=
df3
and P2 = 0,
RP1 = a h ,
Now a = LE where A is the tensile viscosity.
then
(5.72)
388
zy zy
Analysis of polymer melt flow Mould wall
zyxw zyxw
zy zyxwv
Fig. 5.22 Inflation of Parison to Mould Wall
b is the extensional strain rate and is given by
.
E=
change in length per unit time  (R original length
Substituting into (5.72) we get
A dR
RPI = ht R dt
+ dR)dO  RdO  1 dR Rdedt
R dt
(5.73)
Analysis of polymer melt flow
zyxwvu zyx zyxwvu 389
Before this can be integrated, hr needs to be expressed as a function of R or t. Assuming constant volume of the parison
zyx zyxwv zyxwvu Rhr = Rlhl
Hence we can write
or expressing this in terms of the original die dimensions (see Blow Moulding, Chapter 4),
{
Inflation time, t =  1  B& PiDd
($)}
(5.74)
Using the information given and with A = 2.2 x lo5 Ns/m2 (from Fig. 5.3) then 2.2 105 x 1.26 x 2 1  1.262 t= 50 x lo3 x 30 t = 0.08 seconds
(g)}
{
Example 5.10 During the blow moulding of polythene bottles the parison is 0.3 m long and is left hanging for 5 seconds. Estimate the amount of sagging which occurs. The density of polythene is 760 kg/m3
Solution Consider the small element of parison as shown as shown in Fig. 5.21. (a) Elastic Strain From the relationship between stress, strain and modulus Fdx
SL = AE
zyx zyxwv PL2 xdx = 
So total extension = E
2E
0
PL
SOElastic Strain = ER = 2E
390
zy
zyxwvut zyx zyx zyx zyxw zyxw Analysis of polymer melt flow
(b) Viscous Strain
force weight below YY The stress on the element = area area pnDlhl dx = p dx XDlhl
So total stress, cr =
1
p dx = pL
0
Now the viscous strain on the element is given by cr
SE, = 0. dt = dt
h
0
0
Therefore the total strain,
E
= ER
+2E
PLt h
 PL
E=pL
zyxwv
+ E,
+
[;E
I:
(5.75)
zyxwv
Note that this solution applies for values of t less than the relaxation time @ / E ) for the process. This is generally the case for blow moulding. For the situation given,
stress,
cr = pL = 760 x 9.81 x 0.3 = 2.24 x lo3 N/m2
From Fig. 5.3, A = 2.25 x 105 Ns/m2.
.
2.24 103 = 0.01 2.25 x 105 Extrapolating to the left on Fig. 5.3, it may be found that at a strain rate of 0.01, E = 1.9 x lo4 N/m2. So characteristic time = A/E = 11.6 s' Therefore since the parison sag time is less than this, the above expression may be used to calculate the amount of stretching 1 = 0.11 E = 760 x 9.81 x 0.3 [2 x 1.9 x 10" 42.2 x 105 So extension = 0.11 x 0.3 m Also, since cr = h b,
= 33 m
E
=
zyxwvu zyxwvu zyxwv zyxw zyxwv zyxwv zyxw 39 1
Analysis of polymer melt flow
5.12 Analysis of Heat Transfer during Polymer Processing
Most polymer processing methods involve heating and cooling of the polymer melt. So far the effect of the surroundings on the melt has been assumed to be small and experience in the situations analysed has proved this to be a reasonable assumption. However, in most polymer flow studies it is preferable to consider the effect of heat transfer between the melt and its surroundings. It is not proposed to do a detailed analysis of heat transfer techniques here, since these are dealt with in many standard texts on this subject. Instead some simple methods which may be used for heat flow calculations involving plastics are demonstrated. Fouriers equation for nonsteady heat flow in one dimension, x , is a2T _1 _aT a at ax2 where T is temperature and a! is the thermal diffusivity defined as the ratio of thermal conductivity, K,to the heat capacity per unit volume 
a=
K
PCP
where p is density and C p is specific heat. Most materials manufacturers supply data on the thermal diffusivity of their plastics but in the absence of any information a value of 1 x lov7 m2/s may be used for most thermoplastics (see Table 1.8 and Table 5.1). Solutions to Fourier’s equation are in the form of infinite series but are often more conveniently expressed in graphical form. In the solution the following dimensionless groups are used. at Fo = (5.76) (1) Fourier Number, X2
where t is time and x is the radius of the sphere or cylinder (or half thickness of the sheet) considered. In the case of a flat sheet, if the heatingkooling is from one side only then the dimension, x , is taken as the full thickness. (2) Temperature Gradient,
AT =
~
T,  T m Ti  T ,
(5.77)
where Ti = Initial uniform temperature of the melt T, = Temperature of heating or cooling medium T t = Temperature at time t . Fig. 5.23 show the solution to Fourier’s equation in terms of the temperature gradient at the centre line of section considered and the Fourier Number for
392
zy
zyxwvu Analysis of polymer melt flow
zyxwvuts zyxwvut zyxwvutsrqponm 0.6
i
CR
g!
aI
e
0.5
0.4
0.3
0.2
0.1 0
0.2
0.4
0.6
0.8
1
Fourla's number Fig. 5.23 Dimensionless Temperature Data for two Geometries
the cases of a flat sheet and a cylinder respectively. In each case it is assumed that there is no resistance to heat transfer at the boundary between the melt and the heating cooling medium. The way in which this data may be used is illustrated by the following example.
zyxwvu zyx
Example 5.11 A polyethylene injection moulding is in the form of a flat sheet 100 mm square and 3 mm thick. If the melt temperature is 230"C, the mould temperature is 30°C and the plastic may be ejected at a centreline temperature of 90"C, estimate (a) the temperature of the material at the centre of the moulding after 7 seconds (b) the time taken for the centre of the moulding to reach the ejection temperature of 90°C (c) the time taken for the centre of the moulding to cool to 60°C in air at 20°C after ejection from the mould. Comment on the meaning of the answer. The heat transfer coefficient for the air is 20 W/m2 K and the thermal conductivity of the polyethylene is 0.25 W/mK. Solution (a) Fourier Number is
Analysis of polymer melt flow
zy zyxwvu zyxwv zyxw zy zy zyxwv 393
= 0.31
From Fig. 5.23 the temperature gradient is 0.58
Tt  30 230  30 T , = 146" C
0.58 =
(b) For freezeoff to occur the temperature gradient A T = AT=
From Fig. 5.23, Fo = 0.59
Tf Ti44
Ttn  T M
90  30 = 0.3 230  30
at 0.59 = X2
or
t
0.59 x (1.5 x 103)2 1 x 107 = 13.3 s
=
(c) The above analysis relates to the situation where there is little resistance to heat transfer between the plastic and the heating/cooling medium, ie conduction. In situations where the plastic is in contact with a fluid such as air, the main mode of heat transfer will be convection. The interrelationships between conduction and convection may be expressed by the Biot Number, Bi. This is given by hx Bi = (5.78) K where h = heat transfer coefficient (typically 510 W/m2 K for still air and 10 100 W/m2 K for forced air) K = thermal conductivity of the plastic n = full or half thickness of the plastic as described above. A large Biot Number means that conduction controls the energy transfer Wfmm the plastic and large temperature gradients will exist in the plastic. A small Biot Number means that convection is the dominant factor. The above analysis was for conduction heat transfer (Bi + 00). When the plastic moulding is taken out of the mould we need to check the value of Bi. In this case Bi =
20 x 1.5 x 0.25
103
= 0.12
394
zyxwvuts zyxwvu zyxwvu zyxw Analysis of polymer melt flow
The dimensionless temperature gradient is
Fig. 5.24 shows the modified ATIF, graph for a flat sheet for different values of Bi. In this case 1/Bi = 8.33. So from Fig. 5.24
zyxw
Foullers number
Fig. 5.24 Dimensionless Temperature Data for a Flat Sheet (ConductiodConvection)
Hence the plastic cools by 140°C (230°C to 90°C) in 13.3 seconds when it is in contact with the mould but it takes 90 seconds to cool a further 30°C when it emerges out into the air. This highlights the much faster cooling rate achieved in the mould. Some typical moulding data for a range of plastics are given in Table 5.1. Note that the demoulding temperature will be generally about 30°C below the Freezeoff temperature in order to ensure that the moulding is sufficiently solid for handling. The above analysis illustrates how to estimate the cooling time using the relationship between the temperature gradient AT and the Fouriers Number
Analysis of polymer melt flow
zyxwvu 395
zyxwvuts zyxwvu zyx zyxwv zyxwv Table 5.1
Plastic
LDPE Polypropylene Polystyrene PVC POM Acrylic Polycarbonate Nylon 66 ABS
Moulding temperature
Mould temperature
Freezeoff temperature
("C)
("C)
("(3
230 250 230 180 210 250 300 290 230
30 40 50 40
90 135 130 140 130 160 200 240 140
60 50 90 80
60
Thermal diffusivity (m2/s)
1.1 1.1 0.8 1.2
107 107 107 107 0.9 x 107 0.9 107 1.0 107 1.3 107 0.9x 107
F,. A number of empirical relationships have also been proposed. Two of the more useful equations take the form
(a) for flat sheet 4x2
time, t = 1n
R24
or (b) for cylinder
zyxw zyxwv
time, t = 1.7r2 In $4
4
( R A T )
(g)
(5.79)
(5.80)
The reader may wish to check the predictions of freezeoff time for the data in the above Example.
Example 5.12 Estimate the heat transfer from the die to the melt as it passes through the die land in Example 5.5.
Solution
Volume of die land = RDHL = (r 260 0.7 4 1091m3 260 0.7 4 x 109 Residence time = 109.6 x = 2.08 x s at
Fourier number = X2
1 0  ~ 2.08 x (0.35 x 10312 = 0.017
Fo =
1
396
zyxwvu zy zyxwv zyxwv zyxwvu zyxwvut zyxw Analysis of polymer melt flow
From Fig. 5.23 it may be seen that the centre line temperature gradient at this Fourier Number is almost 1.
T3  T2 1 Since AT = T1  T2 then T3 2 T1
Thus the melt temperature after 2.08 x seconds is the same as the initial melt temperature ( T l ) so that as the melt passes through the die land it is relatively unaffected by the temperature of the die. Any temperature rise which occurs in the melt as it passes through this section will be as a result of the work done on the melt and may be estimated using (5.64).
P PCP 3.66 x lo6
Temperature rise = 
So temperature rise =
760 x 2.5 x 103 = 1.9"C
Example 5.13 Derive an expression for the flow length of a power law fluid when it is injected at constant pressure into a rectangular section channel assuming (a) the flow is isothermal (b) there is freezing off as the melt flows (ie nonisothermal flow). Solution (a) As shown earlier the flow rate of a power law fluid in a rectangular section is given by
During any increment of time, dt, the volume of the fluid injected into the channel is Qdt. This will be equal to the increase in volume of the fluid in the channel Qdt = THdl So from above
..
zyxwvu zyxw zyxwvut zyxwv zyxw 397
Analysis of polymer melt flow
The volume flow rate at any instant in time may be determined by substituting for L in equation (5.81). (b) If the melt is freezing off as it flows then the effective channel depth will be h instead of H as shown in Fig. 5.23. Therefore the above expression may be written as (5.83)
This equation cannot be integrated as simply as before because h is now a function of time. Fig. 5.26 shows how the depth of the cavity changes with time as the melt flows. Barrie has investigated this situation and concluded that the freezingoff could be described by a relation of the form Ay = Cr'
(5.84)
Frozen layer H
h
Molten

PlaStk
zyxwvuts Frozen laver
Fig. 5.25 Flow of Molten Polymer into a Cold Mould
where C and s are constants and Ay is the thickness of the frozen layer as shown in Fig. 5.25. For most polymer melt flow situations, Barrie found that s = 113. From (5.84) using the boundary condition that t = t f (freezeoff time) at
zyxwv
Ay = H/2
then C = (H/2t$I3)
zy zy
Analysis of polymer melt flow
398
zyxwvutsr
4
3.5 1
E g
3
8
2
2.5
$
2
3 5
1.5
P f E
2
0
zyxwvut zyxwvu
1 0.5 0
zyxwvut
0
10
5
15
20
Time (s)
Fig. 5.26 Variation of Cavity Depth with Time
also 2Ay = ( H  h) so in (5.84)
,=,(I
(t)’”)
So substituting this expression for h into (5.83), then
This may then be integrated to give
(5.85)
Analysis of polymer melt flow
399
Similar expressions may also be derived for a circular section channel and for the situation where the injection rate is held constant rather than the pressure (see questions at the end of the chapter). In practical injection moulding situations the injection rate would probably be held constant until a preselected value of pressure is reached. After this point, the pressure would be held constant and the injection rate would decrease. Note that for a Newtonian fluid, n = 1, so for the isothermal case, equation (5.82) becomes.
zyxwvu zyxwv zyxwvu zyxwvuts zyxw zyxw zyxw zy (9) 1I2
L = 0.408
H
and for the nonisothermal case, equation (5.86) becomes
(?)
112
L = 0.13
H
For the nonisothermal cases the freezeoff time, t f , may be estimated by the method described in Example 5.1 1.
Example 5.14 A power law fluid with constants ~0 = 1.2 x 104 Ndm2 and n = 0.35 is injected through a centre gate into a disc cavity which has a depth of 2 mm and a diameter of 200 mm. If the injection rate is constant at 6x m3/s, estimate the time taken to fill the cavity and the minimum injection pressure necessary at the gate for (a) Isothermal and (b) Nonisothermal conditions. Solution (a) hothenna2 Situation. If the volume flow rate is Q, then for any increment of time, d t , the volume of material injected into the cavity will be given by (Qdt).During this time period the melt front will have moved from a radius, r, to a radius ( r d r ) . Therefore a volume balance gives the relation
+
Qdt = 2nrHdr
where H is the depth of the cavity. Since the volume flow rate, Q, is constant this expression may be integrated to give
For the conditions given t=
zyxwv zyxwvu
~ ( 1 0 0x 1 0  ~ )(2 ~x
6x = 1.05 seconds
400
zyxwvut zyxw zyxwv zyxwv zyx Analysis of polymer melt flow
It is now necessary to derive an expression for the pressure loss in the cavity. Since the mould fills very quickly it may be assumed that effects due to freezingoff of the melt may be ignored. In Section 5.4(b) it was shown that for the flow of a power law fluid between parallel plates
Q=
(w) n+l
TVoH
Now for the disc, T = 2nr and substituting for VOfrom (5.27)
zyxwv
Now letting P I = 0 at R1 = R and P2 = P at R2 = r
now P = PO at r = 0
So for the conditions given
= 12.42 MN/m2
401
Analysis of polymer melt flow
Note that if POis substituted back into the expression for P then the expression used earlier (Chapter 4) to calculate the mould clamping force is obtained. That is
zyxwvu zyxwvu P=Po{l(t,ln}
zyxw zyxw
(b) Nonisothermal Situation. In this case the injection pressure will need to be higher because as the melt flows the cavity effectively gets thinner due to the freezingoff of the melt as it makes contact with the relatively cold mould.
but when nonisothermal conditions apply, H = H ( t ) , ie the cavity thickness varies with time due to the build up of a frozen layer at the mould. As shown in the previous Example, the variation of cavity thickness with
where 's' is often taken as 113.
zyxwv zyxwvut zyxwv
For the conditions given, Ti = 230°C T , = 90°C T , = 30°C, the freezeoff time may be calculated as shown in Example 5.11. Thus t f = 5.8 seconds. Thus
{
2n+l
1
(t)'")
=
{
1.7
1  (:)'I3}
=0.24
So, for nonisothermal conditions 12.42  51.3 MN/m2 Ap=0.24 5.13 Calculation of Clamping force
(a) Isothermal Situation
z
It may be seen from the above analysis and that in Chapter 4 for the calculation of clamping force on an injection moulding machine the Mean Effective pressure (MEP) across the cavity may be obtained from
{:I:}
(MEP) A = nR2Po where A = projected area (rR2, for a disc mould).
(5.87)
402
zyxwvuts zyxwv zyxw zyxw zyxwvuts zyxw
zyx Analysis of polymer melt flow
Hence, for the isothermal situation
and for a constant injection rate, Q = ItR2H/t
so,
2n
+1
(2n + 1)2"+'
MEP =
(2n + 1 ) 2"+' rn' 2 n . (3  n )
(5.88)
Thus for any plastic where the Power Law constants are known, the clamping force can be calculated for a given radius, R, cavity depth, H , and fill time, C . Fig. 5.27 shows the variation of MEP with flow ratio (RIH) for spreading flow in discs of different depths. The material is polypropylene and the constant injection rate is 3.4 x m3/s. This is a high injection rate but has been chosen because the clamp forces predicted by this diagram are representative of those occurring in real moulding situations (even though it is based 1.0 mm
1.5 mm
60
0
Fig. 5.27 Variation of Cavity Pressure with Flow Ratio
Analysis of polymer melt flow
zyxwvu zyxwv zyxwv zyxw 403
on isothermal conditions). Note that the clamp force is calculated simply by multiplying the mean effective pressure (MEP) by the projected area of the moulding, as illustrated in Chapter 4. For plastics other than polypropylene it would be necessary to produce a similar set of curves using equation (5.88) and the Power Law data in Table 5.2. Table 5.2
zyxw zyxwv
Qpical Power Law Parameters for Plastics Material
Temperature ("C)
LDPE PVC Polypropylene Acetal (POM) Polystyrene ABS PMMA Polycarbonate Nylon 66
qo(Ns" m*)
170 170 230 210 230 230 230
0.85 x 0.36 x 0.85 x 2.0 x
lv' 104
104 104
1.4 x 10" 1.95 x 1v'
3.0 x 10" 3.6 x 10" 0.8 x 10"
290 290
n
0.33 0.67 0.33 0.33 0.33 0.33 0.33 0.5 0.67
(b) Nonisothermal Situation Once again
zyxwv
but in this case, the thickness H is a function of time.
H ( t ) = H {I
 (;)'I3}
and the constant volume flow rate Q = n R 2 H / f where f is the fill time for the cavity.
Fig. 5.28 shows a comparison of the isothermal and nonisothermal situations for polypropylene. When pressure is plotted as a function of injection rate, it
z z y x w v u t s r q p o n m l k j i h zyxwvutsrqpo
zyxwvuts zyxwvuts zyxwvutsrqponm Analysis of polymer melt flow
404
25
7
I
s zyxwv II h
m
20

I
v
f
15
8
d0.
g
..
.+
..
Nonisothermi
10
5: Q
c
3
5
v
zyxwvuts )thermal
0
0.0002
0
0.0001
0.0004
0.0003
O.OOO8
0.0006
0.0005
0.0007
0.001
0.0009
Injection rate (@Is)
Fig. 5.28 Variation of Cavity Pressure Loss with Injection Rate
may be seen that for the isothermal situation the pressure increases as the injection rate increases. However, in the situation where the melt freezes off as it enters the mould, the relationship is quite different. In this case the pressure is high at high injection rates, in a similar manner to the isothermal situation. In fact at extremely high injection rates the two curves would meet because the melt would enter the mould so fast it would not have time to be affected by the melt temperature. However, in the nonisothermal case the pressure is also high at low injection rates. This is because slow injection gives time for significant solidification of the melt and this leads to high pressures. It is clear therefore that in the nonisothermal case there is an optimum injection rate to give minimum pressure. In m3/s for the situation considered Fig. 5.28 this is seen to be about 3.0 x here. This will of course change with melt temperature and mould temperature since these affect the freezeoff time, t f , in the above equations. Some typical values for r)o and n are given in Table 5.2. The viscosity flow curves for these materials are shown in Fig. 5.17. To obtain similar data at other temperatures then a shift factor of the type given in equation (5.27) would have to be used. The temperature effect for polypropylene is shown in Fig. 5.2.
zyxwvu
Example 5.15 During injection moulding of low density polyethylene, 15 kg of material are plasticised per hour. The temperature of the melt entering the
zyxwvut zyxwvu zyxwv zyxwvut
Analysis of polymer melt flow
405
mould is 190°C and the mould temperature is 40°C. If the energy input from the screw is equivalent to 1 kW, calculate (a) the energy required from the heater bands (b) the flow rate of the circulating water in the mould necessary to keep its temperature at 40 f 2"
Solution The steady flow energy equation may be written as qW=Ah
(5.90)
where q is the heat transfer per unit mass W is the work transfer per unit mass h is enthalpy Enthalpy is defined as the amount of heat required to change the temperature of unit mass of material from one temperature to another. Thus the amount of heat required to change the temperature of a material between specified limits is the product of its mass and the enthalpy change. The enthalpy of plastics is frequently given in graphical form. For a perfectly crystalline material there is a sharp change in enthalpy at the melting point due to the latent heat. However, for semicrystalline plastics the rate of enthalpy change with temperature increases up to the melting point after which it varies linearly with temperature increases up to the melting point after which it varies linearly with temperature as shown in Fig. 5.29. For amorphous plastics there is only a change in slope of the enthalpy line at glass transition points. Fig. 5.29 shows that when LDPE is heated from 20°C to 190°C the change in enthalpy is 485 H k g .
zyxwvu zyxwv
Temperature ("c)
Fig. 5.29 Enthalpy Variation with Temperature
406
zy
zyxwvu zyxw zyx z Analysis of polymer melt flow
(a) In equation (5.90) the sign convention is important. Heat is usually taken as positive when it is applied to the system and work is positive when done by the system. Hence in this example where the work is done on the system by the screw it is regarded as negative work. So using (5.90) for a mass of 15 kg per hour q  (4)= 15
(485
1 60
x x
)601
q = 1.02kW
The heater bands are expected to supply this power. (b) At the mould there is no work done so in terms of the total heat absorbed in cooling the melt from 190°Cto 40°C. q = mAh
(485 40) x 60 60 = 1.85 kW
This heat must be removed by the water circulating in the mould at a rate, Q
zyxwvu q = QAh
or by definition of enthalpy
q = QC,AT
where C, is the specific heat (= 4.186 kJ/kg"C for water) and AT is the temperature change (= 4°C i.e. f2"C)
1.85 = Q x 4.186 x 4 Q = 0.11 kg/s = 0.11litreds
It is also possible to estimate the number of cooling channels required. If the thermal conductivity of the mould material is K then the heat removed through the mould per unit time will be given by K * A( A T ) 4=
where AT is the temperature between the melt and the circulating fluid Y is the distance of the cooling channels from the mould A is the area through which the heat is conducted to the coolant. and This is usually taken as half the circumference of the cooling channel multiplied by its length.
Analysis of polymer melt flow
zy zyxwvu zyxwv zyxwvu zyxwv 407
KnDL(AT) 4= 2Y L=
2y9 KnD(AT)
The K value for steel is 11.5 cal/m.s.T, so assuming that the cooling channels have a diameter of 10 mm and they are placed 40 mm from the cavity, then 2 x 40 x 10~x 1.85 x io3 L= 11.5 x 4.2 x n x 10 x x (190  40) = 0.65 m If the length of the cavity is 130 mm then five cooling channels would be needed to provide the necessary heat removal.
Bibliography Pearson, J.R.A. Mechanics of Polymer Processing, Elsevier Applied Science, London (1985) Throne, J.L. Plastics Process Engineering, Marcel Dekker, New York (1979) Fenner, R.T.Principles of Polymer Processing, Macmillan, London, (1979) Tadmor, Z. and Gogos, C.G. Principles of Polymer Processing, Wiley Interscience, New York ( 1979) Brydson, J.A. Flow Properties of Polymer Melts, George Godwin, London (1981) Grober, H. Fundamentals of Heat Transfer, McGrawHill, New York (1961) Cogswell, F.N. Polymer Melt Rheology, George Godwin, London (1981) Carreau, P.J., De Kee, D. and Domoux, M. Can. J. Chem Eng., 57 (1979) p. 135. Rao, N.S., Design Formulasfor Plastics Engineers, Hanser, Munich (1991). Kliene, I., Marshall, D.J. and Friehe, C.A. J. SOC. Plasr. Eng., 21 (1965) p. 1299. Muenstedt, H. Kunsrsroffe, 68 (1978) p. 92.
Questions 5.1 In a particular type of cone and plate rheometer the torque is applied by means of a weight suspended on a piece of cord. The cord passes over a pulley and is wound around a drum which is on the same axis as the cone. There is a direct drive between the two. During a test on polythene at 190°C the following results were obtained by applying a weight and, when the steady state has been achieved, noting the angle of rotation of the cone in 40 seconds. If the diameter of the cone is 50 mm and its included angle is 170", estimate the viscosity of the melt at a shear stress of 104 N/m2.
zyxwvuts zyxwvutsrq zyx
Weight (g)
50
100
200
500
loo0
2000
Angle (e")
0.57
1.25
2.56
7.36
17.0
42.0
5.2 Derive expressions for the velocity profile, shear stress, shear rate and volume flow rate during the isothermal flow of a power law fluid in a rectangular section slit of width W, depth H and length L. During tests on such a section the following data was obtained.
Flow rate (kg/min) Pressure drop (MN/m2)
0.21
0.4
0.58
0.8
1.3
2.3
1.8
3.0
4.0
5.2
7.6
12.0
408
zy zyxwvuts zyxwvu Analysis of polymer melt flow
If the channel has a length of 50 mm, a depth of 2 mm and a width of 6 mm, establish the applicability of the power law to this fluid and determine the relevant constants. The density of the fluid is 940 kg/m3.
5.3 The viscosity characteristics of a polymer melt are measured using both a capillary rheometer and a cone and plate viscometer at the same temperature. The capillary is 2.0 mm diameter and 32.0 mm long. For volumetric flow rates of 70 x m3/s and 200 x m3/s, the pressures measured just before the entry to the capillary are 3.9 M N h Z and 5.7 MN/m*, respectively. The angle between the cone and the plate in the viscometer is 3" and the diameter of the base of the cone is 75 mm. When a torque of 1.18 Nm is applied to the cone, the steady rate of rotation reached is observed to be 0.062 r d s . Assuming that the melt viscosity is a power law function of the rate of shear, calculate the percentage difference in the shear stresses given by the two methods of measurement at the rate of shear obtained in the cone and plate experiment.
zyxwvu zyxwvu
5.4 The correction factor for converting apparent shear rates at the wall of a circular cylindrical capillary to true shear rates is (3n + 1)/4n, where n is the power law index of the polymer melt being extruded. Derive a similar expression for correcting apparent shear rates at the walls of a die whose crosssection is in the form of a very long narrow slit. A slit die is designed on the assumption that the material is Newtonian, using apparent viscous properties derived from capillary rheometer measurements, at a particular wall shear stress, to calculate the volumetric flow rate through the slit for the same wall shear stress. Using the correction factors already derived, obtain an expression for the error involved in this procedure due to the melt being nonNewtonian. Also obtain an expression for the error in pressure drop calculated on the same basis. What is the magnitude of the error in each case for a typical power law index n = 0.37? 5.5 Polyethylene is extruded through a cylindrical die of radius 3 mm and length 37.5 mm at a rate of 2.12 x m3/s. Using the flow curves supplied, calculate the natural time of the process and comment on the meaning of the value obtained.
zyxwvut
5.6 Polythene is passed through a rectangular slit die 5 mm wide, 1 mm deep at a rate of 0.7 x m3/s. If the time taken is 1 second, calculate the natural time and comment on its meaning. 5.7 In a plunger type injection moulding machine the torpedo has a length of 30 mm and a diameter of 23 mm. If, during the moulding of polythene at 170°C (flow curves given), the plunger moves forward at a speed of 50 mm/s estimate the pressure drop along the torpedo. The barrel diameter is 25 mm.
zyxwvu zy zyxwvutsrqp zyxwvu zyxwvu zyx
Analysis of polymer melt flow
409
5.8 The exit region of a die used to extrude a plastic section is 10 mm long and has the crosssectional dimensions shown below. If the channel is being extruded at the rate of 3 d m i n calculate the power absorbed in the die exit and the melt temperature rise in the die. Flow curves for the polymer melt are given in Fig. 5.3. The product pCp for the melt is 3.3 x 106.
5.9 The exit region of a die used to extrude a plastic channel section is 10 mm long and has the dimensions shown below. If the channel is being extruded at the rate of 3 d m i n . calculate the power absorbed in the die exit, and the dimensions of the extrudate as it emerges from the die. The flow curves in Fig. 5.3 may be used.
All dimensions in mm
zyxwvu
5.10 During extrusion blow moulding of 60 mm diameter bottles the extruder output rate is
m3/s. If the die diameter is 30 mm and the die gap is 1.5 mm calculate the wall thickness of the bottles which are produced. The flow curves in Fig. 5.3 should be used. 5.11 Polyethylene is injected into a mould at a temperature of 170°C and a pressure of 100 MN/m2. If the mould cavity has the form of a long channel with a rectangular crosssection 6 mm x 1 m m deep, estimate the length of the flow path after 1 second. The flow may be assumed to be isothermal and over the range of shear rates experienced ( lo3 1 6 sl) the material may be considered to be a power law fluid.
46 x
5.12 Repeat the previous question for the situation in which the mould temperature is 60°C and the freezeoff temperature is 128°C. What difference would it make if it had been assumed that the material was Newtonian with a viscosity of 1.2 x I d Ns/m*. 5.13 During the blow moulding of polypropylene bottles, the parison is extruded at a temperature of 230°C and the mould temperature is 50°C. If the wall thickness of the bottle is 1 mm and the bottles can be ejected at a temperature of 120°C estimate the cooling time in the mould. 5.14 An injection moulding is in the form of a flat sheet 100 mm square and 4 mm thick. The melt temperature is 23OoC, the mould temperature is 30°C and the plastic may be ejected from the mould at a centreline temperature of 90°C. If the runner design criterion is that it should be ejectable at the same instant as the moulding, estimate the required runner diameter. The thermal diffusivity of the melt is 1 x lo' m2/s. 5.15 For a particular polymer melt the power law constants are = 40 kN.s"/m and n = 0.35. If the polymer flows through an injection nozzle of diameter 3 mm and length 25 mm at a rate of 5 x 1 0  ~ m3/s, estimate the pressure drop in the n o d e . 5.16 Polythcne at 170'C is used to injection mould a disc with a diameter of 120 mm and thickness 3 nun. A sprue gate is used to feed the material into the centre of the disc. If the
410
zyxwvuts zy zy Analysis of polymer melt flow
injection rate is constant and the cavity is to be filled in 1 second estimate the minimum injection pressure needed at the nozzle. The flow curves for this grade of polythene are given in Fig. 5.3.
zyxwvutsr zyxw
5.17 During the injection moulding of a polythene container having a volume of 4 x m3, the melt temperature is 170"C, the mould temperature is 50°C and rectangular gates with a land length of 0.6 mm are to be used. If it is desired to have the melt enter the mould at a shear rate of I d sI and freezeoff at the gate after 3 seconds, estimate the dimensions of the gate and the pressure drop across it. It may be assumed that freezeoffoccurs at a temperature of 114°C. The flow curves in Fig. 5.3 should be used.
5.18 Polyethylene at 170°C passes through the annular die shown, at a rate of 10 x m3/s. Using the flow curves provided and assuming the power law index n = 0.33 over the working section of the curves, calculate the total pressure drop through the die. Also estimate the dimensions of the extruded tube.
5.19 A polythene tube of outside diameter 40 mm and wall thickness 0.75 mm is to be extruded at a linear speed of 15 mm/s. Using the 170°C polythene flow curves supplied, calculate suitable die exit dimensions. 5.20 The exit region of a die used to blow plastic film is shown below. If the extruder output is 100 x m3/s of polythene at 170°C estimate the total pressure drop in the die between points A and C. Also calculate the dimensions of the plastic bubble produced. It may be assumed that there is no inflation or drawdown of the bubble. Flow data for polythene is given in Fig. 5.3.
angle = 2"
zyxwv C
Melt
Melt
5.21 A polyethylene moulding material at 170°C passes along the channel shown at a rate of 4x m3/s. Using the flow curves given and assuming n = 0.33 calculate the pressure. drop along the channel.
zyx zyxwvu zyxwvutsr 41 1
Analysis of polymer melt flow
I
all dimensions in mm
1
zyxwvut zyxwvu
5.22 A power law plastic is injected into a circular section channel using a constant pressure, P. Derive an expression for the flow length assuming that
(a) the flow is isothermal (b) the melt is freezing off as it flows along the channel.
5.23 A polymer melt is injected into a circular section channel under constant pressure. What is the ratio of the maximum nonisothermal flow length to the isothermal flow length in the same time for (a) a Newtonian melt and (b) a power law melt with index. n = 0.3.
5.24 A power law fluid with the constants 90 = 104 Ndm2 and n = 0.3 is injected into a circular section channel of diameter 10 mm. Show how the injection rate and injection pressure vary with time if.
(a) the injection pressure is held constant at 140 MN/m2 (b) the injection rate is held constant at m3/s. The flow in each case may be considered to be isothermal. 5.25 Polyethylene at 170°C is used to injection mould a flat plaque measuring 50 mm x 10 mm x 3 mm. A rectangular gate which is 4 mm x 2 mm with a land length of 0.6 mm is situated in the centre of the 50 mm side. The runners are 8 mm diameter and 20 mm long. The material passes from the barrel into the runners in 1 second and the pressure losses in the nozzle and sprue may be taken as the same as those in the runner. If the injection rate is fixed at m3/s, estimate (a) the pressure losses in the runner and gate and (b) the initial packing pressure on the moulded plaque. Flow curves are supplied. 5.26 A lace of polyethylene is extruded with a diameter of 3 mm and a temperature of 190°C. If its centreline must be cooled to 70°C before it can be granulated effectively, calculate the required length of the water bath if the water temperature is 2OoC.The hauloff speed is 0.4 m / s and it may be assumed that the heat transfer from the plastic to the water is by conduction only. 5.27 Using the data in Tables 5.1 and 5.2, calculate the flow lengths which would be expected if the following materials were injected at 100 MN/mz into a wide rectangular crosssection channel, 1 mm deep. Materials  LDPE, polypropylene, polystyrene, PVC, POM, acrylic, polycarbonate, nylon 66 and ABS. Note that the answers will give an indication of the flow ratios for these materials. The flow should be assumed to be nonisothermal. 5.28 It is desired to blow mould a cylindrical plastic container of diameter 100 mm and wall thickness 2.5 mm. If the extruder die has an average diameter of 40 mm and a gap of 2 mm, calculate the output rate needed from the extruder. Comment on the suitability of an inflation pressure in the region of 0.4 MN/m2.The density of the molten plastic may be taken as 790 kg/m3. Use the flow curves in Fig. 5.3. 5.29 During the blow moulding of polyethylene at 170°C the parison is 0.4 m long and is left hanging for 1 second. Estimate the natural time for the process and the amount of sagging which occurs. The density of the melt may be taken at 730 kg/m3.
412
zyxwvuts zyxwvut zyxwv zyxw
zyxw zyxw Analysis of polymer melt flow
5.30 The viscosity, t). of plastic melt is dependent on temperature, T, and pressure, P. The variations for some common plastics are given by equations of the form t ) / t ) ~=
1PAPand
t ) l t ) ~=
leA7
where AT = T  TR(OC), AP = P  PR (htN/m2), and the subscript R signifies a reference value. Spica1 values of the constants A and B are given below. Acrylic
Polypropylene
A (x 103)
28.32
7.53
B (x103)
9.54
6.43
LDPE
11.29 6.02
Nylon
12.97 4.22
Acetal 7.53
3.89
During flow along a particular channel the temperature drops by 40°C and the pressure drops by 50 MN/mz. Estimate the overall change in viscosity of the melt in each case. Detennine the ratio of the pressure change to the temperature change which would cause no change in viscosity for each of the above materials.
zyxwvu
APPENDIX A  Structure of Plastics
A.l Structure of Long Molecules
zyxwv
Polymeric materials consist of long chainlike molecules. Their unique structural configuration affects many of their properties and it is useful to consider in more detail the nature of the chains and how they are built up. The simplest polymer to consider for this purpose is polyethylene. During the polymerisation of the monomer ethylene, the double bond (see Fig. A.l) is opened out enabling the carbon single bonds to link up with neighbouring units to form a long chain of CH2 groups as shown in Fig. A.2. This is a schematic representation and conceals the fact that the atoms are jointed to each other at an angle as shown in Fig. A.3.
Fig. A.l
Ethylene monomer
H
H
H
H
H
I
l
l
1
1
c  c  c c  c I
I
I
I
I
H
H
H
H
H
Fig. A.2
zyxwv zyxwv
Polyethylene molecule
413
414
zyxwvut zy zyxw Structure of Plastics
U
w
H
Fig. A.3 Polyethylene molecule
In all the groups along the chain, the bond angle is fixed. It is determined by considering a carbon atom at the centre of a regular tetrahedron and the four covalent bonds are in the directions of the four corners of the tetrahedron. This sets the bond angle at 109" 28' as shown in Fig. A.4 and this is called the tetrahedral angle.
zyxwvuts Fig. A.4 Tetrahedral angle
For a typical molecular weight of 300,000 there are about 21,000 carbon atoms along the backbone of the chain. Since the length of the CC bond is 0.154 x m the dimensions of an extended zigzag chain would be about 2700 mm long and 0.3 mm diameter. This gives an idea of the long threadlike nature of the molecules. It must be remembered, however, that in any particular polymer, not all molecular chains have the same length. The length of each chain depends on a series of random events during the polymerisation process. One chain may grow rapidly in a region with an abundant supply of monomer
Structure of Plastics
zyxwvu zyxw 415
zyxwvuts
whereas other chains stop growing prematurely as the supply of monomer dries up. This means that a particular sample of synthetic polymer will not have a unique value for its molecular weight. Instead statistical methods are used to determine an average molecular weight and the molecular weight distribution.
A.2 Conformation of the Molecular Chain
The picture presented so far of the polyethylene chain being of a linear zigzag geometry is an idealised one. The conformation of a molecular chain is in fact random provided that the bond tetrahedral angle remains fixed. This is best illustrated by considering a piece of wire with one bend at an angle of 109" 28' as shown in Fig. ASa. 3
zyxwvu Fig. A 3 a ) Rigid Joint at Fixed Angle
If the horizontal arm is rotated about its axis, the other arm will form a cone of revolution. On the polyethylene molecule, the bent wire is similar to the carbon backbone of the chain with carbon atoms at positions 1, 2 and 3. Due to the rotation of the bond 23, atom 3 may be anywhere around the base of the cone of revolution. Similarly the next bond will form a cone of revolution with atom 3 as the apex and atom 4 anywhere around the base of this cone. Fig. AS(b) illustrates how the random shape of the chain is built up. The hydrogen atoms have been omitted for clarity. In practice the picture can take on a further degree of complexity if there is chain branching. This is where a secondary chain initiates from some point along the main chain as shown in Fig. A.6. In rubbers and thermosetting materials these branches link up to other chains to form a three dimensional network. So far the structure of polymers has been described with reference to the material with the simplest molecular structure, i.e. polyethylene. The general principles described also apply to other polymers and the structures of several of the more common polymers are given below.
416
zyx zy zy structure of
/  \
I
\
Plastics
zyxw
Fig. AS@) Random conformation of carbon backbone on molecular chain
C H
Fig. A.6 Chain branch in polyethylene
zyxwvut zyx
structure of Plastics
417
Polypropylene
H
H
H
H
I I I I ccccccI I I I
H
H
I
I
I
I
H CH3 H CH3 H CH3
Polyvinyl Chloride (PVC) H
H
H
H
H
H
H
C1
H
C1
H
C1
F
F
F
F
I I I ccccccI I I
I I
I I
I I
Polytetrafluomethylene(PTFE) F
F
I I I I ccccccI I I I F
Polymethylmethacrylate
I I
I I
zyxwv F
F
F
F
F
0 OCH3 H
CH3 H
I I I cccccc
I
H
I
C
/\
I
H
CH3 H
I I
C
/\
I I
H
0 OCH3 0 OCH3
\/ C
I I
CH3
418
zyxwvut
zyxw zyxwv zyxwvut Structure of Plastics
Polystyrene
H
H
I
I  c  c I H
HC HC
H
H
H
C
H
I I c  c  c I I
I
/c,
H
CH
HC’
CH
HC
I I
‘C€I
I
I
zyxwvu \C/
I
I
H
H
Nylon 66
H
H
H
O
H
I l l I l l CCCNCCCCCCN I l l 1 I H
H
H
H
H
H
I I
H
I I
H
H
H
H
H
O
I l l I ~~
H
I
H
Polyoxymethylene (acetal) H
H
H
H
I I
I
I
H
I
I
H
I
I
H
I
I
H
H
I
I
H
It will be seen from this that a variety of atoms can be present along the carbon backbone and indeed carbon atoms may also be replaced, as in the cases of nylon and acetal. During polymerisation it is possible to direct the way in which monomers join on to a growing chain. This means that side groups (X)may be placed randomly (atactic) or symmetrically along one side of the chain (isotactic) or in regular alternating pattern along the chain (syndiotactic) as shown in Fig. A.7. A good example of this is polypropylene which in the atactic form is an amorphous material of little commercial value but in the isotactic form is an extremely versatile large tonnage plastic material.
Structure of Plastics
zy zyxw zyxw zyx zyxw 419
H
H
H
H
X
H
H
I
I
I
I
I
I
I
ccccccc1
X
(3 H I
1
1
1
1
1
1
H
X
H
H
H
X
At.ctic
H
X
H
H
H
X
l
I
I
I
I
I
ccccccc1
X
1
1
H
H
H
t
X
l
H
H
~
~
syndidretie
(b)
H
H
H
H
H
H
H
1
1
1
1
1
'
1
ccecccc,
1
1
1
l
1
1
X
H
X
H
X
H
X
(C)
IsotrrtiC
Fig. A.7 Possible molecular structures
Polymers can also be produced by combining two or more different monomers in the polymerisation process. If two monomers are used the product is called a copolymer and the second monomer is usually included in the reaction to enhance the properties of the polymer produced by the first monomer alone. It is possible to control the way in which the monomers (A and B) link up and there are four main configurations which are considered useful. These are: (1) Alternating A  B  A  B  A  B
(2) Random A  A  B  A  A  A
B B
 A
(3) Block A  A  A  B  B  B  B  B  B
A
 A
B I
(4)Graft

A  A  A  A  A  A  A I
I
B
B
I
I
B I
B
420
Structure of Plastics
(01
zy
Atactic Polyprapylene
zyxwvutsr
Ibl lsotactlc Polypropylene
Fig. A.8 Polypropylene structures
A.3 Arrangement of Molecular Chains
zyxwvut
A picture of an individual molecular chain has been built up as a long randomly twisted threadlike molecule with a carbon backbone. It must be realised, however, that each chain must coexist with other chains in the bulk material and the arrangement and interaction of the chains has a considerable effect on the properties of the material. Probably the most significant factor is whether the material is crystalline or amorphous. At first glance it may seem difficult to imagine how the long randomly twisted chains could exist in any uniform pattern. In fact Xray diffraction studies of many polymers show sharp features associated with regions of three dimensional order (crystallinity) and diffuse features characteristic of disordered (amorphous) regions. By considering the polyethylene molecule again it is possible to see how the long chains can physically coexist in an ordered crystalline fashion. This is illustrated in Fig. A.9. During the 1940’s it was proposed that partially crystalline polymers consisted of regions where the molecular chains where gathered in an ordered
Structure of Plastics
42 1
zyxwvu zyxwv Fig. A.9 Crystalline structure of polyethylene
fashion whereas adjacent regions had a random distribution of chains. The crystalline regions were considered to be so small that an individual chain could contribute to both crystalline and amorphous areas as shown in Fig. A. 10. This was known as the Fringed Micelle Model and was generally accepted until the late 1950's when for the first time single polymer crystals were prepared from solution. These crystals took the form of thin platelets, their thickness being about 10 mm and their lateral dimensions as large as 0.01 mm. The most important discovery from the growth of these single crystals was that the chains were aligned perpendicular to the flat faces of the platelet. Since the length of an individual chain could be lo00 times greater than the thickness of the platelet the only conclusion was that the chains were folded. Appropriately, this was called the Folded Chain Theory and is illustrated in Fig. A.ll. There are several proposals to account for the coexistence of crystalline and amorphous regions in the latter theory. In one case, the structure is considered to be a totally crystalline phase with defects. These defects which include such features as dislocations, loose chain ends, imperfect folds, chain entanglements etc, are regarded as the diffuse (amorphous) regions viewed in Xray diffraction studies. As an alternative it has been suggested that crystalline
zy zyx
422
Structure of Plastics
zyx zyxwvu .Crystalline wbn
Fig. A.10 Fringed micelle model
10
Fig. A. 11 Folded chain model
(folded chains) and amorphous (random chains) regions can exist in a similar manner to that proposed in the fringed micelle theory. In reality, time will probably show that in the complex structure of partially crystalline polymers, the crystalline regions consist of aligned and folded chains and the amorphous regions consist of crystal defects and randomly entangled chains. Many crystalline polymers when viewed in cross polarised light, display characteristic Maltese crosses due to the presence of spherulites. These spherulites, shown in Fig. A.12, may vary in size from fractions of a micron to several millimetres in diameter, depending on the cooling rate from the melt. Slow cooling tends to produce larger spherulites than fast cooling. It is believed that the spherulites grow in all directions from a central nucleus, by the twisting of the folded chain platelets as shown in Fig. A.13. The size of a spherulite will be limited by the growth of adjacent spherulites. If the polymer melt is cooled very quickly it may undercool, i.e. remain molten at a temperature below its melting point. This results in a shower of nucleation sites becoming available and a mass of spherulites will start to grow. The solid polymer will then consist of a large number of small spherulites.
Structure of Plastics
zyxwvut 423
Fig. A. 12 Qpical illustration of spherulites
zyxw
Twisted tddcd chain growth from nucleus
zyxwv
Fig. A.13 Structure of spherulite
The ease with which a polymer will form into crystalline regions depends on the structure of the molecular chain. It can be seen, for example, that if the polyethylene molecule has a high degree of branching then it makes it difficult to form into the ordered fashion shown in Fig. A.9. Also, if the side
424
zyxwvutsr Structure of Plastics
groups are large, it is not easy for a polymer with an atactic structure to form ordered regions. On the other hand isotactic and syndiotactic structures do have sufficient symmetry to be capable of crystallisation. Another important feature of long chain molecules is the ease with which they can be rearranged by the application of stress. If a plastic is stretched the molecules will tend to align themselves in the direction of the stress and this is referred to as orientation. Molecular orientation leads to anisotropy of mechanical properties. This can be used to advantage in the production of fibres and film or may be the undesirable result of a moulding process. However, it is important that orientation should not be confused with crystallinity. It is possible to have an orientated polymer which shows no evidence of crystalline regions when Xray diffraction studies are carried out. Equally, a polymer may be crystalline but optical measurements will show no signs of orientation. Orientation can be introduced into plastics such as polyethylene and polypropylene (both semicrystalline) by cold drawing at room temperature. Other brittle plastics such as polymethyl methacrylate and polystyrene (both amorphous) cannot be cold drawn but can be drawn at elevated temperatures.
zyxwv
zyxwv zyxwv
APPENDIX B  Solution of Differential Equations
zyxw zyxwv zyxw zyxwvuts zyxwvu
The following type of differential equation is encountered in the text, for example, in the analysis of the models for viscoelastic behaviour: AdY + B y  C = 0 dx where A, B and C are constants. This has the solution
y=BB
eB.xfA
where the constant ‘K’ can be determined from the known boundary conditions in the specific case.
425
zyxwv zyx
APPENDIX C  StresdStrain Relationships
zyxwvu zyx zyxwvuts zyxw zyxw
(i) Uniaxial Stresses When a material is subjected to a uniaxial stress, there will be a strain in the direction of the stress and a strain of the opposite sense in the perpendicular directions. The latter is referred to as the Poisson's Ratio effect. E"
1 = EO"
where
E = modulus of material.
where
v = Poisson's ratio (typical values are given in Chapter 2). E,
= u
(;
.
.>
The Zdirection is perpendicular to the page. For simplicity the material is assumed to be isotropic, ie same properties in all directions. However, in some cases for plastics and almost always for fibre composites, the properties will be anisotropic. Thus E and u will have different values in the x, y and z direction. Also, it should also be remembered that only at short times can E and u be assumed to be constants. They will both change with time and so for longterm loading, appropriate values should be used.
(ii) Biaxial stresses If the material is subjected to biaxial stresses in both the x and y directions then the strains will be 426
Stress/Strain Relationships
zyxwvu zyxwv zyxwvu zyxwvut zyxw zyx zyxw 427
Ex
1 1 = ox  va, E E
That is, the total strain will be the sum of the tensile strain due to ox and the negative strain due to the Poisson's ratio effect caused by 0,. Similarly Ey
1 1 = ay  vox E E v = (ox + oy)
This situation is sometimes referred to as plane stress because there are only stresses in one plane. It is important to note, however, that there are strains in all three coordinate directions.
i ,
zyxwvutsrqpon
(iii) 'hiaxial stresses
If there are stresses in the x , y and z directions then the above approach is continued so that 1 1 1 1 v Ex = 0,  v  o y  vo  0,  (a + oz) E E E '  E E
428
zyxwvuts zyxwvu zyxwvutsrqp zyxwvutsrq StresdStrain Relationships
1 = Eay 
V
Ey
1 =2 0 2
V
Ez
+az)
 (ay +ax) E
In the above situation, if the stresses are such that E , = 0 then this condition is referred to as plane strain. This is because strains are experienced in only one plane even though there are stresses in all three coordinate directions.
zyxwvu
APPENDIX D  Stresses in Cylindrical Shapes
zyxwvu zyxwv zyxwv
(i) In a thin wall cylinder ( r > 10 h) subjected to internal pressure, p , the stresses are given by Pr ag = h Pr a, = 
2h a, =  p (at bore)
a, = 0 (at outside)
I
I
zyxwv 429
430
zyxwvu zyxw zyxwvut zyxwvu zyx Stresses in Cylindrical Shapes
Note that a, is small compared to 0 0 or a, and so it is often ignored. Hoop strain, Ar 1 V &e =  =  0 0  a r E E a
Eh
Axial strain, 1 V E E Pr Ea = 11  2vj 2Eh (ii) In a thick wall cylinder subjected to both internal and external pressures the stresses are given by E,
= aa  a0
= k2  1 ( P i (1
+ $)  pok ( 1 +
a, = k2  1 { P i ( l  $ )
zy
z)}
pok(l$)}
where k = ro/ri. The axial stress will depend on the end constraints but if we consider the most common situation where there are end caps and the cylinder is free to change in length then for internal pressure only (ie p o = 0):
zy zy
Pi a, = k2  1
For the zero external pressure situation, the axial strain will be given by 1 V V = aa  0, ne E E E ( 1  2v) (Pi 1 Ea = E(k2  1 ) E,
zyxwv
APPENDIX E  Introduction to Matrix Algebra
zyxwvut zyxwvuts zyxwv zyxw zyxwv
E.1 Matrix definitions
A matrix is an array of terms as shown below: a12 a22
a13
a21 a31
a32
a33
.. . .. .* .
am1
am2
am3
...
all
[AI =
a23
aln
a2n a3n
amn
If n = 1 then we have a matrix consisting of a single column of terms and this referred to as a column matrix. If rn = 1 then the matrix is called a row matrix.
If in the analysis of a problem there is a set of simultaneous equations then the use of matrices can be a very convenient shorthand way of expressing and solving the equations. For example, consider the following set of equations:
+ ~ 1 2 x +2 + + UlnXn y2 = Q21XI + a22x2 + a 2 3 x 3 + + a2nXn y 3 = a 3 1 x 1 + a32X2 + a 3 3 x 3 f + a3nXn y1 = ~ I I X I
~13x3
* * *
* ' *
' ' '
zyxwvu Ym
amlxl
+am2x2 + ~
+ +
~ 3 x .3.
amnXn
These may be written in matrix form as follows:
IY} = [AItxJ where (y} and (x} are column matrices.
[E.11 43 1
432
zyxwvut z zy zyxw zyxwvu Introduction to Matrix Algebra
E.2 Matrix multiplication
The matrix equation [E.1] involves the multiplication of the matrices [A] and ( x ) . To do this one must apply the simple rules of matrix multiplication. These are:
(a) two matrices may only be multiplied if the number of columns in the first is equal to the number of rows in the second; ( b ) the terms in the product matrix resulting from the multiplication of matrix [A] with a matrix [B] are given by
Then
zyxw
E 3 Matrix addition and subtraction Matrix algebra also involves the addition and subtraction of matrices. The rules for this are as follows:
(a) matrices may only be added or subtracted if they are of the same order,
i.e. they each contain the same number of rows and columns; ( b ) the terms in the resulting matrix are given by
The following example illustrates the use of these rules:
zyxwvuts zyxwvu zy zyx zyxwvut zyx 433
Introduction to Matrix Algebra
Then
E.4 Inversion of a matrix Referring back to the set of simultaneous equations at the beginning of this appendix, the objective is usually to solve these for the unknown x terms. This is where the use of matrices has a major advantage because referring to equation [E.1] we may rewrite this as (XI = [Al'IYI
~.41
This equation expresses the solution to the set of simultaneous equations in that each of the unknown x terms is now given by a new matrix [AI' multiplied by the known y terms. The new matrix is called the inverse of matrix [A]. The determination of the terms in the inverse matrix is beyond the scope of this brief introduction. Suffice to say that it may be obtained very quickly on a computer and hence the solution to a set of simultaneousequations is determined quickly using equation [E.4].
zyxwvut
E.5 Symmetric matrix
A square matrix is one in which the number of columns is equal to the number of rows. An important type of square matrix which arises quite often in the finite element method is a symmetric matrix. Such matrices possess the property that ai, = aji. An example of such a matrix is given below: 2 4
7 1 6  5 L3 9 5 41 2 4 7  3 5 1 sym. 6
[
:]
which is often written as
zyxwv zy
APPENDIX F  Abbreviations for some Common Polymers
ABS ASA CA CAB CAP CN CP EC EP EVA FEP HDPE
LDPE LLDPE MDPE MF PA PAEK PAI PAN PB PBA PBT PCTEE PE PEEK PEI PEK PES
434
PET PF PI PIB PMMA
Poly(ethy1ene terephtlhalate) Phenolformaldehyde Polyimide Polyisobutylene Poly(methy1 methacrylate), acrylic Poly4methylpentene1 Polyoxymethylene: polyformaldehyde, acetal Polypropylene Polyphenylene ether Polyphenylene oxide Poly(pheny1ene sulphide) Poly(pheny1ene sulphone) Polystyrene Polysulfone Polytetrafluoroethylene Polyurethane Poly(viny1 acetate) Poly(viny1 alcohol) Poly(viny1 butyral) Poly(viny1 chloride) Poly(viny1idene chloride) Poly(vinylidene fluoride) Poly(viny1 formal) Polyvinylcarbazole Styrene Acrylonitrile Styrene butadiene rubber Styrenebutadienestyrene Ureaformaldehyde Unsaturated polyester
zyxwvut zyxw zyxwvut zy
HIPS
Pc
Acrylonitrile butadiene styrene Acrylonitrile styrene acrylade Cellulose acetate Cellulose acetate butyrate Cellulose acetate propionate Cellulose nitrate Cellulose propionate Ethyl cellulose Epoxide, epoxy Ethylene vinyl acetate Fluorinated ethylene propylene High density PE High impact PS Low density PE Linear low density PE Medium density PE Melamineformaldehyde Polyamide Polyaryletherketone Polyamideimide Polyacrylonitrile Polybutene1 Poly(buty1ene acrylate) Poly(buty1ene terephtlhalate) Polycarbonate Polychlorotrifluoroethylene Polyethylene Polyetheretherketone Polyetherimide Polyetherketone Polyethersulfone
PMP POM
PP PPE PPO PPS PPSU PS PSU
PTFE
PUR PVAC PVAL PVB PVC PVDC PVDF PVFM PVK SAN SBR
SBS UF UP
zyxwv
Solutions to Questions
zy
zyxwvu zyxwv
(2.1) Using the desirability factor Df (Equation 1.16)
Df =
($)
zyxwvut
So uPVC would be the best choice on a cost basis.
Weight, W = density x volume = (2 x 103L)N From 1 week isochronous for polypropylene, E = 427.5 MN/m2
so
384 x 427.5 x 12.3 x lo3 x 4 2 x 103 L = 1.417 m
L4
=
435
zy zyx zyx zyxw zyxw Solutions to Questions
436
7 = 16.94 mm
(2.3)
r l
2s
wL2 W where w = 24 L wL27 2 x
M=
1
I I
zyxwvutsrqp x 14172 x 16.94 24 x 12.3 x 103
= 0.23 MN/m2
A this stress, E = 550 MN/m2, s % error =
so
6=
wL3 384EZ

427.5  550 = 28.7% 427.5
2x x 1417 x 14173 = 3.1 mm 384 x 550 x 12.3 x 103
(2.4) From 3 year isochronous at 1.5%, a = 4.9 MN/m2 a0
PR h
PR
=  SO h =  =  go
0.5 x 40  4.08 mm 4.9
If the density = 905 kg/m3 ie a reduction of 4 kg/m3 then there would be a (4 x 4)% reduction in design stress. So new design stress = (0.84 x 4.9) MN/m2 New h =
so Original weight = 909 x New weight = 905 x
so
IC x
IC x
% change =
0.5 x 40 = 4.86 mm 4.9 x 0.84
80 x 4.08 x
80 x 4.86 x
 (909x 4.08) x 100 = +18.6% (909x 4.08)
(905 x 4.86)
zy
Note that this question involved a biaxial state of stress in the material and hence, strictly speaking, the creep curves used are not appropriate. However, creep curves for biaxial states of stress are rarely available, and one possible approach is to calculate an equivalent stress, a,, using a van Mises type criterion 1
d
a, = 
{(a1
 a d 2 + (a2  0312 + ( 0 3  adz)
In the case of a cylinder under pressure,
(TI
= pR/h,
a2
= pR/2h, a3 = 0,so
In most cases it is probably sufficiently accurate to use approach will provide a builtin safety factor.
rather than a, and this
zyx zyxwvu zyxwvu zyxwvutsr zyxwvu 437
Solutions to Questions (2.5) Central Deflection,
WL3 s= 
48EI
so,
zyxwv zyxwvuts zyx
This strain will occur in the outer fibres at midspan. = po2r2
(2.6) For rotating pipe, 00=
909
(2 ~ x603 0 0 )0 (150 x
= 2 MN/m2
It is necessary to know how long the material can withstand this stress before it reaches a strain of EO = ADID = 1.21300 = 0.4% From the creep curves t =2.1 x 106 seconds = 24 days
(2.7)
12.5 1250
= 1%)
h=
2pgHR2 EAD
From 1 year isochronous at 1% strain, E = 360 MN/m2 Making the 20% correction for change in density from 909 kg/m3 to 904 kg/m3, E = 288 MN/m2
so
h=
2 x lo00 x 9.81 x 3 x 0.6252 = 6.39 IIUII 288 x 106 x 12.5 x
(2.8) From the 3 year isochronous curve for polypropylene, the initial modulus, E = 466.7 MN/m2. Making the (5 x 4)% allowance for the different density, E = 0.8 x 466.7 = 373.3 MN/m2.
0.365 x 373.3 Now
PR 2h
g==
= 8.48 IIUII
20 x 103 x 700 = 0.825 MN/m2 2 x 8.48
At this stress the modulus has the same value as the initial modulus so no further iterations are necessary. When the pipe is cooled it will contract by an amount given by ET = a ( A T ) and when this equals the fixed strain, &e, the pipe would leak ie
A T =  0*00417 46.3"C 9 x 105
So minimum temperature = 20  46.3 = 26.3"C
438
zyxwvutsr zyxwvuts zyxwv zyxw zyxwvu zyxwvu Solutions to Questions
(2.9) The compressive stress in the bar is given by u=
l o x 10
Now
 1.4 MN/m2
zyxw
bd3 l o x 103 I= = 833.3 IIUII~ 12 12 PcL2 140 x 2252 E== 861.7 MN/m2 n21 n2 x 833.3 u 1.4 x 100 E== = 0.16% E 861.7 ~
For buckling,
From the creep curves this strain is reached at 104 seconds 104
So time = = 2.78 hours 3600 (Note: E < 0.5% so no correction to tensile creep data is needed).
(2.10) critical stress, P, a,== A
and
I=
4n2EI AL2
zyx
W h3 12
4n2EWh3 n2E h = 12whL2 = 3(i)
so
L For many plastics u,/E = 30 x
to 35 x
for shortterm loading
so For longer term loading, E will decrease more than uc so uJE will get larger. This will cause the acceptable h/L to decrease. (2.1 1)
K~EI K~EI Pc = so a, = 
L2
AL2
n2d2 Now for circular rod, cc = 16L2 = /0.005 x 16 x 1502 n2
zyxwv = 13.5 mm
zyxwvut zy zyxwv zyxwv zyxwvutsr
Solutions to Questions
439
From 1 year isochronous at 0.5% strain, E = 370 MN/m2
so
k2 x
370 x
IC x
13S4
zyxwvu zyx P, =
(2.12)
3(3
h =
64 x l 5 P
= 227 N
+ u)PR2  3 x 3.4 x 0.04 x 752 = 6.91 mm 8u
8x6
From 1 year isochronous curve at a stress of 6 MN/mz, E = 6/0.018 = 333.3 MN/m2
so
s=
3 x 0.6 x 5.4 x 0.04 x 754 =7mm 16 x 333.3 x 6.912
(2.13) The maximum stress or strain is not specified so an iterative approach is needed. From the 1 year isochronous for PP the initial modulus is 370 MN/m2 P=
so
but at
so
U =
16Eh3S
3(3
+ v)PR2  3 x 3.4 x 0.0363 x 322 = 7.58 MN/m2
zyxwvut
8 x 2S2 7.58 u = 7.58 MN/m2, E =  305.6 MN/m2 0.0248 16 x 2 S 3 x 4 P= (305.6) = 3 x MN/m2 3 x 0.6 x 5.4 x 324 8h2
U =
but
16 x 370 x 2S3 x 4
= 0.036 MN/m2 3(1  u)(5 + v ) P  3 x 0.6 x 5.4 x 324
3 x 3.4 x 322 (3 x lo’) = 6.27 MN/m2 8 x 2.52
6.27 E =  319.6 MN/m2 + P = 3.14 x low2+ u = 6.55 MN/m2 0.0196 E = 321.2 MN/m2 + P = 3.15 x
MN/m2 + (I = 6.58 MN/m2
E = 321.2 MN/m2 + P = 3.15 x low2MN/m2 &e =
so (2.14)
AD =
AD
Pr
 = (2 D 2hE
Pr2 hE
 u), So AD = (2
3.15 x x 322 (1.6) = 6.43 x 2.5 x 321.2
bd3 I==12
 v) mm
12 x d3  d 3 12
From the 1 year isochronous curve, the initial modulus = 370 MN/m2 NOW
5WL3 d 3 = 384E6 yc = M =I
5 x 150 x ZOO3 So d = 19.16 mm, where W = wL 384 x 370 x 6 WL 150x200 = 5.1 MN/m2 16d2  16dz
zyxwvu zy zy zyxw zyxwvuts Solutions to Questions
440 At
(I
= 5.1 MN/mz + E = 342.3 MN/m2 + d = 19.67 mm
(I
= 4.85 MN/m2 + E = 346.2 MN/m2 + d = 19.6 mm
(I
= 4.88 MN/m2 + E = 346.4 MN/m2 + d = 19.6 mm
(2.15) Once again an iterative type solution is required. 1.5)
W=
(;)“”>
{0.48(?) 2.4W 32
= 0.0795E
 0.267
(I=
zyxw
From the 1 year isochronous curve, the initial modulus is 370 MN/m2
so
W = 29.43 N + (I = 7.86 MN/m2 + E = 302.3 MN/m2
W = 24.03 N + 0 = 6.42 MN/m2 + E = 324.1 MN/m2
W = 25.76 N + (I = 6.88 MN/mz + E = 317.0 MN/m2 W = 25.2 N + (I = 6.73 MN/m2 + E = 317.4 MN/m2
W = 25.2 N + (I = 6.73 MN/m2
So W = 25.2 N (2.16) This is a stress relaxation problem but the isometric curves may be used.
From 2% isometric, after 10 seconds, E = 16*75 837.5 MN/m2 0.02 W=
Afterlweek, so
Ed4S  837.5 x 34 x 10 = 3 N 128(1 + w)R3N  128(1.4)53 x 10
E =  8S5  427.5 MN/m2 0.02 427.5 x 34 x 10 W= = 1.55 N 128(1.4)53x 10
zy
(2.17) From the 1 day isochronous curve, the maximum stress at which the material is linear is 4 MN/m2. This may be converted to an equivalent shear stress by the relation (I
r=2(1
Now
If W = 4.5 N,
+ u)  2(1.4)  1.43 MN/m2
zyxw
16 x 3 x 7.5 a x 1.43 d = 4.31 IYNII 16 x 4.5 x 7.5 T = = 2.15 MN/m2 ~r(4.31)~
16WR r=
ad3 ’
SO d3 =
zyx zyxwvu zyxwvu zyxw zyxwvu 441
Solutions to Questions
zyxw
Equivalent tensile stress = u = 2.15 x 2 x 1.4 = 6 MN/m2. From the 1 day isochronous at this stress,
E=
‘
0.0094
638.3 MN/m2
128(1+ v)R3N  _K Ed4 E
s=
K  K so
where E2 = 638.3 MN/m2 and 1.4 = = 700 MN/m2 0.002
zyxwvut
So % change = +9.67% (2.18) At short times,
E=
’*‘
0.004
1400MN/m2
Allowing for temperature, E a = 1400 x 0.44= 616 MN/m2 Overall strain, E = ET  E, = 0 ET = E, aAT = u/E = P / A E
so
n(10)2 x 616 x 1.35 x P = AEaAT = 4
x 40 = 261 N
(Note: u = (261 x 4 ) / ~ ( 1 0 = ) ~3.3 MN/m2. Therefore since the strain is less than 0.5% no correction to the tensile data is needed for compressive loading). After 1 year Em = 370 MN/m2, E a = 222 MN/m2
so
4
(Note: Once again the strain is less than 0.5%so no correction is needed for compressive loading). (2.19)
E@ =
AD 0.05 == 0.417% D
12
From the 0.417% isometric curve, the stress after 1 year is 1.45 MN/m2 The pipe would leak if the hoop stress caused by atmospheric pressure (0.1 MN/m2) exceeded the stress in the pipe wall after 1 year. PR 0.1 x 6 P = 0.1 MN/m2, a@ =  =  0.4 MNlm2 For h 1.5 Hence, leakage would not occur.
442
zy zyxwvutsr Solutions to Questions
zyxwvut zyxwv zyxw zyxwv
(2.20) This is a stress relaxation problem, but the question states that creep data may
be used
Then from a 1.6% isometric taken from the creep curves it may be determined that the stress after 10 seconds is 15.1 MN/m2 and after 1 year it is 5.4 MN/m2. (a) Initial pressure at interface = p = (ha)/R = 3.02 MN/m2
Thus normal force at interface, F = p x 2xRL = 3.02 x 2x x 5 x 15 = 1.423 kN
So axial force, W = pF = 0.3 x 1.423 kN = 0.427 kN
(b) Similarly, after 1 year for u = 5.4 MN/m2 the axial force W = 0.153 kN.
(2.21) (a) As illustrated in Example 2.7, the extraction force, F, is given by
zyxwvu F =xppDW
so
1.2
103
=4 m / m 2
= ~(0.24)(40)(10)
Treating the bush as a thick wall cylinder subjected to this value of external pressure, then Benham et al. show that at the outer surface of the bush, the stresses are:
radial stress, a, =  p
zyx zyxwvu zyxwvut zyxwvu zyxwvu 443
Solutions to Questions
Hence, the hoop strain, &e, is given by
AR R
&e =  =  
E
~ a ,
E
zyxwvu zyxwvu zyxwvu
The negative sign simply means that this is a reduction. 4 x 20
1.142+1
AR=m{ (1.1421)0’4}
so
AR = 0.29 ITM (b>
AR = a.R.AT AT =
0.29
loo x
106 x 20
= 143°C
Hence the nylon bush would need to be cooled by 143°C to achieve the necessary of 123°C. contraction to have easy assembly. This suggests a cooled tempem(c) At the bore of the bush, Benham et al. shows the stresses to be 2k2p a@ = k2  1’ hence
Ar _  a0  =vu,
zyx
a, = 0
2k2P E(k2  1)
r
E
A, =
2( 1.14)*17.5(4) = 0.3 ITM 2 x 103(1.142 1)
E
Therefore the internal diameter of the bush will be 35  2(0.3) = 34.4 mm.
(d) If the longterm modulus of the nylon is 1 GN/m2 then for the same interference conditions, the interface pressure would be reduced to half its initial value ie 2 MN/m2. This means that the separation force would be half the design value ie 600 N. (2.22) If the acetal ring is considered as a thick wall cylinder, then at the inner surface there will be hoop stresses and radial stresses if it is constrained in a uniform manner: hoop stress, ae = p
{
z}
zyxwvu radial stress, a, =  p
where p is the effective internal pressure k is the ratio of the outer to inner radii
Hence, the hoop strain, E @ , at the inner surface is given by &e =
Ar ae a, =   vr
E
E
zyxwvut zy z zyxwvuts zyxw
444 so,
Solutions to Questions
..=${(=)+"} + k2
1
When the bobbin is cooled by 60°C the effective constrained contraction of the inner surface of the acetal will be Ar = (a,,  as)rAT A r = (80  11)106(10)(60) = 0.0414 mm
so,
{ ()
0.0414 = P(W 3 x IO3
1.52+ 1 +o.33 1.5' 1
}
zyxwvut zyxwvu p = 4.24 MN/m'
+
u o = p {k2 m}1 =4.24(~)
hence,
=11MN/m2
(2.23) Plot log i vs. loga and straight line confirms the Power Law with A = 3 x lo", II = 0.774 EI
so
 EO = i t = Ad"' = 0.95 x lo*
+ (3 x 10'1(5)0.774)(9x lo6  1 x IO6)
= 1.033%
z
(2.24) A plot of log E against log t is a straight line for u = 5.6 MN/m2 So E ( t ) = At" where A = 0.238 and N = 0.114. After 3 days (= 2.59 x I d seconds) strain = 0.988%
So from (5) Fr = 1

F, =
E ( T ) ~ l p ( t ) 0.988  E R ( ~ ) ET 0.988
t, =
(2 x 2.59  2.59) x 1 6 =1 2.59 x l@
+ t i  (tR+ 1)"
0.988((2)0."4  1) = E r ( t ) = 0.0813% Alternatively: Strain after 2 x 2.59 x 1 6 seconds = 1.069%. Now recovery may be regarded as reversal of creep, So residual strain = 1.069  0.988 = 0.0812% 15 x 153 10.5 x 10.53 (2.25) I = ___ 12 12
For solid beam,
I
10.5 +12
0 450 909
(10.5Q = 3454.1 mm4
04 =  = 3454.1, D = 14.27 IIUII 12
zyxwvu zyxwvut zyxwvu zyxw zyxwvut
Solutions to Questions
445
zyxwvutsr zyxwvuts Weight of solid beam = 14.27’ x
loe6 x 909 = 185.1 g
Weight of foamed beam =
x 909)
(4 x 2.25 x 12.75 x
+ (450 x 10.5’
x
= 153.9 g
96 Saving = 16.9% (2.26)
My
WL2 x7.5 24 x 3126.3
u== I
W=
7 x 3126.3 x 24 = 1.12 kN/mm 2502 x 7.5 7 0.015
From the 1 week isochronous, E = = 466.7 MN/m’ WL4 384EI
6=
1.12 x 2504
 384 x 466.7 x 3126.3 = 7.8 mm
(2.27) Weight of solid beam = 909 x 12 x 8 x 300 x
x lo3 = 26.18 g
Weight of composite = (909 x 2 x 2 x 12 x 300 x 106)+(500 x h12 x 300 x h = 7.27 nun, so composite beam depth = 11.27 mm. The ratio of stifhesses will be equal to the ratio of second moment of area bd3 I solid .  =  12 Icomposite
=
12 x 83 12
 512 mm4
12 x 11.273 12 x 7.273 12 12
+
(g)’
12 x 7.273
12
1163.45 Ic =/___ Is 512
 2.27
(2.28) (a) Solid
Consider a flexural loading situation as above, so
W  48EI _  cx E I
s
L3
= 1163.45
zy zyxwvuts zyxw zyxwv zyxwvuts zyxwv
446
zy Solutions to Questions
So Solid
Weight = p, x H x 1 x 1 = p,H = 12p,
S Ratio = E (12) PS
(b) Foamed
EI = Ef
(g)(E) (T) =
E,
1 x 123
12 Weight = p f x H x 1 x 1 = 12pf = p, 1.5
(T)
Ratio = E,  12 x 1.5
Ps (c) Composite
= (8) ES
zyx zyxwv PS
b’ =
Weight = ps(4
(2)
(I)
+ (8 x 0.44))x 1 x 1 = 7 . 5 6 ~ ~
120.3ES E, Ratio =  (15.9)7.56~~ PS
So ratio foam: solid: composite = 8:12:15.9 (2.29) (a) Sandwich Beam of Minimum Weight for a given stiffness KWL3 deflection, S = KI where K is a factor depending on loading and supports. For E s ~ ,>,> E,,
EI
Ebdh2/2
S=
2KWL3 E&,,bdh2
zyxwvut zyx zyxwvutsr zyxwvut
Solutions to Questions Total mass
447
+
m = pCoEbhL p*,,bdL
From deflection equation (1)
d =  2KWL3 Esbnbh26
so
zyxw zyxwv zyxwvu
To minimise the weight with respect to h, then amlah = 0 am ah
 = pbL

4 p a n KWL4 =O Esbn6h3
Pcmh = 4skh
or
weight of core = 2 x weight of skin
(b) Sandwich Beam of Minimum Weight for a Given Strength Assuming the core does not fail in shear, failure occurs in bending when the stress in the skin reaches its yield strength cy,ie
M
a, = bdh
where M = bending moment.
Mass of beam m = pbhL
+ psbnbdL
Using
M d=bhu,
To minimise the weight with respect to h, b l a h = 0
zyxwvuts zyxwvu zyxwvutsrqp zyxwvuts Solutions to Questions
448
ph
or
=b
d
weight of core = weight of skin.
(2.30)
(b) Voigt
(a) Maxwell
4
12 cU) =  1 2 x 5 0 ) = 1.26% 2000 90x109
+
EllJo =
00
l2 + l2 106(100) = 1.933% 2000 90x109
but  = 0.6%
e
6150
zyxwvut
= 1.933  0.6 = 1.333%
(2.31) Maxwell Strain (50 s) = Kelvin Strain (50 s)
(2.32)
From graph U O / = ~ 0.01 2 ~==~ooMN/~~
so
At
0.01
E
= 0.0089, t = 3000 s 0.0089 = 0.01 { 1  eMoo(t/q)}
zyxwvu zyx zyxwvu zyxwvutsrqpo
zyxwvut
Solutions to Questions
449
Relaxation time
.C
e
3
Time
so
7.36
10~= 5/,,
q = 270 GNs/m2
Relaxation time = for
00 E
= 1350 seconds
= 4.5 MN/mZ
4.5 =. 200
{ 1  ,(15@3/135o } = 0.0151
(2.33) (a) StressStrain equations
zyxw
61
=elel
02
= 52E2
a3
= 5343
(b) Equilibrium equations
a = 61 = a2 (c) Geometry of Deformation E
From above B=&1+&2
but
L.1
= ir1/61
6
b=
51
and
+ t7 + 52t7( E ff
i + 52 c =  +irrl
L.2
61
“(“‘52)
17
+
+ a3
zyxw
= ~1
and ~2 = 8 3
= (al/q)  (42/t))e2 (from Kelvin model)
 El)

z
This is the governing equation for the Standard Model.
450
zyxwvuts zyxwvut zyxwvut zyxwv zyxwv zyxwv zyxwv Solutions to Questions
The solution to this differential equation will have the form
where T = q / h and a0/6l is the initial strain when the stress is applied. The unrelaxed creep modulus is obtained by putting t = 0. Hence, unrelaxed modulus E" =  a0
E(0)
h
The relaxed modulus is obtained by putting t = 00. Hence, relaxed modulus ER = 00
616 2
 61 + 62 *
E(0O)
(2.34) From figure below redrawn from the creep curves q=
0
E
2: 4.3
x 10" Ns/mz
00
.$ =  = 1400 x lo6 N/mz EO
So from text using the fact that for a strain of 0.48,
a0 21 5.5
MN/mz (from creep data)
= aoe(o/'lt
= 5.5e(1400~106x900)/4.3x1012 = 4.1
m/,,,2
1.0
0.75 C
'e s
05
025
zyxwvutsrqpo lime
(2.35) From the graph below, and the theory of the 4element model, 4.2/0.003 = 1400 MN/m2
.$I
= UO/EI =
4.2 00 00 h = Retarded Creep = EZ  (0.72  0.3)102 = 1000 m / m 2 VI=
00
ds/dt

4.2 3.167 x
q1 = 4.775 x lo9 MNs/m*
= 1.326 x lo6 (MN/m2)hr
zyxwvu zyx zyxw
Solutions to Questions
45 1
zyxwv zyxwvuts
Finally from the expression for the 4element model
taking a value of strain from the knee of the curve E
= 0.0055 at t = 4 x 104 seconds (11.1 hrs)
So 72 = 4.525 x lo7 MNs/m2
For u = 5.6 MN/m2 at 3 x 16 seconds
1.4

1.2

Xr 1.0

.
c
Slop..
o.2
0
Ll
100
200
pr dt
zyxwvutsrq
(2.36)
E(?) = At" a(r)= Bt
zyxwvu Mo
452
zyxwvuts zy
zyxwv zyxwvu zyx Solutions to Questions
& ( I )=
BT*+' A(n 1)

+
This will be a nonlinear response for all nonzero values of n. (2.37) For the Maxwell Model
&=r]ln
zy
(K  3+r]lnK
Using and
x
Kr] =
I
Time (s)
I
zyxwv
Strain (%)
loo0 x I d = 10
I
1 ;1 : 1
Stress (MN/m2)
0.06
100
0.08 0.1
2;
7.98 8.65
initial tangent modulus = 7.00/0.0004 = 17.5 GN/mz 0.1% secant modulus = 8.65/0.001 = 8.65 GN/m2 Note that in this question an alternative solution may be carried out using the creep modulus but this causes slight inaccuracies.
zyxwvu zyxwvu "I
Solutions to Questions
453
10
zyxwv zyxwvut zyxwvu zyxwv zyxwvuts zyxw zyx K Strain
Alternative Solution:
tr) Now for Maxwell Model E ( t ) = 
?I+&
So for case in question, the strain hstory is
0 < t < ti
so
6r)
a(t)=
E(f)
.K
= K t , d&(u)/du= K
.du =
I0 n + 6 ( t ,  u ) = K6r) [log,(r)
so
a(t)= Kr)boge
j! ( + " 0
r)
B 1
+ et1  B )
(y )]
This equation predicts the following data
100
0.06 0.08 0.1
7.88 9.56 10.98
 6u
)K
du.
454
zyxwvuts zyxwvu zyxwvut zyxw z zyxwv zyxwv zyxwv Solutions to Questions
From a plot of this data
Initial tangent modulus = lo  17.54 GN/m2 0.00057 10.98 =  10.98 GN/mz 0.001
0.1% secant modulus
~(40) = 0.5 x 40 (3A
4 t 2 )= ( K I T
+
2 x 45, 000
+K z T )
~ ( 7 0= ) (0.5 x 60
+ 1 x 60)
) = 1.55%  Kztz (! + ”> 5 211
+70
3000
45,000
90,000
= 3.22%
zyxwvu zyxw
which, for t3 = 120 s, T = 60 s and T’ = 90 s, gives 4120) = 3% (2.39)
~ ( t l= ) Kltl
(F + “) 2rl
~(60) = 0.4 x 60 .5(t2) =
E(
Kit'

6o
(3i00 + 2 x 50,000
’>
(iF + firl  2a
130) = 0.4( 100)

) = 2.12%
ha
E(t2
 t‘)
130    lO(50, 000 + 350(30)) + 
(3i00
50,000
)
100,000
= 6.61 (2.40)
a(t)=
20 800
* t ,
da(t)  20 dt 800
3500~50,000
Solutions to Questions
zyxwv zyxwv zyxwvutsrqp zyxw zyxwv 455
=
E@,)
20
dt I0 E ( t L 0 ) 800 *
~
.
1.05
E(500) =
zyxwv
"1
500
1.05 x lo00 800
= 0.0162 = 1.62%
20 (b) After 800 s, the change in stress is (Kt) where K = . 800 uz
so
E(U2)
=
zyxwvu
J.E(t  t l ) dt 0
" t0.05
 . K . dt
=
E(t  t 2 )
103
0
+
/
u2
r2
E(
t2
 t2)0.05
(t
103
. (K)dt
1.05 x 103
1.05 x 103 then for u 2 = loo0 s,
dt
12
fz
= 800 a
10oO) = 0.0336  6.21 x
= 0.0274 = 2.74%
(2.41) 10
zyxwvutsr zyxwvu For a KelvinVoigt model
~ ( t=) 6 [I  e  r / T ~  l
where T = 17 15 = 30
I
I
"\I
0 t , a
+loo
"3
150
(a) Using Boltzmanns Superposition Principle
where
a(t)=  K t
SO
d N ) = K
dt
time@)*
456
zyxwvuts zy Solutions to Questions
= 6.43
(b)
.&)
= (1 *O
t
zyxwvu zyxw zyxw zyxw 104 = 0.064%
)+I

dt
E ( t  r l ) dt
fZ
fl
For the period after tz (= 100 s) the change in stress is Kr.
do(t)  K for this third period
so
dt
Substituting u3 = 150 s, K = 0.1,t l = 50 s, r2 = 100 s ~(150)= 4.49 x i=N
(2.42)
~ ( t=)
{ E(t } 1
a; i~
15{ 25{
10
= (v 5V
u;
where E ( t  u i ) =
+ 5(4500  2000) } +
= 0.045%
+
5V
v + 5(t  u i )
{
2o V+8(45E  3 0 w
5V 5(4500  4OOo)
5V
+ 45005 + v + 35006  1 . 5 ~ 375% + 2~
+ 30005  2.5~ 12505)
zyxwvu zyxwvutsr zyxwvu zyxwvu zyxwvu 451
Solutions to Questions
(2.43) From the information provided
F, =
 0.8  0.058 = 0.9275
E A T )EAT)
zyx zyxwvu zyxwvut t
T
0.8
 100  200100 =1
also
tR=
but,
F, = 1 + r ;  ( t R + 1)"
0.9275 = 1
T
zyxw
+ 1  (2)" + n = 0.1
Also, since ~ ~ ( 1 0= 0 )0.8% and ~ ~ ( 1 0 = 0 )A(lOO)o.' then A = 0.504766 (for u = 10 MN/m2)
Therefore after 2400 seconds at 10 MN/m2
~(2400)= 0.504766(2400)0~1 = 1.1%
For 2400 seconds on and 7200 seconds off, t' = 9600 seconds. x=10
~ ~ ( 9x. 6104) = ~ ~ ( 2 4 0 0 )
SO
x=l
x=lO
t'x
"
[(y)  ($  l)"]
[(4x)" (4x  l)"] = 0.108%.
~ ~ ( 9x. 6lo4)= 1.1 x= 1
(2.44) From question (2.20) at 5.6 MN/m2 the grade of PP may be repnsented by E ( t ) = 0.238(t)0.114 So, after lo00 seconds, ~ ( t=) 0.523% After 10 cycles in the given sequence (t' = 1500 seconds) x=lO
[ ( 1 . 5 ~ ) ~. "(~1 . 5 ~ l)0."4] = 0.691%
~ ( 1 . 5x 104) = (0.523) +OS23 x= 1
Then if a straight line is drawn from the point 0.523, lo00 to 0.691, 1O,o00 on Fig. 2.4 then this may be extrapolated to 1% strain which occurs at approximately t = 9 x 16 seconds. This is the total creep time (ignoring recovery) and so the number of cycles for this time is (9 = I ~ ) / ~ O = O 900 O cycles Notes
lo00 cycles
~ ~ ( 1 x. 5106) = 0.495% ~ ~ ( 1x. 5106) = 1.018%
1500 cycles
~ ~ ( 2 . 2x 5106) = 0.5329% ~ ~ ( 2 . 2x 5106) = 1.056%
Equivalent modulus after 900 cycles = 5/0.01 = 500 MN/m2
458
zyxwvutsr zyxwvuts zyxwvutsr zyxwv Solutions to Questions
1
C
'E s 3i
_____
zyxwvutsr zyxwv zyx 100
101
i o ~ 103
105
104
i o ~ 107
Total creep time
(2.45) For the PP creep curves in Fig. 2.4, n = 0.114 at Q = 7 MN/m2, ~ ~ ( 2 . 1x6 104) = 0.99% after 11 cycles of creep (10 cycles of load removal), t = 66 hrs = 2.37 x 1 6 s. (using equation in text or from computer p g r a m ) ~ ~ ( 2 . 3x71 6 ) = 1.105% A line joining 0.99, 2.16 x 10' to 1.105, 2.375 x lo6 on Fig. 2.4 allows strain at 365 days (ie 365 days @ 6 hrs per day = 7.88 x lo6 seconds) to be extrapolated to 1.29%. The computer program predicts ~ ~ ( 7 . 8x8lo6) = 1.294%
at
u = 8.4 MN/m2, ~ ~ ( 2 . 3x7lo5) = 1.406% and ~ ~ ( 2 . 1x6104) = 1.26%
Extrapolation on Fig. 2.4 to 7.88 x 106 seconds gives ~ ~ ( 7 . 8x8106) = 1.62%. Computer program gives ~ ~ ( 7 . 8 8x) lo6) = l . a % Extrapolation between these two values to get ~ ~ ( 7 . 8x8106) = 1.5% gives u = 7.8 MN/mZ. So since
u = PD
2h '
h=
0.5 x 150 = 4.8 mm 2 x 7.8
For continuous loading for 1 year (= 3.15 x 5.08 MN/m2 which gives h = 7.38 mm So material saving =
(2.46)
lo7 s)
7.38  4.8 = 35% 7.38 = uoei(@+a) E
=
the design stress would be
z
As shown in the previous question, the governing equation for this type of Standard Linear Solid is given by: 52
tj
rl
51
&+E=+

zyxwvu zyxwvut zyxwvu zyxwvu z
Solutions to Questions
459
,o,$w+d)
Dividing across by &oeic* and letting E* = 
&Od=
then E* is given by
E* =
61P
i
+ tlh
(h + 62) + w
i
Multiplying top and bottom by the conjugate of the denominator,
E2 tans== EI
(61
+ h M l V  6162vo + h.2)+ q 2 3 h
51h01
(2.47) The straight line graph of stress against log (time) confirms the relationship
}
Att=800,u=60 SO, B = O.467(MN/m2)' A t t = 8 . 9 ~1 @ , ~ = 4 5 A= 1.225 x l@ s
(2.48) ZhurkovBueche equation gives t = toe(uOro)/m
comparing this with t = ABu t = toeu0IRTand B = y/RT
zyxwvu zy zyxwvutsr zyxw zyx zyxwvutsrq zyxw Solutions to Questions
460 so
to=
1.225 x 1015 = 2.22 x 10l2 s 150 x Id (8.314 x 293)

A
(2)
Also y = BRT = 0.467 x 8.314 x 293 x
= 1137.6 x
m3/mol
so at u = 44 MN/m2, T = 40°C t = 2.22 x 1012exp
150 x
Id  1137.6 x
x 44 x 106
8.314 x 313
= 1.06 x 16 s
(2.49) 3 years = 0.95 x 108 seconds From Fig. 3.10 creep rupture strength = 8 MN/m2 Using a safety factor of 1.5 the design stress = 8/1.5 = 5.33 MN/m2 for the pipe, hoop stress = pR/h OS( 100) 5.33 = h h = 9.4 mm
(2.50) The critical defect size in the material may be caalated from K1, = ~ ( 7 ~ a , ) ” ~ ac
= 3.18 mm  (1)’: 20 IC 2
1(1/2)m
tf = c(uyJr(1/2)m(m  2) {ai
2
3.15 x 10’ = ai
3 x 1011(20)3.2(1.2)~1.6 = 0.631IU II r p =  1(  ) KI, 2n uy
ABS,
‘P=
polypropylene,
rp = (o‘2)2 = 6.37 mm
(0*13)2
2n
 (3.18 x I O  ~ )  O . ~ )
zyxwv =(0.023)2
(2.51) acrylic,
2n
 a,1(1/2)m}
2n
 2.69 mm
(2.52) Using fracture mechanics
Kl, = u(nac)”2
 0.084 mm
zyx zyxwvu zyxwvut zyxwvu zyxwvut zyxwvu 461
Solutions to Questions
Table 3.1 gives KI,for acrylic as 0.9  1.6 MN/m"") a, =
(g)2= 0.08 mm (up
to 0.25
mm)
So inherent flaw sizes are probably in the range 0.16 mm0.5 mm.
FL (2.53) Stress range = 60 FL Stress amplitude = mean stress = 120 To allow for mean stress use
a, = Uf
{1
zyxw
z}
.. . . . .(1)
Now at 1 x lo7 cycles of = 16 MN/mz also 1 x lo7 cycles at 5 H f represents 2 x I d seconds
a, = 42 MN/mz
so
16 FL 2 120 x 42 F = 16.13 N
FL 120
so (2.54) Bending stress = MY I so
1 xd/2 32 a , = =  N/m2
but
a,
nd4/64 nd3 32 x 0.75 a, = N/mz nd3 'Uf
(1 
2)
x 0.75 (32 nd3 ) = 25 '* ('  nd3 x 35 x 106
2*5
d = 11.43 mm
so if Kf = 2 2.5 x
x 0.75 (32 nd3 )=
(1  nd3 x 35 x 106
d = 13.1 mm (2.55) uf = 43.4  3.8 log lo7 = 16.8 MN/m2
At 5 Hz,lo7 cycles would take 2 x 106 seconds
zyxwvuts zy zyxwvuts zyxwvut zyxwv zyxwv zyxwvut Solutions to Questions
462
from (3.1) t = 1.225 x 1015e0.467u~ So a,  43.3 m / m 2 Now
a,=' 0 °
n( 10)2
a,== My I
so
 6.37 MN/m2
= 10.2
64M(5
1 0 6 (~N / ~ Z )
K(io x 103)4
(12)
U,Uf
(
6.37 x 2) 16.8 x 106 l1.8 43.3 M = 0.32 Nm
2 x 10.2 x 106M =
(2.56)
4(Pe)r nT4 P  4(Pe)r Minimum stress = 2nr2 I& a,,+afi, P a, = =2 4nr2
Maximum stress =
a, =
P +zr2
a,,
+Per d
 a& 2
aa=uf (1$)
zyxwvu zy uf = 43.4  3.81og(l x lo8) = 13 MN/m2
At 10 Hz,10" cycles would take lo7 seconds so from t = 1.225 x a, = 39.9 m / m 2
so
'(
(
2.5 x 2 2nr2 3p + ! 2~1.4 E~)=13~106
from which P = 235.7 N
(2.57)
lOI5 exp(0.467ac),
+ 3.5 = 1 + 2(c/0.25)"*
+
1  2.539.9 x lo6 (G P E)) 4m2
Kt = 1 2(c/r)'I2
+ c = 0.39
(2.58) 4.5 kg = 44.145 N (i) loss of energy due to friction, etc = (44.145)(0.3  0.29) = 0.44 J (ii) energy absorbed due to specimen fracture = (44.145)(0.29  0.2) = 3.973 J impact strength =
3.973 = 165.5 kJ/m2 (12 x 2)104
(iii) Initial pendulum energy = 0.25 x 44.145 = 11.036 J
zyxwvut zyxwvu zyxwvut zyxwvu zyxw zyxwvut zyxw zyxw 463
Solutions to Questions
Loss of energy due to friction + specimen fracture = 0.44 + 3.947 = 4.414 J Remaining energy = 11.036  4.414 = 6.6218 J 6.6218 So height of swing = = 0.15 m 44.145 (2.59) K =
so where so (2.60)
[
p(m~)'/~ 1.12  0.23 (t)+ 10.6 (t)' 21.7 Wh 1.75 x lo6 =
[f
(R x
100 x 5 x 106
(3' +
io x 1 0  3 p
(31=
P = 4.89 kN
K , = D&
+ a, =
(E)1 K
= 8.15 mm
from equation (3.28)
N=
 (25 x 106)o.66) 2((8.15 x 103)0.66 2 x 106(10)'%'.66(1.32)
= 57,794 cycles = 16.05 hours I (l/Z)n
[((?lZ :)
 a i1(1/2)n
2 (2.61)
N=
c0"7&2(2
 n)
1
30.4
(
464
zyxwvut zy zyxwvut zyxwv zyxwvu zyxwv zyxwvut Solutions to Questions
da dN
from the graph  = 2 x
(AK)2.513
0.256
 (20 x 106)o.S
u2.513
XU2  2 ((E)x 106 x ~ ' . ~ (  0 . 5 1 3 )
2x
(I
= 2.13 MN/mz
zy
(2.62)For a sheet, K = u f ( ~ a ) ~ / ~ where uf = fatigue limit. Knowing K this would give the critical defect size, a,, in the material. Equating this to the critical version of the expression for the pressure vessel u ~ ( x u , ) ' /=~ 2 0 e ( k c ) ' / 2 ue= us
(5) ($) = 10
Now,
P=
= 0.627 MN/m2
2 x 4 x 0.627 = 41.8 kN/m2 120
(E (3'"
K, = u(xu,)'/~
(2.63)
tan

P 1/2 43 = 5 (1.05) 30 x 5 P=49kN (3.1) The energy absorbing ability of a material is given by
Hence the following table may be drawn up
a2/2E
E
U
~
I
Carbon (HS) Carbon (HM) Kevlar EGlass SGlass
I
2.9 2.2 3.0 2.0 3.3
I
230 380 130 80 91
I
1.83 x 0.64 x 102 3.46 x io2 2.5 x lod2 6.0 x
From this table it may be seen that carbon fibre has low energy absorbing capability compared with the other fibres. However, the other fibres are not as stiff. Hence it is
zy zyx zyx
Solutions to Questions
zyxwv zyxwv 465
quite common to use hybrid fibre composites, eg glass and carbon fibres in order to get a better combination of properties.
(3.2) It is necessary to calculate the volume fraction for each of the fibres. Firstly for the carbon 20 1800 = 0.181 vfc= 20 30 50 1800 2540 1300 Similarly for the glass fibres
++
30 20 1800 Hence, using the rule of mixtures
++
pc = 0.181(1800)
2540 30 2540
50 1300
= 0.192
+ 0.192(2540)+ 0.627(1300)
= 1629 kg/m3
(3.3) p f = 1800 kg/m3, p, = 1250 kg/m3, p, = 1600 kg/m3 Using rule of mixtures
= P f V f + Pm(1 V f ) 1600 = 1800Vf + 1250(1  V f ) ~c
V f = 0.636
to get weight fraction W f = PfV f Pc
w,
hence
= E ( 0 . 6 3 6 ) = 0.716 1600
= 0.284
Weight ratio W,: Wf = 0.284: 0.716 Hence for 1 kg epoxy, the weight of carbon = 2.52 kg (3.4) Using rule of mixtures
+ pmV, = 2540(0.5) + 1250(0.4) = 2024 kg/m3 E , = E f V f + E,V, = PiO(0.6) + 6.1(0.4) = 50.44 GN/m2 K , = K f V f = 1.05(0.6) + 0.25(0.4) = 0.73 W/m”K p, = p f V f
zyxwvut
(3.5) Using the rule of mixtures
E, = E f V f
Also,
but
+ E,(1
a, = OfV, E,
+ 6(0.6) = 51.6 GN/m2
 V f )= 120(0.4)
+4
= E, = Ef
1  Vf)
466 so,
zyxwvutsr zyx zy Solutions to Questions
(3.6) In the composite
zyxwvuts zyxwvuts zyxwvut zyxwv
(3.7)
Since
ie
so
= 60(25)0.3 + 60(0.7) = 492 MN/mz
Also
Ec = EfVf
+E m ( 1 
Vf)
= (76 x 0.3) + z ( 0 . 7 ) = 24.93 GN/mZ 25
(3.8)
0)
VI2
= Uf V f
+ um(l  V f ) +
= (0.23M0.58) 0.35(0.42) = 0.28
(ii)
+
+
El = E f Vf EmVm = 230(0.58) 3.8(0.42) = 135 GN/m2 EfEm (230)(3.8) E2 = = 8.8 GN/mz V f E , VmE/ (0.58)(3.8) (0.42)(230)
+
UZI
= VIZ = 0.28

(g)
= 0.02
+
zyxwvu 467
Solutions to Questions
zyxw zyxwvutsrq zyxwv
(3.9)The local compliance matrix is
and Q = S  '
Then
8.81 105 S = 2.72 x 5.44 x 105
 [
Directly by matrix manipulation E,
= 2.238 x
E,
= 7.578 x
lo4
Alternatively using the Constitutive Equation Approach
[
1
m2/MN
yxy = 2.241 x
and
A=D.h
zyxw zyxwv
5.44 x 10~ 4.05 x 1.70 x 104
2.72 10~ 1.04 x 4.05 x 105
2.78 x 104 1.17 x 104 1.16 x 104 104 2.06~104 8.624~ld 1.16 x lo' 8.62 x Id 1.45 x lo'
A = 1.17 x Also, a = A' (since [B] = 0)
1 1
5.87 105 1.81 x 105 3.63 x 105 6.99x 2.7 x lo' mm/N 1.81 x 1.13 x 104 3.63 105 2.7 x 105 1 1 1 ai2 G,, =  uxy = , u p = Ex = a,, . h' =a U . h' m*h' a11 E, = 11.3 GMN/m2, E , = 9.53 GN/m2, Gxy= 5.8 GN/m2 vxy = 0.308
vYr = 0.259
For the applied Fomes N , and N ,
[ ] [ 21 (= [ "1 YXY
E,
= 2.238 x
= a. NXY E,
= 7.578 x
a.
h Y
.h )
a12 a22
zyxw
yxy = 2.241 x
468
zyxwvut zy Solutions to Questions
(3.10) The properties of the ply in the fibre and transverse directions are
El = 200 GN/m2 E2 = 11 GN/m2
zyx
G12 = 8 GN/m2 ~ 1= 2 0.32
The local compliance matrix is
S=
zyxw zyx zy zyxwv I zyxwv and
0
0

1
(312
??=e'
S o , G = T ; ' . Q . T E and Then
[ ;]
]:[
=s.
YXY
 [
3.13 x
S = 6.45 4.28
x
105
6.45 x 7.42 x 3.15 x 105
Directly by matrix manipulation ex = 2.507 x
E,
Q=S'
TXY
4.28 x 3.15 x 1.05 x 104
m2/ MN
yxr= 3.424 x
= 5.164 x
and
Ex = 31.9 GN/m2, E, = 13.5 GN/m2, Gxy = 9.5 GN/m2, vXy= 0.206,
vYx= 0.087
Alternatively using the Constitutive Equation Approach
A=Qh 7.2 x 10" 1.19 x 105
2.42 x 1 6 7.2 x 10" 5.22 x 104 4.48 x 10" 1.19 x 1 6 4.48 x 104 8.09 x 10"
 h3 D=Q.
12 8.07 x 10" 2.4 x 104 3.99 x 10" 2.4 x 104 1.74 x 104 1.49 x 10" 3.99 x 10" 1.49 x 104 2.69 x 10"
1
N/ IIUII
1
NIIIIII
zyx zyxwvut zyxwvu zyxwvu 469
Solutions to Questions
zyxw zyx zyxwvu I,;[zyxwvu I;[
a = A' 3.22 x 2.14 x 3.71 x 1.58 x mm/N 1.58 x 105 5.27 x 105 d := D' 4.7 105 9.68 x 106 6.42 x 105 d = 9.68 x 1.11 x 4.73 x (Nmm)' 1.58 x 104 6.42 105 4.73 x 105 1 1 1 a12 a12 v,, = up =E , =  E , =  G all . h ' a22 a22. h' x y  a66. h all E, = 31.9 GN/mz, E, = 13.5 GN/m2, G,, = 9.5 GN/m2
1.56 x a = 3.22 x 2.14 105
[
[
1 1
v,, = 0.206,
vp = 0.087
It may be Seen that these agree with the previous values. For the applied Force N,
[;,I
=a.
E, = 5.164 x = 2.507 x For the applied Moment M, = 180 Nm/m E,
K,
= 8.46 mI,
K,
.")
(=a.
= 1.743 mI,
v,, = 4.854,
yxy = 3.424 x lop3
K,,
= 12 m',
v,, = 0.206
It may be seen that when the moment is applied, the major Poisson's ratio sponds as it should to the value when the inplane stress, a,, is applied.
LJ, corre,
(ii) If an additional moment My is applied, then the D and d matrices do not change and so once again
K,
= 6.04 mI,
vYx= 0.23,
K,
= 26 ml,
K,,
= 23 m'
vxY= 4.32
(3.11) (i) Symmetric (ii) Nonsymmetric (there is an uneven number of plies) (iii) Symmetric (could also be written as [0/90/45/  4531  453/45/90/0], (3.12) This is treated as a 4 layer situation with = 0.7, hi = 0.2, h2 = 0, h3 = 0.2, h4 = 0.7 mm
For
zyx
zyxwvutsr zyx zy zyx zyxwv zyxwvu
470
Solutions to Questions
]
Material A
 [4.16; Id 1.66 x Id Q1 = 1.66 x Id 4.16 x Id 0
0 0
1.25 x

and
Q4=81
As the laminate is symmetrical, B
Id
[
0

Q3 = a 2
= 0 and
4
A=
[ [
Eaf.(hf  hf1)
Material B
683.5 239.5 , Q 2 = 239.5 683.5 0
0]
222.2
a = A'
and
f=l
:] :
4.44 ld 1.76 x Id N/mm 1.76~Id 4 . 6 4 ~Id 0 1.33 x Id 2.67 104 1.06 x 104 a = 1.06 104 2.67 x 104 0 7.46 x 104
A=
;
The strains are then obtained from
[ 21 [ $1
I.
=a.
N*Y
YXY
ey = 8.257 x
ex = 3.028 x
lod3,
and the stresses are given by
zyxw yxy = 0.016
Stresses in Material A
, a = 26.38 MN/m2
a,, = 39.45 MN/m2
ray = 19.6MN/m2 Stresses in Material B ah = 4.04 7hY
MN/m2
oby = 6.36 MN/m2
YXY
thy= 3.48 MN/m2
(3.13) Compliance Matrix
S=
0
0

1
G 2
Stamss Matrix
zyx zyxwvut zyxw zyx
Solutions to Questions
zyx zyxwvu 47 1
Overall SrifSness Matrix
Overall Compliance Matrix

Q = T i ’ .Q .T,
S = Ql
The Extension Stiffness Matrix is then obtained from [AI = 0.@(60)
which gives
+ 0.4Q(30) + 0.4Q(O)+ 0.4Q(30)+ 0.4Q(60)+ 0.4Q(90)
[
:]
1.36; 16 4.19 x 104 A = 4.19 x 104 1.36 x Id 0 4.71 x 104
N/mm
As [B] = 0 in this symmetric laminate, the compliance matrix is obtained by inverting [A]
a = A’
[
8.10; a = 2.49 x
2.49 x 8.10 x 0
2.11 x 105
The stiffness terms in the global directions are (for h = 2.4 mm)
1 E, = all . h’ 1
E, = a z z . h’
E, = 5.14 x 104 MN/m2 E , = 5.14.104 MN/m2
1
zyxwvutsrqpon
G,, =  G,, = 1.96.104 MN/m2 a66. h’ a12
v, = ,
a1 I
a12 v, = a22 ’ and the strains may be obtained as
E,
V,
= 0.308
V,
= 0.308
cy = 5.98
= 1.94 x
(3.14) Using the S and Q matrices to calculate 8
A= f=1
yxy
and
D, . (hf  hf,),
= 1.12
107
for each layer, then a = A’
472
zyxwv zyxw zyx
zyxwvuts zy zyxwvu zyxwv Solutions to Questions
[ 21 [ $1 =a
EXY
=a
[ :]
NXY
 H whereH=fullthicknessoflaminate
NXY
ey = 1.286 x
cX = 8.989 x
;
yxy = 1.774 x
lop4
Note, to assist the reader, the values of the terms in the matrices are
[ [
:
4.65 1 6 2.47 x 10s A = 2.47 x ld 2.82 x 10s ]N/m 0 2.81 x 1 6 4.03 a = 3.54 x
(3.15)
E=
zyxw
3.54 x 6.65 x 0
3.54 x 106
Taking the xdirection as the hoop direction ax =
pr
7=
3x600
= 600 m / m 2
pr 3x600 a,== 300 MN/m2 2t 6
From the data given Compliance Matrix
Stifiess Matrix
S=
0
0

1
G 2
Overall Stifiess Matrix
Overall Compliance Matrix

S(e) = Q(e)l 1 d 2.71 x Id
Q(0) = Ti' * Q * TE
9.82 x 103 6.95 x 2.21 x 104 7.91 x ld 2.71 x Id 7.91 x Id 7.50 x Id
1
The Extension Stiffness matrix is then given by
;+
[
A = 2 *Q(60) 2 *Q(60)
+
6 *Q(O) 2.35 105 4.25 x 10" A = 4.25 x 10" 1.37 x 10s 0 4.80 x 104
The compliance matrix is obtained by inverting [A]
[
;
4.49 a = 1.39 x
a = A' 1.39 x 7.70 x 0
2.08 x 1 6
Solutions to Questions
zy zyxwvut 473
and the strains may be obtained as
zyxwvuts zyxwv zyxw
zyxw 1
ex = 0.023 or 2.34
= 0.015 or 1.5% Yxy
=0
(3.16) (a) This is a symmetric laminate and the 8.77 x 104 2.98 x 104 2.98 x 104 2.22 x 104 4.31 x 10" 1.35 x 10"
terms are as follows: 4.31 x 104 1.35 x 104 2.96 x 104
8.77 x 1O4 2.98 x 1O4 4.31 x 1O4 2.98 x 1O4 2.22 x 1O4 1.35 x 1O4 4.31 x 104 1.35 x 104 2.96 x 104
1 1
8.77 x 1O4 2.98 x 1O4 4.31 x 1O4 2.98 x 1O4 2.22 x 1O4 1.35 x 1O4 2.% x 104 4.31 x 104 1.35 x 104 8.77 x 104 2.98 x 104 4.31 x 104 2.98 x 104 2.22 x 104 1.35 x 104 4.31 x 104 1.35 x 104 2.96 x 104 The A, B, D matrices are
1
4
A=
ZQf. (hf  hf1) f=1
So that with ho=o.2,
h1=0.1,
h*=0,
h3=0.1,
hq=0.2
zyxw
The A, B, D matrices and hence the al, d  l , matrices may be determined as:
a=
;
5.25 105 7.06 x 105
1.18 x 104
0
7.06 x 105 2.07 104 0
5.58
8.42
103
105
5.59
103
4.18 x 103 7.62 104
1
474
zyxwvuts zy Solutions to Questions
Then using
zyxw zyxwvut
(b) T h i s laminate is unsymmetrical. In the above analysis, D2 and D3 are reversed and this has the effect of making [ B I Z 0. The matrix values are.
[ [
3.51
; ;
10'' 1.19 x 10'' 10'' 8.88 x lo3
A = 1.19 x
5.75 105 a = 7.15 x
0
1.18 x 104
7.15 x 105 2.07 x 0 9.74 x 105
)
0 0 863.8 0 0 271 0 863.8 271 1.91 x 104 0 0 3.49 x 105 b=[ 0 0 1.91 x 104 3.49 x 105 0 0 0 1.91 x 10" 3.49 x 105 0 0 1.91 x 104 3.49 x 105 467.9 159.3 D = (159.3 118.5 0 0 1.58.2 4.31 103 5.36 x 103 d = 5.36 x 0.016 7.30 x 103 0 B=(
:)
;
[
1
zyx zy
Using the above equation relating strains and curvatures to N and M we get Ex
= 2.3 x
K~
= 0,
K~
= 2.86 x = 0 and
K~~
= 7.67 x
yxy = o
mm'
The difference in this case therefore is that we start to see some twisting of the laminate due to the nonsymmetric nature of the layup.
zyxwvu zyx zyxw zyx zyxwvut
Solutions to Questions
415
zyxwvut
(3.17) This is a nonsymmetric laminate. The Q matrices are given in the text and the
A , B and D matrices are determined from 3
A=
CQf. (hf  hf1)
f=1
 E x 
CY YXY
Kx Ky Kxy
zyxwvu zyxwvutsrqponm  a11 a21

ab1 ~
I
I
a12 ai6
bii
a22
b21
a26
b12 bn
bib
 N,
b26
Ny
a62
a66
bbi
b6z
bM
Nxy
b12
bla
dii
d12
d16
M,
h b
d21
d22
d2b
BM
d61
db2
da
hl
a2
bbl
b62

My
Mxy
where N x = 30 N/mm
476
zyxwvuts zy zyxw zyxwvu Solutions to Questions
(
D=
236.0 47.7 47.7 50.3 29.3 13.9
29.3 13.9 47.2
1 zyxwvu zyx 4.65 x 8.37 x lob3 8.00 x 0.031 2.68 103 8.00 x 4.65 x lob3 2.68 x low3 0.036
(3.18) (a) Maximum Stress Criterion The local stresses are given by
61T = 20.1,
62T = 0.52,
a2
01
312 = 1.36 r12
As the second term is less than 1, a tensile failure in the 2direction would be expected. (b) Maximum Strain Criterion
From the data given
= 2.49 x w 3 ,
22T
= 5.84 x 10 5
= 3.777 x io3,
p12 = 7.14
gZc = 5.66
10~
The 12 strains are given by
IT
g2T = 0.5,
 = 24.9, 91
92
"'  1.36 nz
Hence once again a failure is predicted in the 2direction. (c) 'hiHill Criterion
The TsaiHill equation gives
Therefore failure is predicted.
(3.19) (i) For an applied stress of a, = 1 MN/m2,the stresses in the 12 direction are given by
GtT
&T
01
02
 = 1867,  = 200,
212 = 92.4
r12
Hence an applied stress of a, = 92 MN/m2 would initiate a shear failure before tensile or compressive failures occurred.
zyxwvu zyxwvu zy
zyx
zyxwvu zyxw zyxwvut zyxwvutsrq 3 zyx
Solutions to Questions
477
(ii) Maximum Strain Criterion From the data given
ilT
$IT
32T
E l
E2
=  = 0.035, i 2 T =  = 5.56 x
iZc = 32c  = 0.011
$IC dlc = = 5.5
E l
E2
.. = ?12 = 0.01
y12
GI2
Also,
[I] [
so
=s
[
=
 = 92.4 YlZ
E2
E1
105
?12
i2T = 253,
;IT
 = 2082,
[ EJ]
zyx
Hence once again a stress of a, = 92 MN/m2 is the limiting condition. (iii) TsaiHill Criterion Letting X be the multiplier for a,
(x z ) 2  (x+)?
+
z)2(F)2
(
+
=1
Solving for X gives X = 83.8. Hence the limiting condition is a, = 83 MN/m2.
(3.20) Let N, = 1.2 N/mm (ie a, = 1 N/mm2). By calculating the matrix [a] we get (for 30" ply).
[
F]
1.235
[ [ [ 3 [ 3 [ 3&] = 102483
=a
Then
=T,
ZIT
~ 2 3 7 9 , E1
x 105
zyxw =
x
?12
  3624,
Ek
 =606
E2
Y12
Hence the limiting condition is a, = 606 MN/m2. Also,
[:]=Q,["] TXY
and YXY
[::]=To[:] r12
TXY
478
zyxwvuts zyxwv Solutions to Questions
which gives
[
[
0.787 = O.CW] 0.148
MN/m2
zyxw zyx zyxwvu zyxw TI2
Hence the Maximum Stress Criterion also predicts 6, = 606 MN/m2 as the limiting condition. For the TsaiHill Criterion, letting X = multiplier on stress a,, then solving
gives X = 583. This predicts a stress of ax= 583 MN/m2.
If this is repeated for all the plies then we get
Table 1 Maximum permissible values of a,, to cause failure in each PlY
zyxwvut zyxw
MaKstressorMax.
'l$aiHIu
Strain
e = 0" 9 = 30" e = 30"
a, = 1201 MN/mz a, = 606 h4N/mz a, = 606 m / m 2
a, = 1067 a, = 583 ax= 583
The limiting condition is thus ax= 583 MN/m2 as predicted by TsaiHill. (3.21)
(E (s))
K , = a(~a,)'/~
tan
zyxwv 'I2
'/2
=% Wbr a c ) ' / 2
(E (g))
P
tan
43 = (Z x 5 x 30 x 5 P=49kN (3.22)
CSM: K , = a(n~,)'/~ + a, =
N=
112 (1.05)
13.5 1 (=)  = 9.06 x 103 m a
2((9.06 x 103)5.35 (lo00 x 106)5.35) 3.3 x 10'8(80)12.7fi.3s(10.7)
= 3 x 1 6 cycles
zy zyxwvut zyxwvu zyxwvu
zyxwvuts zyxwv 479
Solutions to Questions
so in a similar way
a, = 34.9 x
Woven Roving:
N = 1.14 x lo6 cycles
(4.1)
QD
= 1/2n2D2NHsin4cos4
= 1/2n2(50 x 103)2(100/60)(2.4x 103)sin 17.7~0s17.7
= 1.43 x
QP
m3/s
nDH3 sin24 1%
=
(f)
(2.4 x 103)3sin217.7 12(200)
n (50 x 
zyxwvuts zyx = 1.67 x
Total flow = QD
 Qp
m3/s
= 1.26 x
m3/s
The shear rate in the metering zone will be given by
.
ZDN C O S 4  TT (50 X H
v d
y==
H
w3)(1OO/60)COS 17.7 2.4 x 103
ZrPR4  KP (4.2) For the die, Q = 8Lv
for the extruder. x lo00 x 50 x 100 6n x 200 x = 171 h4N/m2 60 x (2.4)2 x 0.3191
Pmax
=
Qmax
= 1/2n2D2NHsin4cos4 = 1.436 x
m3/s
From graph, operating point is P = 43 MN/m2,Q = 1.075 m3/s
New operating point is
P = 85 MN/m2,Q = 1.075 m3/s (4.3) Extruder: Qmax = 1/2n2D2NHsin 4cos 4 = 1/2n2(25)' = 2.98 x
(2)
(2)sin 17'42'cos 17"42'
m3/s
480
Solutions to Questions
(g)
6~(25)(500)
(400 x
22 x tan 17’42’
= 123 MN/mz
Die:
zy
zyxwv zyxwv zyxwvutsr zyxwv 
Q=2{$}P
lod6)
Hence the characteristics shown may be drawn. The operating point is at the intersection of the two characteristics.
Output, Q = 2.13 x (4.4)
but
m3/s
Q = 1/2lsdNH sin qi cos qi  nDH3 sin’ qi ( 1 3
zyxwvu zyx
Solutions to Questions
48 1
zyxw zyxwv zyxwvu 0
Q = 1 / 2 d N H sin4cos4 
so
nDH3 sin’# 12q
.Qq
KIL
AH sin 4 cos 4 1 +BH3sin2q5
nD
A = 1/2x’D2N and B = 
where
12LKl
so
_  (1 +BH3sin’4)AH(2cos24 1) AHsin~cosQ,(2H3Bsin~cos~) dQ =O (1 BH3 sin24) d4 
+
+ BH3 sin’ 4)(2 cos’ 4  1) = 2H3Bsin’ COS' 4 (1 + BH’ sin’ 4)A sin 4 cos 4  AH sin 4 cos 4(3BHz sin’ 4) dQ =O (1
Also
dH
so
(1 + BH3 sin24)
(1 + BH3 sin’ 4) = 3BH3sin24
Using (2) in (1)
zyxw
(3BH3sinZt$)(2cos2(b 1) = W3Bsin24cos’4 thus
(3BH3sin2 COS 24) = W 3 Bsin’
(1)
COS' Q,
2cos24 = 2cosz4 + 3(1  2sin24) = 2(1  sin24)
(2)
482
zy zyxwvu zyxwv Solutions to Questions
which can be solved to give 4 = 30" Also
(4.5)
[l + BH3sin24] = 3BH3sin24
zyxwvu zyxwv
F = nR2P0 (L) = 1r(0.25)~(50x lo6) m+l = 2.26 MN
AB = l o o m
(4.6) A
zy
CBA 150 How ratio = =  = 50 3 3 Clamp force =lrR2Po
100
= 1.06 MN
(4.7)
(9 (ii)
c.s.a. 1/41rd
IrD
s.a.
0.250
DC = Dtan lo",BC = D / c o s 10"
+ D2 tan 10"= D2(1 + tan 10") s.a. = 20 + 2D/ cos 10 + 2 0 tan 10" c.s.a. o z ( 1 + tan 10") s.a. 2D(1 + (cos + tan lo") C.S.U.
=d
= 0.268 D (iii)
FG = (D/4)tan3Oo c.s.a. = d(l.5)/4tan30° s.a. = 6(D/2)
c.s.a. _s.a.
=3 0
8tan30
 0.216 D
zyxwvu zyxwvu zyxw 483
Solutions to Questions
c.s.a. = d
/ 2
s,a. = 2 0
+D = 3 D
zyxwv zyxwv zyxwvutsr zyxw zyxwvut zyxw  _ OZ
c.s.a. s.a.
Vd = 2 7 5 m=
(4.8)
60
2 n x 0.15 x 5
= 0.078 m/s
60
Q = 2000 kghour = 0.3% x
but
Q = H W V d SO H =
= 0.167 D
m3/s
0.396 x = 5.04 mm 1 x 0.078
x = d(5.04 4.5)150 = 9 mm
w = 1.786 (ie x / H )
Now
so
(4.9) For
P,
3 x 1.5 x 104 x 0.078 (3.57  0.64(1.786 5.77(0.33))) 4.5 x 103 = 0.93 MN/m2
+
=
Ho = 0.8, x =
Jm = 10.9 mm, w = 5.45
= 24.3 MN/m2 (same equation as above) H~ = 1.2 mm, , P = 4.9 m / m 2 Ho = 1.6 mm, , P = 0.86 MN/mZ
P,,
For For For
H o = 1.9 mm, , P
= 0.073 MN/mz
(4.10) Initial volume of sheet = ($)4=750Z
Since the dome formed is a free surface it m a y be assumed to have a constant thickness, t Final volume =
(T) t
nOZ t = 7roz b t = 2 mm 2
(4.1 1)
CY
= tan'
($) = 80.54'
L = 35 um, to = 3 mm H = 3Otanb = 180 a 1
rb
= 0.58 mm
484
zyxwvuts zyx Solutions to Questions
zyxwv zyxwvuts zyxw zyxwv
When sheet just touches the base S, = (D(1
+ cosa)/ sina)  R = 40.82
Lc = 40.27 mm and thus t~ = 0.48 mm
so
zyxw zyxwv
(4.12) (a) BsH = 1.8 So Parison thickness = 1.8 x 2 = 3.6 mm
= 1.34, Parison diameter = 38 x 1.34 = 50.98 mm
BsT = (b) h =
GThd
(2)
= (1.34p x 2 x
(5)
= 2.62
2uh 2 x 10 x 2.62 = 0.75 MN/m2 (c) P =  70 Dln die gap OMD=2 (4.13) OTD film thickness x (blowup)*
so &Ib&
= 2.24 x 99 = 221.76 mm
ZDb Lay flat width = = 348.3 mm 2
zyx zyxwvu zyxwvu 485
Solutions to Questions AP =
(4.14)
6qVL(2h  H ) H3
(s) zyxwvut (z) zyxw (s) zyxwvut zyxwv zyxwv zyxwvu  6 x 100 x 0.5 x 6 x 102(0.6 0.5)103 (0.513
109
= 14.4 MN/m2
(4.15)
= exp
= exp
where a = k/pC, = thermal diffusivity and H = wall thickness = 1/B
28.4 x 8.6 x lo% 300  250 = exp 300  23 3 x 103 x 230 t = 484.4 s = 8.07 minutes
mass 150 x volume = = 1200 P
(4.16)
X R ~ H=
so,
H=
Also
3qv2 8nFH4
t = 
150 x 103 x 109
1200
zyxwv
150 x 106 = 1.77 mm a x 1200 x (150)2
3 x 104 x (150 x = 19 s 8a x 106 x 100 x 103 x 1.774 x (1200)2
(5.1)
.
Also
m3
e
e
a
40x5
y==
e
200
r(N/m2)
500 lo00 ~
2000
374.5 749 1498 3745 7490 14980
105 105
0.57 1.25 2.56 7.36 17.0
2.85 103 6.25 x 103 1.28 x 3.68 x 8.5 x 102
1.31 x 1.2 x 1.17 x 1.02 x 8.8 x
42.0
0.21
7.13 x 104
A graph of q vs. r gives
r = 1 x lo4 N/m2 and q = 8 x 104 Ns/m2
105 105
104
486
zyxwvutsr zyxwvut zyxwv zyxwv zyxw Solutions to Questions
(5.2) For a Power Law fluid
y a (r)""
so, or
Q a (AP)'/"
l o g e o< l/n log AP
So the slope of a graph of (log Q) against (log A P ) will be a straight line of slope l/n if the Power Law is obeyed. From the attached graph l/n = 1.268 SO n = 0.7886 Consider the point, Q = 0.8 kglmin and AP = 5.2 MN/m2. r = H ( A P ) 2L
x 5.2 x 106 =  2 x 210~ x 50 x 103
los N,m2
Pressun drop I MN I rnz 1
+ 1 ) 6Q =
NOW?= (2n
3n
so
TH2
+
(2(0.7886) 1 ) 3(0.7886)
(
60 x 0.94 x 6 x 22
= 3863 sl
zyxwv zyxwvutsr zyxwvu zyxwvuts zyxwv zyxwvut
Solutions to Questions
487
zyxw zyxw zyxwv
(5.3) Cone and Plate
0.062 x 180 True shear rate, i, =  = = 1.18 S' a 3n 3T 3 x 1.18 Shear Stress, r = = 10.7 kN/m2 2nR3 2n x (37.5 x 103)3 Ram Extruder .
4Q 4 x 70 x = 89.1 s' nR3 7c x Q = 70 x 109 PR 3 . 9 ~l e x 1 r== = 60.9 kN/m2 2L 2 x 32 y==
Q = 200 x 109
1:
4 x 200 x 109 = 254.6 sl 109
5.7 = 89.1 m/,,,2 2 x 32
but r = roV
(
(60.9)  = 89.1 ) n 89.1 254.6
So n = 0.362 and TO = 11.98 Now the cone and plate gives true shear rate whereas the ram extruder uses apparent shear rate. The NonNewtonian correction factor is = 0.69 3(0.362) 1 Therefore the true shear rate on the cone and plate is equivalent to a shear rate of 0.69(1.18) = 0.817 on the ram extruder
+
At
i, = 0.817 r = 11.98(0.817)0.362 = 11.13 kN/m2
11.13  10.7 = 4.06% 10.7 (5.4) If the material is assumed Newtonian and the shear rates are equated then % difference =
6Q2 =THz
4Ql nR3
4TH2Qi Qz = 6nR3 If the material is NonNewtonian then the true shear rates should be equated
zyxwvuts zy zyxwvutsrq zyxwvut zyxwvutsrq zyxwvuts zyxwv zyxw zyx zyxwvuts Solutions to Questions
488
So for n = 0.37 correction factor = 0.9094 Error = 1  0.9094 = 0.0906 + 9.06%
Now
i, 01 Q and r a
and
Po( r then P a Q"
so
for
Correction Factor =
01
Q"
((3 (23
n = 0.37 Factor = 0.%55
Error = 1  0.9655 = 0.0345 + 3.45% 4 x 2.12 x 106 = 100 s' nR3  n(3 x 103)3 4Q
(5.5)
y=
From flow curves
r]
so
= 1.3 x I d Ns/mZ,G = 3 x 104 Nlm'
G
1.3 x 103 = 4.3 x 3x104
v
n(3
'I
Natural time =  = Dwell time =  =
Q
103)2 x 37 2.12 x 106
s
103
= 0.5 s
So flow is mostly plastic.
y =   6Q
6 x 0.75 x lo' TH2  (5 x 103)(1 x
(5.6) From flow curves
r]
= 0.9 s
= 2 x 10" Ns/m', G = 1 x 10" Nlm' tl Natural time = = 2 seconds G
so
Dwell time = 1 second so flow is predominantly elastic. (5.7)
n 4
Q = A V =  x 25' x y. =   6Q

TH~
x 50 x
6 x 24.54 x x 25 x 103 x 1 x 106
= 24.54 x
= 1953 S'
From flow curves at y = 1953 s', r = 3.2 x 1 6 N/m2.
PH
T=+P=
2L
3.2 x 1 6 x 2 x 30 = 19.2 MNlm' 1
m3/s
zyxwvuts zyxwvu zyxwvut zyxwvuts 489
Solutions to Questions
(5.8) Flow rate = 3 d m i n
Area = 2 ((15
Q=
zyxwv
+ 15) + n(8.3))
3 x 112 x 106
60
p =  6Q
T H ~ (30
m2
= 112 x
= 5.6
106m3/s
6 x 5.6 x + 26) x 22 x 109
= 150 S' from flow curves, at
9 = 150 sl, r = 1.5 x
2Lr AP==
H
105 N/m2
2 x 10 x 1.5 x 105 = 1.5 MN/m2 2
Power = P Q Power = 1.5 x lo6 x 5.6 x = 8.4 Nmls (= 8.4 W)
The temperature rise A T is then given by 1.5 x 106 = 0.45"C 3 . 3 x 106
AP AT==
pc,
(5.9) Flow rate = 3 d m i n
zyxw
+
Area = (30 x 2) 2( 13 x 2) = 112 x
Q=
3 x 112 x 106
60
y. =  6Q
TH2

m2
zyxw
= 5.6 = lob6 m3/s
6 x 5.6 x (30+26) x 22 x
= 150 S'
from flow curves, at 9 = 150 s', r = 1.5 x 10s N/m2
2Lr 2 x 10 x 1.5 x 16 AP= = 1.5 MN/mZ H 2 Power = P Q = 1.5 x 106 x 5.6 x = 8.4 N d s = 8.4 W
zyxwvuts zyxwvut zyxwvuts zyxwvu zyxwvu zyxw zyxwvutsrq zyx
490
Solutions to Questions
From flow curves, at 9 = 150
G = 3.05 x 104 N/m2
SO,
YR = T/G = 4.92
From graphs for swell ratio BST = 1.41, BSH = 1.99 Thus approximate dimensions of extrudate would be 42.3 mm deep x 21.2 mm wide x 3.98 mm thick.
y. =  6Q
TH2 6 x 46 x (n x 30)(1.5 x 103)2
= 1.3
So from the flow curves, at
103 sl
= 1300 sl
r = 2.6 x 16 Nm2 G = 5 x IO4 Nrn' T
YR
=  = 5.2
G
From swell ratio curves at
YR = 5.2, BST = 1.41, BSH = 2
zyxwv
(g) ( 0.33/1.33
L=
100
106
104
(f)
0.33/1.33
= 355 mm
zyxwvut zyx zyxwvu zyx zyxwv
zyxwvut
Solutions to Questions
so
49 1
AT= 7'3T~ =12860 = 0.62 + Fo = 0.295 = atf TI T2 17060 X2 0.295 x O S 2 x tf = = 0.74 seconds 107 1 0 0 x 106 3 x 104
zyxw
6 x 0.74 x 0.333 x 1.33 2.32 x 1.99 x 1.662
For a Newtonian fluid, n = 1 112
L=0.13(:)
100 x 106 x 0.74 1.2 x 102
H=0.13 120  50 230  50
 0.39
(5.13)
AT=
so,
Fo = 0.48 =  where x = 1 mm
= 80.6 mm
= 101.9 mm
at
X2
0.48 x 1 x = 4.8 seconds 1 x 107 T3 T2 9030  0.3 AT=Ti  T 2 23030 t=
(5.14)
at
Fo = 0.58 = X2
0.58 x (2 x 1092 t= = 23.2 s 1 x 107 for the runner, AT also equals 0.3 so Fo = 0.29. To cause freezeoff in 23.2 seconds then 1 x 107 x 23.2
zyxwvu zyxwv z zyxwvutsrq 0.29 =
R = 2.83 mm
R2
runner diameter = 5.66 mm
(5.15) Since the power law equations are going to be used rather than the flow curves, it is necessary to use the true shear rates. ie
'
=
3n
+1
4Q
)(
3(0.35)+ 1
(7 a=) ( 4(0.35)
4x5x 1.53 x 109
II x
= 2.76 x 104 s'
Now r = rei." = 40 x IO3 (2.76 x 104)0'35 = 1.43 MN/m2 PR 2Lx So P =  = R 2L (5.16) Volume flow rate,
Nowr=
XR*H e=t

(60
2 x 25 x 1.43 1.5
= 47.8 MN/m2
103)2 (3 x 103) = 3.39 x 1 0  ~m3/s 1
492
zyxwvuts zy zy zyxwvut zyxwvutsr zyxw zyxw Solutions to Questions
From Fig. 5.3, qo = 3 x 104 NdmZ (ie q at 1; = 1 sI) and n = 0.33. So from illustrative example (5.3)
= 1.05 MN/mz 114  50 AT=170  50
(5.17)
 0.531 + Fo = 0.35 = at X
gate depth = 2x = 1.85 mm
Now
+=6Q + T =  6Q THZ
yH2

6x4x x lo9 = 1.26 m m loo0 x 3 x 1(1.85)3
From Fig. 5.3 at 1; = lo00 s', r = 2.9 x 10s N/mz PH 2Lr sop== 2L H
r=
2 x 0.6 x 2.9 x 1 6 = 0.19 MN/rnz 1.85
(5.18) Ho = HI +2Ltana
Ho = 0.5 +3Otan3" = 2.07 mm T = x D = 4 O x = 1261~n
zy
6 x 10 x = 1910 S' 126 x 103(0.5 x lO3)2 Z
h=1910(%)
= I 1 1 s',
1 ~ ~ = 3 ( l l l ) t a n 3 " = 2 s ~ ' ~ u ~ = 0 . 4 5 M N / m Z
&z = i h t a n a = 1/3(191O)tan3"= 33 s' + uz = 7.5 MN/mZ For the tapered section, Po =
4+(qA)'I2
+
(313 1)
 4 x lll(1150 x 2.25 x
= 3.6 MN/mz
1.99
zy zyxwvut zyxwvut zyxwv zyxwvuts 493
Solutions to Questions
0.66tan 3"
2n tana
= 6.3 MN/mZ
PE = 1/2a,(1 
($.)*)= 1/2x 7.5 (1  (
s)2)
= 3.53 MN/m2
Parallel Section,
zyxwvu zyxwvutsr zyxwvutsrq 2 x 6 x lov3x 3.6 x 105 = 8.6 MNlm2 0.5 x 103
2Lt
p,==
H
Total Pressure loss = 22.1 MN/rn2
At exit,
so
i, = 1910 So t = 3.6 x lo5 N/mZ,G = 5 x
lo4 N/m2
36
yR =  = 7.2 + BH = 2.43,BT = 1.56
.5
So wall thickness = 1.21 mm, diameter = 62.4mm (5.19)Assuming no swelling at the die exit .
6V
6 x 15 x = 120 sL 0.75 x 103
y==
H
From the flow curves, t = 1.3 x Id N/mz G = 3 x 104 N/m2 So yR = r/G = 4.4 and SO BH = 1.85,BT = 1.36
. .
New H = New V = 15 x
0.7s x 103 = 0.41 x 1.85 x 1.85 x 1.36 = 37.7 x
6 x 37.7 x 0.41 x 103
so,
y=
T h i s gives
T = 2.2 x
so,
yR = 5.5
m m/s
= 552 s'
105 N/mZ, G = 4 x 104 N/m2
and BH = 2.08,BT = 1.455
0.75 x 13 = 0.36 x lod3m 2.08 = 45.39 x New V = 15 x 2.08 x 1.455 x 6 x 45.39 y= = 756.6 s' so, 0.36 And so on until the iteration converges, at which point New H =
H = 0.405 x
m, D = 29.2 m m
mls
494
zyxwvuts z zyx zyx zyxwvut zyxwv zyxwv
(5.20)
Solutions to Questions
6 x 100 x y =  6Q = 764 sl THI II (250 x 103) (1 x 103)’
so from flow curves T = 2.4 x le N/m’
2Lr 2 x 5 x 2.4 x le p,, =  = = 2.4 MN/mZ H 1 H3 = H2 2Ltana (where a = 1/2 angle)
+ H3 = 1 + 2(12)tan(l)” = 1.42 IIUII
At
zyx zyxw
Bz, i/ = 764 S’, L. = 1/3j.tana
= 1/3(764)tan( 1) = 4.45 s’
so
P,, = 2n tana [ l 
 2.4 x
105
2(0.33) tan(1) = 4.3 m / m 2
P& = 2 2 [I 
(37 [
 (L)””] 1.42
(3’1
1 x 106 =2 [I= 0.25 MN/m’
(A)’]
Total Pressure loss = 6.95 MN/m2 6Q y== THZ
At die exit,
6 x 100 x n(250 x 103) x (1 x 103)’
= 764 sl
From flow curves, T = 2.4 x I d N/m’
G = 4.1 x 104 N/m2 T
yR==
G
2.4 x le = 5.85 4.1 x 104
From swelling ratio curves BSH = 2.19 and BST = 1.48
so
Bubble thickness = 1 x 2.19 = 2.19 mm Bubble diameter = 250 x 1.48 = 370 mm
Solutions to Questions (5.21)
zyxwvu zyx 495
zyxwv zyxw zyxwv zyxw
Po = 4j,(r]A)1/2(3n 1)
4 x 600(4 x 1 6 x 2.25 x 1.w
2Lr pSI  =
x 2.4 x I d = 2.4 MN/m2 2 x 103
+
2x
H
PE =
(1

(
$)2)
= 11.4 MN,m2
zyx
( (y)')
= 1/2(43.6 x lo6) 1 
= 19.8 MN/m2
Total pressure loss = 58 MN/m2 (5.22) (a) As shown in the text, the flow rate of a power law fluid in a circular section is given by
Now for a volume flow rate, Q, the volume in any increment of time, dt, is Qdt and this is equal to nR2de Qdt = nR2dC
So from (1)
496
so
zyxwvuts zy zy Solutions to Questions
(b) If the crosssection is freezingoff then the radius of the channel will be changing with time and is given by
So since
ie
zyxwvut zyxwvut
(5.23) From the equations in the previous example
For a Newtonian fluid. n = 1 so .tf/t= 0.316 For a NonNewtonian fluid, n = 0.3f!,/e = 0.424 (5.24) (a) As shown in the previous examples, if the pressure is held constant
but So substituting for .t gives
140 x 106
1/13
7.53 x 105 t0.76!3
zyxwvu zyxwvu zyxwvut
zy zyxwvuts zyxwv z zyxw
Solutions to Questions
497
(b) As shown in the text for the flow of a power law fluid in a capillary
2q@
but
..
=
(3n + 1 ($)
nnR3n+l
Qdt = rR2de SO d e = (Qdt)/ZR2)
2q0@ =
2q0Q"dt =
3 d P . nR2 . R3"+' (m) nn
(e) ltR3n+3. dP
which may be. integrated to give 2
ioq7 10511.3 n(5 x 103)3.9
0.3
(6%)
= (29.36t) MN/mz The variations of Q and P in each case are shown in the attached graph.
498
zyxwvuts zy zyxwvu Solutions to Questions
zyxwvu zyxw zyxwv zyxwv m3
(5.25) Volume of cavity = 50 x 10 x 3 x
So time to fill this = 1.5 seconds Gate: volume = 2 x 4 x 0.6 x lo' m3 seconds So time to pass through = 4.8 x
.
6Q TH2
y==
x lo9
6x
4 x 22
= 375 s'
From flow curves, r = 2.1 x 10s N/m2
2Lr p== H
..
2 x 0.6 x 2.1 x 1 6 = 0.13 MN/m2 2
Runner: volume = ~ ( 4x)20~x time to fill this = 1 second
m3
zyxwvut .
4Q
y==
4 x 1x
x lo9
x(4I3
xR3
= 20 s'
2 x 20 x 7.6 x 104 = 0.6 MN/m2 5 Sprue, etc: time to pass through = 1 second pressure loss = 0.6 MN/m2
so
t = 7.6 x
lo4 N/m2 + P =
Total time to fill = 1 + 1 + 1.5 = 3.5 seconds Now, as shown in previous example, for a constant flow rate situation the pressure buildup in the machine is given by
For PE,n = 0.33 and qo = 3 x 104 (from flow curves)
Therefore after 3.5 seconds P = 4.7 MN/m2. But Pressures losses = (0.6 + 0.6 + 0.13) = 1.33 MN/m2 So packing pressure = 3.37 MN/m2 Tt  T m Ti  T m
(5.26) The temperature gradient, AT = 70  20 AT=190  20
 0.29
From Fig. 5.23, t=
0.29 x (1.5 x 1 x 107
= 6 ~
Solutions to Questions
zy zyxwvut zyxwvu 499
zyxwvut
Since the hauloff speed is 0.4 m/s, the water bath would need to be at least (0.4 x 6) m long ie 2.4 m. (5.27) Using the equation derived in the text:
zyxw zyxwvut L
n(n
+ 1)’
where the freezeoff time may be calculated from 4~’ t f = ln AZCY
;[
()I
4
TmT~ Tf  T M
Using the data given, the flow ratios will be Material
Flow Ratio (LIH)
LDPE polypropylene polYStyrene
240 220 165
POM acrylic polycarbonate
121 86 32
60
PVC
nylon 66
30
123
ABS
zyxwv
Note the qo and n data from Table 5.2 has been used even though the temperatures quoted are not always the same as the moulding temperature. h = BiThd
(5.28)
BST={
so
(2)
2.5 x 100 2 x 4 0 = 1.46
From Fig. 5.1 1 at BST = 1.46, YR = 5.5 = t / G From the flow curves the value of shear stress to give r/G = 5.5 is 7 = 2.25 x 1 6 N/m2 (also G = 4.1 x 104 N/m*). From the flow curves at T = 2.25 x 1 6 N/m2, 6Q 9 = 620 = + Q = 52 x
TH2
2uh p== Dm
2 x 2.5 x 4 x 100
lo6
m’/s = 147 kghour = 0.2 x
lo6 N/m2
So the suggested pressure would cause melt fracture. (5.29) Stress = pL = 730 x 9.81 x 0.4 = 2.86 x 104 N/m2
From flow curves A = 2.25 x 1 6 and E = 4.6 x 104
500
zyxwvutsr zy zyxwvu zyxw zyxw zyxwv zyxw Solutions to Questions
So characteristic time = A/E = 4.95
Also E = pL
so
(& + i) = 730
1 4.6 x 104 k 2.25 x 1@ 6L = 0.044 x 0.4 = 0.017m = 17 mm x
9.81 x 0.4
[2
x
(5.30)For the overall change of temperature and pressure q / q R = l@AT+BAP
For acrylic,
,,IqR
= 10[(28.32~40)+(9.54~50)110~ = 4 53
Similarly for the others V / q R = 0.95,1.415,2.03and 1.28,
Also for
q/qR A '
= 1, AAT
BAP
 =   28'32  2.97 MN/m2"C AT 9.54 Similarly for the others, ( A P ) / ( A T )= 1.17,1.87,3.07and 1.93 For acrylic
Index
zyxwvu
zyxwvu zyxw
ABS, 3, 11, 16, 20, 26, 33, 131, 135, 149, 283, 295, 308 Acetal, 4, 14, 59, 61, 76, 149, 418 Acrylic, 4, 15, 33, 34, 59, 90,124, 136, 149, 283, 308 Activation energy, 136 Alloys, 11 Aminos, 17 Amorphous, 4, 15, 137, 405,420 Antioxidants, 3 Antistatic agents, 3 APC, 8, 328 Apparent shear rate, 371 Apparent viscosity, 352, 371 Aspect ratio, 171 Atactic, 418 Autoclave moulding, 332 Axial stress and strain, 219,430
Bakelite, 2, 17 Bearings, 29 Bending stiffness matrix, 197 Biot number, 393 Blister forming, 307 Blow moulding, 268, 304, 385, 387 Blowup ratio, 267 BMC, 334 Boltzmann’s Superposition Principle, 95 Breaker plate, 250 Brittle behaviour, 135 Buckling of ribs, 79 Bulk modulus, 57
Calcium stearate, 3 Calendering, 313, 315 Capillary viscometer 369 Carbon fibres, 28, 39, 168, 181, 189, 192, 228, 233, 328 Carreau, 352 Celluloid, 2 Cellulose, 1 Centrifugal casting, 337 Charpy impact, 152, 155, 157 Chemical resistance, 5 Chopped fibres, 329 Chopped strand mat, 329 Clamping forces, 293, 326, 401 Clamping systems, 284 Coefficient of friction, 28, 72 Coefficient of thermal conductivity, 31 Coefficient of thermal expansion, 33, 61 Coextrusion, 275 COI, 34 Cold drawing, 44 Cold press moulding, 332 Complex modulus, 111 Compliance, 52 Compliance matrix, 183 Composites, 8, 168, 327 Compression moulding, 323, 334 Compression zone, 246 Compressive modulus, 57, 68 Concentric cylinder viscometer, 370 Cone and plate viscometer, 369 Conicylindrical dies, 357
50 1
502
zyxwvuts zy
Contact moulding, 330 Copolymer, 4 19 Corrugation design, 81 Coupling agents, 3 Coupling effects, 200 Coupling matrix, 196, 209 Crack extension force, 122 Crazing, 137 Creep, 24, 41, 86, 88, 93, 232 Creep compliance, 52 Creep contraction ratio, 58 Creep failure, 134 Creep fracture, 25, 134, 136 Creep modulus, 49, 87, 88, 106 Creep rupture, 25, 134 Critical fibre length, 227 Critical flaw size, 133 Critical oxygen index, 34 Critical volume fraction, 176 Crosslinked polyethylene, 13 Crosslinking, 5, 170, 326 Crystalline polymers, 4,405,420 Cyclic frequency, 110, 140 Deborah number, 368 Degradation, 26 Degree of polymerisation, 2 Density, 22, 30,67, 171 Desirability factor, 39 Die entry losses, 360, 382 Die swell, 363, 383 Dielectric strength, 32 Distribution tube system, 292 DMC, 9, 304, 324,334 Drag flow, 252, 274 Drape forming, 307 Drawdown, 267,270, 382 Dual sheet forming, 309 Ductility, 24 Ductility factor, 133 Dynamic loading, 110 Effective creep modulus, 106 Elastomers, 9, 10 Electrical properties, 32, 173 Electromagnetic interference, 33 EMI, 33, 299 Empirical analysis, 103 Endurance limit, 141 Energy, 18
Index
Engineering plastics, 6 Environmental stress cracking, 27, 135 Epoxides, 17, 173 Equivalent section, 67 ESC, 27 EVA, 11, 26 Extenders, 3 Extensional flow, 359 Extensional stiffness matrix, 196, 205, 209 Extensional strain rate, 345, 388 Extrudeddie characteristics, 257 Extrusion, 246, 377 Extrusion blow moulding, 268 Extrusion coating, 273 Extrusion stretch blow moulding, 272
Fatigue, 5, 26, 138 Fatigue limit, 141 Fatigue of composites, 238 Feed zone, 246 Fibres, 3, 25, 168 Filament, 328 Filament winding, 330, 337 Fillers, 3, 169 Film blowing, 265, 379 Filter pack, 250 Fire retardant, 34 Flame retardants, 3 Flammability, 34 Flashing, 293 Flexural modulus, 10, 22, 45, 57 Flow coefficient, 260 Flow defects, 375 Fluorocarbons, 5 Foam, 9,26, 68, 298 Folded chain theory, 421 Fourier number, 391 Fractional recovery, 104 Fracture, 119, 131 Fracture mechanics, 121. 145, 154 Freezeoff time, 397 Friction. 28 Fringed micelle model, 421 Gas injection moulding, 299 Gates, 286 Gelcoat, 330 Glass fibres, 25, 28, 39, 168, 173, 231, 233
Index
zyxwvut zyx zyxwvu
Glass transition temperature, 30, 117 GMT, 8, 328 Granule production, 264 Grp, 25, 28, 29, 238, 330 Hand layup, 330 HDPE, 12, 135, 308 Heat transfer coefficient, 393 Hoop strain, 219,430 Hoop stress, 65, 219, 272,429 Hot press moulding, 333 Hot runner moulds, 290 Hydrolysis, 26, 283
Imaginary modulus, 112 Impact, 147 Impact behaviour of composites, 240 Injection blow moulding, 303 Injection moulding, 278, 330, 338, 377, 392,404 Injection stretch blow moulding, 273 Insulated runner moulds, 291 Interfacial shear strength, 227, 231 Interference fit, 64 Intermittent loading, 95 Isochronous curves, 48 Isometric curves, 48 Isotactic, 418 Izod impact, 152 Kelvin model, 87 Kevlar, 9, 168, 190, 233 Lag angle, 110, 112 Lamina analysis, 182 Laminate analysis, 202 Latent heat of fusion, 405 Lateral strain ratio, 58 LCP, 12 LDPE, 12, 26, 33, 132, 135, 308 Leakage flow, 255 LEFM, 121, 145, 154 Linear elastic fracture mechanics, 127 Liquid crystal polymers, 12 LLDPE, 12, 26 Load transfer fibre length, 227 Longitudinal modulus, 179 Loss factor, 112, 114 Loss modulus, 112
503
Loss tangent, 112, 114 Lubricants, 3
zyxw
Matched die forming, 309 Material selection, 22 Maximum strain criterion, 233 Maximum stress criterion, 233 Maxwell model, 85, 112 Mean effective pressure, 294, 401 Mean stress, 143 Melt flow index, 373 Melt flow rate, 373 Melt fracture, 375 Metallocene, 13 Metering zone, 246 Mixing zones, 248 Modulus, 20, 39, 41, 47, 59, 67, 283 Molar gas constant, 136 Monomers, 2 Mould clamping force, 293 Moulds, 285 Muenstedt polynomial, 353 Multidaylight moulds, 290 Multilayer materials, 218 Multilayer mouldings, 66
Natural time, 368 Neck ring process, 272 Negative forming, 306 Newtonian flow, 346, 367 Nip gap, 313 NonNewtonian flow, 35 1 Nonsymmetric laminates, 223 Nozzles, 283 Nylon, 4, 13, 26, 28, 34, 64,135, 149, 171,228, 261, 283, 295, 418
zyx
Olefinics, 16 Optical properties, 34 Orientation, 424 Oxidation, 26, 27 Parison, 268 Parkesine, 2 PBT, 8, 11. 15 PEEK, 7, 8, 15, 27, 28, 174, 177, 181, 189. 328 Permeability, 35 Perspex, 2
504
zy zyxwvutsrq zyxwvuts Index
PET, 8, 11, 15, 269, 283. 308 Phase lag, 110 Phenol formaldehyde, 17,326 Phenolics, 8, 17 Pigments, 3 Plane strain, 126, 132, 154,428 Plane stress, 130, 132, 154, 427 Plastic zone, 133 Plasticisers, 3 Plastics, 1, 3 Plate constitutive equations, 197, 210 Plug assisted forming, 307 Plunger injection moulding, 280. 376 Poisson’s ratio, 57, 58, 59, 126, 173, 183,426
Polyamide, 5, 13, 283 Polyamideimide, 7 Polyarylether, 7 Polycarbonate, 4, 9, 10, 16, 26, 34, 283, 295, 308
Polyester, 5, 15, 17 Polyether sulphone, 16, 28, 59 Polyetheretherketone, 7, 15 Polyetherimide, 7 Polyethernitrile, 7 Polyethylene, 3, 4, 7, 12, 32, 269, 283, 295, 392,416
Polyimide, 7 Polymerisation, 2, 3 Polymers, 1, 3 Polymethylene methacrylate, 4, 15, 59, 417
Polyphenylene, 5 Polyphenylene oxide (PPO), 8, 9, 16 Polyphenylene sulphide, 7, 28 Polypropylene, 2, 5, 7, 9, 10, 13, 20.47, 54, 58, 59, 66, 71, 118, 135, 269, 283,295 Polystyrene, 2, 4, 15, 34, 59, 130, 149, 283, 295.418 Polyurethane, 16, 17, 26 Polyvinyl chloride, 3,4,7, 15, 33,44,59, 135, 149, 269, 283, 295, 308,417 Positive forming, 307 Power law, 293, 351, 396, 399,403 Pressure bag moulding, 33 1 Pressure flow, 254, 234 Pressure forming, 308 Profile production, 264 Pseudoelastic design, 53 PTFE, 1, 15, 28, 32, 33, 417 Pultrusion, 330, 337
PVC, 3, 4, 7, 15. 33, 44, 59. 135, 149, 269,283,295,308,417
PVDF, 26,28
Rabinowitsch correction factor, 372 Ram extruder, 371 Reaction injection moulding, 302 Reactive extrusion, 278 Real modulus, 112 Reciprocating screw injection, 28 1 Recoverable shear strain, 345 Recovery, 24,43, 87, 89,94 Reduced time, 104 Refractive index, 34 Reinforcement, 3 Relaxation, 42, 87, 89, 93 Relaxation modulus, 49 Relaxation time, 87, 367 Relaxed modulus, 51 Residence time, 367 Residual strain, 109 Resin injection, 335 Resistance, 32 Retardation time, 88 Rheological models, 35 1 Rib design, 74
RIM,302
zyxw zyx
Rotational moulding, 3 18 Rotational viscometer, 369 Roving, 328 RRIM, 302 Rule of mixtures, 173, 226 Runners, 287. 377 Safe working stresses, 135 S A N , 34
Sandwich mouldings, 66,298 SCORIM, 301 Screws, 282
Secant modulus, 21. 55 Semicrystalline, 4, 11 Sharkskin, 375 Shear modulus, 57, 59, 68. 180, 183, 217,345
Shear rate, 344 Shear stress, 345 Shear viscosity, 345 Shellac, 1 Shift factor, 116 Short fibre composites, 226
Index
zyxwvut zyx 505
zyxwvu
Shrinkage, 4 Shutoff nozzles, 284 Single ply analysis, 182 Sizing, 169 Skin forming, 307 Slush moulding, 323 SMC,9, 33, 334 Snap fits, 71 Specific heat, 31, 391 Spherulites, 423 Sprayup moulding, 331 Sprues, 288 Stabilisers, 3 Standad linea^ solid, 92, 112 Static electricity. 3 Static fatigue, 134 Stiffness, 18, 23, 38 Stiffness matrix, 184 Storage modulus, 112 Strain, 19.42, 85,203,426 Strain energy release rate, 122 Strain rate, 20, 85, 152, 344 Strain transformation matrix, 186 Strength, 18,37, 173,232 Strength of laminates, 236 Stress, 19, 42, 85, 203 Stress concentration factor, 121, 148 Stress intensity factor, 127, 146 Stress relaxation, 25,42 Stress transformation matrix, 185 Structural foam, 9, 26,68,297 Superposition principle, 95 Swelling ratios, 270,363, 384 Symmetric laminates, 203 Syndiotactic, 418
Tietemperature superposition, 116 Toughness, 26, 154, 155, 283 Tow, 328 TPR, 10 Tracking, 32 Transfer moulding, 326 Transverse modulus, 179 Triaxial stresses, 149,427 TsaiHill criterion, 233 Twin screw extruders, 262
Unidirectional composites, 182, 188 unidirectional plies, 202 Unrelaxed modulus, 51 Urea formaldehyde, 17
zyxwvut zyxwvut
Tangent modulus, 21 Tensile modulus, 57, 59, 171, 345 Tensile strength, 22, 171 Tensile viscosity, 345, 387 Thermal conductivity, 31, 173, 391, 393 Thermal diffisivity, 3 1, 391 Thermal strains, 61 Thermal stresses, 61 Thermofonning, 306, 309 Thermoplasticrubber, 10, 16 Thermoplastics, 3 Thermosetting plastics, 5 , 7, 17, 170, 304, 328
Vacuum bag moulding, 331 vacuum forming, 306 Vacuum injection, 336 Van der Waals forces, 3 Vent wne, 249 Venting, 288 Viscoelasticity, 25,42, 84 Viscosity, 42, 344 Voigt model, 87 Volume fraction, 171 Vulcanisation, 10
Waveform, 142 Wear, 5,28 Weathering. 27 Wedge shaped die, 362 Weight fraction, 171 Williams. Landel and Ferry, 117 W L F equation, 117
XLPE, 13
Yam,328 Yield locus, 132 Young’s modulus, 20, 426 Zener model, 92 Ziegler Natta catalysts, 13
zyxwvu
This book presents in a single volume t properties and processing behaviour o The aim is to give engineers and understanding of basic principles wkhout the unduly complex levels of mathematics or chemistry set plastics in their proper context as engineering makri
zyxwv
This textbook pioneered the approach whereby botn 1, and processing of reinforced and unreinforced plastics ai: LO in a single volume. It assumes no prior knowledg emphasises the practical aspects of the subject. In this third edition over half the book has been rewrit been updated and reorganised. introduction to the types of plastics and describe how a designer goes for a particular application. Later chap more advanced aspects of mechanica polymer melt flow. All techniques dev numerous worked examples, and proble each chapter  the solutions to which
zyxwvutsr zyxwvut zyxwvu
Contents 0 General properties of plastics 0 of plastics Mechanical behaviour of c plastics 0 Analysis of polymer melt Structure of plastics and Solutions to
zyxwvut zyxwvuts
An imprint of Elsevier
www.bh.com
Suenee